#------------------------------------------------------------------------------
#$Date: 2017-02-07 17:13:06 +0200 (Tue, 07 Feb 2017) $
#$Revision: 191892 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103538.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103538
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.5 La3 Nb0.5 O14'
_chemical_formula_weight         1070.65
_chemical_name_systematic        ?
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   8.084
_cell_length_b                   8.084
_cell_length_c                   5.069
_cell_measurement_temperature    293(2)
_cell_volume                     286.9
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         6.8E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.569
_diffrn_measured_fraction_theta_max 0.569
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71070
_diffrn_reflns_av_R_equivalents  0.0424
_diffrn_reflns_av_sigmaI/netI    0.0299
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       4
_diffrn_reflns_limit_l_min       -4
_diffrn_reflns_number            1608
_diffrn_reflns_theta_full        32.00
_diffrn_reflns_theta_max         32.00
_diffrn_reflns_theta_min         2.91
_exptl_absorpt_coefficient_mu    24.163
_exptl_crystal_density_diffrn    6.197
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             474
_refine_diff_density_max         1.263
_refine_diff_density_min         -1.036
_refine_diff_density_rms         0.283
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.01(7)
_refine_ls_extinction_coef       0.108(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.003
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     39
_refine_ls_number_reflns         408
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.003
_refine_ls_R_factor_all          0.0311
_refine_ls_R_factor_gt           0.0308
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0750P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0796
_refine_ls_wR_factor_ref         0.0800
_reflns_number_gt                405
_reflns_number_total             408
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-6.8cad4.cif
_cod_data_source_block           6.8cad4
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

Saulius Gra\<zulis
;
_cod_original_formula_sum        'Ga5.50 La3 Nb0.50 O14'
_cod_database_code               2103538
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La La -0.42868(8) 0.0000 0.0000 0.0238(3) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0232(7) Uani 0.50 6 d SP
Ga2 Ga -0.6667 -0.3333 0.4709(6) 0.0220(6) Uani 1 3 d S
Ga3 Ga -0.76526(18) 0.0000 -0.5000 0.0253(5) Uani 1 2 d S
Nb Nb 0.0000 0.0000 0.0000 0.0232(7) Uani 0.50 6 d SP
O1 O -0.3333 0.3333 0.184(4) 0.031(4) Uani 1 3 d S
O2 O -0.4574(10) -0.3072(12) 0.308(3) 0.034(3) Uani 1 1 d .
O3 O -0.7820(11) 0.1458(9) 0.241(3) 0.035(3) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La O3 67.0(5) 3_565 5_445
O3 La O2 106.8(4) 3_565 3_455
O3 La O2 139.7(3) 5_445 3_455
O3 La O2 139.7(3) 3_565 5_455
O3 La O2 106.8(4) 5_445 5_455
O2 La O2 101.8(5) 3_455 5_455
O3 La O1 124.2(2) 3_565 2_455
O3 La O1 79.1(3) 5_445 2_455
O2 La O1 72.5(5) 3_455 2_455
O2 La O1 91.0(4) 5_455 2_455
O3 La O1 79.1(3) 3_565 .
O3 La O1 124.2(2) 5_445 .
O2 La O1 91.0(4) 3_455 .
O2 La O1 72.5(5) 5_455 .
O1 La O1 154.17(9) 2_455 .
O3 La O2 65.4(3) 3_565 .
O3 La O2 79.9(3) 5_445 .
O2 La O2 62.8(3) 3_455 .
O2 La O2 154.89(12) 5_455 .
O1 La O2 66.0(4) 2_455 .
O1 La O2 124.4(5) . .
O3 La O2 79.9(3) 3_565 6
O3 La O2 65.4(3) 5_445 6
O2 La O2 154.89(12) 3_455 6
O2 La O2 62.8(3) 5_455 6
O1 La O2 124.4(5) 2_455 6
O1 La O2 66.0(4) . 6
O2 La O2 138.4(3) . 6
O3 La Ga2 85.9(3) 3_565 .
O3 La Ga2 110.9(3) 5_445 .
O2 La Ga2 30.71(18) 3_455 .
O2 La Ga2 130.2(2) 5_455 .
O1 La Ga2 66.0(5) 2_455 .
O1 La Ga2 109.3(4) . .
O2 La Ga2 32.05(17) . .
O2 La Ga2 165.6(2) 6 .
O3 La Ga2 110.9(3) 3_565 2_565
O3 La Ga2 85.9(3) 5_445 2_565
O2 La Ga2 130.2(2) 3_455 2_565
O2 La Ga2 30.71(18) 5_455 2_565
O1 La Ga2 109.3(4) 2_455 2_565
O1 La Ga2 66.0(5) . 2_565
O2 La Ga2 165.6(2) . 2_565
O2 La Ga2 32.05(17) 6 2_565
Ga2 La Ga2 160.40(3) . 2_565
O3 La Ga1 33.5(2) 3_565 .
O3 La Ga1 33.5(2) 5_445 .
O2 La Ga1 129.1(2) 3_455 .
O2 La Ga1 129.1(2) 5_455 .
O1 La Ga1 102.92(4) 2_455 .
O1 La Ga1 102.92(4) . .
O2 La Ga1 69.20(15) . .
O2 La Ga1 69.20(15) 6 .
Ga2 La Ga1 99.800(13) . .
Ga2 La Ga1 99.800(13) 2_565 .
O3 La Nb 33.5(2) 3_565 .
O3 La Nb 33.5(2) 5_445 .
O2 La Nb 129.1(2) 3_455 .
O2 La Nb 129.1(2) 5_455 .
O1 La Nb 102.92(4) 2_455 .
O1 La Nb 102.92(4) . .
O2 La Nb 69.20(15) . .
O2 La Nb 69.20(15) 6 .
Ga2 La Nb 99.800(13) . .
Ga2 La Nb 99.800(13) 2_565 .
Ga1 La Nb 0.0 . .
O3 Ga1 O3 107.2(6) 4_445 5_445
O3 Ga1 O3 85.9(5) 4_445 1_655
O3 Ga1 O3 162.7(4) 5_445 1_655
O3 Ga1 O3 162.7(4) 4_445 2_565
O3 Ga1 O3 85.9(5) 5_445 2_565
O3 Ga1 O3 83.9(6) 1_655 2_565
O3 Ga1 O3 83.9(6) 4_445 6_655
O3 Ga1 O3 85.9(5) 5_445 6_655
O3 Ga1 O3 107.2(6) 1_655 6_655
O3 Ga1 O3 85.9(5) 2_565 6_655
O3 Ga1 O3 85.9(5) 4_445 3_565
O3 Ga1 O3 83.9(6) 5_445 3_565
O3 Ga1 O3 85.9(5) 1_655 3_565
O3 Ga1 O3 107.2(6) 2_565 3_565
O3 Ga1 O3 162.7(4) 6_655 3_565
O3 Ga1 La 41.9(3) 4_445 2
O3 Ga1 La 98.7(2) 5_445 2
O3 Ga1 La 98.7(2) 1_655 2
O3 Ga1 La 126.4(3) 2_565 2
O3 Ga1 La 41.9(3) 6_655 2
O3 Ga1 La 126.4(3) 3_565 2
O3 Ga1 La 98.7(2) 4_445 .
O3 Ga1 La 41.9(3) 5_445 .
O3 Ga1 La 126.4(3) 1_655 .
O3 Ga1 La 98.7(2) 2_565 .
O3 Ga1 La 126.4(3) 6_655 .
O3 Ga1 La 41.9(3) 3_565 .
La Ga1 La 120.0 2 .
O3 Ga1 La 126.4(3) 4_445 4
O3 Ga1 La 126.4(3) 5_445 4
O3 Ga1 La 41.9(3) 1_655 4
O3 Ga1 La 41.9(3) 2_565 4
O3 Ga1 La 98.7(2) 6_655 4
O3 Ga1 La 98.7(2) 3_565 4
La Ga1 La 120.0 2 4
La Ga1 La 120.0 . 4
O3 Ga1 O2 67.0(4) 4_445 2
O3 Ga1 O2 51.5(3) 5_445 2
O3 Ga1 O2 145.8(3) 1_655 2
O3 Ga1 O2 116.3(4) 2_565 2
O3 Ga1 O2 51.7(3) 6_655 2
O3 Ga1 O2 111.2(2) 3_565 2
La Ga1 O2 47.26(15) 2 2
La Ga1 O2 79.90(12) . 2
La Ga1 O2 148.67(16) 4 2
O3 Ga1 O2 51.7(3) 4_445 3
O3 Ga1 O2 145.8(3) 5_445 3
O3 Ga1 O2 51.5(3) 1_655 3
O3 Ga1 O2 111.2(2) 2_565 3
O3 Ga1 O2 67.0(4) 6_655 3
O3 Ga1 O2 116.3(4) 3_565 3
La Ga1 O2 47.26(15) 2 3
La Ga1 O2 148.67(15) . 3
La Ga1 O2 79.90(12) 4 3
O2 Ga1 O2 94.5(3) 2 3
O3 Ga1 O2 111.2(2) 4_445 5
O3 Ga1 O2 116.3(4) 5_445 5
O3 Ga1 O2 67.0(4) 1_655 5
O3 Ga1 O2 51.7(3) 2_565 5
O3 Ga1 O2 51.5(3) 6_655 5
O3 Ga1 O2 145.8(3) 3_565 5
La Ga1 O2 79.90(12) 2 5
La Ga1 O2 148.67(16) . 5
La Ga1 O2 47.26(15) 4 5
O2 Ga1 O2 102.8(2) 2 5
O2 Ga1 O2 62.7(3) 3 5
O2 Ga2 O2 100.5(5) 4_445 .
O2 Ga2 O2 100.5(5) 4_445 3_455
O2 Ga2 O2 100.5(5) . 3_455
O2 Ga2 O1 117.4(4) 4_445 2_456
O2 Ga2 O1 117.4(4) . 2_456
O2 Ga2 O1 117.4(4) 3_455 2_456
O2 Ga2 O1 62.6(4) 4_445 2_455
O2 Ga2 O1 62.6(4) . 2_455
O2 Ga2 O1 62.6(4) 3_455 2_455
O1 Ga2 O1 180.0 2_456 2_455
O2 Ga2 La 57.0(4) 4_445 4_445
O2 Ga2 La 43.5(3) . 4_445
O2 Ga2 La 107.3(4) 3_455 4_445
O1 Ga2 La 134.80(3) 2_456 4_445
O1 Ga2 La 45.20(4) 2_455 4_445
O2 Ga2 La 43.5(3) 4_445 2_455
O2 Ga2 La 107.3(4) . 2_455
O2 Ga2 La 57.0(4) 3_455 2_455
O1 Ga2 La 134.80(3) 2_456 2_455
O1 Ga2 La 45.20(3) 2_455 2_455
La Ga2 La 75.83(5) 4_445 2_455
O2 Ga2 La 107.3(4) 4_445 .
O2 Ga2 La 57.0(4) . .
O2 Ga2 La 43.5(3) 3_455 .
O1 Ga2 La 134.80(4) 2_456 .
O1 Ga2 La 45.20(3) 2_455 .
La Ga2 La 75.83(5) 4_445 .
La Ga2 La 75.83(5) 2_455 .
O2 Ga2 O3 102.1(4) 4_445 6_556
O2 Ga2 O3 152.0(3) . 6_556
O2 Ga2 O3 59.2(4) 3_455 6_556
O1 Ga2 O3 65.1(2) 2_456 6_556
O1 Ga2 O3 114.9(2) 2_455 6_556
La Ga2 O3 154.7(2) 4_445 6_556
La Ga2 O3 78.9(2) 2_455 6_556
La Ga2 O3 100.17(15) . 6_556
O2 Ga2 O3 59.2(4) 4_445 2_456
O2 Ga2 O3 102.1(4) . 2_456
O2 Ga2 O3 152.0(3) 3_455 2_456
O1 Ga2 O3 65.1(2) 2_456 2_456
O1 Ga2 O3 114.9(2) 2_455 2_456
La Ga2 O3 78.9(2) 4_445 2_456
La Ga2 O3 100.17(15) 2_455 2_456
La Ga2 O3 154.7(2) . 2_456
O3 Ga2 O3 103.6(3) 6_556 2_456
O2 Ga2 O3 152.0(3) 4_445 5_446
O2 Ga2 O3 59.2(4) . 5_446
O2 Ga2 O3 102.1(3) 3_455 5_446
O1 Ga2 O3 65.1(2) 2_456 5_446
O1 Ga2 O3 114.9(2) 2_455 5_446
La Ga2 O3 100.17(15) 4_445 5_446
La Ga2 O3 154.7(2) 2_455 5_446
La Ga2 O3 78.9(2) . 5_446
O3 Ga2 O3 103.6(3) 6_556 5_446
O3 Ga2 O3 103.6(3) 2_456 5_446
O2 Ga2 La 97.8(3) 4_445 4_446
O2 Ga2 La 88.0(4) . 4_446
O2 Ga2 La 157.9(4) 3_455 4_446
O1 Ga2 La 41.87(3) 2_456 4_446
O1 Ga2 La 138.13(3) 2_455 4_446
La Ga2 La 92.930(6) 4_445 4_446
La Ga2 La 139.598(6) 2_455 4_446
La Ga2 La 139.597(6) . 4_446
O3 Ga2 La 105.0(2) 6_556 4_446
O3 Ga2 La 39.46(16) 2_456 4_446
O3 Ga2 La 64.8(2) 5_446 4_446
O3 Ga3 O3 132.9(6) 6 1_554
O3 Ga3 O2 108.5(3) 6 3_454
O3 Ga3 O2 101.2(5) 1_554 3_454
O3 Ga3 O2 101.2(5) 6 5_455
O3 Ga3 O2 108.5(3) 1_554 5_455
O2 Ga3 O2 100.5(7) 3_454 5_455
O3 Ga3 O3 73.5(4) 6 2_465
O3 Ga3 O3 77.7(6) 1_554 2_465
O2 Ga3 O3 177.9(3) 3_454 2_465
O2 Ga3 O3 78.3(4) 5_455 2_465
O3 Ga3 O3 77.7(6) 6 4_344
O3 Ga3 O3 73.5(4) 1_554 4_344
O2 Ga3 O3 78.3(4) 3_454 4_344
O2 Ga3 O3 177.9(3) 5_455 4_344
O3 Ga3 O3 103.1(3) 2_465 4_344
O3 Ga3 Nb 109.9(4) 6 1_454
O3 Ga3 Nb 35.0(2) 1_554 1_454
O2 Ga3 Nb 88.0(4) 3_454 1_454
O2 Ga3 Nb 143.3(3) 5_455 1_454
O3 Ga3 Nb 92.1(2) 2_465 1_454
O3 Ga3 Nb 38.6(2) 4_344 1_454
O3 Ga3 Nb 35.0(2) 6 1_455
O3 Ga3 Nb 109.9(4) 1_554 1_455
O2 Ga3 Nb 143.3(3) 3_454 1_455
O2 Ga3 Nb 88.0(4) 5_455 1_455
O3 Ga3 Nb 38.6(2) 2_465 1_455
O3 Ga3 Nb 92.1(2) 4_344 1_455
Nb Ga3 Nb 106.35(4) 1_454 1_455
O3 Ga3 O1 159.6(5) 6 1_554
O3 Ga3 O1 63.0(4) 1_554 1_554
O2 Ga3 O1 75.5(3) 3_454 1_554
O2 Ga3 O1 58.6(5) 5_455 1_554
O3 Ga3 O1 102.5(2) 2_465 1_554
O3 Ga3 O1 122.4(4) 4_344 1_554
Nb Ga3 O1 90.1(3) 1_454 1_554
Nb Ga3 O1 136.3(2) 1_455 1_554
O3 Ga3 O1 63.0(4) 6 2_455
O3 Ga3 O1 159.6(5) 1_554 2_455
O2 Ga3 O1 58.6(5) 3_454 2_455
O2 Ga3 O1 75.5(3) 5_455 2_455
O3 Ga3 O1 122.4(4) 2_465 2_455
O3 Ga3 O1 102.5(2) 4_344 2_455
Nb Ga3 O1 136.3(2) 1_454 2_455
Nb Ga3 O1 90.1(3) 1_455 2_455
O1 Ga3 O1 105.7(2) 1_554 2_455
O3 Ga3 O3 45.0(2) 6 5_345
O3 Ga3 O3 88.3(5) 1_554 5_345
O2 Ga3 O3 134.4(3) 3_454 5_345
O2 Ga3 O3 118.7(4) 5_455 5_345
O3 Ga3 O3 47.49(18) 2_465 5_345
O3 Ga3 O3 61.8(4) 4_344 5_345
Nb Ga3 O3 74.64(19) 1_454 5_345
Nb Ga3 O3 32.74(18) 1_455 5_345
O1 Ga3 O3 144.14(15) 1_554 5_345
O1 Ga3 O3 107.7(3) 2_455 5_345
O3 Ga3 O3 88.3(5) 6 3_464
O3 Ga3 O3 45.0(2) 1_554 3_464
O2 Ga3 O3 118.7(4) 3_454 3_464
O2 Ga3 O3 134.4(3) 5_455 3_464
O3 Ga3 O3 61.8(4) 2_465 3_464
O3 Ga3 O3 47.49(18) 4_344 3_464
Nb Ga3 O3 32.74(18) 1_454 3_464
Nb Ga3 O3 74.64(19) 1_455 3_464
O1 Ga3 O3 107.7(3) 1_554 3_464
O1 Ga3 O3 144.14(15) 2_455 3_464
O3 Ga3 O3 45.4(4) 5_345 3_464
O3 Nb O3 107.2(6) 4_445 5_445
O3 Nb O3 85.9(5) 4_445 1_655
O3 Nb O3 162.7(4) 5_445 1_655
O3 Nb O3 162.7(4) 4_445 2_565
O3 Nb O3 85.9(5) 5_445 2_565
O3 Nb O3 83.9(6) 1_655 2_565
O3 Nb O3 83.9(6) 4_445 6_655
O3 Nb O3 85.9(5) 5_445 6_655
O3 Nb O3 107.2(6) 1_655 6_655
O3 Nb O3 85.9(5) 2_565 6_655
O3 Nb O3 85.9(5) 4_445 3_565
O3 Nb O3 83.9(6) 5_445 3_565
O3 Nb O3 85.9(5) 1_655 3_565
O3 Nb O3 107.2(6) 2_565 3_565
O3 Nb O3 162.7(4) 6_655 3_565
O3 Nb Ga3 98.0(3) 4_445 4_445
O3 Nb Ga3 31.8(2) 5_445 4_445
O3 Nb Ga3 160.1(3) 1_655 4_445
O3 Nb Ga3 87.2(3) 2_565 4_445
O3 Nb Ga3 54.2(3) 6_655 4_445
O3 Nb Ga3 113.8(3) 3_565 4_445
O3 Nb Ga3 31.8(2) 4_445 4_446
O3 Nb Ga3 98.0(3) 5_445 4_446
O3 Nb Ga3 87.2(3) 1_655 4_446
O3 Nb Ga3 160.1(3) 2_565 4_446
O3 Nb Ga3 113.8(3) 6_655 4_446
O3 Nb Ga3 54.2(3) 3_565 4_446
Ga3 Nb Ga3 106.35(4) 4_445 4_446
O3 Nb Ga3 54.2(3) 4_445 1_656
O3 Nb Ga3 160.1(3) 5_445 1_656
O3 Nb Ga3 31.8(2) 1_655 1_656
O3 Nb Ga3 113.8(3) 2_565 1_656
O3 Nb Ga3 98.0(3) 6_655 1_656
O3 Nb Ga3 87.2(3) 3_565 1_656
Ga3 Nb Ga3 145.124(18) 4_445 1_656
Ga3 Nb Ga3 62.54(3) 4_446 1_656
O3 Nb Ga3 113.8(3) 4_445 1_655
O3 Nb Ga3 87.2(3) 5_445 1_655
O3 Nb Ga3 98.0(3) 1_655 1_655
O3 Nb Ga3 54.2(3) 2_565 1_655
O3 Nb Ga3 31.8(2) 6_655 1_655
O3 Nb Ga3 160.1(3) 3_565 1_655
Ga3 Nb Ga3 62.54(3) 4_445 1_655
Ga3 Nb Ga3 145.124(18) 4_446 1_655
Ga3 Nb Ga3 106.35(4) 1_656 1_655
O3 Nb Ga3 87.2(3) 4_445 2_565
O3 Nb Ga3 113.8(3) 5_445 2_565
O3 Nb Ga3 54.2(3) 1_655 2_565
O3 Nb Ga3 98.0(3) 2_565 2_565
O3 Nb Ga3 160.1(3) 6_655 2_565
O3 Nb Ga3 31.8(2) 3_565 2_565
Ga3 Nb Ga3 145.123(18) 4_445 2_565
Ga3 Nb Ga3 62.54(3) 4_446 2_565
Ga3 Nb Ga3 62.54(3) 1_656 2_565
Ga3 Nb Ga3 145.123(18) 1_655 2_565
O3 Nb Ga3 160.1(3) 4_445 2_564
O3 Nb Ga3 54.2(3) 5_445 2_564
O3 Nb Ga3 113.8(3) 1_655 2_564
O3 Nb Ga3 31.8(2) 2_565 2_564
O3 Nb Ga3 87.2(3) 6_655 2_564
O3 Nb Ga3 98.0(3) 3_565 2_564
Ga3 Nb Ga3 62.54(3) 4_445 2_564
Ga3 Nb Ga3 145.123(18) 4_446 2_564
Ga3 Nb Ga3 145.123(18) 1_656 2_564
Ga3 Nb Ga3 62.54(3) 1_655 2_564
Ga3 Nb Ga3 106.35(4) 2_565 2_564
Ga2 O1 La 111.3(5) 2_566 .
Ga2 O1 La 111.3(5) 2_566 2_565
La O1 La 107.6(5) . 2_565
Ga2 O1 La 111.2(5) 2_566 4_455
La O1 La 107.6(5) . 4_455
La O1 La 107.6(5) 2_565 4_455
Ga2 O1 O2 147.4(3) 2_566 5_455
La O1 O2 51.3(3) . 5_455
La O1 O2 101.0(7) 2_565 5_455
La O1 O2 61.3(4) 4_455 5_455
Ga2 O1 O2 147.4(3) 2_566 6
La O1 O2 61.3(4) . 6
La O1 O2 51.3(3) 2_565 6
La O1 O2 101.0(7) 4_455 6
O2 O1 O2 55.6(5) 5_455 6
Ga2 O1 O2 147.4(3) 2_566 2_565
La O1 O2 101.0(7) . 2_565
La O1 O2 61.3(4) 2_565 2_565
La O1 O2 51.3(3) 4_455 2_565
O2 O1 O2 55.6(5) 5_455 2_565
O2 O1 O2 55.6(5) 6 2_565
Ga2 O1 O2 31.8(3) 2_566 6_556
La O1 O2 97.8(3) . 6_556
La O1 O2 89.7(3) 2_565 6_556
La O1 O2 142.4(7) 4_455 6_556
O2 O1 O2 149.08(10) 5_455 6_556
O2 O1 O2 115.6(2) 6 6_556
O2 O1 O2 149.07(10) 2_565 6_556
Ga2 O1 O2 31.8(3) 2_566 5_456
La O1 O2 89.7(3) . 5_456
La O1 O2 142.4(7) 2_565 5_456
La O1 O2 97.8(3) 4_455 5_456
O2 O1 O2 115.6(2) 5_455 5_456
O2 O1 O2 149.08(10) 6 5_456
O2 O1 O2 149.07(10) 2_565 5_456
O2 O1 O2 54.3(5) 6_556 5_456
Ga2 O1 O2 31.8(3) 2_566 2_566
La O1 O2 142.4(7) . 2_566
La O1 O2 97.8(3) 2_565 2_566
La O1 O2 89.7(3) 4_455 2_566
O2 O1 O2 149.07(10) 5_455 2_566
O2 O1 O2 149.07(10) 6 2_566
O2 O1 O2 115.6(2) 2_565 2_566
O2 O1 O2 54.3(5) 6_556 2_566
O2 O1 O2 54.3(5) 5_456 2_566
Ga2 O1 O3 84.8(5) 2_566 3_565
La O1 O3 47.86(15) . 3_565
La O1 O3 81.97(17) 2_565 3_565
La O1 O3 155.3(6) 4_455 3_565
O2 O1 O3 95.0(4) 5_455 3_565
O2 O1 O3 66.8(3) 6 3_565
O2 O1 O3 122.4(6) 2_565 3_565
O2 O1 O3 57.6(3) 6_556 3_565
O2 O1 O3 86.2(4) 5_456 3_565
O2 O1 O3 111.9(6) 2_566 3_565
Ga2 O1 O3 84.8(5) 2_566 .
La O1 O3 81.97(17) . .
La O1 O3 155.3(6) 2_565 .
La O1 O3 47.86(15) 4_455 .
O2 O1 O3 66.8(3) 5_455 .
O2 O1 O3 122.4(6) 6 .
O2 O1 O3 95.0(4) 2_565 .
O2 O1 O3 111.9(6) 6_556 .
O2 O1 O3 57.6(3) 5_456 .
O2 O1 O3 86.2(4) 2_566 .
O3 O1 O3 119.20(14) 3_565 .
Ga2 O1 O3 84.8(5) 2_566 4_455
La O1 O3 155.3(6) . 4_455
La O1 O3 47.86(15) 2_565 4_455
La O1 O3 81.97(17) 4_455 4_455
O2 O1 O3 122.4(6) 5_455 4_455
O2 O1 O3 95.0(4) 6 4_455
O2 O1 O3 66.8(3) 2_565 4_455
O2 O1 O3 86.2(4) 6_556 4_455
O2 O1 O3 111.9(6) 5_456 4_455
O2 O1 O3 57.6(3) 2_566 4_455
O3 O1 O3 119.20(14) 3_565 4_455
O3 O1 O3 119.20(14) . 4_455
Ga2 O1 Ga2 180.0 2_566 2_565
La O1 Ga2 68.8(5) . 2_565
La O1 Ga2 68.8(5) 2_565 2_565
La O1 Ga2 68.7(5) 4_455 2_565
O2 O1 Ga2 32.6(3) 5_455 2_565
O2 O1 Ga2 32.6(3) 6 2_565
O2 O1 Ga2 32.6(3) 2_565 2_565
O2 O1 Ga2 148.2(3) 6_556 2_565
O2 O1 Ga2 148.2(3) 5_456 2_565
O2 O1 Ga2 148.2(3) 2_566 2_565
O3 O1 Ga2 95.2(5) 3_565 2_565
O3 O1 Ga2 95.2(5) . 2_565
O3 O1 Ga2 95.2(5) 4_455 2_565
Ga2 O1 Ga3 63.2(3) 2_566 2_565
La O1 Ga3 78.03(10) . 2_565
La O1 Ga3 72.76(10) 2_565 2_565
La O1 Ga3 173.6(7) 4_455 2_565
O2 O1 Ga3 125.1(3) 5_455 2_565
O2 O1 Ga3 84.3(2) 6 2_565
O2 O1 Ga3 131.5(4) 2_565 2_565
O2 O1 Ga3 31.7(2) 6_556 2_565
O2 O1 Ga3 79.0(4) 5_456 2_565
O2 O1 Ga3 83.9(5) 2_566 2_565
O3 O1 Ga3 30.7(2) 3_565 2_565
O3 O1 Ga3 131.9(5) . 2_565
O3 O1 Ga3 94.0(3) 4_455 2_565
Ga2 O1 Ga3 116.8(3) 2_565 2_565
Ga2 O1 Ga3 63.2(3) 2_566 1_556
La O1 Ga3 72.76(10) . 1_556
La O1 Ga3 173.6(7) 2_565 1_556
La O1 Ga3 78.03(10) 4_455 1_556
O2 O1 Ga3 84.3(2) 5_455 1_556
O2 O1 Ga3 131.5(4) 6 1_556
O2 O1 Ga3 125.1(3) 2_565 1_556
O2 O1 Ga3 83.9(5) 6_556 1_556
O2 O1 Ga3 31.7(2) 5_456 1_556
O2 O1 Ga3 79.0(4) 2_566 1_556
O3 O1 Ga3 94.0(3) 3_565 1_556
O3 O1 Ga3 30.7(2) . 1_556
O3 O1 Ga3 131.9(5) 4_455 1_556
Ga2 O1 Ga3 116.8(3) 2_565 1_556
Ga3 O1 Ga3 101.3(4) 2_565 1_556
Ga2 O1 Ga3 63.2(3) 2_566 4_456
La O1 Ga3 173.6(7) . 4_456
La O1 Ga3 78.03(10) 2_565 4_456
La O1 Ga3 72.76(10) 4_455 4_456
O2 O1 Ga3 131.5(4) 5_455 4_456
O2 O1 Ga3 125.1(3) 6 4_456
O2 O1 Ga3 84.3(2) 2_565 4_456
O2 O1 Ga3 79.0(4) 6_556 4_456
O2 O1 Ga3 83.9(5) 5_456 4_456
O2 O1 Ga3 31.7(2) 2_566 4_456
O3 O1 Ga3 131.9(5) 3_565 4_456
O3 O1 Ga3 94.0(3) . 4_456
O3 O1 Ga3 30.7(2) 4_455 4_456
Ga2 O1 Ga3 116.8(3) 2_565 4_456
Ga3 O1 Ga3 101.3(4) 2_565 4_456
Ga3 O1 Ga3 101.3(4) 1_556 4_456
Ga2 O1 O2 79.9(4) 2_566 3_455
La O1 O2 42.73(18) . 3_455
La O1 O2 148.7(3) 2_565 3_455
La O1 O2 94.03(16) 4_455 3_455
O2 O1 O2 69.6(4) 5_455 3_455
O2 O1 O2 103.4(4) 6 3_455
O2 O1 O2 124.0(5) 2_565 3_455
O2 O1 O2 86.2(4) 6_556 3_455
O2 O1 O2 50.7(4) 5_456 3_455
O2 O1 O2 104.7(5) 2_566 3_455
O3 O1 O2 69.72(19) 3_565 3_455
O3 O1 O2 49.48(19) . 3_455
O3 O1 O2 161.6(7) 4_455 3_455
Ga2 O1 O2 100.1(4) 2_565 3_455
Ga3 O1 O2 88.2(3) 2_565 3_455
Ga3 O1 O2 30.36(16) 1_556 3_455
Ga3 O1 O2 131.1(5) 4_456 3_455
Ga2 O1 O2 79.9(4) 2_566 4
La O1 O2 94.03(16) . 4
La O1 O2 42.73(18) 2_565 4
La O1 O2 148.7(3) 4_455 4
O2 O1 O2 124.0(5) 5_455 4
O2 O1 O2 69.6(4) 6 4
O2 O1 O2 103.4(4) 2_565 4
O2 O1 O2 50.7(4) 6_556 4
O2 O1 O2 104.7(5) 5_456 4
O2 O1 O2 86.2(4) 2_566 4
O3 O1 O2 49.48(19) 3_565 4
O3 O1 O2 161.6(7) . 4
O3 O1 O2 69.72(19) 4_455 4
Ga2 O1 O2 100.1(4) 2_565 4
Ga3 O1 O2 30.36(16) 2_565 4
Ga3 O1 O2 131.1(5) 1_556 4
Ga3 O1 O2 88.2(3) 4_456 4
O2 O1 O2 117.0(2) 3_455 4
Ga2 O1 O2 79.9(4) 2_566 1_565
La O1 O2 148.7(3) . 1_565
La O1 O2 94.03(16) 2_565 1_565
La O1 O2 42.73(18) 4_455 1_565
O2 O1 O2 103.4(4) 5_455 1_565
O2 O1 O2 124.0(5) 6 1_565
O2 O1 O2 69.6(4) 2_565 1_565
O2 O1 O2 104.7(5) 6_556 1_565
O2 O1 O2 86.2(4) 5_456 1_565
O2 O1 O2 50.7(4) 2_566 1_565
O3 O1 O2 161.6(7) 3_565 1_565
O3 O1 O2 69.72(19) . 1_565
O3 O1 O2 49.48(19) 4_455 1_565
Ga2 O1 O2 100.1(4) 2_565 1_565
Ga3 O1 O2 131.1(5) 2_565 1_565
Ga3 O1 O2 88.2(3) 1_556 1_565
Ga3 O1 O2 30.36(16) 4_456 1_565
O2 O1 O2 117.0(2) 3_455 1_565
O2 O1 O2 117.0(2) 4 1_565
Ga2 O1 O3 119.4(3) 2_566 2_465
La O1 O3 81.2(3) . 2_465
La O1 O3 120.9(6) 2_565 2_465
La O1 O3 26.76(16) 4_455 2_465
O2 O1 O3 40.0(3) 5_455 2_465
O2 O1 O3 91.8(5) 6 2_465
O2 O1 O3 59.7(3) 2_565 2_465
O2 O1 O3 148.4(5) 6_556 2_465
O2 O1 O3 94.1(2) 5_456 2_465
O2 O1 O3 109.1(3) 2_566 2_465
O3 O1 O3 129.0(4) 3_565 2_465
O3 O1 O3 36.5(4) . 2_465
O3 O1 O3 107.9(3) 4_455 2_465
Ga2 O1 O3 60.6(3) 2_565 2_465
Ga3 O1 O3 158.05(14) 2_565 2_465
Ga3 O1 O3 65.52(14) 1_556 2_465
Ga3 O1 O3 98.62(13) 4_456 2_465
O2 O1 O3 71.6(2) 3_455 2_465
O2 O1 O3 160.6(7) 4 2_465
O2 O1 O3 68.3(2) 1_565 2_465
Ga2 O1 O3 119.4(3) 2_566 5_445
La O1 O3 26.76(16) . 5_445
La O1 O3 81.2(3) 2_565 5_445
La O1 O3 120.9(6) 4_455 5_445
O2 O1 O3 59.7(3) 5_455 5_445
O2 O1 O3 40.0(3) 6 5_445
O2 O1 O3 91.8(5) 2_565 5_445
O2 O1 O3 94.1(2) 6_556 5_445
O2 O1 O3 109.1(3) 5_456 5_445
O2 O1 O3 148.4(5) 2_566 5_445
O3 O1 O3 36.5(4) 3_565 5_445
O3 O1 O3 107.9(3) . 5_445
O3 O1 O3 129.0(4) 4_455 5_445
Ga2 O1 O3 60.6(3) 2_565 5_445
Ga3 O1 O3 65.52(14) 2_565 5_445
Ga3 O1 O3 98.62(13) 1_556 5_445
Ga3 O1 O3 158.05(14) 4_456 5_445
O2 O1 O3 68.3(2) 3_455 5_445
O2 O1 O3 71.6(2) 4 5_445
O2 O1 O3 160.6(7) 1_565 5_445
O3 O1 O3 98.0(4) 2_465 5_445
Ga2 O1 O3 119.4(3) 2_566 6_665
La O1 O3 120.9(6) . 6_665
La O1 O3 26.76(16) 2_565 6_665
La O1 O3 81.2(3) 4_455 6_665
O2 O1 O3 91.8(5) 5_455 6_665
O2 O1 O3 59.7(3) 6 6_665
O2 O1 O3 40.0(3) 2_565 6_665
O2 O1 O3 109.1(3) 6_556 6_665
O2 O1 O3 148.4(5) 5_456 6_665
O2 O1 O3 94.1(2) 2_566 6_665
O3 O1 O3 107.9(3) 3_565 6_665
O3 O1 O3 129.0(4) . 6_665
O3 O1 O3 36.5(4) 4_455 6_665
Ga2 O1 O3 60.6(3) 2_565 6_665
Ga3 O1 O3 98.62(13) 2_565 6_665
Ga3 O1 O3 158.05(14) 1_556 6_665
Ga3 O1 O3 65.52(14) 4_456 6_665
O2 O1 O3 160.6(7) 3_455 6_665
O2 O1 O3 68.3(2) 4 6_665
O2 O1 O3 71.6(2) 1_565 6_665
O3 O1 O3 98.0(4) 2_465 6_665
O3 O1 O3 98.0(4) 5_445 6_665
Ga2 O1 Ga3 137.59(18) 2_566 2_564
La O1 Ga3 56.8(3) . 2_564
La O1 Ga3 52.1(3) 2_565 2_564
La O1 Ga3 111.1(6) 4_455 2_564
O2 O1 Ga3 61.7(4) 5_455 2_564
O2 O1 Ga3 10.45(19) 6 2_564
O2 O1 Ga3 65.9(4) 2_565 2_564
O2 O1 Ga3 105.89(17) 6_556 2_564
O2 O1 Ga3 140.53(18) 5_456 2_564
O2 O1 Ga3 146.76(19) 2_566 2_564
O3 O1 Ga3 56.5(3) 3_565 2_564
O3 O1 Ga3 127.0(5) . 2_564
O3 O1 Ga3 98.6(4) 4_455 2_564
Ga2 O1 Ga3 42.41(18) 2_565 2_564
Ga3 O1 Ga3 74.37(14) 2_565 2_564
Ga3 O1 Ga3 129.3(2) 1_556 2_564
Ga3 O1 Ga3 129.3(2) 4_456 2_564
O2 O1 Ga3 99.5(3) 3_455 2_564
O2 O1 Ga3 62.4(3) 4 2_564
O2 O1 Ga3 133.3(5) 1_565 2_564
O3 O1 Ga3 99.9(5) 2_465 2_564
O3 O1 Ga3 32.6(2) 5_445 2_564
O3 O1 Ga3 65.4(2) 6_665 2_564
Ga2 O1 Ga3 137.59(18) 2_566 .
La O1 Ga3 52.1(3) . .
La O1 Ga3 111.1(6) 2_565 .
La O1 Ga3 56.8(3) 4_455 .
O2 O1 Ga3 10.45(19) 5_455 .
O2 O1 Ga3 65.9(4) 6 .
O2 O1 Ga3 61.7(4) 2_565 .
O2 O1 Ga3 146.76(19) 6_556 .
O2 O1 Ga3 105.89(18) 5_456 .
O2 O1 Ga3 140.53(18) 2_566 .
O3 O1 Ga3 98.6(4) 3_565 .
O3 O1 Ga3 56.5(3) . .
O3 O1 Ga3 127.0(5) 4_455 .
Ga2 O1 Ga3 42.41(18) 2_565 .
Ga3 O1 Ga3 129.3(2) 2_565 .
Ga3 O1 Ga3 74.37(14) 1_556 .
Ga3 O1 Ga3 129.3(2) 4_456 .
O2 O1 Ga3 62.4(3) 3_455 .
O2 O1 Ga3 133.3(5) 4 .
O2 O1 Ga3 99.5(3) 1_565 .
O3 O1 Ga3 32.6(2) 2_465 .
O3 O1 Ga3 65.4(3) 5_445 .
O3 O1 Ga3 99.9(5) 6_665 .
Ga3 O1 Ga3 71.5(3) 2_564 .
Ga2 O1 Ga3 137.59(18) 2_566 4_455
La O1 Ga3 111.1(6) . 4_455
La O1 Ga3 56.8(3) 2_565 4_455
La O1 Ga3 52.1(3) 4_455 4_455
O2 O1 Ga3 65.9(4) 5_455 4_455
O2 O1 Ga3 61.7(4) 6 4_455
O2 O1 Ga3 10.45(19) 2_565 4_455
O2 O1 Ga3 140.53(18) 6_556 4_455
O2 O1 Ga3 146.76(19) 5_456 4_455
O2 O1 Ga3 105.89(17) 2_566 4_455
O3 O1 Ga3 127.0(5) 3_565 4_455
O3 O1 Ga3 98.6(4) . 4_455
O3 O1 Ga3 56.5(3) 4_455 4_455
Ga2 O1 Ga3 42.41(18) 2_565 4_455
Ga3 O1 Ga3 129.3(2) 2_565 4_455
Ga3 O1 Ga3 129.3(2) 1_556 4_455
Ga3 O1 Ga3 74.37(14) 4_456 4_455
O2 O1 Ga3 133.3(5) 3_455 4_455
O2 O1 Ga3 99.5(3) 4 4_455
O2 O1 Ga3 62.4(3) 1_565 4_455
O3 O1 Ga3 65.4(2) 2_465 4_455
O3 O1 Ga3 99.9(5) 5_445 4_455
O3 O1 Ga3 32.6(2) 6_665 4_455
Ga3 O1 Ga3 71.5(3) 2_564 4_455
Ga3 O1 Ga3 71.5(3) . 4_455
Ga2 O1 Ga1 101.3(3) 2_566 1_455
La O1 Ga1 71.04(13) . 1_455
La O1 Ga1 144.7(7) 2_565 1_455
La O1 Ga1 45.20(4) 4_455 1_455
O2 O1 Ga1 49.43(19) 5_455 1_455
O2 O1 Ga1 105.0(4) 6 1_455
O2 O1 Ga1 84.0(3) 2_565 1_455
O2 O1 Ga1 125.6(4) 6_556 1_455
O2 O1 Ga1 72.10(17) 5_456 1_455
O2 O1 Ga1 103.1(3) 2_566 1_455
O3 O1 Ga1 115.08(16) 3_565 1_455
O3 O1 Ga1 17.4(3) . 1_455
O3 O1 Ga1 125.71(15) 4_455 1_455
Ga2 O1 Ga1 78.7(3) 2_565 1_455
Ga3 O1 Ga1 137.14(19) 2_565 1_455
Ga3 O1 Ga1 41.70(5) 1_556 1_455
Ga3 O1 Ga1 106.21(9) 4_456 1_455
O2 O1 Ga1 48.97(16) 3_455 1_455
O2 O1 Ga1 164.53(14) 4 1_455
O2 O1 Ga1 78.23(12) 1_565 1_455
O3 O1 Ga1 24.52(12) 2_465 1_455
O3 O1 Ga1 94.8(2) 5_445 1_455
O3 O1 Ga1 122.5(4) 6_665 1_455
Ga3 O1 Ga1 110.0(4) 2_564 1_455
Ga3 O1 Ga1 39.11(9) . 1_455
Ga3 O1 Ga1 89.9(2) 4_455 1_455
Ga2 O1 Nb 101.3(3) 2_566 1_455
La O1 Nb 71.04(13) . 1_455
La O1 Nb 144.7(7) 2_565 1_455
La O1 Nb 45.20(4) 4_455 1_455
O2 O1 Nb 49.43(19) 5_455 1_455
O2 O1 Nb 105.0(4) 6 1_455
O2 O1 Nb 84.0(3) 2_565 1_455
O2 O1 Nb 125.6(4) 6_556 1_455
O2 O1 Nb 72.10(17) 5_456 1_455
O2 O1 Nb 103.1(3) 2_566 1_455
O3 O1 Nb 115.08(16) 3_565 1_455
O3 O1 Nb 17.4(3) . 1_455
O3 O1 Nb 125.71(15) 4_455 1_455
Ga2 O1 Nb 78.7(3) 2_565 1_455
Ga3 O1 Nb 137.14(19) 2_565 1_455
Ga3 O1 Nb 41.70(5) 1_556 1_455
Ga3 O1 Nb 106.21(9) 4_456 1_455
O2 O1 Nb 48.97(16) 3_455 1_455
O2 O1 Nb 164.53(14) 4 1_455
O2 O1 Nb 78.23(12) 1_565 1_455
O3 O1 Nb 24.52(12) 2_465 1_455
O3 O1 Nb 94.8(2) 5_445 1_455
O3 O1 Nb 122.5(4) 6_665 1_455
Ga3 O1 Nb 110.0(4) 2_564 1_455
Ga3 O1 Nb 39.11(9) . 1_455
Ga3 O1 Nb 89.9(2) 4_455 1_455
Ga1 O1 Nb 0.0 1_455 1_455
Ga2 O1 Ga1 101.3(3) 2_566 .
La O1 Ga1 45.20(4) . .
La O1 Ga1 71.04(13) 2_565 .
La O1 Ga1 144.7(7) 4_455 .
O2 O1 Ga1 84.0(3) 5_455 .
O2 O1 Ga1 49.43(19) 6 .
O2 O1 Ga1 105.0(4) 2_565 .
O2 O1 Ga1 72.10(17) 6_556 .
O2 O1 Ga1 103.1(3) 5_456 .
O2 O1 Ga1 125.6(4) 2_566 .
O3 O1 Ga1 17.4(3) 3_565 .
O3 O1 Ga1 125.71(15) . .
O3 O1 Ga1 115.08(16) 4_455 .
Ga2 O1 Ga1 78.7(3) 2_565 .
Ga3 O1 Ga1 41.70(5) 2_565 .
Ga3 O1 Ga1 106.21(9) 1_556 .
Ga3 O1 Ga1 137.14(19) 4_456 .
O2 O1 Ga1 78.23(12) 3_455 .
O2 O1 Ga1 48.97(16) 4 .
O2 O1 Ga1 164.53(14) 1_565 .
O3 O1 Ga1 122.5(4) 2_465 .
O3 O1 Ga1 24.52(12) 5_445 .
O3 O1 Ga1 94.8(2) 6_665 .
Ga3 O1 Ga1 39.11(9) 2_564 .
Ga3 O1 Ga1 89.9(2) . .
Ga3 O1 Ga1 110.0(4) 4_455 .
Ga1 O1 Ga1 116.24(17) 1_455 .
Nb O1 Ga1 116.24(17) 1_455 .
Ga2 O1 Nb 101.3(3) 2_566 .
La O1 Nb 45.20(4) . .
La O1 Nb 71.04(13) 2_565 .
La O1 Nb 144.7(7) 4_455 .
O2 O1 Nb 84.0(3) 5_455 .
O2 O1 Nb 49.43(19) 6 .
O2 O1 Nb 105.0(4) 2_565 .
O2 O1 Nb 72.10(17) 6_556 .
O2 O1 Nb 103.1(3) 5_456 .
O2 O1 Nb 125.6(4) 2_566 .
O3 O1 Nb 17.4(3) 3_565 .
O3 O1 Nb 125.71(15) . .
O3 O1 Nb 115.08(16) 4_455 .
Ga2 O1 Nb 78.7(3) 2_565 .
Ga3 O1 Nb 41.70(5) 2_565 .
Ga3 O1 Nb 106.21(9) 1_556 .
Ga3 O1 Nb 137.14(19) 4_456 .
O2 O1 Nb 78.23(12) 3_455 .
O2 O1 Nb 48.97(16) 4 .
O2 O1 Nb 164.53(14) 1_565 .
O3 O1 Nb 122.5(4) 2_465 .
O3 O1 Nb 24.52(12) 5_445 .
O3 O1 Nb 94.8(2) 6_665 .
Ga3 O1 Nb 39.11(9) 2_564 .
Ga3 O1 Nb 89.9(2) . .
Ga3 O1 Nb 110.0(4) 4_455 .
Ga1 O1 Nb 116.24(17) 1_455 .
Nb O1 Nb 116.24(17) 1_455 .
Ga1 O1 Nb 0.0 . .
Ga2 O1 Ga1 101.3(3) 2_566 1_565
La O1 Ga1 144.7(7) . 1_565
La O1 Ga1 45.20(4) 2_565 1_565
La O1 Ga1 71.04(13) 4_455 1_565
O2 O1 Ga1 105.0(4) 5_455 1_565
O2 O1 Ga1 84.0(3) 6 1_565
O2 O1 Ga1 49.43(19) 2_565 1_565
O2 O1 Ga1 103.1(3) 6_556 1_565
O2 O1 Ga1 125.6(4) 5_456 1_565
O2 O1 Ga1 72.10(17) 2_566 1_565
O3 O1 Ga1 125.71(15) 3_565 1_565
O3 O1 Ga1 115.08(15) . 1_565
O3 O1 Ga1 17.4(3) 4_455 1_565
Ga2 O1 Ga1 78.7(3) 2_565 1_565
Ga3 O1 Ga1 106.21(9) 2_565 1_565
Ga3 O1 Ga1 137.14(19) 1_556 1_565
Ga3 O1 Ga1 41.70(5) 4_456 1_565
O2 O1 Ga1 164.53(14) 3_455 1_565
O2 O1 Ga1 78.23(12) 4 1_565
O2 O1 Ga1 48.97(16) 1_565 1_565
O3 O1 Ga1 94.8(2) 2_465 1_565
O3 O1 Ga1 122.5(4) 5_445 1_565
O3 O1 Ga1 24.52(12) 6_665 1_565
Ga3 O1 Ga1 89.9(2) 2_564 1_565
Ga3 O1 Ga1 110.0(4) . 1_565
Ga3 O1 Ga1 39.11(9) 4_455 1_565
Ga1 O1 Ga1 116.24(17) 1_455 1_565
Nb O1 Ga1 116.24(17) 1_455 1_565
Ga1 O1 Ga1 116.24(17) . 1_565
Nb O1 Ga1 116.24(17) . 1_565
Ga2 O1 Nb 101.3(3) 2_566 1_565
La O1 Nb 144.7(7) . 1_565
La O1 Nb 45.20(4) 2_565 1_565
La O1 Nb 71.04(13) 4_455 1_565
O2 O1 Nb 105.0(4) 5_455 1_565
O2 O1 Nb 84.0(3) 6 1_565
O2 O1 Nb 49.43(19) 2_565 1_565
O2 O1 Nb 103.1(3) 6_556 1_565
O2 O1 Nb 125.6(4) 5_456 1_565
O2 O1 Nb 72.10(17) 2_566 1_565
O3 O1 Nb 125.71(15) 3_565 1_565
O3 O1 Nb 115.08(15) . 1_565
O3 O1 Nb 17.4(3) 4_455 1_565
Ga2 O1 Nb 78.7(3) 2_565 1_565
Ga3 O1 Nb 106.21(9) 2_565 1_565
Ga3 O1 Nb 137.14(19) 1_556 1_565
Ga3 O1 Nb 41.70(5) 4_456 1_565
O2 O1 Nb 164.53(14) 3_455 1_565
O2 O1 Nb 78.23(12) 4 1_565
O2 O1 Nb 48.97(16) 1_565 1_565
O3 O1 Nb 94.8(2) 2_465 1_565
O3 O1 Nb 122.5(4) 5_445 1_565
O3 O1 Nb 24.52(12) 6_665 1_565
Ga3 O1 Nb 89.9(2) 2_564 1_565
Ga3 O1 Nb 110.0(4) . 1_565
Ga3 O1 Nb 39.11(9) 4_455 1_565
Ga1 O1 Nb 116.24(17) 1_455 1_565
Nb O1 Nb 116.24(17) 1_455 1_565
Ga1 O1 Nb 116.24(17) . 1_565
Nb O1 Nb 116.24(17) . 1_565
Ga1 O1 Nb 0.0 1_565 1_565
Ga2 O1 O2 82.5(3) 2_566 .
La O1 O2 29.3(2) . .
La O1 O2 115.40(14) 2_565 .
La O1 O2 125.82(17) 4_455 .
O2 O1 O2 79.1(3) 5_455 .
O2 O1 O2 82.8(3) 6 .
O2 O1 O2 130.0(5) 2_565 .
O2 O1 O2 70.1(3) 6_556 .
O2 O1 O2 66.3(3) 5_456 .
O2 O1 O2 114.2(5) 2_566 .
O3 O1 O2 34.96(16) 3_565 .
O3 O1 O2 84.28(18) . .
O3 O1 O2 152.1(3) 4_455 .
Ga2 O1 O2 97.5(3) 2_565 .
Ga3 O1 O2 58.09(13) 2_565 .
Ga3 O1 O2 61.74(13) 1_556 .
Ga3 O1 O2 145.7(6) 4_456 .
O2 O1 O2 34.8(2) 3_455 .
O2 O1 O2 83.6(2) 4 .
O2 O1 O2 149.7(5) 1_565 .
O3 O1 O2 100.01(19) 2_465 .
O3 O1 O2 42.8(2) 5_445 .
O3 O1 O2 138.7(3) 6_665 .
Ga3 O1 O2 75.01(18) 2_564 .
Ga3 O1 O2 77.46(19) . .
Ga3 O1 O2 139.9(5) 4_455 .
Ga1 O1 O2 81.26(9) 1_455 .
Nb O1 O2 81.26(9) 1_455 .
Ga1 O1 O2 44.49(10) . .
Nb O1 O2 44.49(10) . .
Ga1 O1 O2 160.41(13) 1_565 .
Nb O1 O2 160.41(13) 1_565 .
Ga2 O1 O2 82.5(3) 2_566 3_565
La O1 O2 125.82(17) . 3_565
La O1 O2 29.3(2) 2_565 3_565
La O1 O2 115.40(14) 4_455 3_565
O2 O1 O2 130.0(5) 5_455 3_565
O2 O1 O2 79.1(3) 6 3_565
O2 O1 O2 82.8(3) 2_565 3_565
O2 O1 O2 66.3(3) 6_556 3_565
O2 O1 O2 114.2(5) 5_456 3_565
O2 O1 O2 70.1(3) 2_566 3_565
O3 O1 O2 84.28(18) 3_565 3_565
O3 O1 O2 152.1(3) . 3_565
O3 O1 O2 34.96(16) 4_455 3_565
Ga2 O1 O2 97.5(3) 2_565 3_565
Ga3 O1 O2 61.74(13) 2_565 3_565
Ga3 O1 O2 145.7(6) 1_556 3_565
Ga3 O1 O2 58.09(13) 4_456 3_565
O2 O1 O2 149.7(4) 3_455 3_565
O2 O1 O2 34.8(2) 4 3_565
O2 O1 O2 83.6(2) 1_565 3_565
O3 O1 O2 138.7(3) 2_465 3_565
O3 O1 O2 100.01(19) 5_445 3_565
O3 O1 O2 42.8(2) 6_665 3_565
Ga3 O1 O2 77.46(19) 2_564 3_565
Ga3 O1 O2 139.9(5) . 3_565
Ga3 O1 O2 75.01(18) 4_455 3_565
Ga1 O1 O2 160.41(13) 1_455 3_565
Nb O1 O2 160.41(13) 1_455 3_565
Ga1 O1 O2 81.26(9) . 3_565
Nb O1 O2 81.26(9) . 3_565
Ga1 O1 O2 44.49(10) 1_565 3_565
Nb O1 O2 44.49(10) 1_565 3_565
O2 O1 O2 118.33(14) . 3_565
Ga2 O1 O2 82.5(3) 2_566 4_455
La O1 O2 115.40(14) . 4_455
La O1 O2 125.82(17) 2_565 4_455
La O1 O2 29.3(2) 4_455 4_455
O2 O1 O2 82.8(3) 5_455 4_455
O2 O1 O2 130.0(5) 6 4_455
O2 O1 O2 79.1(3) 2_565 4_455
O2 O1 O2 114.2(5) 6_556 4_455
O2 O1 O2 70.1(3) 5_456 4_455
O2 O1 O2 66.3(3) 2_566 4_455
O3 O1 O2 152.1(3) 3_565 4_455
O3 O1 O2 34.96(16) . 4_455
O3 O1 O2 84.28(18) 4_455 4_455
Ga2 O1 O2 97.5(3) 2_565 4_455
Ga3 O1 O2 145.7(6) 2_565 4_455
Ga3 O1 O2 58.09(13) 1_556 4_455
Ga3 O1 O2 61.74(13) 4_456 4_455
O2 O1 O2 83.6(2) 3_455 4_455
O2 O1 O2 149.7(4) 4 4_455
O2 O1 O2 34.8(2) 1_565 4_455
O3 O1 O2 42.8(2) 2_465 4_455
O3 O1 O2 138.7(3) 5_445 4_455
O3 O1 O2 100.01(19) 6_665 4_455
Ga3 O1 O2 139.9(5) 2_564 4_455
Ga3 O1 O2 75.01(19) . 4_455
Ga3 O1 O2 77.46(19) 4_455 4_455
Ga1 O1 O2 44.49(10) 1_455 4_455
Nb O1 O2 44.49(10) 1_455 4_455
Ga1 O1 O2 160.41(14) . 4_455
Nb O1 O2 160.41(14) . 4_455
Ga1 O1 O2 81.26(9) 1_565 4_455
Nb O1 O2 81.26(9) 1_565 4_455
O2 O1 O2 118.33(14) . 4_455
O2 O1 O2 118.33(14) 3_565 4_455
Ga2 O1 La 30.18(13) 2_566 1_556
La O1 La 81.1(3) . 1_556
La O1 La 123.2(4) 2_565 1_556
La O1 La 123.2(4) 4_455 1_556
O2 O1 La 123.76(18) 5_455 1_556
O2 O1 La 129.3(2) 6 1_556
O2 O1 La 174.5(2) 2_565 1_556
O2 O1 La 34.2(3) 6_556 1_556
O2 O1 La 25.4(2) 5_456 1_556
O2 O1 La 61.8(4) 2_566 1_556
O3 O1 La 62.8(3) 3_565 1_556
O3 O1 La 80.2(4) . 1_556
O3 O1 La 113.2(6) 4_455 1_556
Ga2 O1 La 149.83(13) 2_565 1_556
Ga3 O1 La 53.9(2) 2_565 1_556
Ga3 O1 La 50.4(2) 1_556 1_556
Ga3 O1 La 93.3(4) 4_456 1_556
O2 O1 La 54.4(3) 3_455 1_556
O2 O1 La 81.5(4) 4 1_556
O2 O1 La 106.0(5) 1_565 1_556
O3 O1 La 115.9(2) 2_465 1_556
O3 O1 La 92.2(2) 5_445 1_556
O3 O1 La 142.8(4) 6_665 1_556
Ga3 O1 La 119.16(6) 2_564 1_556
Ga3 O1 La 116.80(6) . 1_556
Ga3 O1 La 167.6(3) 4_455 1_556
Ga1 O1 La 91.89(18) 1_455 1_556
Nb O1 La 91.89(18) 1_455 1_556
Ga1 O1 La 80.11(15) . 1_556
Nb O1 La 80.11(15) . 1_556
Ga1 O1 La 130.4(4) 1_565 1_556
Nb O1 La 130.4(4) 1_565 1_556
O2 O1 La 52.5(2) . 1_556
O2 O1 La 100.2(4) 3_565 1_556
O2 O1 La 95.3(3) 4_455 1_556
Ga2 O1 La 30.18(13) 2_566 2_566
La O1 La 123.2(4) . 2_566
La O1 La 81.1(3) 2_565 2_566
La O1 La 123.2(4) 4_455 2_566
O2 O1 La 174.5(2) 5_455 2_566
O2 O1 La 123.76(18) 6 2_566
O2 O1 La 129.3(2) 2_565 2_566
O2 O1 La 25.4(2) 6_556 2_566
O2 O1 La 61.8(4) 5_456 2_566
O2 O1 La 34.2(3) 2_566 2_566
O3 O1 La 80.2(4) 3_565 2_566
O3 O1 La 113.2(6) . 2_566
O3 O1 La 62.8(3) 4_455 2_566
Ga2 O1 La 149.82(13) 2_565 2_566
Ga3 O1 La 50.4(2) 2_565 2_566
Ga3 O1 La 93.3(4) 1_556 2_566
Ga3 O1 La 53.9(2) 4_456 2_566
O2 O1 La 106.0(5) 3_455 2_566
O2 O1 La 54.4(3) 4 2_566
O2 O1 La 81.5(4) 1_565 2_566
O3 O1 La 142.8(4) 2_465 2_566
O3 O1 La 115.9(2) 5_445 2_566
O3 O1 La 92.2(2) 6_665 2_566
Ga3 O1 La 116.80(6) 2_564 2_566
Ga3 O1 La 167.6(3) . 2_566
Ga3 O1 La 119.16(6) 4_455 2_566
Ga1 O1 La 130.4(4) 1_455 2_566
Nb O1 La 130.4(4) 1_455 2_566
Ga1 O1 La 91.89(18) . 2_566
Nb O1 La 91.89(18) . 2_566
Ga1 O1 La 80.10(15) 1_565 2_566
Nb O1 La 80.10(15) 1_565 2_566
O2 O1 La 95.3(3) . 2_566
O2 O1 La 52.5(2) 3_565 2_566
O2 O1 La 100.2(4) 4_455 2_566
La O1 La 51.6(2) 1_556 2_566
Ga2 O1 La 30.17(13) 2_566 4_456
La O1 La 123.2(4) . 4_456
La O1 La 123.2(4) 2_565 4_456
La O1 La 81.1(3) 4_455 4_456
O2 O1 La 129.3(2) 5_455 4_456
O2 O1 La 174.5(2) 6 4_456
O2 O1 La 123.76(18) 2_565 4_456
O2 O1 La 61.8(4) 6_556 4_456
O2 O1 La 34.2(3) 5_456 4_456
O2 O1 La 25.4(2) 2_566 4_456
O3 O1 La 113.2(6) 3_565 4_456
O3 O1 La 62.8(3) . 4_456
O3 O1 La 80.2(4) 4_455 4_456
Ga2 O1 La 149.82(13) 2_565 4_456
Ga3 O1 La 93.3(4) 2_565 4_456
Ga3 O1 La 53.9(2) 1_556 4_456
Ga3 O1 La 50.4(2) 4_456 4_456
O2 O1 La 81.5(4) 3_455 4_456
O2 O1 La 106.0(5) 4 4_456
O2 O1 La 54.4(3) 1_565 4_456
O3 O1 La 92.2(2) 2_465 4_456
O3 O1 La 142.8(4) 5_445 4_456
O3 O1 La 115.9(2) 6_665 4_456
Ga3 O1 La 167.6(3) 2_564 4_456
Ga3 O1 La 119.16(6) . 4_456
Ga3 O1 La 116.80(6) 4_455 4_456
Ga1 O1 La 80.10(15) 1_455 4_456
Nb O1 La 80.10(15) 1_455 4_456
Ga1 O1 La 130.4(4) . 4_456
Nb O1 La 130.4(4) . 4_456
Ga1 O1 La 91.89(18) 1_565 4_456
Nb O1 La 91.89(18) 1_565 4_456
O2 O1 La 100.2(4) . 4_456
O2 O1 La 95.3(3) 3_565 4_456
O2 O1 La 52.5(2) 4_455 4_456
La O1 La 51.6(2) 1_556 4_456
La O1 La 51.6(2) 2_566 4_456
Ga2 O1 O3 52.7(2) 2_566 2_466
La O1 O3 104.0(2) . 2_466
La O1 O3 148.3(4) 2_565 2_466
La O1 O3 64.3(3) 4_455 2_466
O2 O1 O3 100.8(2) 5_455 2_466
O2 O1 O3 156.4(4) 6 2_466
O2 O1 O3 115.2(2) 2_565 2_466
O2 O1 O3 83.3(5) 6_556 2_466
O2 O1 O3 33.9(2) 5_456 2_466
O2 O1 O3 53.4(3) 2_566 2_466
O3 O1 O3 118.7(4) 3_565 2_466
O3 O1 O3 34.0(4) . 2_466
O3 O1 O3 100.7(4) 4_455 2_466
Ga2 O1 O3 127.3(2) 2_565 2_466
Ga3 O1 O3 111.9(5) 2_565 2_466
Ga3 O1 O3 31.45(14) 1_556 2_466
Ga3 O1 O3 70.3(3) 4_456 2_466
O2 O1 O3 61.8(2) 3_455 2_466
O2 O1 O3 132.6(6) 4 2_466
O2 O1 O3 58.5(3) 1_565 2_466
O3 O1 O3 66.63(12) 2_465 2_466
O3 O1 O3 130.07(10) 5_445 2_466
O3 O1 O3 130.07(10) 6_665 2_466
Ga3 O1 O3 159.1(2) 2_564 2_466
Ga3 O1 O3 90.49(13) . 2_466
Ga3 O1 O3 113.45(11) 4_455 2_466
Ga1 O1 O3 51.39(13) 1_455 2_466
Nb O1 O3 51.39(13) 1_455 2_466
Ga1 O1 O3 134.2(3) . 2_466
Nb O1 O3 134.2(3) . 2_466
Ga1 O1 O3 106.47(18) 1_565 2_466
Nb O1 O3 106.47(18) 1_565 2_466
O2 O1 O3 91.2(2) . 2_466
O2 O1 O3 123.3(4) 3_565 2_466
O2 O1 O3 36.20(19) 4_455 2_466
La O1 O3 59.2(2) 1_556 2_466
La O1 O3 79.5(3) 2_566 2_466
La O1 O3 28.88(16) 4_456 2_466
Ga2 O1 O3 52.7(2) 2_566 6_666
La O1 O3 148.3(4) . 6_666
La O1 O3 64.3(3) 2_565 6_666
La O1 O3 104.0(2) 4_455 6_666
O2 O1 O3 156.4(4) 5_455 6_666
O2 O1 O3 115.2(2) 6 6_666
O2 O1 O3 100.8(2) 2_565 6_666
O2 O1 O3 53.4(3) 6_556 6_666
O2 O1 O3 83.3(5) 5_456 6_666
O2 O1 O3 33.9(2) 2_566 6_666
O3 O1 O3 100.7(4) 3_565 6_666
O3 O1 O3 118.7(4) . 6_666
O3 O1 O3 34.0(4) 4_455 6_666
Ga2 O1 O3 127.3(2) 2_565 6_666
Ga3 O1 O3 70.3(3) 2_565 6_666
Ga3 O1 O3 111.9(5) 1_556 6_666
Ga3 O1 O3 31.45(14) 4_456 6_666
O2 O1 O3 132.6(6) 3_455 6_666
O2 O1 O3 58.5(3) 4 6_666
O2 O1 O3 61.8(2) 1_565 6_666
O3 O1 O3 130.07(10) 2_465 6_666
O3 O1 O3 130.07(10) 5_445 6_666
O3 O1 O3 66.63(12) 6_665 6_666
Ga3 O1 O3 113.45(11) 2_564 6_666
Ga3 O1 O3 159.1(2) . 6_666
Ga3 O1 O3 90.49(13) 4_455 6_666
Ga1 O1 O3 134.2(3) 1_455 6_666
Nb O1 O3 134.2(3) 1_455 6_666
Ga1 O1 O3 106.47(18) . 6_666
Nb O1 O3 106.47(18) . 6_666
Ga1 O1 O3 51.39(13) 1_565 6_666
Nb O1 O3 51.39(13) 1_565 6_666
O2 O1 O3 123.3(4) . 6_666
O2 O1 O3 36.20(19) 3_565 6_666
O2 O1 O3 91.2(2) 4_455 6_666
La O1 O3 79.5(3) 1_556 6_666
La O1 O3 28.88(16) 2_566 6_666
La O1 O3 59.2(2) 4_456 6_666
O3 O1 O3 87.1(3) 2_466 6_666
Ga2 O1 O3 52.7(2) 2_566 5_446
La O1 O3 64.3(3) . 5_446
La O1 O3 104.0(2) 2_565 5_446
La O1 O3 148.3(4) 4_455 5_446
O2 O1 O3 115.2(2) 5_455 5_446
O2 O1 O3 100.8(2) 6 5_446
O2 O1 O3 156.4(4) 2_565 5_446
O2 O1 O3 33.9(2) 6_556 5_446
O2 O1 O3 53.4(3) 5_456 5_446
O2 O1 O3 83.3(5) 2_566 5_446
O3 O1 O3 34.0(4) 3_565 5_446
O3 O1 O3 100.7(4) . 5_446
O3 O1 O3 118.7(4) 4_455 5_446
Ga2 O1 O3 127.3(2) 2_565 5_446
Ga3 O1 O3 31.45(14) 2_565 5_446
Ga3 O1 O3 70.3(3) 1_556 5_446
Ga3 O1 O3 111.9(5) 4_456 5_446
O2 O1 O3 58.5(3) 3_455 5_446
O2 O1 O3 61.8(2) 4 5_446
O2 O1 O3 132.6(6) 1_565 5_446
O3 O1 O3 130.07(10) 2_465 5_446
O3 O1 O3 66.63(12) 5_445 5_446
O3 O1 O3 130.07(10) 6_665 5_446
Ga3 O1 O3 90.49(13) 2_564 5_446
Ga3 O1 O3 113.45(11) . 5_446
Ga3 O1 O3 159.1(2) 4_455 5_446
Ga1 O1 O3 106.47(18) 1_455 5_446
Nb O1 O3 106.47(18) 1_455 5_446
Ga1 O1 O3 51.39(13) . 5_446
Nb O1 O3 51.39(13) . 5_446
Ga1 O1 O3 134.2(3) 1_565 5_446
Nb O1 O3 134.2(3) 1_565 5_446
O2 O1 O3 36.20(19) . 5_446
O2 O1 O3 91.2(2) 3_565 5_446
O2 O1 O3 123.3(4) 4_455 5_446
La O1 O3 28.88(16) 1_556 5_446
La O1 O3 59.2(2) 2_566 5_446
La O1 O3 79.5(3) 4_456 5_446
O3 O1 O3 87.1(3) 2_466 5_446
O3 O1 O3 87.1(3) 6_666 5_446
Ga2 O1 O3 116.0(3) 2_566 6
La O1 O3 49.74(17) . 6
La O1 O3 132.4(7) 2_565 6
La O1 O3 59.7(2) 4_455 6
O2 O1 O3 31.5(2) 5_455 6
O2 O1 O3 84.3(4) 6 6
O2 O1 O3 81.0(4) 2_565 6
O2 O1 O3 129.6(3) 6_556 6
O2 O1 O3 84.3(2) 5_456 6
O2 O1 O3 125.5(3) 2_566 6
O3 O1 O3 96.9(2) 3_565 6
O3 O1 O3 39.4(3) . 6
O3 O1 O3 140.5(4) 4_455 6
Ga2 O1 O3 64.0(3) 2_565 6
Ga3 O1 O3 125.02(9) 2_565 6
Ga3 O1 O3 52.84(16) 1_556 6
Ga3 O1 O3 128.55(9) 4_456 6
O2 O1 O3 43.5(3) 3_455 6
O2 O1 O3 143.1(3) 4 6
O2 O1 O3 99.0(2) 1_565 6
O3 O1 O3 33.0(2) 2_465 6
O3 O1 O3 71.7(3) 5_445 6
O3 O1 O3 120.5(5) 6_665 6
Ga3 O1 O3 87.7(3) 2_564 6
Ga3 O1 O3 21.62(14) . 6
Ga3 O1 O3 89.9(3) 4_455 6
Ga1 O1 O3 23.52(11) 1_455 6
Nb O1 O3 23.52(11) 1_455 6
Ga1 O1 O3 94.30(19) . 6
Nb O1 O3 94.30(19) . 6
Ga1 O1 O3 125.7(3) 1_565 6
Nb O1 O3 125.7(3) 1_565 6
O2 O1 O3 67.17(15) . 6
O2 O1 O3 161.5(5) 3_565 6
O2 O1 O3 67.14(15) 4_455 6
La O1 O3 96.69(18) 1_556 6
La O1 O3 146.0(4) 2_566 6
La O1 O3 101.10(17) 4_456 6
O3 O1 O3 72.34(11) 2_466 6
O3 O1 O3 157.7(3) 6_666 6
O3 O1 O3 100.08(16) 5_446 6
Ga2 O1 O3 116.0(3) 2_566 5_455
La O1 O3 132.4(7) . 5_455
La O1 O3 59.6(2) 2_565 5_455
La O1 O3 49.74(17) 4_455 5_455
O2 O1 O3 84.3(4) 5_455 5_455
O2 O1 O3 81.0(4) 6 5_455
O2 O1 O3 31.5(2) 2_565 5_455
O2 O1 O3 125.5(3) 6_556 5_455
O2 O1 O3 129.6(3) 5_456 5_455
O2 O1 O3 84.3(2) 2_566 5_455
O3 O1 O3 140.5(4) 3_565 5_455
O3 O1 O3 96.9(2) . 5_455
O3 O1 O3 39.4(3) 4_455 5_455
Ga2 O1 O3 64.0(3) 2_565 5_455
Ga3 O1 O3 128.55(9) 2_565 5_455
Ga3 O1 O3 125.02(9) 1_556 5_455
Ga3 O1 O3 52.84(16) 4_456 5_455
O2 O1 O3 143.1(3) 3_455 5_455
O2 O1 O3 99.0(2) 4 5_455
O2 O1 O3 43.5(3) 1_565 5_455
O3 O1 O3 71.7(3) 2_465 5_455
O3 O1 O3 120.5(5) 5_445 5_455
O3 O1 O3 33.0(2) 6_665 5_455
Ga3 O1 O3 89.9(3) 2_564 5_455
Ga3 O1 O3 87.7(3) . 5_455
Ga3 O1 O3 21.62(14) 4_455 5_455
Ga1 O1 O3 94.30(19) 1_455 5_455
Nb O1 O3 94.30(19) 1_455 5_455
Ga1 O1 O3 125.7(3) . 5_455
Nb O1 O3 125.7(3) . 5_455
Ga1 O1 O3 23.51(11) 1_565 5_455
Nb O1 O3 23.51(11) 1_565 5_455
O2 O1 O3 161.5(5) . 5_455
O2 O1 O3 67.14(15) 3_565 5_455
O2 O1 O3 67.17(15) 4_455 5_455
La O1 O3 146.0(4) 1_556 5_455
La O1 O3 101.10(17) 2_566 5_455
La O1 O3 96.69(18) 4_456 5_455
O3 O1 O3 100.08(16) 2_466 5_455
O3 O1 O3 72.34(11) 6_666 5_455
O3 O1 O3 157.7(3) 5_446 5_455
O3 O1 O3 102.2(3) 6 5_455
Ga2 O1 O3 116.0(3) 2_566 2_565
La O1 O3 59.6(2) . 2_565
La O1 O3 49.74(17) 2_565 2_565
La O1 O3 132.4(7) 4_455 2_565
O2 O1 O3 81.0(4) 5_455 2_565
O2 O1 O3 31.5(2) 6 2_565
O2 O1 O3 84.3(4) 2_565 2_565
O2 O1 O3 84.3(2) 6_556 2_565
O2 O1 O3 125.5(3) 5_456 2_565
O2 O1 O3 129.6(3) 2_566 2_565
O3 O1 O3 39.4(3) 3_565 2_565
O3 O1 O3 140.5(4) . 2_565
O3 O1 O3 96.9(2) 4_455 2_565
Ga2 O1 O3 64.0(3) 2_565 2_565
Ga3 O1 O3 52.84(16) 2_565 2_565
Ga3 O1 O3 128.55(9) 1_556 2_565
Ga3 O1 O3 125.02(9) 4_456 2_565
O2 O1 O3 99.0(2) 3_455 2_565
O2 O1 O3 43.5(3) 4 2_565
O2 O1 O3 143.1(3) 1_565 2_565
O3 O1 O3 120.5(5) 2_465 2_565
O3 O1 O3 33.0(2) 5_445 2_565
O3 O1 O3 71.7(3) 6_665 2_565
Ga3 O1 O3 21.62(14) 2_564 2_565
Ga3 O1 O3 89.9(3) . 2_565
Ga3 O1 O3 87.7(3) 4_455 2_565
Ga1 O1 O3 125.7(3) 1_455 2_565
Nb O1 O3 125.7(3) 1_455 2_565
Ga1 O1 O3 23.51(11) . 2_565
Nb O1 O3 23.51(11) . 2_565
Ga1 O1 O3 94.30(19) 1_565 2_565
Nb O1 O3 94.30(19) 1_565 2_565
O2 O1 O3 67.14(15) . 2_565
O2 O1 O3 67.17(15) 3_565 2_565
O2 O1 O3 161.5(5) 4_455 2_565
La O1 O3 101.10(17) 1_556 2_565
La O1 O3 96.69(18) 2_566 2_565
La O1 O3 146.0(4) 4_456 2_565
O3 O1 O3 157.7(3) 2_466 2_565
O3 O1 O3 100.08(16) 6_666 2_565
O3 O1 O3 72.34(11) 5_446 2_565
O3 O1 O3 102.2(3) 6 2_565
O3 O1 O3 102.2(3) 5_455 2_565
Ga2 O1 Ga2 72.7(2) 2_566 1_565
La O1 Ga2 136.43(4) . 1_565
La O1 Ga2 110.78(3) 2_565 1_565
La O1 Ga2 40.9(2) 4_455 1_565
O2 O1 Ga2 101.0(2) 5_455 1_565
O2 O1 Ga2 136.3(5) 6 1_565
O2 O1 Ga2 80.62(16) 2_565 1_565
O2 O1 Ga2 102.1(5) 6_556 1_565
O2 O1 Ga2 71.9(3) 5_456 1_565
O2 O1 Ga2 49.0(2) 2_566 1_565
O3 O1 Ga2 156.9(7) 3_565 1_565
O3 O1 Ga2 54.70(17) . 1_565
O3 O1 Ga2 65.01(18) 4_455 1_565
Ga2 O1 Ga2 107.3(2) 2_565 1_565
Ga3 O1 Ga2 132.8(5) 2_565 1_565
Ga3 O1 Ga2 71.37(15) 1_556 1_565
Ga3 O1 Ga2 40.40(7) 4_456 1_565
O2 O1 Ga2 100.4(2) 3_455 1_565
O2 O1 Ga2 128.4(3) 4 1_565
O2 O1 Ga2 16.85(17) 1_565 1_565
O3 O1 Ga2 61.90(15) 2_465 1_565
O3 O1 Ga2 159.7(3) 5_445 1_565
O3 O1 Ga2 88.29(11) 6_665 1_565
Ga3 O1 Ga2 146.5(4) 2_564 1_565
Ga3 O1 Ga2 94.54(12) . 1_565
Ga3 O1 Ga2 75.23(8) 4_455 1_565
Ga1 O1 Ga2 65.81(3) 1_455 1_565
Nb O1 Ga2 65.81(3) 1_455 1_565
Ga1 O1 Ga2 174.0(5) . 1_565
Nb O1 Ga2 174.0(5) . 1_565
Ga1 O1 Ga2 65.81(3) 1_565 1_565
Nb O1 Ga2 65.81(3) 1_565 1_565
O2 O1 Ga2 132.9(3) . 1_565
O2 O1 Ga2 97.71(16) 3_565 1_565
O2 O1 Ga2 21.37(11) 4_455 1_565
La O1 Ga2 94.3(3) 1_556 1_565
La O1 Ga2 82.9(3) 2_566 1_565
La O1 Ga2 43.72(12) 4_456 1_565
O3 O1 Ga2 42.01(14) 2_466 1_565
O3 O1 Ga2 70.11(18) 6_666 1_565
O3 O1 Ga2 122.9(4) 5_446 1_565
O3 O1 Ga2 88.47(10) 6 1_565
O3 O1 Ga2 58.55(12) 5_455 1_565
O3 O1 Ga2 159.9(2) 2_565 1_565
Ga2 O1 Ga2 72.7(2) 2_566 .
La O1 Ga2 40.9(2) . .
La O1 Ga2 136.43(3) 2_565 .
La O1 Ga2 110.78(3) 4_455 .
O2 O1 Ga2 80.62(16) 5_455 .
O2 O1 Ga2 101.0(2) 6 .
O2 O1 Ga2 136.3(5) 2_565 .
O2 O1 Ga2 71.9(3) 6_556 .
O2 O1 Ga2 49.0(2) 5_456 .
O2 O1 Ga2 102.1(5) 2_566 .
O3 O1 Ga2 54.70(17) 3_565 .
O3 O1 Ga2 65.01(18) . .
O3 O1 Ga2 156.9(7) 4_455 .
Ga2 O1 Ga2 107.3(2) 2_565 .
Ga3 O1 Ga2 71.37(15) 2_565 .
Ga3 O1 Ga2 40.40(7) 1_556 .
Ga3 O1 Ga2 132.8(5) 4_456 .
O2 O1 Ga2 16.85(17) 3_455 .
O2 O1 Ga2 100.4(2) 4 .
O2 O1 Ga2 128.4(3) 1_565 .
O3 O1 Ga2 88.29(11) 2_465 .
O3 O1 Ga2 61.90(15) 5_445 .
O3 O1 Ga2 159.7(3) 6_665 .
Ga3 O1 Ga2 94.54(12) 2_564 .
Ga3 O1 Ga2 75.23(8) . .
Ga3 O1 Ga2 146.5(4) 4_455 .
Ga1 O1 Ga2 65.81(3) 1_455 .
Nb O1 Ga2 65.81(3) 1_455 .
Ga1 O1 Ga2 65.81(2) . .
Nb O1 Ga2 65.81(2) . .
Ga1 O1 Ga2 174.0(5) 1_565 .
Nb O1 Ga2 174.0(5) 1_565 .
O2 O1 Ga2 21.37(11) . .
O2 O1 Ga2 132.9(3) 3_565 .
O2 O1 Ga2 97.71(16) 4_455 .
La O1 Ga2 43.72(12) 1_556 .
La O1 Ga2 94.3(3) 2_566 .
La O1 Ga2 82.9(3) 4_456 .
O3 O1 Ga2 70.11(18) 2_466 .
O3 O1 Ga2 122.9(4) 6_666 .
O3 O1 Ga2 42.01(14) 5_446 .
O3 O1 Ga2 58.55(12) 6 .
O3 O1 Ga2 159.9(2) 5_455 .
O3 O1 Ga2 88.47(10) 2_565 .
Ga2 O1 Ga2 111.6(2) 1_565 .
Ga2 O1 Ga2 72.7(2) 2_566 1_665
La O1 Ga2 110.78(3) . 1_665
La O1 Ga2 40.9(2) 2_565 1_665
La O1 Ga2 136.43(3) 4_455 1_665
O2 O1 Ga2 136.3(5) 5_455 1_665
O2 O1 Ga2 80.62(16) 6 1_665
O2 O1 Ga2 101.0(2) 2_565 1_665
O2 O1 Ga2 49.0(2) 6_556 1_665
O2 O1 Ga2 102.1(5) 5_456 1_665
O2 O1 Ga2 71.9(3) 2_566 1_665
O3 O1 Ga2 65.01(18) 3_565 1_665
O3 O1 Ga2 156.9(7) . 1_665
O3 O1 Ga2 54.70(17) 4_455 1_665
Ga2 O1 Ga2 107.3(2) 2_565 1_665
Ga3 O1 Ga2 40.40(7) 2_565 1_665
Ga3 O1 Ga2 132.8(5) 1_556 1_665
Ga3 O1 Ga2 71.37(15) 4_456 1_665
O2 O1 Ga2 128.4(3) 3_455 1_665
O2 O1 Ga2 16.85(17) 4 1_665
O2 O1 Ga2 100.4(2) 1_565 1_665
O3 O1 Ga2 159.7(3) 2_465 1_665
O3 O1 Ga2 88.29(11) 5_445 1_665
O3 O1 Ga2 61.90(15) 6_665 1_665
Ga3 O1 Ga2 75.23(8) 2_564 1_665
Ga3 O1 Ga2 146.5(4) . 1_665
Ga3 O1 Ga2 94.54(12) 4_455 1_665
Ga1 O1 Ga2 174.0(5) 1_455 1_665
Nb O1 Ga2 174.0(5) 1_455 1_665
Ga1 O1 Ga2 65.81(2) . 1_665
Nb O1 Ga2 65.81(2) . 1_665
Ga1 O1 Ga2 65.81(2) 1_565 1_665
Nb O1 Ga2 65.81(2) 1_565 1_665
O2 O1 Ga2 97.71(16) . 1_665
O2 O1 Ga2 21.37(11) 3_565 1_665
O2 O1 Ga2 132.9(3) 4_455 1_665
La O1 Ga2 82.9(3) 1_556 1_665
La O1 Ga2 43.72(12) 2_566 1_665
La O1 Ga2 94.3(3) 4_456 1_665
O3 O1 Ga2 122.9(4) 2_466 1_665
O3 O1 Ga2 42.01(14) 6_666 1_665
O3 O1 Ga2 70.11(18) 5_446 1_665
O3 O1 Ga2 159.9(2) 6 1_665
O3 O1 Ga2 88.47(10) 5_455 1_665
O3 O1 Ga2 58.55(12) 2_565 1_665
Ga2 O1 Ga2 111.6(2) 1_565 1_665
Ga2 O1 Ga2 111.6(2) . 1_665
Ga2 O1 O1 111.8(5) 2_566 2_465
La O1 O1 117.7(6) . 2_465
La O1 O1 96.1(4) 2_565 2_465
La O1 O1 12.92(4) 4_455 2_465
O2 O1 O1 68.3(4) 5_455 2_465
O2 O1 O1 98.4(7) 6 2_465
O2 O1 O1 44.4(3) 2_565 2_465
O2 O1 O1 139.9(6) 6_556 2_465
O2 O1 O1 105.1(4) 5_456 2_465
O2 O1 O1 85.6(3) 2_566 2_465
O3 O1 O1 162.5(8) 3_565 2_465
O3 O1 O1 59.85(15) . 2_465
O3 O1 O1 69.45(17) 4_455 2_465
Ga2 O1 O1 68.2(5) 2_565 2_465
Ga3 O1 O1 163.4(2) 2_565 2_465
Ga3 O1 O1 89.26(10) 1_556 2_465
Ga3 O1 O1 63.73(12) 4_456 2_465
O2 O1 O1 106.91(17) 3_455 2_465
O2 O1 O1 136.0(2) 4 2_465
O2 O1 O1 35.4(2) 1_565 2_465
O3 O1 O1 38.56(18) 2_465 2_465
O3 O1 O1 126.0(7) 5_445 2_465
O3 O1 O1 69.3(3) 6_665 2_465
Ga3 O1 O1 108.8(6) 2_564 2_465
Ga3 O1 O1 65.7(3) . 2_465
Ga3 O1 O1 42.6(3) 4_455 2_465
Ga1 O1 O1 58.12(8) 1_455 2_465
Nb O1 O1 58.12(8) 1_455 2_465
Ga1 O1 O1 146.8(7) . 2_465
Nb O1 O1 146.8(7) . 2_465
Ga1 O1 O1 58.12(8) 1_565 2_465
Nb O1 O1 58.12(8) 1_565 2_465
O2 O1 O1 138.4(2) . 2_465
O2 O1 O1 102.51(12) 3_565 2_465
O2 O1 O1 35.0(2) 4_455 2_465
La O1 O1 130.2(5) 1_556 2_465
La O1 O1 116.8(4) 2_566 2_465
La O1 O1 82.4(3) 4_456 2_465
O3 O1 O1 71.2(3) 2_466 2_465
O3 O1 O1 94.0(2) 6_666 2_465
O3 O1 O1 158.2(5) 5_446 2_465
O3 O1 O1 71.6(3) 6 2_465
O3 O1 O1 37.15(15) 5_455 2_465
O3 O1 O1 128.6(6) 2_565 2_465
Ga2 O1 O1 39.1(2) 1_565 2_465
Ga2 O1 O1 123.619(10) . 2_465
Ga2 O1 O1 123.619(11) 1_665 2_465
Ga2 O1 O1 111.8(5) 2_566 2_455
La O1 O1 12.92(5) . 2_455
La O1 O1 117.7(6) 2_565 2_455
La O1 O1 96.1(4) 4_455 2_455
O2 O1 O1 44.4(3) 5_455 2_455
O2 O1 O1 68.3(4) 6 2_455
O2 O1 O1 98.4(7) 2_565 2_455
O2 O1 O1 105.1(4) 6_556 2_455
O2 O1 O1 85.6(3) 5_456 2_455
O2 O1 O1 139.9(6) 2_566 2_455
O3 O1 O1 59.85(15) 3_565 2_455
O3 O1 O1 69.45(17) . 2_455
O3 O1 O1 162.5(8) 4_455 2_455
Ga2 O1 O1 68.2(5) 2_565 2_455
Ga3 O1 O1 89.26(10) 2_565 2_455
Ga3 O1 O1 63.73(12) 1_556 2_455
Ga3 O1 O1 163.4(2) 4_456 2_455
O2 O1 O1 35.4(2) 3_455 2_455
O2 O1 O1 106.91(17) 4 2_455
O2 O1 O1 136.0(2) 1_565 2_455
O3 O1 O1 69.3(3) 2_465 2_455
O3 O1 O1 38.56(18) 5_445 2_455
O3 O1 O1 126.0(7) 6_665 2_455
Ga3 O1 O1 65.7(3) 2_564 2_455
Ga3 O1 O1 42.6(3) . 2_455
Ga3 O1 O1 108.8(6) 4_455 2_455
Ga1 O1 O1 58.12(8) 1_455 2_455
Nb O1 O1 58.12(8) 1_455 2_455
Ga1 O1 O1 58.12(9) . 2_455
Nb O1 O1 58.12(9) . 2_455
Ga1 O1 O1 146.8(7) 1_565 2_455
Nb O1 O1 146.8(7) 1_565 2_455
O2 O1 O1 35.0(2) . 2_455
O2 O1 O1 138.4(2) 3_565 2_455
O2 O1 O1 102.51(12) 4_455 2_455
La O1 O1 82.4(3) 1_556 2_455
La O1 O1 130.2(5) 2_566 2_455
La O1 O1 116.8(4) 4_456 2_455
O3 O1 O1 94.0(2) 2_466 2_455
O3 O1 O1 158.2(5) 6_666 2_455
O3 O1 O1 71.2(3) 5_446 2_455
O3 O1 O1 37.15(15) 6 2_455
O3 O1 O1 128.6(6) 5_455 2_455
O3 O1 O1 71.6(3) 2_565 2_455
Ga2 O1 O1 123.619(11) 1_565 2_455
Ga2 O1 O1 39.1(2) . 2_455
Ga2 O1 O1 123.618(11) 1_665 2_455
O1 O1 O1 107.0(5) 2_465 2_455
Ga2 O1 O1 111.8(5) 2_566 2_565
La O1 O1 96.1(4) . 2_565
La O1 O1 12.92(4) 2_565 2_565
La O1 O1 117.7(6) 4_455 2_565
O2 O1 O1 98.4(7) 5_455 2_565
O2 O1 O1 44.4(3) 6 2_565
O2 O1 O1 68.3(4) 2_565 2_565
O2 O1 O1 85.6(3) 6_556 2_565
O2 O1 O1 139.9(6) 5_456 2_565
O2 O1 O1 105.1(4) 2_566 2_565
O3 O1 O1 69.45(17) 3_565 2_565
O3 O1 O1 162.5(8) . 2_565
O3 O1 O1 59.85(15) 4_455 2_565
Ga2 O1 O1 68.2(5) 2_565 2_565
Ga3 O1 O1 63.73(12) 2_565 2_565
Ga3 O1 O1 163.4(2) 1_556 2_565
Ga3 O1 O1 89.26(10) 4_456 2_565
O2 O1 O1 136.0(2) 3_455 2_565
O2 O1 O1 35.4(2) 4 2_565
O2 O1 O1 106.91(17) 1_565 2_565
O3 O1 O1 126.0(7) 2_465 2_565
O3 O1 O1 69.3(3) 5_445 2_565
O3 O1 O1 38.56(18) 6_665 2_565
Ga3 O1 O1 42.6(3) 2_564 2_565
Ga3 O1 O1 108.8(6) . 2_565
Ga3 O1 O1 65.7(3) 4_455 2_565
Ga1 O1 O1 146.8(7) 1_455 2_565
Nb O1 O1 146.8(7) 1_455 2_565
Ga1 O1 O1 58.12(8) . 2_565
Nb O1 O1 58.12(8) . 2_565
Ga1 O1 O1 58.12(8) 1_565 2_565
Nb O1 O1 58.12(8) 1_565 2_565
O2 O1 O1 102.51(12) . 2_565
O2 O1 O1 35.0(2) 3_565 2_565
O2 O1 O1 138.4(2) 4_455 2_565
La O1 O1 116.8(4) 1_556 2_565
La O1 O1 82.4(3) 2_566 2_565
La O1 O1 130.2(5) 4_456 2_565
O3 O1 O1 158.2(5) 2_466 2_565
O3 O1 O1 71.2(3) 6_666 2_565
O3 O1 O1 94.0(2) 5_446 2_565
O3 O1 O1 128.6(6) 6 2_565
O3 O1 O1 71.6(3) 5_455 2_565
O3 O1 O1 37.15(15) 2_565 2_565
Ga2 O1 O1 123.619(11) 1_565 2_565
Ga2 O1 O1 123.619(11) . 2_565
Ga2 O1 O1 39.1(2) 1_665 2_565
O1 O1 O1 107.0(5) 2_465 2_565
O1 O1 O1 107.0(5) 2_455 2_565
Ga2 O1 O1 180.0 2_566 1_554
La O1 O1 68.8(5) . 1_554
La O1 O1 68.8(5) 2_565 1_554
La O1 O1 68.7(5) 4_455 1_554
O2 O1 O1 32.6(3) 5_455 1_554
O2 O1 O1 32.6(3) 6 1_554
O2 O1 O1 32.6(3) 2_565 1_554
O2 O1 O1 148.2(3) 6_556 1_554
O2 O1 O1 148.2(3) 5_456 1_554
O2 O1 O1 148.2(3) 2_566 1_554
O3 O1 O1 95.2(5) 3_565 1_554
O3 O1 O1 95.2(5) . 1_554
O3 O1 O1 95.2(5) 4_455 1_554
Ga2 O1 O1 0.0 2_565 1_554
Ga3 O1 O1 116.8(3) 2_565 1_554
Ga3 O1 O1 116.8(3) 1_556 1_554
Ga3 O1 O1 116.8(3) 4_456 1_554
O2 O1 O1 100.1(4) 3_455 1_554
O2 O1 O1 100.1(4) 4 1_554
O2 O1 O1 100.1(4) 1_565 1_554
O3 O1 O1 60.6(3) 2_465 1_554
O3 O1 O1 60.6(3) 5_445 1_554
O3 O1 O1 60.6(3) 6_665 1_554
Ga3 O1 O1 42.41(18) 2_564 1_554
Ga3 O1 O1 42.41(18) . 1_554
Ga3 O1 O1 42.41(18) 4_455 1_554
Ga1 O1 O1 78.7(3) 1_455 1_554
Nb O1 O1 78.7(3) 1_455 1_554
Ga1 O1 O1 78.7(3) . 1_554
Nb O1 O1 78.7(3) . 1_554
Ga1 O1 O1 78.7(3) 1_565 1_554
Nb O1 O1 78.7(3) 1_565 1_554
O2 O1 O1 97.5(3) . 1_554
O2 O1 O1 97.5(3) 3_565 1_554
O2 O1 O1 97.5(3) 4_455 1_554
La O1 O1 149.83(13) 1_556 1_554
La O1 O1 149.82(13) 2_566 1_554
La O1 O1 149.82(13) 4_456 1_554
O3 O1 O1 127.3(2) 2_466 1_554
O3 O1 O1 127.3(2) 6_666 1_554
O3 O1 O1 127.3(2) 5_446 1_554
O3 O1 O1 64.0(3) 6 1_554
O3 O1 O1 64.0(3) 5_455 1_554
O3 O1 O1 64.0(3) 2_565 1_554
Ga2 O1 O1 107.3(2) 1_565 1_554
Ga2 O1 O1 107.3(2) . 1_554
Ga2 O1 O1 107.3(2) 1_665 1_554
O1 O1 O1 68.2(5) 2_465 1_554
O1 O1 O1 68.2(5) 2_455 1_554
O1 O1 O1 68.2(5) 2_565 1_554
Ga2 O1 O1 0.0 2_566 1_556
La O1 O1 111.3(5) . 1_556
La O1 O1 111.3(5) 2_565 1_556
La O1 O1 111.2(5) 4_455 1_556
O2 O1 O1 147.4(3) 5_455 1_556
O2 O1 O1 147.4(3) 6 1_556
O2 O1 O1 147.4(3) 2_565 1_556
O2 O1 O1 31.8(3) 6_556 1_556
O2 O1 O1 31.8(3) 5_456 1_556
O2 O1 O1 31.8(3) 2_566 1_556
O3 O1 O1 84.8(5) 3_565 1_556
O3 O1 O1 84.8(5) . 1_556
O3 O1 O1 84.8(5) 4_455 1_556
Ga2 O1 O1 180.0 2_565 1_556
Ga3 O1 O1 63.2(3) 2_565 1_556
Ga3 O1 O1 63.2(3) 1_556 1_556
Ga3 O1 O1 63.2(3) 4_456 1_556
O2 O1 O1 79.9(4) 3_455 1_556
O2 O1 O1 79.9(4) 4 1_556
O2 O1 O1 79.9(4) 1_565 1_556
O3 O1 O1 119.4(3) 2_465 1_556
O3 O1 O1 119.4(3) 5_445 1_556
O3 O1 O1 119.4(3) 6_665 1_556
Ga3 O1 O1 137.59(18) 2_564 1_556
Ga3 O1 O1 137.59(18) . 1_556
Ga3 O1 O1 137.59(18) 4_455 1_556
Ga1 O1 O1 101.3(3) 1_455 1_556
Nb O1 O1 101.3(3) 1_455 1_556
Ga1 O1 O1 101.3(3) . 1_556
Nb O1 O1 101.3(3) . 1_556
Ga1 O1 O1 101.3(3) 1_565 1_556
Nb O1 O1 101.3(3) 1_565 1_556
O2 O1 O1 82.5(3) . 1_556
O2 O1 O1 82.5(3) 3_565 1_556
O2 O1 O1 82.5(3) 4_455 1_556
La O1 O1 30.18(13) 1_556 1_556
La O1 O1 30.18(13) 2_566 1_556
La O1 O1 30.18(13) 4_456 1_556
O3 O1 O1 52.7(2) 2_466 1_556
O3 O1 O1 52.7(2) 6_666 1_556
O3 O1 O1 52.7(2) 5_446 1_556
O3 O1 O1 116.0(3) 6 1_556
O3 O1 O1 116.0(3) 5_455 1_556
O3 O1 O1 116.0(3) 2_565 1_556
Ga2 O1 O1 72.7(2) 1_565 1_556
Ga2 O1 O1 72.7(2) . 1_556
Ga2 O1 O1 72.7(2) 1_665 1_556
O1 O1 O1 111.8(5) 2_465 1_556
O1 O1 O1 111.8(5) 2_455 1_556
O1 O1 O1 111.8(5) 2_565 1_556
O1 O1 O1 179.999(1) 1_554 1_556
Ga2 O1 Ga3 72.4(2) 2_566 4_446
La O1 Ga3 45.42(19) . 4_446
La O1 Ga3 101.69(4) 2_565 4_446
La O1 Ga3 145.92(5) 4_455 4_446
O2 O1 Ga3 96.73(19) 5_455 4_446
O2 O1 Ga3 83.98(19) 6 4_446
O2 O1 Ga3 138.8(5) 2_565 4_446
O2 O1 Ga3 52.48(18) 6_556 4_446
O2 O1 Ga3 66.9(2) 5_456 4_446
O2 O1 Ga3 103.3(5) 2_566 4_446
O3 O1 Ga3 20.5(2) 3_565 4_446
O3 O1 Ga3 101.0(2) . 4_446
O3 O1 Ga3 131.6(3) 4_455 4_446
Ga2 O1 Ga3 107.6(2) 2_565 4_446
Ga3 O1 Ga3 37.58(6) 2_565 4_446
Ga3 O1 Ga3 73.89(16) 1_556 4_446
Ga3 O1 Ga3 131.4(5) 4_456 4_446
O2 O1 Ga3 52.39(16) 3_455 4_446
O2 O1 Ga3 64.64(16) 4 4_446
O2 O1 Ga3 151.6(6) 1_565 4_446
O3 O1 Ga3 120.57(14) 2_465 4_446
O3 O1 Ga3 47.17(17) 5_445 4_446
O3 O1 Ga3 128.06(13) 6_665 4_446
Ga3 O1 Ga3 74.20(7) 2_564 4_446
Ga3 O1 Ga3 96.71(11) . 4_446
Ga3 O1 Ga3 145.7(4) 4_455 4_446
Ga1 O1 Ga3 100.80(4) 1_455 4_446
Nb O1 Ga3 100.80(4) 1_455 4_446
Ga1 O1 Ga3 36.26(3) . 4_446
Nb O1 Ga3 36.26(3) . 4_446
Ga1 O1 Ga3 142.86(8) 1_565 4_446
Nb O1 Ga3 142.86(8) 1_565 4_446
O2 O1 Ga3 20.59(11) . 4_446
O2 O1 Ga3 98.66(16) 3_565 4_446
O2 O1 Ga3 131.8(3) 4_455 4_446
La O1 Ga3 45.63(11) 1_556 4_446
La O1 Ga3 77.8(2) 2_566 4_446
La O1 Ga3 97.2(3) 4_456 4_446
O3 O1 Ga3 98.4(3) 2_466 4_446
O3 O1 Ga3 104.1(3) 6_666 4_446
O3 O1 Ga3 20.01(12) 5_446 4_446
O3 O1 Ga3 87.75(10) 6 4_446
O3 O1 Ga3 161.0(2) 5_455 4_446
O3 O1 Ga3 59.48(11) 2_565 4_446
Ga2 O1 Ga3 138.9(4) 1_565 4_446
Ga2 O1 Ga3 36.07(5) . 4_446
Ga2 O1 Ga3 77.61(12) 1_665 4_446
O1 O1 Ga3 158.77(12) 2_465 4_446
O1 O1 Ga3 54.14(16) 2_455 4_446
O1 O1 Ga3 89.50(7) 2_565 4_446
O1 O1 Ga3 107.6(2) 1_554 4_446
O1 O1 Ga3 72.4(2) 1_556 4_446
Ga2 O1 Ga3 72.4(2) 2_566 2_465
La O1 Ga3 101.69(4) . 2_465
La O1 Ga3 145.92(5) 2_565 2_465
La O1 Ga3 45.42(19) 4_455 2_465
O2 O1 Ga3 83.98(19) 5_455 2_465
O2 O1 Ga3 138.8(5) 6 2_465
O2 O1 Ga3 96.73(19) 2_565 2_465
O2 O1 Ga3 103.3(5) 6_556 2_465
O2 O1 Ga3 52.48(18) 5_456 2_465
O2 O1 Ga3 66.9(2) 2_566 2_465
O3 O1 Ga3 131.6(3) 3_565 2_465
O3 O1 Ga3 20.5(2) . 2_465
O3 O1 Ga3 101.0(2) 4_455 2_465
Ga2 O1 Ga3 107.6(2) 2_565 2_465
Ga3 O1 Ga3 131.4(5) 2_565 2_465
Ga3 O1 Ga3 37.58(6) 1_556 2_465
Ga3 O1 Ga3 73.89(16) 4_456 2_465
O2 O1 Ga3 64.64(16) 3_455 2_465
O2 O1 Ga3 151.6(6) 4 2_465
O2 O1 Ga3 52.39(16) 1_565 2_465
O3 O1 Ga3 47.17(17) 2_465 2_465
O3 O1 Ga3 128.06(13) 5_445 2_465
O3 O1 Ga3 120.57(14) 6_665 2_465
Ga3 O1 Ga3 145.7(4) 2_564 2_465
Ga3 O1 Ga3 74.20(7) . 2_465
Ga3 O1 Ga3 96.71(11) 4_455 2_465
Ga1 O1 Ga3 36.26(3) 1_455 2_465
Nb O1 Ga3 36.26(3) 1_455 2_465
Ga1 O1 Ga3 142.86(8) . 2_465
Nb O1 Ga3 142.86(8) . 2_465
Ga1 O1 Ga3 100.80(4) 1_565 2_465
Nb O1 Ga3 100.80(4) 1_565 2_465
O2 O1 Ga3 98.66(16) . 2_465
O2 O1 Ga3 131.8(3) 3_565 2_465
O2 O1 Ga3 20.59(11) 4_455 2_465
La O1 Ga3 77.8(2) 1_556 2_465
La O1 Ga3 97.2(3) 2_566 2_465
La O1 Ga3 45.63(11) 4_456 2_465
O3 O1 Ga3 20.01(12) 2_466 2_465
O3 O1 Ga3 98.4(3) 6_666 2_465
O3 O1 Ga3 104.1(3) 5_446 2_465
O3 O1 Ga3 59.48(11) 6 2_465
O3 O1 Ga3 87.75(10) 5_455 2_465
O3 O1 Ga3 161.0(2) 2_565 2_465
Ga2 O1 Ga3 36.07(5) 1_565 2_465
Ga2 O1 Ga3 77.61(12) . 2_465
Ga2 O1 Ga3 138.9(4) 1_665 2_465
O1 O1 Ga3 54.14(16) 2_465 2_465
O1 O1 Ga3 89.50(7) 2_455 2_465
O1 O1 Ga3 158.77(12) 2_565 2_465
O1 O1 Ga3 107.6(2) 1_554 2_465
O1 O1 Ga3 72.4(2) 1_556 2_465
Ga3 O1 Ga3 111.3(2) 4_446 2_465
Ga2 O1 Ga3 72.4(2) 2_566 1_666
La O1 Ga3 145.92(5) . 1_666
La O1 Ga3 45.42(19) 2_565 1_666
La O1 Ga3 101.69(4) 4_455 1_666
O2 O1 Ga3 138.8(5) 5_455 1_666
O2 O1 Ga3 96.73(19) 6 1_666
O2 O1 Ga3 83.98(19) 2_565 1_666
O2 O1 Ga3 66.9(2) 6_556 1_666
O2 O1 Ga3 103.3(5) 5_456 1_666
O2 O1 Ga3 52.48(18) 2_566 1_666
O3 O1 Ga3 101.0(2) 3_565 1_666
O3 O1 Ga3 131.6(3) . 1_666
O3 O1 Ga3 20.5(2) 4_455 1_666
Ga2 O1 Ga3 107.6(2) 2_565 1_666
Ga3 O1 Ga3 73.89(16) 2_565 1_666
Ga3 O1 Ga3 131.4(5) 1_556 1_666
Ga3 O1 Ga3 37.58(6) 4_456 1_666
O2 O1 Ga3 151.6(6) 3_455 1_666
O2 O1 Ga3 52.39(16) 4 1_666
O2 O1 Ga3 64.64(16) 1_565 1_666
O3 O1 Ga3 128.06(13) 2_465 1_666
O3 O1 Ga3 120.57(14) 5_445 1_666
O3 O1 Ga3 47.17(17) 6_665 1_666
Ga3 O1 Ga3 96.71(11) 2_564 1_666
Ga3 O1 Ga3 145.7(4) . 1_666
Ga3 O1 Ga3 74.20(7) 4_455 1_666
Ga1 O1 Ga3 142.86(8) 1_455 1_666
Nb O1 Ga3 142.86(8) 1_455 1_666
Ga1 O1 Ga3 100.80(4) . 1_666
Nb O1 Ga3 100.80(4) . 1_666
Ga1 O1 Ga3 36.26(3) 1_565 1_666
Nb O1 Ga3 36.26(3) 1_565 1_666
O2 O1 Ga3 131.8(3) . 1_666
O2 O1 Ga3 20.59(11) 3_565 1_666
O2 O1 Ga3 98.66(16) 4_455 1_666
La O1 Ga3 97.2(3) 1_556 1_666
La O1 Ga3 45.63(11) 2_566 1_666
La O1 Ga3 77.8(2) 4_456 1_666
O3 O1 Ga3 104.1(3) 2_466 1_666
O3 O1 Ga3 20.01(12) 6_666 1_666
O3 O1 Ga3 98.4(3) 5_446 1_666
O3 O1 Ga3 161.0(2) 6 1_666
O3 O1 Ga3 59.48(11) 5_455 1_666
O3 O1 Ga3 87.75(10) 2_565 1_666
Ga2 O1 Ga3 77.61(12) 1_565 1_666
Ga2 O1 Ga3 138.9(4) . 1_666
Ga2 O1 Ga3 36.07(5) 1_665 1_666
O1 O1 Ga3 89.50(7) 2_465 1_666
O1 O1 Ga3 158.77(12) 2_455 1_666
O1 O1 Ga3 54.14(16) 2_565 1_666
O1 O1 Ga3 107.6(2) 1_554 1_666
O1 O1 Ga3 72.4(2) 1_556 1_666
Ga3 O1 Ga3 111.3(2) 4_446 1_666
Ga3 O1 Ga3 111.3(2) 2_465 1_666
Ga2 O1 O3 56.6(3) 2_566 6_556
La O1 O3 75.3(2) . 6_556
La O1 O3 166.9(6) 2_565 6_556
La O1 O3 83.0(2) 4_455 6_556
O2 O1 O3 90.9(2) 5_455 6_556
O2 O1 O3 135.7(3) 6 6_556
O2 O1 O3 131.4(3) 2_565 6_556
O2 O1 O3 77.2(4) 6_556 6_556
O2 O1 O3 24.9(2) 5_456 6_556
O2 O1 O3 74.0(4) 2_566 6_556
O3 O1 O3 91.4(3) 3_565 6_556
O3 O1 O3 36.5(3) . 6_556
O3 O1 O3 129.1(5) 4_455 6_556
Ga2 O1 O3 123.4(3) 2_565 6_556
Ga3 O1 O3 95.8(4) 2_565 6_556
Ga3 O1 O3 6.87(17) 1_556 6_556
Ga3 O1 O3 98.5(4) 4_456 6_556
O2 O1 O3 32.6(2) 3_455 6_556
O2 O1 O3 125.1(5) 4 6_556
O2 O1 O3 88.7(3) 1_565 6_556
O3 O1 O3 72.03(12) 2_465 6_556
O3 O1 O3 100.25(16) 5_445 6_556
O3 O1 O3 160.23(19) 6_665 6_556
Ga3 O1 O3 132.12(14) 2_564 6_556
Ga3 O1 O3 81.03(14) . 6_556
Ga3 O1 O3 134.85(16) 4_455 6_556
Ga1 O1 O3 48.44(14) 1_455 6_556
Nb O1 O3 48.44(14) 1_455 6_556
Ga1 O1 O3 104.95(15) . 6_556
Nb O1 O3 104.95(15) . 6_556
Ga1 O1 O3 136.9(2) 1_565 6_556
Nb O1 O3 136.9(2) 1_565 6_556
O2 O1 O3 60.97(18) . 6_556
O2 O1 O3 139.1(5) 3_565 6_556
O2 O1 O3 60.93(17) 4_455 6_556
La O1 O3 43.92(19) 1_556 6_556
La O1 O3 86.6(4) 2_566 6_556
La O1 O3 49.5(2) 4_456 6_556
O3 O1 O3 30.46(17) 2_466 6_556
O3 O1 O3 106.2(4) 6_666 6_556
O3 O1 O3 65.3(3) 5_446 6_556
O3 O1 O3 59.45(9) 6 6_556
O3 O1 O3 128.07(7) 5_455 6_556
O3 O1 O3 128.07(7) 2_565 6_556
Ga2 O1 O3 71.97(17) 1_565 6_556
Ga2 O1 O3 39.71(11) . 6_556
Ga2 O1 O3 126.0(4) 1_665 6_556
O1 O1 O3 93.6(2) 2_465 6_556
O1 O1 O3 67.4(2) 2_455 6_556
O1 O1 O3 159.3(4) 2_565 6_556
O1 O1 O3 123.4(3) 1_554 6_556
O1 O1 O3 56.6(3) 1_556 6_556
Ga3 O1 O3 70.95(18) 4_446 6_556
Ga3 O1 O3 40.39(11) 2_465 6_556
Ga3 O1 O3 126.0(4) 1_666 6_556
Ga2 O1 O3 56.6(3) 2_566 5_456
La O1 O3 166.9(6) . 5_456
La O1 O3 83.0(2) 2_565 5_456
La O1 O3 75.3(2) 4_455 5_456
O2 O1 O3 135.7(3) 5_455 5_456
O2 O1 O3 131.4(3) 6 5_456
O2 O1 O3 90.9(2) 2_565 5_456
O2 O1 O3 74.0(4) 6_556 5_456
O2 O1 O3 77.2(4) 5_456 5_456
O2 O1 O3 24.9(2) 2_566 5_456
O3 O1 O3 129.1(5) 3_565 5_456
O3 O1 O3 91.4(3) . 5_456
O3 O1 O3 36.5(3) 4_455 5_456
Ga2 O1 O3 123.4(3) 2_565 5_456
Ga3 O1 O3 98.5(4) 2_565 5_456
Ga3 O1 O3 95.8(4) 1_556 5_456
Ga3 O1 O3 6.87(17) 4_456 5_456
O2 O1 O3 125.1(5) 3_455 5_456
O2 O1 O3 88.7(3) 4 5_456
O2 O1 O3 32.6(2) 1_565 5_456
O3 O1 O3 100.25(16) 2_465 5_456
O3 O1 O3 160.23(19) 5_445 5_456
O3 O1 O3 72.03(12) 6_665 5_456
Ga3 O1 O3 134.85(16) 2_564 5_456
Ga3 O1 O3 132.12(14) . 5_456
Ga3 O1 O3 81.03(14) 4_455 5_456
Ga1 O1 O3 104.95(15) 1_455 5_456
Nb O1 O3 104.95(15) 1_455 5_456
Ga1 O1 O3 136.9(2) . 5_456
Nb O1 O3 136.9(2) . 5_456
Ga1 O1 O3 48.44(14) 1_565 5_456
Nb O1 O3 48.44(14) 1_565 5_456
O2 O1 O3 139.1(5) . 5_456
O2 O1 O3 60.93(17) 3_565 5_456
O2 O1 O3 60.97(18) 4_455 5_456
La O1 O3 86.6(4) 1_556 5_456
La O1 O3 49.5(2) 2_566 5_456
La O1 O3 43.92(19) 4_456 5_456
O3 O1 O3 65.3(3) 2_466 5_456
O3 O1 O3 30.46(17) 6_666 5_456
O3 O1 O3 106.2(4) 5_446 5_456
O3 O1 O3 128.07(7) 6 5_456
O3 O1 O3 59.45(8) 5_455 5_456
O3 O1 O3 128.07(7) 2_565 5_456
Ga2 O1 O3 39.71(11) 1_565 5_456
Ga2 O1 O3 126.0(4) . 5_456
Ga2 O1 O3 71.97(17) 1_665 5_456
O1 O1 O3 67.4(2) 2_465 5_456
O1 O1 O3 159.3(4) 2_455 5_456
O1 O1 O3 93.6(2) 2_565 5_456
O1 O1 O3 123.4(3) 1_554 5_456
O1 O1 O3 56.6(3) 1_556 5_456
Ga3 O1 O3 126.0(4) 4_446 5_456
Ga3 O1 O3 70.95(18) 2_465 5_456
Ga3 O1 O3 40.38(11) 1_666 5_456
O3 O1 O3 92.6(3) 6_556 5_456
Ga2 O1 O3 56.6(3) 2_566 2_566
La O1 O3 83.0(2) . 2_566
La O1 O3 75.3(2) 2_565 2_566
La O1 O3 166.9(6) 4_455 2_566
O2 O1 O3 131.4(3) 5_455 2_566
O2 O1 O3 90.9(2) 6 2_566
O2 O1 O3 135.7(3) 2_565 2_566
O2 O1 O3 24.9(2) 6_556 2_566
O2 O1 O3 74.0(4) 5_456 2_566
O2 O1 O3 77.2(4) 2_566 2_566
O3 O1 O3 36.5(3) 3_565 2_566
O3 O1 O3 129.1(5) . 2_566
O3 O1 O3 91.4(3) 4_455 2_566
Ga2 O1 O3 123.4(3) 2_565 2_566
Ga3 O1 O3 6.87(17) 2_565 2_566
Ga3 O1 O3 98.5(4) 1_556 2_566
Ga3 O1 O3 95.8(4) 4_456 2_566
O2 O1 O3 88.7(3) 3_455 2_566
O2 O1 O3 32.6(2) 4 2_566
O2 O1 O3 125.1(5) 1_565 2_566
O3 O1 O3 160.23(19) 2_465 2_566
O3 O1 O3 72.03(12) 5_445 2_566
O3 O1 O3 100.25(16) 6_665 2_566
Ga3 O1 O3 81.03(14) 2_564 2_566
Ga3 O1 O3 134.85(16) . 2_566
Ga3 O1 O3 132.12(14) 4_455 2_566
Ga1 O1 O3 136.9(2) 1_455 2_566
Nb O1 O3 136.9(2) 1_455 2_566
Ga1 O1 O3 48.44(14) . 2_566
Nb O1 O3 48.44(14) . 2_566
Ga1 O1 O3 104.95(15) 1_565 2_566
Nb O1 O3 104.95(15) 1_565 2_566
O2 O1 O3 60.93(17) . 2_566
O2 O1 O3 60.97(18) 3_565 2_566
O2 O1 O3 139.1(5) 4_455 2_566
La O1 O3 49.5(2) 1_556 2_566
La O1 O3 43.92(19) 2_566 2_566
La O1 O3 86.6(4) 4_456 2_566
O3 O1 O3 106.2(4) 2_466 2_566
O3 O1 O3 65.3(3) 6_666 2_566
O3 O1 O3 30.45(17) 5_446 2_566
O3 O1 O3 128.07(7) 6 2_566
O3 O1 O3 128.07(7) 5_455 2_566
O3 O1 O3 59.45(8) 2_565 2_566
Ga2 O1 O3 126.0(4) 1_565 2_566
Ga2 O1 O3 71.97(17) . 2_566
Ga2 O1 O3 39.71(11) 1_665 2_566
O1 O1 O3 159.3(4) 2_465 2_566
O1 O1 O3 93.6(2) 2_455 2_566
O1 O1 O3 67.4(2) 2_565 2_566
O1 O1 O3 123.4(3) 1_554 2_566
O1 O1 O3 56.6(3) 1_556 2_566
Ga3 O1 O3 40.39(11) 4_446 2_566
Ga3 O1 O3 126.0(4) 2_465 2_566
Ga3 O1 O3 70.95(18) 1_666 2_566
O3 O1 O3 92.6(3) 6_556 2_566
O3 O1 O3 92.6(3) 5_456 2_566
Ga2 O1 O3 87.0(3) 2_566 1_655
La O1 O3 65.30(9) . 1_655
La O1 O3 61.72(9) 2_565 1_655
La O1 O3 161.7(7) 4_455 1_655
O2 O1 O3 104.5(3) 5_455 1_655
O2 O1 O3 60.7(2) 6 1_655
O2 O1 O3 111.9(4) 2_565 1_655
O2 O1 O3 55.5(2) 6_556 1_655
O2 O1 O3 99.0(3) 5_456 1_655
O2 O1 O3 106.0(4) 2_566 1_655
O3 O1 O3 21.34(18) 3_565 1_655
O3 O1 O3 140.5(2) . 1_655
O3 O1 O3 98.39(19) 4_455 1_655
Ga2 O1 O3 93.0(3) 2_565 1_655
Ga3 O1 O3 23.79(16) 2_565 1_655
Ga3 O1 O3 113.6(2) 1_556 1_655
Ga3 O1 O3 116.3(2) 4_456 1_655
O2 O1 O3 91.01(16) 3_455 1_655
O2 O1 O3 29.09(16) 4 1_655
O2 O1 O3 145.9(3) 1_565 1_655
O3 O1 O3 143.7(4) 2_465 1_655
O3 O1 O3 45.7(2) 5_445 1_655
O3 O1 O3 88.28(19) 6_665 1_655
Ga3 O1 O3 50.65(15) 2_564 1_655
Ga3 O1 O3 111.1(3) . 1_655
Ga3 O1 O3 113.1(3) 4_455 1_655
Ga1 O1 O3 135.50(11) 1_455 1_655
Nb O1 O3 135.50(11) 1_455 1_655
Ga1 O1 O3 21.35(11) . 1_655
Nb O1 O3 21.35(11) . 1_655
Ga1 O1 O3 104.44(9) 1_565 1_655
Nb O1 O3 104.44(9) 1_565 1_655
O2 O1 O3 56.29(11) . 1_655
O2 O1 O3 63.45(11) 3_565 1_655
O2 O1 O3 168.9(5) 4_455 1_655
La O1 O3 73.6(2) 1_556 1_655
La O1 O3 71.83(19) 2_566 1_655
La O1 O3 117.1(4) 4_456 1_655
O3 O1 O3 132.9(4) 2_466 1_655
O3 O1 O3 85.2(2) 6_666 1_655
O3 O1 O3 46.1(2) 5_446 1_655
O3 O1 O3 114.99(16) 6 1_655
O3 O1 O3 121.31(18) 5_455 1_655
O3 O1 O3 29.3(3) 2_565 1_655
Ga2 O1 O3 154.3(4) 1_565 1_655
Ga2 O1 O3 75.61(10) . 1_655
Ga2 O1 O3 45.56(9) 1_665 1_655
O1 O1 O3 155.7(5) 2_465 1_655
O1 O1 O3 78.08(9) 2_455 1_655
O1 O1 O3 49.79(11) 2_565 1_655
O1 O1 O3 93.0(3) 1_554 1_655
O1 O1 O3 87.0(3) 1_556 1_655
Ga3 O1 O3 40.00(9) 4_446 1_655
Ga3 O1 O3 150.0(3) 2_465 1_655
Ga3 O1 O3 81.46(10) 1_666 1_655
O3 O1 O3 110.0(2) 6_556 1_655
O3 O1 O3 115.6(2) 5_456 1_655
O3 O1 O3 30.6(3) 2_566 1_655
Ga2 O1 O3 87.0(3) 2_566 4_345
La O1 O3 61.72(9) . 4_345
La O1 O3 161.7(7) 2_565 4_345
La O1 O3 65.30(9) 4_455 4_345
O2 O1 O3 60.7(2) 5_455 4_345
O2 O1 O3 111.9(4) 6 4_345
O2 O1 O3 104.5(3) 2_565 4_345
O2 O1 O3 106.0(4) 6_556 4_345
O2 O1 O3 55.5(2) 5_456 4_345
O2 O1 O3 99.0(3) 2_566 4_345
O3 O1 O3 98.39(19) 3_565 4_345
O3 O1 O3 21.34(18) . 4_345
O3 O1 O3 140.5(2) 4_455 4_345
Ga2 O1 O3 93.0(3) 2_565 4_345
Ga3 O1 O3 116.3(2) 2_565 4_345
Ga3 O1 O3 23.79(16) 1_556 4_345
Ga3 O1 O3 113.6(2) 4_456 4_345
O2 O1 O3 29.09(16) 3_455 4_345
O2 O1 O3 145.9(3) 4 4_345
O2 O1 O3 91.01(16) 1_565 4_345
O3 O1 O3 45.7(2) 2_465 4_345
O3 O1 O3 88.28(19) 5_445 4_345
O3 O1 O3 143.7(4) 6_665 4_345
Ga3 O1 O3 113.1(3) 2_564 4_345
Ga3 O1 O3 50.65(15) . 4_345
Ga3 O1 O3 111.1(3) 4_455 4_345
Ga1 O1 O3 21.35(11) 1_455 4_345
Nb O1 O3 21.35(11) 1_455 4_345
Ga1 O1 O3 104.45(9) . 4_345
Nb O1 O3 104.45(9) . 4_345
Ga1 O1 O3 135.50(11) 1_565 4_345
Nb O1 O3 135.50(11) 1_565 4_345
O2 O1 O3 63.45(11) . 4_345
O2 O1 O3 168.9(5) 3_565 4_345
O2 O1 O3 56.29(11) 4_455 4_345
La O1 O3 71.83(19) 1_556 4_345
La O1 O3 117.1(4) 2_566 4_345
La O1 O3 73.6(2) 4_456 4_345
O3 O1 O3 46.1(2) 2_466 4_345
O3 O1 O3 132.9(4) 6_666 4_345
O3 O1 O3 85.2(2) 5_446 4_345
O3 O1 O3 29.3(3) 6 4_345
O3 O1 O3 114.99(16) 5_455 4_345
O3 O1 O3 121.31(18) 2_565 4_345
Ga2 O1 O3 75.61(10) 1_565 4_345
Ga2 O1 O3 45.56(9) . 4_345
Ga2 O1 O3 154.3(4) 1_665 4_345
O1 O1 O3 78.08(9) 2_465 4_345
O1 O1 O3 49.79(11) 2_455 4_345
O1 O1 O3 155.7(5) 2_565 4_345
O1 O1 O3 93.0(3) 1_554 4_345
O1 O1 O3 87.0(3) 1_556 4_345
Ga3 O1 O3 81.46(10) 4_446 4_345
Ga3 O1 O3 39.99(9) 2_465 4_345
Ga3 O1 O3 150.0(3) 1_666 4_345
O3 O1 O3 30.6(3) 6_556 4_345
O3 O1 O3 110.0(2) 5_456 4_345
O3 O1 O3 115.6(2) 2_566 4_345
O3 O1 O3 119.72(5) 1_655 4_345
Ga2 O1 O3 87.0(3) 2_566 3_575
La O1 O3 161.7(7) . 3_575
La O1 O3 65.30(9) 2_565 3_575
La O1 O3 61.71(9) 4_455 3_575
O2 O1 O3 111.9(4) 5_455 3_575
O2 O1 O3 104.5(3) 6 3_575
O2 O1 O3 60.7(2) 2_565 3_575
O2 O1 O3 99.0(3) 6_556 3_575
O2 O1 O3 106.0(4) 5_456 3_575
O2 O1 O3 55.5(2) 2_566 3_575
O3 O1 O3 140.5(2) 3_565 3_575
O3 O1 O3 98.39(19) . 3_575
O3 O1 O3 21.34(19) 4_455 3_575
Ga2 O1 O3 93.0(3) 2_565 3_575
Ga3 O1 O3 113.6(2) 2_565 3_575
Ga3 O1 O3 116.3(2) 1_556 3_575
Ga3 O1 O3 23.79(16) 4_456 3_575
O2 O1 O3 145.9(3) 3_455 3_575
O2 O1 O3 91.01(16) 4 3_575
O2 O1 O3 29.09(16) 1_565 3_575
O3 O1 O3 88.28(19) 2_465 3_575
O3 O1 O3 143.7(4) 5_445 3_575
O3 O1 O3 45.7(2) 6_665 3_575
Ga3 O1 O3 111.1(3) 2_564 3_575
Ga3 O1 O3 113.1(3) . 3_575
Ga3 O1 O3 50.65(15) 4_455 3_575
Ga1 O1 O3 104.44(9) 1_455 3_575
Nb O1 O3 104.44(9) 1_455 3_575
Ga1 O1 O3 135.50(11) . 3_575
Nb O1 O3 135.50(11) . 3_575
Ga1 O1 O3 21.35(11) 1_565 3_575
Nb O1 O3 21.35(11) 1_565 3_575
O2 O1 O3 168.9(5) . 3_575
O2 O1 O3 56.29(11) 3_565 3_575
O2 O1 O3 63.45(11) 4_455 3_575
La O1 O3 117.1(4) 1_556 3_575
La O1 O3 73.6(2) 2_566 3_575
La O1 O3 71.83(19) 4_456 3_575
O3 O1 O3 85.2(2) 2_466 3_575
O3 O1 O3 46.1(2) 6_666 3_575
O3 O1 O3 132.9(4) 5_446 3_575
O3 O1 O3 121.31(18) 6 3_575
O3 O1 O3 29.3(3) 5_455 3_575
O3 O1 O3 114.99(16) 2_565 3_575
Ga2 O1 O3 45.56(9) 1_565 3_575
Ga2 O1 O3 154.3(4) . 3_575
Ga2 O1 O3 75.61(10) 1_665 3_575
O1 O1 O3 49.79(11) 2_465 3_575
O1 O1 O3 155.7(5) 2_455 3_575
O1 O1 O3 78.08(9) 2_565 3_575
O1 O1 O3 93.0(3) 1_554 3_575
O1 O1 O3 87.0(3) 1_556 3_575
Ga3 O1 O3 150.0(3) 4_446 3_575
Ga3 O1 O3 81.46(10) 2_465 3_575
Ga3 O1 O3 40.00(9) 1_666 3_575
O3 O1 O3 115.6(2) 6_556 3_575
O3 O1 O3 30.6(3) 5_456 3_575
O3 O1 O3 110.0(2) 2_566 3_575
O3 O1 O3 119.72(5) 1_655 3_575
O3 O1 O3 119.72(5) 4_345 3_575
Ga2 O1 O2 141.64(17) 2_566 3_454
La O1 O2 38.1(3) . 3_454
La O1 O2 102.4(6) 2_565 3_454
La O1 O2 73.7(4) 4_455 3_454
O2 O1 O2 13.34(17) 5_455 3_454
O2 O1 O2 52.6(3) 6 3_454
O2 O1 O2 66.4(4) 2_565 3_454
O2 O1 O2 135.91(16) 6_556 3_454
O2 O1 O2 111.1(2) 5_456 3_454
O2 O1 O2 156.95(14) 2_566 3_454
O3 O1 O2 82.1(3) 3_565 3_454
O3 O1 O2 70.8(3) . 3_454
O3 O1 O2 132.8(6) 4_455 3_454
Ga2 O1 O2 38.36(17) 2_565 3_454
Ga3 O1 O2 112.6(2) 2_565 3_454
Ga3 O1 O2 81.9(2) 1_556 3_454
Ga3 O1 O2 144.8(3) 4_456 3_454
O2 O1 O2 61.7(3) 3_455 3_454
O2 O1 O2 116.3(4) 4 3_454
O2 O1 O2 116.3(4) 1_565 3_454
O3 O1 O2 50.4(3) 2_465 3_454
O3 O1 O2 47.8(2) 5_445 3_454
O3 O1 O2 99.0(4) 6_665 3_454
Ga3 O1 O2 56.2(2) 2_564 3_454
Ga3 O1 O2 17.77(10) . 3_454
Ga3 O1 O2 76.8(3) 4_455 3_454
Ga1 O1 O2 53.88(17) 1_455 3_454
Nb O1 O2 53.88(17) 1_455 3_454
Ga1 O1 O2 72.3(2) . 3_454
Nb O1 O2 72.3(2) . 3_454
Ga1 O1 O2 115.6(4) 1_565 3_454
Nb O1 O2 115.6(4) 1_565 3_454
O2 O1 O2 66.38(18) . 3_454
O2 O1 O2 131.4(4) 3_565 3_454
O2 O1 O2 92.7(3) 4_455 3_454
La O1 O2 113.99(9) 1_556 3_454
La O1 O2 161.24(14) 2_566 3_454
La O1 O2 132.86(9) 4_456 3_454
O3 O1 O2 104.11(17) 2_466 3_454
O3 O1 O2 165.5(4) 6_666 3_454
O3 O1 O2 102.25(15) 5_446 3_454
O3 O1 O2 31.78(17) 6 3_454
O3 O1 O2 96.4(4) 5_455 3_454
O3 O1 O2 72.9(3) 2_565 3_454
Ga2 O1 O2 112.3(2) 1_565 3_454
Ga2 O1 O2 70.28(14) . 3_454
Ga2 O1 O2 131.1(3) 1_665 3_454
O1 O1 O2 81.4(4) 2_465 3_454
O1 O1 O2 32.2(3) 2_455 3_454
O1 O1 O2 96.9(5) 2_565 3_454
O1 O1 O2 38.36(17) 1_554 3_454
O1 O1 O2 141.64(17) 1_556 3_454
Ga3 O1 O2 83.46(13) 4_446 3_454
Ga3 O1 O2 90.04(14) 2_465 3_454
Ga3 O1 O2 145.6(4) 1_666 3_454
O3 O1 O2 87.82(17) 6_556 3_454
O3 O1 O2 148.8(2) 5_456 3_454
O3 O1 O2 118.59(18) 2_566 3_454
O3 O1 O2 93.4(2) 1_655 3_454
O3 O1 O2 59.78(19) 4_345 3_454
O3 O1 O2 124.7(4) 3_575 3_454
Ga2 O1 O2 141.64(17) 2_566 4_554
La O1 O2 73.7(4) . 4_554
La O1 O2 38.1(3) 2_565 4_554
La O1 O2 102.4(6) 4_455 4_554
O2 O1 O2 66.4(4) 5_455 4_554
O2 O1 O2 13.34(17) 6 4_554
O2 O1 O2 52.6(3) 2_565 4_554
O2 O1 O2 111.1(2) 6_556 4_554
O2 O1 O2 156.95(13) 5_456 4_554
O2 O1 O2 135.91(16) 2_566 4_554
O3 O1 O2 70.8(3) 3_565 4_554
O3 O1 O2 132.8(6) . 4_554
O3 O1 O2 82.1(3) 4_455 4_554
Ga2 O1 O2 38.36(17) 2_565 4_554
Ga3 O1 O2 81.9(2) 2_565 4_554
Ga3 O1 O2 144.8(3) 1_556 4_554
Ga3 O1 O2 112.6(2) 4_456 4_554
O2 O1 O2 116.3(4) 3_455 4_554
O2 O1 O2 61.7(3) 4 4_554
O2 O1 O2 116.3(4) 1_565 4_554
O3 O1 O2 99.0(4) 2_465 4_554
O3 O1 O2 50.4(3) 5_445 4_554
O3 O1 O2 47.8(2) 6_665 4_554
Ga3 O1 O2 17.77(10) 2_564 4_554
Ga3 O1 O2 76.8(3) . 4_554
Ga3 O1 O2 56.2(2) 4_455 4_554
Ga1 O1 O2 115.6(4) 1_455 4_554
Nb O1 O2 115.6(4) 1_455 4_554
Ga1 O1 O2 53.88(17) . 4_554
Nb O1 O2 53.88(17) . 4_554
Ga1 O1 O2 72.3(2) 1_565 4_554
Nb O1 O2 72.3(2) 1_565 4_554
O2 O1 O2 92.7(3) . 4_554
O2 O1 O2 66.38(18) 3_565 4_554
O2 O1 O2 131.4(4) 4_455 4_554
La O1 O2 132.86(9) 1_556 4_554
La O1 O2 113.99(9) 2_566 4_554
La O1 O2 161.24(14) 4_456 4_554
O3 O1 O2 165.5(4) 2_466 4_554
O3 O1 O2 102.25(15) 6_666 4_554
O3 O1 O2 104.11(17) 5_446 4_554
O3 O1 O2 96.4(4) 6 4_554
O3 O1 O2 72.9(3) 5_455 4_554
O3 O1 O2 31.78(17) 2_565 4_554
Ga2 O1 O2 131.1(3) 1_565 4_554
Ga2 O1 O2 112.3(2) . 4_554
Ga2 O1 O2 70.28(14) 1_665 4_554
O1 O1 O2 96.9(5) 2_465 4_554
O1 O1 O2 81.4(4) 2_455 4_554
O1 O1 O2 32.2(3) 2_565 4_554
O1 O1 O2 38.36(17) 1_554 4_554
O1 O1 O2 141.64(17) 1_556 4_554
Ga3 O1 O2 90.04(14) 4_446 4_554
Ga3 O1 O2 145.6(4) 2_465 4_554
Ga3 O1 O2 83.46(13) 1_666 4_554
O3 O1 O2 148.8(2) 6_556 4_554
O3 O1 O2 118.59(18) 5_456 4_554
O3 O1 O2 87.82(17) 2_566 4_554
O3 O1 O2 59.78(19) 1_655 4_554
O3 O1 O2 124.7(4) 4_345 4_554
O3 O1 O2 93.4(2) 3_575 4_554
O2 O1 O2 65.0(3) 3_454 4_554
Ga2 O1 O2 141.64(17) 2_566 1_564
La O1 O2 102.4(6) . 1_564
La O1 O2 73.7(4) 2_565 1_564
La O1 O2 38.1(3) 4_455 1_564
O2 O1 O2 52.6(3) 5_455 1_564
O2 O1 O2 66.4(4) 6 1_564
O2 O1 O2 13.34(17) 2_565 1_564
O2 O1 O2 156.95(14) 6_556 1_564
O2 O1 O2 135.91(16) 5_456 1_564
O2 O1 O2 111.1(2) 2_566 1_564
O3 O1 O2 132.8(6) 3_565 1_564
O3 O1 O2 82.1(3) . 1_564
O3 O1 O2 70.8(3) 4_455 1_564
Ga2 O1 O2 38.36(17) 2_565 1_564
Ga3 O1 O2 144.8(3) 2_565 1_564
Ga3 O1 O2 112.6(2) 1_556 1_564
Ga3 O1 O2 81.9(2) 4_456 1_564
O2 O1 O2 116.3(4) 3_455 1_564
O2 O1 O2 116.3(4) 4 1_564
O2 O1 O2 61.7(3) 1_565 1_564
O3 O1 O2 47.8(2) 2_465 1_564
O3 O1 O2 99.0(4) 5_445 1_564
O3 O1 O2 50.4(3) 6_665 1_564
Ga3 O1 O2 76.8(3) 2_564 1_564
Ga3 O1 O2 56.2(2) . 1_564
Ga3 O1 O2 17.77(10) 4_455 1_564
Ga1 O1 O2 72.3(2) 1_455 1_564
Nb O1 O2 72.3(2) 1_455 1_564
Ga1 O1 O2 115.6(4) . 1_564
Nb O1 O2 115.6(4) . 1_564
Ga1 O1 O2 53.88(17) 1_565 1_564
Nb O1 O2 53.88(17) 1_565 1_564
O2 O1 O2 131.4(4) . 1_564
O2 O1 O2 92.7(3) 3_565 1_564
O2 O1 O2 66.38(18) 4_455 1_564
La O1 O2 161.24(14) 1_556 1_564
La O1 O2 132.86(9) 2_566 1_564
La O1 O2 113.99(9) 4_456 1_564
O3 O1 O2 102.25(15) 2_466 1_564
O3 O1 O2 104.11(17) 6_666 1_564
O3 O1 O2 165.5(4) 5_446 1_564
O3 O1 O2 72.9(3) 6 1_564
O3 O1 O2 31.78(17) 5_455 1_564
O3 O1 O2 96.4(4) 2_565 1_564
Ga2 O1 O2 70.28(14) 1_565 1_564
Ga2 O1 O2 131.1(3) . 1_564
Ga2 O1 O2 112.3(2) 1_665 1_564
O1 O1 O2 32.2(3) 2_465 1_564
O1 O1 O2 96.9(5) 2_455 1_564
O1 O1 O2 81.4(4) 2_565 1_564
O1 O1 O2 38.36(17) 1_554 1_564
O1 O1 O2 141.64(17) 1_556 1_564
Ga3 O1 O2 145.6(4) 4_446 1_564
Ga3 O1 O2 83.46(13) 2_465 1_564
Ga3 O1 O2 90.04(14) 1_666 1_564
O3 O1 O2 118.59(18) 6_556 1_564
O3 O1 O2 87.82(17) 5_456 1_564
O3 O1 O2 148.8(2) 2_566 1_564
O3 O1 O2 124.7(4) 1_655 1_564
O3 O1 O2 93.4(2) 4_345 1_564
O3 O1 O2 59.78(19) 3_575 1_564
O2 O1 O2 65.0(3) 3_454 1_564
O2 O1 O2 65.0(3) 4_554 1_564
Ga2 O1 O1 55.6(4) 2_566 2_466
La O1 O1 137.5(3) . 2_466
La O1 O1 114.73(16) 2_565 2_466
La O1 O1 57.22(9) 4_455 2_466
O2 O1 O1 115.2(3) 5_455 2_466
O2 O1 O1 152.1(5) 6 2_466
O2 O1 O1 96.8(2) 2_565 2_466
O2 O1 O1 85.3(6) 6_556 2_466
O2 O1 O1 58.0(4) 5_456 2_466
O2 O1 O1 33.9(3) 2_566 2_466
O3 O1 O1 140.1(8) 3_565 2_466
O3 O1 O1 58.2(2) . 2_466
O3 O1 O1 66.9(2) 4_455 2_466
Ga2 O1 O1 124.4(4) 2_565 2_466
Ga3 O1 O1 116.6(7) 2_565 2_466
Ga3 O1 O1 65.5(3) 1_556 2_466
Ga3 O1 O1 37.16(12) 4_456 2_466
O2 O1 O1 95.8(4) 3_455 2_466
O2 O1 O1 118.8(5) 4 2_466
O2 O1 O1 28.3(2) 1_565 2_466
O3 O1 O1 75.20(17) 2_465 2_466
O3 O1 O1 164.1(2) 5_445 2_466
O3 O1 O1 97.22(12) 6_665 2_466
Ga3 O1 O1 161.5(4) 2_564 2_466
Ga3 O1 O1 107.23(17) . 2_466
Ga3 O1 O1 90.45(18) 4_455 2_466
Ga1 O1 O1 72.942(4) 1_455 2_466
Nb O1 O1 72.942(4) 1_455 2_466
Ga1 O1 O1 156.9(6) . 2_466
Nb O1 O1 156.9(6) . 2_466
Ga1 O1 O1 72.942(4) 1_565 2_466
Nb O1 O1 72.942(4) 1_565 2_466
O2 O1 O1 123.2(5) . 2_466
O2 O1 O1 94.3(3) 3_565 2_466
O2 O1 O1 32.36(15) 4_455 2_466
La O1 O1 78.4(4) 1_556 2_466
La O1 O1 68.1(4) 2_566 2_466
La O1 O1 27.0(2) 4_456 2_466
O3 O1 O1 34.02(18) 2_466 2_466
O3 O1 O1 61.3(3) 6_666 2_466
O3 O1 O1 106.4(6) 5_446 2_466
O3 O1 O1 96.46(11) 6 2_466
O3 O1 O1 71.63(16) 5_455 2_466
O3 O1 O1 161.2(3) 2_565 2_466
Ga2 O1 O1 17.15(13) 1_565 2_466
Ga2 O1 O1 103.1(4) . 2_466
Ga2 O1 O1 103.1(4) 1_665 2_466
O1 O1 O1 56.26(10) 2_465 2_466
O1 O1 O1 126.4(2) 2_455 2_466
O1 O1 O1 126.38(19) 2_565 2_466
O1 O1 O1 124.4(4) 1_554 2_466
O1 O1 O1 55.6(4) 1_556 2_466
Ga3 O1 O1 123.9(5) 4_446 2_466
Ga3 O1 O1 37.66(2) 2_465 2_466
Ga3 O1 O1 73.81(19) 1_666 2_466
O3 O1 O1 64.1(3) 6_556 2_466
O3 O1 O1 33.43(15) 5_456 2_466
O3 O1 O1 109.7(6) 2_566 2_466
O3 O1 O1 139.7(6) 1_655 2_466
O3 O1 O1 76.64(14) 4_345 2_466
O3 O1 O1 51.60(11) 3_575 2_466
O2 O1 O1 124.7(2) 3_454 2_466
O2 O1 O1 144.1(3) 4_554 2_466
O2 O1 O1 87.2(2) 1_564 2_466
Ga2 O1 O1 55.6(4) 2_566 2_456
La O1 O1 57.22(9) . 2_456
La O1 O1 137.5(3) 2_565 2_456
La O1 O1 114.73(16) 4_455 2_456
O2 O1 O1 96.8(2) 5_455 2_456
O2 O1 O1 115.2(3) 6 2_456
O2 O1 O1 152.1(5) 2_565 2_456
O2 O1 O1 58.0(4) 6_556 2_456
O2 O1 O1 33.9(3) 5_456 2_456
O2 O1 O1 85.3(6) 2_566 2_456
O3 O1 O1 58.2(2) 3_565 2_456
O3 O1 O1 66.9(2) . 2_456
O3 O1 O1 140.1(8) 4_455 2_456
Ga2 O1 O1 124.4(4) 2_565 2_456
Ga3 O1 O1 65.5(3) 2_565 2_456
Ga3 O1 O1 37.16(12) 1_556 2_456
Ga3 O1 O1 116.6(7) 4_456 2_456
O2 O1 O1 28.3(2) 3_455 2_456
O2 O1 O1 95.8(3) 4 2_456
O2 O1 O1 118.8(5) 1_565 2_456
O3 O1 O1 97.22(12) 2_465 2_456
O3 O1 O1 75.20(17) 5_445 2_456
O3 O1 O1 164.1(2) 6_665 2_456
Ga3 O1 O1 107.23(17) 2_564 2_456
Ga3 O1 O1 90.45(18) . 2_456
Ga3 O1 O1 161.5(4) 4_455 2_456
Ga1 O1 O1 72.943(4) 1_455 2_456
Nb O1 O1 72.943(4) 1_455 2_456
Ga1 O1 O1 72.942(3) . 2_456
Nb O1 O1 72.942(3) . 2_456
Ga1 O1 O1 156.9(6) 1_565 2_456
Nb O1 O1 156.9(6) 1_565 2_456
O2 O1 O1 32.36(15) . 2_456
O2 O1 O1 123.2(5) 3_565 2_456
O2 O1 O1 94.3(3) 4_455 2_456
La O1 O1 27.0(2) 1_556 2_456
La O1 O1 78.4(4) 2_566 2_456
La O1 O1 68.1(4) 4_456 2_456
O3 O1 O1 61.3(3) 2_466 2_456
O3 O1 O1 106.4(6) 6_666 2_456
O3 O1 O1 34.02(18) 5_446 2_456
O3 O1 O1 71.63(16) 6 2_456
O3 O1 O1 161.3(3) 5_455 2_456
O3 O1 O1 96.46(11) 2_565 2_456
Ga2 O1 O1 103.1(4) 1_565 2_456
Ga2 O1 O1 17.15(13) . 2_456
Ga2 O1 O1 103.1(4) 1_665 2_456
O1 O1 O1 126.38(19) 2_465 2_456
O1 O1 O1 56.26(10) 2_455 2_456
O1 O1 O1 126.4(2) 2_565 2_456
O1 O1 O1 124.4(4) 1_554 2_456
O1 O1 O1 55.6(4) 1_556 2_456
Ga3 O1 O1 37.66(2) 4_446 2_456
Ga3 O1 O1 73.81(19) 2_465 2_456
Ga3 O1 O1 123.9(5) 1_666 2_456
O3 O1 O1 33.43(15) 6_556 2_456
O3 O1 O1 109.7(6) 5_456 2_456
O3 O1 O1 64.1(3) 2_566 2_456
O3 O1 O1 76.64(14) 1_655 2_456
O3 O1 O1 51.60(11) 4_345 2_456
O3 O1 O1 139.7(6) 3_575 2_456
O2 O1 O1 87.2(2) 3_454 2_456
O2 O1 O1 124.7(2) 4_554 2_456
O2 O1 O1 144.1(3) 1_564 2_456
O1 O1 O1 91.2(5) 2_466 2_456
Ga2 O1 O1 55.6(4) 2_566 2_566
La O1 O1 114.73(16) . 2_566
La O1 O1 57.22(9) 2_565 2_566
La O1 O1 137.5(3) 4_455 2_566
O2 O1 O1 152.1(5) 5_455 2_566
O2 O1 O1 96.8(2) 6 2_566
O2 O1 O1 115.2(3) 2_565 2_566
O2 O1 O1 33.9(3) 6_556 2_566
O2 O1 O1 85.3(6) 5_456 2_566
O2 O1 O1 58.0(4) 2_566 2_566
O3 O1 O1 66.9(2) 3_565 2_566
O3 O1 O1 140.1(8) . 2_566
O3 O1 O1 58.2(2) 4_455 2_566
Ga2 O1 O1 124.4(4) 2_565 2_566
Ga3 O1 O1 37.16(12) 2_565 2_566
Ga3 O1 O1 116.6(7) 1_556 2_566
Ga3 O1 O1 65.5(3) 4_456 2_566
O2 O1 O1 118.8(5) 3_455 2_566
O2 O1 O1 28.3(2) 4 2_566
O2 O1 O1 95.8(3) 1_565 2_566
O3 O1 O1 164.1(2) 2_465 2_566
O3 O1 O1 97.22(12) 5_445 2_566
O3 O1 O1 75.20(17) 6_665 2_566
Ga3 O1 O1 90.45(18) 2_564 2_566
Ga3 O1 O1 161.5(4) . 2_566
Ga3 O1 O1 107.23(17) 4_455 2_566
Ga1 O1 O1 156.9(6) 1_455 2_566
Nb O1 O1 156.9(6) 1_455 2_566
Ga1 O1 O1 72.942(3) . 2_566
Nb O1 O1 72.942(3) . 2_566
Ga1 O1 O1 72.942(3) 1_565 2_566
Nb O1 O1 72.942(3) 1_565 2_566
O2 O1 O1 94.3(3) . 2_566
O2 O1 O1 32.36(15) 3_565 2_566
O2 O1 O1 123.2(5) 4_455 2_566
La O1 O1 68.1(4) 1_556 2_566
La O1 O1 27.0(2) 2_566 2_566
La O1 O1 78.4(4) 4_456 2_566
O3 O1 O1 106.4(6) 2_466 2_566
O3 O1 O1 34.02(18) 6_666 2_566
O3 O1 O1 61.3(3) 5_446 2_566
O3 O1 O1 161.2(3) 6 2_566
O3 O1 O1 96.46(11) 5_455 2_566
O3 O1 O1 71.63(16) 2_565 2_566
Ga2 O1 O1 103.1(4) 1_565 2_566
Ga2 O1 O1 103.1(4) . 2_566
Ga2 O1 O1 17.15(13) 1_665 2_566
O1 O1 O1 126.38(19) 2_465 2_566
O1 O1 O1 126.38(19) 2_455 2_566
O1 O1 O1 56.26(10) 2_565 2_566
O1 O1 O1 124.4(4) 1_554 2_566
O1 O1 O1 55.6(4) 1_556 2_566
Ga3 O1 O1 73.81(19) 4_446 2_566
Ga3 O1 O1 123.9(5) 2_465 2_566
Ga3 O1 O1 37.66(2) 1_666 2_566
O3 O1 O1 109.7(6) 6_556 2_566
O3 O1 O1 64.1(3) 5_456 2_566
O3 O1 O1 33.43(15) 2_566 2_566
O3 O1 O1 51.60(11) 1_655 2_566
O3 O1 O1 139.7(6) 4_345 2_566
O3 O1 O1 76.64(14) 3_575 2_566
O2 O1 O1 144.1(3) 3_454 2_566
O2 O1 O1 87.2(2) 4_554 2_566
O2 O1 O1 124.7(2) 1_564 2_566
O1 O1 O1 91.2(5) 2_466 2_566
O1 O1 O1 91.2(5) 2_456 2_566
Ga2 O1 O3 146.59(15) 2_566 3_564
La O1 O3 46.2(4) . 3_564
La O1 O3 66.6(4) 2_565 3_564
La O1 O3 100.5(6) 4_455 3_564
O2 O1 O3 45.8(3) 5_455 3_564
O2 O1 O3 15.62(19) 6 3_564
O2 O1 O3 63.3(4) 2_565 3_564
O2 O1 O3 117.1(2) 6_556 3_564
O2 O1 O3 135.7(2) 5_456 3_564
O2 O1 O3 163.28(17) 2_566 3_564
O3 O1 O3 61.8(3) 3_565 3_564
O3 O1 O3 110.5(4) . 3_564
O3 O1 O3 110.5(4) 4_455 3_564
Ga2 O1 O3 33.41(15) 2_565 3_564
Ga3 O1 O3 85.6(2) 2_565 3_564
Ga3 O1 O3 115.9(3) 1_556 3_564
Ga3 O1 O3 140.2(3) 4_456 3_564
O2 O1 O3 87.9(3) 3_455 3_564
O2 O1 O3 78.2(3) 4 3_564
O2 O1 O3 132.8(5) 1_565 3_564
O3 O1 O3 85.1(4) 2_465 3_564
O3 O1 O3 28.6(3) 5_445 3_564
O3 O1 O3 74.7(3) 6_665 3_564
Ga3 O1 O3 16.55(9) 2_564 3_564
Ga3 O1 O3 55.3(2) . 3_564
Ga3 O1 O3 71.3(3) 4_455 3_564
Ga1 O1 O3 93.5(3) 1_455 3_564
Nb O1 O3 93.5(3) 1_455 3_564
Ga1 O1 O3 45.46(18) . 3_564
Nb O1 O3 45.46(18) . 3_564
Ga1 O1 O3 98.6(3) 1_565 3_564
Nb O1 O3 98.6(3) 1_565 3_564
O2 O1 O3 70.3(3) . 3_564
O2 O1 O3 93.5(2) 3_565 3_564
O2 O1 O3 127.2(4) 4_455 3_564
La O1 O3 120.78(11) 1_556 3_564
La O1 O3 132.08(8) 2_566 3_564
La O1 O3 169.38(11) 4_456 3_564
O3 O1 O3 143.2(2) 2_466 3_564
O3 O1 O3 129.63(18) 6_666 3_564
O3 O1 O3 94.4(2) 5_446 3_564
O3 O1 O3 71.2(3) 6 3_564
O3 O1 O3 92.2(3) 5_455 3_564
O3 O1 O3 35.4(2) 2_565 3_564
Ga2 O1 O3 140.5(4) 1_565 3_564
Ga2 O1 O3 86.75(18) . 3_564
Ga2 O1 O3 91.68(16) 1_665 3_564
O1 O1 O3 101.4(6) 2_465 3_564
O1 O1 O3 52.7(4) 2_455 3_564
O1 O1 O3 58.5(4) 2_565 3_564
O1 O1 O3 33.41(15) 1_554 3_564
O1 O1 O3 146.59(15) 1_556 3_564
Ga3 O1 O3 75.52(16) 4_446 3_564
Ga3 O1 O3 129.4(3) 2_465 3_564
Ga3 O1 O3 111.92(19) 1_666 3_564
O3 O1 O3 120.1(2) 6_556 3_564
O3 O1 O3 146.7(2) 5_456 3_564
O3 O1 O3 92.5(2) 2_566 3_564
O3 O1 O3 62.09(15) 1_655 3_564
O3 O1 O3 97.3(3) 4_345 3_564
O3 O1 O3 118.3(3) 3_575 3_564
O2 O1 O3 39.66(17) 3_454 3_564
O2 O1 O3 28.90(13) 4_554 3_564
O2 O1 O3 71.4(3) 1_564 3_564
O1 O1 O3 157.5(5) 2_466 3_564
O1 O1 O3 102.0(3) 2_456 3_564
O1 O1 O3 106.4(2) 2_566 3_564
Ga2 O1 O3 146.59(15) 2_566 1_554
La O1 O3 66.6(4) . 1_554
La O1 O3 100.5(6) 2_565 1_554
La O1 O3 46.2(4) 4_455 1_554
O2 O1 O3 15.62(19) 5_455 1_554
O2 O1 O3 63.3(4) 6 1_554
O2 O1 O3 45.8(3) 2_565 1_554
O2 O1 O3 163.28(17) 6_556 1_554
O2 O1 O3 117.1(2) 5_456 1_554
O2 O1 O3 135.7(2) 2_566 1_554
O3 O1 O3 110.5(4) 3_565 1_554
O3 O1 O3 61.8(3) . 1_554
O3 O1 O3 110.5(4) 4_455 1_554
Ga2 O1 O3 33.41(15) 2_565 1_554
Ga3 O1 O3 140.2(3) 2_565 1_554
Ga3 O1 O3 85.6(2) 1_556 1_554
Ga3 O1 O3 115.9(3) 4_456 1_554
O2 O1 O3 78.2(3) 3_455 1_554
O2 O1 O3 132.8(5) 4 1_554
O2 O1 O3 87.9(3) 1_565 1_554
O3 O1 O3 28.6(3) 2_465 1_554
O3 O1 O3 74.7(3) 5_445 1_554
O3 O1 O3 85.1(4) 6_665 1_554
Ga3 O1 O3 71.3(3) 2_564 1_554
Ga3 O1 O3 16.55(9) . 1_554
Ga3 O1 O3 55.3(2) 4_455 1_554
Ga1 O1 O3 45.46(18) 1_455 1_554
Nb O1 O3 45.46(18) 1_455 1_554
Ga1 O1 O3 98.6(3) . 1_554
Nb O1 O3 98.6(3) . 1_554
Ga1 O1 O3 93.5(3) 1_565 1_554
Nb O1 O3 93.5(3) 1_565 1_554
O2 O1 O3 93.5(2) . 1_554
O2 O1 O3 127.2(4) 3_565 1_554
O2 O1 O3 70.3(3) 4_455 1_554
La O1 O3 132.08(8) 1_556 1_554
La O1 O3 169.37(11) 2_566 1_554
La O1 O3 120.78(11) 4_456 1_554
O3 O1 O3 94.4(2) 2_466 1_554
O3 O1 O3 143.2(2) 6_666 1_554
O3 O1 O3 129.63(18) 5_446 1_554
O3 O1 O3 35.4(2) 6 1_554
O3 O1 O3 71.2(3) 5_455 1_554
O3 O1 O3 92.2(3) 2_565 1_554
Ga2 O1 O3 86.75(18) 1_565 1_554
Ga2 O1 O3 91.68(16) . 1_554
Ga2 O1 O3 140.5(4) 1_665 1_554
O1 O1 O3 52.7(4) 2_465 1_554
O1 O1 O3 58.5(4) 2_455 1_554
O1 O1 O3 101.4(6) 2_565 1_554
O1 O1 O3 33.41(15) 1_554 1_554
O1 O1 O3 146.59(15) 1_556 1_554
Ga3 O1 O3 111.92(19) 4_446 1_554
Ga3 O1 O3 75.52(16) 2_465 1_554
Ga3 O1 O3 129.4(3) 1_666 1_554
O3 O1 O3 92.5(2) 6_556 1_554
O3 O1 O3 120.1(2) 5_456 1_554
O3 O1 O3 146.7(2) 2_566 1_554
O3 O1 O3 118.3(3) 1_655 1_554
O3 O1 O3 62.09(15) 4_345 1_554
O3 O1 O3 97.3(3) 3_575 1_554
O2 O1 O3 28.90(13) 3_454 1_554
O2 O1 O3 71.4(3) 4_554 1_554
O2 O1 O3 39.66(18) 1_564 1_554
O1 O1 O3 102.0(3) 2_466 1_554
O1 O1 O3 106.4(2) 2_456 1_554
O1 O1 O3 157.5(5) 2_566 1_554
O3 O1 O3 57.0(3) 3_564 1_554
Ga2 O1 O3 146.59(15) 2_566 4_454
La O1 O3 100.5(6) . 4_454
La O1 O3 46.2(4) 2_565 4_454
La O1 O3 66.6(4) 4_455 4_454
O2 O1 O3 63.3(4) 5_455 4_454
O2 O1 O3 45.8(3) 6 4_454
O2 O1 O3 15.62(19) 2_565 4_454
O2 O1 O3 135.7(2) 6_556 4_454
O2 O1 O3 163.28(17) 5_456 4_454
O2 O1 O3 117.1(2) 2_566 4_454
O3 O1 O3 110.5(4) 3_565 4_454
O3 O1 O3 110.5(4) . 4_454
O3 O1 O3 61.8(3) 4_455 4_454
Ga2 O1 O3 33.41(15) 2_565 4_454
Ga3 O1 O3 115.9(3) 2_565 4_454
Ga3 O1 O3 140.2(3) 1_556 4_454
Ga3 O1 O3 85.6(2) 4_456 4_454
O2 O1 O3 132.8(5) 3_455 4_454
O2 O1 O3 87.9(3) 4 4_454
O2 O1 O3 78.2(3) 1_565 4_454
O3 O1 O3 74.7(3) 2_465 4_454
O3 O1 O3 85.1(4) 5_445 4_454
O3 O1 O3 28.6(3) 6_665 4_454
Ga3 O1 O3 55.3(2) 2_564 4_454
Ga3 O1 O3 71.3(3) . 4_454
Ga3 O1 O3 16.55(9) 4_455 4_454
Ga1 O1 O3 98.6(3) 1_455 4_454
Nb O1 O3 98.6(3) 1_455 4_454
Ga1 O1 O3 93.5(3) . 4_454
Nb O1 O3 93.5(3) . 4_454
Ga1 O1 O3 45.46(18) 1_565 4_454
Nb O1 O3 45.46(18) 1_565 4_454
O2 O1 O3 127.2(4) . 4_454
O2 O1 O3 70.3(3) 3_565 4_454
O2 O1 O3 93.5(2) 4_455 4_454
La O1 O3 169.38(11) 1_556 4_454
La O1 O3 120.78(11) 2_566 4_454
La O1 O3 132.08(8) 4_456 4_454
O3 O1 O3 129.63(18) 2_466 4_454
O3 O1 O3 94.4(2) 6_666 4_454
O3 O1 O3 143.2(2) 5_446 4_454
O3 O1 O3 92.2(3) 6 4_454
O3 O1 O3 35.4(2) 5_455 4_454
O3 O1 O3 71.2(3) 2_565 4_454
Ga2 O1 O3 91.68(16) 1_565 4_454
Ga2 O1 O3 140.5(4) . 4_454
Ga2 O1 O3 86.75(18) 1_665 4_454
O1 O1 O3 58.5(4) 2_465 4_454
O1 O1 O3 101.4(6) 2_455 4_454
O1 O1 O3 52.7(4) 2_565 4_454
O1 O1 O3 33.41(15) 1_554 4_454
O1 O1 O3 146.59(15) 1_556 4_454
Ga3 O1 O3 129.4(3) 4_446 4_454
Ga3 O1 O3 111.92(19) 2_465 4_454
Ga3 O1 O3 75.52(16) 1_666 4_454
O3 O1 O3 146.7(2) 6_556 4_454
O3 O1 O3 92.5(2) 5_456 4_454
O3 O1 O3 120.1(2) 2_566 4_454
O3 O1 O3 97.3(3) 1_655 4_454
O3 O1 O3 118.3(4) 4_345 4_454
O3 O1 O3 62.09(15) 3_575 4_454
O2 O1 O3 71.4(3) 3_454 4_454
O2 O1 O3 39.66(18) 4_554 4_454
O2 O1 O3 28.90(13) 1_564 4_454
O1 O1 O3 106.4(2) 2_466 4_454
O1 O1 O3 157.5(5) 2_456 4_454
O1 O1 O3 102.0(3) 2_566 4_454
O3 O1 O3 57.0(3) 3_564 4_454
O3 O1 O3 57.0(3) 1_554 4_454
Ga2 O1 O3 87.2(2) 2_566 4_445
La O1 O3 41.45(17) . 4_445
La O1 O3 86.86(10) 2_565 4_445
La O1 O3 149.1(4) 4_455 4_445
O2 O1 O3 89.6(3) 5_455 4_445
O2 O1 O3 66.5(2) 6 4_445
O2 O1 O3 122.0(5) 2_565 4_445
O2 O1 O3 61.8(2) 6_556 4_445
O2 O1 O3 84.9(3) 5_456 4_445
O2 O1 O3 115.8(5) 2_566 4_445
O3 O1 O3 6.6(2) 3_565 4_445
O3 O1 O3 113.4(2) . 4_445
O3 O1 O3 125.7(2) 4_455 4_445
Ga2 O1 O3 92.8(2) 2_565 4_445
Ga3 O1 O3 36.73(13) 2_565 4_445
Ga3 O1 O3 89.56(15) 1_556 4_445
Ga3 O1 O3 138.0(4) 4_456 4_445
O2 O1 O3 63.97(15) 3_455 4_445
O2 O1 O3 56.00(16) 4 4_445
O2 O1 O3 166.5(6) 1_565 4_445
O3 O1 O3 122.5(2) 2_465 4_445
O3 O1 O3 32.7(3) 5_445 4_445
O3 O1 O3 112.06(17) 6_665 4_445
Ga3 O1 O3 56.46(13) 2_564 4_445
Ga3 O1 O3 92.71(19) . 4_445
Ga3 O1 O3 127.9(4) 4_455 4_445
Ga1 O1 O3 108.54(10) 1_455 4_445
Nb O1 O3 108.54(10) 1_455 4_445
Ga1 O1 O3 18.28(10) . 4_445
Nb O1 O3 18.28(10) . 4_445
Ga1 O1 O3 131.34(12) 1_565 4_445
Nb O1 O3 131.34(12) 1_565 4_445
O2 O1 O3 29.13(12) . 4_445
O2 O1 O3 90.75(12) 3_565 4_445
O2 O1 O3 147.3(2) 4_455 4_445
La O1 O3 62.85(16) 1_556 4_445
La O1 O3 85.3(2) 2_566 4_445
La O1 O3 114.2(3) 4_456 4_445
O3 O1 O3 116.1(2) 2_466 4_445
O3 O1 O3 106.9(2) 6_666 4_445
O3 O1 O3 34.9(2) 5_446 4_445
O3 O1 O3 90.24(18) 6 4_445
O3 O1 O3 143.8(3) 5_455 4_445
O3 O1 O3 41.68(19) 2_565 4_445
Ga2 O1 O3 156.8(4) 1_565 4_445
Ga2 O1 O3 49.58(9) . 4_445
Ga2 O1 O3 71.65(10) 1_665 4_445
O1 O1 O3 157.9(6) 2_465 4_445
O1 O1 O3 53.28(13) 2_455 4_445
O1 O1 O3 74.12(8) 2_565 4_445
O1 O1 O3 92.8(2) 1_554 4_445
O1 O1 O3 87.2(2) 1_556 4_445
Ga3 O1 O3 18.02(10) 4_446 4_445
Ga3 O1 O3 127.09(19) 2_465 4_445
Ga3 O1 O3 107.65(14) 1_666 4_445
O3 O1 O3 87.5(2) 6_556 4_445
O3 O1 O3 134.6(3) 5_456 4_445
O3 O1 O3 42.2(2) 2_566 4_445
O3 O1 O3 27.48(11) 1_655 4_445
O3 O1 O3 92.33(11) 4_345 4_445
O3 O1 O3 147.01(14) 3_575 4_445
O2 O1 O3 76.55(19) 3_454 4_445
O2 O1 O3 72.03(18) 4_554 4_445
O2 O1 O3 131.1(4) 1_564 4_445
O1 O1 O3 141.2(6) 2_466 4_445
O1 O1 O3 54.88(9) 2_456 4_445
O1 O1 O3 73.31(12) 2_566 4_445
O3 O1 O3 59.62(13) 3_564 4_445
O3 O1 O3 105.2(3) 1_554 4_445
O3 O1 O3 111.5(3) 4_454 4_445
Ga2 O1 O3 87.2(2) 2_566 3_465
La O1 O3 86.86(10) . 3_465
La O1 O3 149.1(4) 2_565 3_465
La O1 O3 41.45(17) 4_455 3_465
O2 O1 O3 66.5(2) 5_455 3_465
O2 O1 O3 122.0(5) 6 3_465
O2 O1 O3 89.6(3) 2_565 3_465
O2 O1 O3 115.8(5) 6_556 3_465
O2 O1 O3 61.8(2) 5_456 3_465
O2 O1 O3 84.9(3) 2_566 3_465
O3 O1 O3 125.7(2) 3_565 3_465
O3 O1 O3 6.6(2) . 3_465
O3 O1 O3 113.4(2) 4_455 3_465
Ga2 O1 O3 92.8(2) 2_565 3_465
Ga3 O1 O3 138.0(4) 2_565 3_465
Ga3 O1 O3 36.73(13) 1_556 3_465
Ga3 O1 O3 89.56(15) 4_456 3_465
O2 O1 O3 56.00(16) 3_455 3_465
O2 O1 O3 166.5(6) 4 3_465
O2 O1 O3 63.97(15) 1_565 3_465
O3 O1 O3 32.7(3) 2_465 3_465
O3 O1 O3 112.07(17) 5_445 3_465
O3 O1 O3 122.5(2) 6_665 3_465
Ga3 O1 O3 127.9(4) 2_564 3_465
Ga3 O1 O3 56.46(13) . 3_465
Ga3 O1 O3 92.71(19) 4_455 3_465
Ga1 O1 O3 18.28(10) 1_455 3_465
Nb O1 O3 18.28(10) 1_455 3_465
Ga1 O1 O3 131.34(12) . 3_465
Nb O1 O3 131.34(12) . 3_465
Ga1 O1 O3 108.54(10) 1_565 3_465
Nb O1 O3 108.54(10) 1_565 3_465
O2 O1 O3 90.75(12) . 3_465
O2 O1 O3 147.3(2) 3_565 3_465
O2 O1 O3 29.12(12) 4_455 3_465
La O1 O3 85.3(2) 1_556 3_465
La O1 O3 114.2(3) 2_566 3_465
La O1 O3 62.85(16) 4_456 3_465
O3 O1 O3 34.9(2) 2_466 3_465
O3 O1 O3 116.1(2) 6_666 3_465
O3 O1 O3 106.9(2) 5_446 3_465
O3 O1 O3 41.68(19) 6 3_465
O3 O1 O3 90.24(18) 5_455 3_465
O3 O1 O3 143.8(3) 2_565 3_465
Ga2 O1 O3 49.58(9) 1_565 3_465
Ga2 O1 O3 71.65(10) . 3_465
Ga2 O1 O3 156.8(4) 1_665 3_465
O1 O1 O3 53.28(13) 2_465 3_465
O1 O1 O3 74.12(8) 2_455 3_465
O1 O1 O3 157.9(6) 2_565 3_465
O1 O1 O3 92.8(2) 1_554 3_465
O1 O1 O3 87.2(2) 1_556 3_465
Ga3 O1 O3 107.65(14) 4_446 3_465
Ga3 O1 O3 18.02(10) 2_465 3_465
Ga3 O1 O3 127.09(19) 1_666 3_465
O3 O1 O3 42.2(2) 6_556 3_465
O3 O1 O3 87.5(2) 5_456 3_465
O3 O1 O3 134.6(3) 2_566 3_465
O3 O1 O3 147.01(14) 1_655 3_465
O3 O1 O3 27.48(11) 4_345 3_465
O3 O1 O3 92.33(11) 3_575 3_465
O2 O1 O3 72.03(18) 3_454 3_465
O2 O1 O3 131.1(4) 4_554 3_465
O2 O1 O3 76.55(19) 1_564 3_465
O1 O1 O3 54.88(9) 2_466 3_465
O1 O1 O3 73.31(13) 2_456 3_465
O1 O1 O3 141.2(6) 2_566 3_465
O3 O1 O3 111.5(3) 3_564 3_465
O3 O1 O3 59.62(13) 1_554 3_465
O3 O1 O3 105.2(3) 4_454 3_465
O3 O1 O3 119.76(4) 4_445 3_465
Ga2 O1 O3 87.2(2) 2_566 1_665
La O1 O3 149.1(4) . 1_665
La O1 O3 41.45(17) 2_565 1_665
La O1 O3 86.86(10) 4_455 1_665
O2 O1 O3 122.0(5) 5_455 1_665
O2 O1 O3 89.6(3) 6 1_665
O2 O1 O3 66.5(2) 2_565 1_665
O2 O1 O3 84.9(3) 6_556 1_665
O2 O1 O3 115.8(5) 5_456 1_665
O2 O1 O3 61.8(2) 2_566 1_665
O3 O1 O3 113.4(2) 3_565 1_665
O3 O1 O3 125.7(2) . 1_665
O3 O1 O3 6.6(2) 4_455 1_665
Ga2 O1 O3 92.8(2) 2_565 1_665
Ga3 O1 O3 89.56(15) 2_565 1_665
Ga3 O1 O3 138.0(4) 1_556 1_665
Ga3 O1 O3 36.73(13) 4_456 1_665
O2 O1 O3 166.5(6) 3_455 1_665
O2 O1 O3 63.97(15) 4 1_665
O2 O1 O3 56.00(16) 1_565 1_665
O3 O1 O3 112.06(16) 2_465 1_665
O3 O1 O3 122.5(2) 5_445 1_665
O3 O1 O3 32.7(3) 6_665 1_665
Ga3 O1 O3 92.71(19) 2_564 1_665
Ga3 O1 O3 127.9(4) . 1_665
Ga3 O1 O3 56.46(13) 4_455 1_665
Ga1 O1 O3 131.33(12) 1_455 1_665
Nb O1 O3 131.33(12) 1_455 1_665
Ga1 O1 O3 108.54(10) . 1_665
Nb O1 O3 108.54(10) . 1_665
Ga1 O1 O3 18.28(10) 1_565 1_665
Nb O1 O3 18.28(10) 1_565 1_665
O2 O1 O3 147.3(2) . 1_665
O2 O1 O3 29.13(12) 3_565 1_665
O2 O1 O3 90.75(12) 4_455 1_665
La O1 O3 114.2(3) 1_556 1_665
La O1 O3 62.85(16) 2_566 1_665
La O1 O3 85.3(2) 4_456 1_665
O3 O1 O3 106.9(2) 2_466 1_665
O3 O1 O3 34.9(2) 6_666 1_665
O3 O1 O3 116.1(2) 5_446 1_665
O3 O1 O3 143.8(3) 6 1_665
O3 O1 O3 41.67(19) 5_455 1_665
O3 O1 O3 90.25(18) 2_565 1_665
Ga2 O1 O3 71.65(10) 1_565 1_665
Ga2 O1 O3 156.8(4) . 1_665
Ga2 O1 O3 49.58(9) 1_665 1_665
O1 O1 O3 74.12(8) 2_465 1_665
O1 O1 O3 157.9(6) 2_455 1_665
O1 O1 O3 53.28(13) 2_565 1_665
O1 O1 O3 92.8(2) 1_554 1_665
O1 O1 O3 87.2(2) 1_556 1_665
Ga3 O1 O3 127.09(19) 4_446 1_665
Ga3 O1 O3 107.65(14) 2_465 1_665
Ga3 O1 O3 18.02(10) 1_666 1_665
O3 O1 O3 134.6(3) 6_556 1_665
O3 O1 O3 42.2(2) 5_456 1_665
O3 O1 O3 87.5(2) 2_566 1_665
O3 O1 O3 92.33(11) 1_655 1_665
O3 O1 O3 147.01(14) 4_345 1_665
O3 O1 O3 27.48(11) 3_575 1_665
O2 O1 O3 131.1(4) 3_454 1_665
O2 O1 O3 76.55(19) 4_554 1_665
O2 O1 O3 72.03(18) 1_564 1_665
O1 O1 O3 73.31(12) 2_466 1_665
O1 O1 O3 141.2(6) 2_456 1_665
O1 O1 O3 54.88(9) 2_566 1_665
O3 O1 O3 105.2(3) 3_564 1_665
O3 O1 O3 111.5(3) 1_554 1_665
O3 O1 O3 59.62(13) 4_454 1_665
O3 O1 O3 119.76(4) 4_445 1_665
O3 O1 O3 119.76(4) 3_465 1_665
Ga2 O1 La 99.1(2) 2_566 2_455
La O1 La 37.84(3) . 2_455
La O1 La 142.3(5) 2_565 2_455
La O1 La 79.97(12) 4_455 2_455
O2 O1 La 49.32(16) 5_455 2_455
O2 O1 La 91.2(3) 6 2_455
O2 O1 La 103.3(4) 2_565 2_455
O2 O1 La 106.6(3) 6_556 2_455
O2 O1 La 68.17(18) 5_456 2_455
O2 O1 La 119.4(3) 2_566 2_455
O3 O1 La 79.03(14) 3_565 2_455
O3 O1 La 44.25(16) . 2_455
O3 O1 La 161.72(18) 4_455 2_455
Ga2 O1 La 80.9(2) 2_565 2_455
Ga3 O1 La 103.72(7) 2_565 2_455
Ga3 O1 La 40.45(9) 1_556 2_455
Ga3 O1 La 137.6(2) 4_456 2_455
O2 O1 La 20.7(3) 3_455 2_455
O2 O1 La 128.49(12) 4 2_455
O2 O1 La 113.36(12) 1_565 2_455
O3 O1 La 54.65(12) 2_465 2_455
O3 O1 La 64.31(13) 5_445 2_455
O3 O1 La 141.1(5) 6_665 2_455
Ga3 O1 La 90.5(2) 2_564 2_455
Ga3 O1 La 41.74(4) . 2_455
Ga3 O1 La 112.7(3) 4_455 2_455
Ga1 O1 La 36.06(3) 1_455 2_455
Nb O1 La 36.06(3) 1_455 2_455
Ga1 O1 La 81.82(7) . 2_455
Nb O1 La 81.82(7) . 2_455
Ga1 O1 La 149.0(3) 1_565 2_455
Nb O1 La 149.0(3) 1_565 2_455
O2 O1 La 45.85(10) . 2_455
O2 O1 La 162.99(10) 3_565 2_455
O2 O1 La 78.60(9) 4_455 2_455
La O1 La 75.07(10) 1_556 2_455
La O1 La 126.5(3) 2_566 2_455
La O1 La 94.26(16) 4_456 2_455
O3 O1 La 68.83(12) 2_466 2_455
O3 O1 La 151.4(4) 6_666 2_455
O3 O1 La 76.78(12) 5_446 2_455
O3 O1 La 23.44(11) 6 2_455
O3 O1 La 125.5(3) 5_455 2_455
O3 O1 La 97.35(18) 2_565 2_455
Ga2 O1 La 98.94(3) 1_565 2_455
Ga2 O1 La 35.12(3) . 2_455
Ga2 O1 La 143.52(10) 1_665 2_455
O1 O1 La 92.65(17) 2_465 2_455
O1 O1 La 25.82(9) 2_455 2_455
O1 O1 La 132.6(4) 2_565 2_455
O1 O1 La 80.9(2) 1_554 2_455
O1 O1 La 99.1(2) 1_556 2_455
Ga3 O1 La 66.16(2) 4_446 2_455
Ga3 O1 La 63.861(17) 2_465 2_455
Ga3 O1 La 171.4(4) 1_666 2_455
O3 O1 La 45.57(12) 6_556 2_455
O3 O1 La 133.7(2) 5_456 2_455
O3 O1 La 105.72(13) 2_566 2_455
O3 O1 La 99.63(8) 1_655 2_455
O3 O1 La 23.98(9) 4_345 2_455
O3 O1 La 140.50(10) 3_575 2_455
O2 O1 La 42.98(12) 3_454 2_455
O2 O1 La 104.5(3) 4_554 2_455
O2 O1 La 96.2(2) 1_564 2_455
O1 O1 La 100.56(9) 2_466 2_455
O1 O1 La 48.89(12) 2_456 2_455
O1 O1 La 138.0(3) 2_566 2_455
O3 O1 La 75.78(19) 3_564 2_455
O3 O1 La 57.56(13) 1_554 2_455
O3 O1 La 112.6(3) 4_454 2_455
O3 O1 La 72.49(9) 4_445 2_455
O3 O1 La 49.54(8) 3_465 2_455
O3 O1 La 166.7(2) 1_665 2_455
Ga2 O1 La 99.1(2) 2_566 4
La O1 La 79.97(12) . 4
La O1 La 37.84(3) 2_565 4
La O1 La 142.3(5) 4_455 4
O2 O1 La 103.3(4) 5_455 4
O2 O1 La 49.32(16) 6 4
O2 O1 La 91.2(3) 2_565 4
O2 O1 La 68.17(18) 6_556 4
O2 O1 La 119.4(3) 5_456 4
O2 O1 La 106.6(3) 2_566 4
O3 O1 La 44.25(16) 3_565 4
O3 O1 La 161.72(18) . 4
O3 O1 La 79.03(14) 4_455 4
Ga2 O1 La 80.9(2) 2_565 4
Ga3 O1 La 40.45(9) 2_565 4
Ga3 O1 La 137.6(2) 1_556 4
Ga3 O1 La 103.72(7) 4_456 4
O2 O1 La 113.36(12) 3_455 4
O2 O1 La 20.7(2) 4 4
O2 O1 La 128.49(12) 1_565 4
O3 O1 La 141.1(5) 2_465 4
O3 O1 La 54.65(12) 5_445 4
O3 O1 La 64.31(13) 6_665 4
Ga3 O1 La 41.74(4) 2_564 4
Ga3 O1 La 112.7(3) . 4
Ga3 O1 La 90.5(2) 4_455 4
Ga1 O1 La 149.0(3) 1_455 4
Nb O1 La 149.0(3) 1_455 4
Ga1 O1 La 36.06(3) . 4
Nb O1 La 36.06(3) . 4
Ga1 O1 La 81.82(7) 1_565 4
Nb O1 La 81.82(7) 1_565 4
O2 O1 La 78.60(9) . 4
O2 O1 La 45.85(10) 3_565 4
O2 O1 La 162.99(10) 4_455 4
La O1 La 94.26(16) 1_556 4
La O1 La 75.07(10) 2_566 4
La O1 La 126.5(3) 4_456 4
O3 O1 La 151.4(4) 2_466 4
O3 O1 La 76.78(12) 6_666 4
O3 O1 La 68.83(11) 5_446 4
O3 O1 La 125.5(3) 6 4
O3 O1 La 97.35(18) 5_455 4
O3 O1 La 23.44(11) 2_565 4
Ga2 O1 La 143.52(10) 1_565 4
Ga2 O1 La 98.94(3) . 4
Ga2 O1 La 35.12(3) 1_665 4
O1 O1 La 132.6(4) 2_465 4
O1 O1 La 92.65(17) 2_455 4
O1 O1 La 25.82(9) 2_565 4
O1 O1 La 80.9(2) 1_554 4
O1 O1 La 99.1(2) 1_556 4
Ga3 O1 La 63.861(17) 4_446 4
Ga3 O1 La 171.4(4) 2_465 4
Ga3 O1 La 66.16(2) 1_666 4
O3 O1 La 133.7(2) 6_556 4
O3 O1 La 105.72(13) 5_456 4
O3 O1 La 45.57(12) 2_566 4
O3 O1 La 23.98(9) 1_655 4
O3 O1 La 140.50(10) 4_345 4
O3 O1 La 99.63(8) 3_575 4
O2 O1 La 96.2(2) 3_454 4
O2 O1 La 42.98(12) 4_554 4
O2 O1 La 104.5(3) 1_564 4
O1 O1 La 138.0(3) 2_466 4
O1 O1 La 100.56(9) 2_456 4
O1 O1 La 48.88(12) 2_566 4
O3 O1 La 57.56(13) 3_564 4
O3 O1 La 112.6(3) 1_554 4
O3 O1 La 75.78(19) 4_454 4
O3 O1 La 49.54(8) 4_445 4
O3 O1 La 166.7(2) 3_465 4
O3 O1 La 72.49(9) 1_665 4
La O1 La 117.53(11) 2_455 4
Ga2 O1 La 99.1(2) 2_566 1_565
La O1 La 142.3(5) . 1_565
La O1 La 79.97(12) 2_565 1_565
La O1 La 37.84(3) 4_455 1_565
O2 O1 La 91.2(3) 5_455 1_565
O2 O1 La 103.3(4) 6 1_565
O2 O1 La 49.32(16) 2_565 1_565
O2 O1 La 119.4(3) 6_556 1_565
O2 O1 La 106.6(3) 5_456 1_565
O2 O1 La 68.17(18) 2_566 1_565
O3 O1 La 161.72(18) 3_565 1_565
O3 O1 La 79.03(14) . 1_565
O3 O1 La 44.25(16) 4_455 1_565
Ga2 O1 La 80.9(2) 2_565 1_565
Ga3 O1 La 137.6(2) 2_565 1_565
Ga3 O1 La 103.72(7) 1_556 1_565
Ga3 O1 La 40.45(9) 4_456 1_565
O2 O1 La 128.49(12) 3_455 1_565
O2 O1 La 113.36(12) 4 1_565
O2 O1 La 20.7(2) 1_565 1_565
O3 O1 La 64.31(13) 2_465 1_565
O3 O1 La 141.1(5) 5_445 1_565
O3 O1 La 54.65(12) 6_665 1_565
Ga3 O1 La 112.7(3) 2_564 1_565
Ga3 O1 La 90.5(2) . 1_565
Ga3 O1 La 41.74(4) 4_455 1_565
Ga1 O1 La 81.82(7) 1_455 1_565
Nb O1 La 81.82(7) 1_455 1_565
Ga1 O1 La 149.0(3) . 1_565
Nb O1 La 149.0(3) . 1_565
Ga1 O1 La 36.06(3) 1_565 1_565
Nb O1 La 36.06(3) 1_565 1_565
O2 O1 La 162.99(10) . 1_565
O2 O1 La 78.60(9) 3_565 1_565
O2 O1 La 45.85(10) 4_455 1_565
La O1 La 126.5(3) 1_556 1_565
La O1 La 94.26(16) 2_566 1_565
La O1 La 75.07(10) 4_456 1_565
O3 O1 La 76.78(12) 2_466 1_565
O3 O1 La 68.83(11) 6_666 1_565
O3 O1 La 151.4(4) 5_446 1_565
O3 O1 La 97.35(18) 6 1_565
O3 O1 La 23.44(11) 5_455 1_565
O3 O1 La 125.5(3) 2_565 1_565
Ga2 O1 La 35.12(3) 1_565 1_565
Ga2 O1 La 143.52(9) . 1_565
Ga2 O1 La 98.94(3) 1_665 1_565
O1 O1 La 25.82(9) 2_465 1_565
O1 O1 La 132.6(4) 2_455 1_565
O1 O1 La 92.65(17) 2_565 1_565
O1 O1 La 80.9(2) 1_554 1_565
O1 O1 La 99.1(2) 1_556 1_565
Ga3 O1 La 171.4(4) 4_446 1_565
Ga3 O1 La 66.16(2) 2_465 1_565
Ga3 O1 La 63.860(18) 1_666 1_565
O3 O1 La 105.72(13) 6_556 1_565
O3 O1 La 45.57(12) 5_456 1_565
O3 O1 La 133.7(2) 2_566 1_565
O3 O1 La 140.50(10) 1_655 1_565
O3 O1 La 99.63(8) 4_345 1_565
O3 O1 La 23.98(9) 3_575 1_565
O2 O1 La 104.5(3) 3_454 1_565
O2 O1 La 96.2(2) 4_554 1_565
O2 O1 La 42.98(12) 1_564 1_565
O1 O1 La 48.89(12) 2_466 1_565
O1 O1 La 138.0(3) 2_456 1_565
O1 O1 La 100.56(9) 2_566 1_565
O3 O1 La 112.6(3) 3_564 1_565
O3 O1 La 75.78(19) 1_554 1_565
O3 O1 La 57.55(13) 4_454 1_565
O3 O1 La 166.7(2) 4_445 1_565
O3 O1 La 72.49(9) 3_465 1_565
O3 O1 La 49.54(8) 1_665 1_565
La O1 La 117.53(11) 2_455 1_565
La O1 La 117.53(11) 4 1_565
Ga2 O1 O2 84.2(2) 2_566 4_445
La O1 O2 33.3(2) . 4_445
La O1 O2 138.1(2) 2_565 4_445
La O1 O2 101.60(9) 4_455 4_445
O2 O1 O2 67.9(2) 5_455 4_445
O2 O1 O2 94.5(3) 6 4_445
O2 O1 O2 123.5(4) 2_565 4_445
O2 O1 O2 84.7(3) 6_556 4_445
O2 O1 O2 57.5(3) 5_456 4_445
O2 O1 O2 111.8(4) 2_566 4_445
O3 O1 O2 60.19(15) 3_565 4_445
O3 O1 O2 59.21(16) . 4_445
O3 O1 O2 169.0(6) 4_455 4_445
Ga2 O1 O2 95.8(2) 2_565 4_445
Ga3 O1 O2 81.45(13) 2_565 4_445
Ga3 O1 O2 40.72(11) 1_556 4_445
Ga3 O1 O2 140.4(4) 4_456 4_445
O2 O1 O2 10.60(16) 3_455 4_445
O2 O1 O2 108.7(2) 4 4_445
O2 O1 O2 127.5(3) 1_565 4_445
O3 O1 O2 77.31(14) 2_465 4_445
O3 O1 O2 58.02(17) 5_445 4_445
O3 O1 O2 153.9(5) 6_665 4_445
Ga3 O1 O2 89.81(17) 2_564 4_445
Ga3 O1 O2 62.38(12) . 4_445
Ga3 O1 O2 133.7(4) 4_455 4_445
Ga1 O1 O2 56.47(7) 1_455 4_445
Nb O1 O2 56.47(7) 1_455 4_445
Ga1 O1 O2 67.77(9) . 4_445
Nb O1 O2 67.77(9) . 4_445
Ga1 O1 O2 172.0(3) 1_565 4_445
Nb O1 O2 172.0(3) 1_565 4_445
O2 O1 O2 25.27(11) . 4_445
O2 O1 O2 143.0(2) 3_565 4_445
O2 O1 O2 93.79(13) 4_455 4_445
La O1 O2 56.09(14) 1_556 4_445
La O1 O2 107.1(3) 2_566 4_445
La O1 O2 90.1(2) 4_456 4_445
O3 O1 O2 72.13(17) 2_466 4_445
O3 O1 O2 135.5(4) 6_666 4_445
O3 O1 O2 53.84(14) 5_446 4_445
O3 O1 O2 46.27(14) 6 4_445
O3 O1 O2 148.4(3) 5_455 4_445
O3 O1 O2 88.40(15) 2_565 4_445
Ga2 O1 O2 110.96(16) 1_565 4_445
Ga2 O1 O2 12.86(11) . 4_445
Ga2 O1 O2 121.81(18) 1_665 4_445
O1 O1 O2 114.49(13) 2_465 4_445
O1 O1 O2 28.2(3) 2_455 4_445
O1 O1 O2 125.40(18) 2_565 4_445
O1 O1 O2 95.8(2) 1_554 4_445
O1 O1 O2 84.2(2) 1_556 4_445
Ga3 O1 O2 44.34(8) 4_446 4_445
Ga3 O1 O2 75.14(11) 2_465 4_445
Ga3 O1 O2 151.6(4) 1_666 4_445
O3 O1 O2 42.37(15) 6_556 4_445
O3 O1 O2 134.0(4) 5_456 4_445
O3 O1 O2 82.95(16) 2_566 4_445
O3 O1 O2 81.52(11) 1_655 4_445
O3 O1 O2 38.20(11) 4_345 4_445
O3 O1 O2 156.5(2) 3_575 4_445
O2 O1 O2 58.05(10) 3_454 4_445
O2 O1 O2 107.0(3) 4_554 4_445
O2 O1 O2 118.3(3) 1_564 4_445
O1 O1 O2 106.1(3) 2_466 4_445
O1 O1 O2 29.15(19) 2_456 4_445
O1 O1 O2 115.1(3) 2_566 4_445
O3 O1 O2 79.3(2) 3_564 4_445
O3 O1 O2 78.83(17) 1_554 4_445
O3 O1 O2 129.2(4) 4_454 4_445
O3 O1 O2 54.17(11) 4_445 4_445
O3 O1 O2 65.59(11) 3_465 4_445
O3 O1 O2 169.7(4) 1_665 4_445
La O1 O2 22.96(9) 2_455 4_445
La O1 O2 103.22(8) 4 4_445
La O1 O2 137.75(8) 1_565 4_445
Ga2 O1 O2 84.2(2) 2_566 1_665
La O1 O2 101.60(9) . 1_665
La O1 O2 33.3(2) 2_565 1_665
La O1 O2 138.1(2) 4_455 1_665
O2 O1 O2 123.5(4) 5_455 1_665
O2 O1 O2 67.9(2) 6 1_665
O2 O1 O2 94.5(3) 2_565 1_665
O2 O1 O2 57.5(3) 6_556 1_665
O2 O1 O2 111.8(4) 5_456 1_665
O2 O1 O2 84.7(3) 2_566 1_665
O3 O1 O2 59.21(16) 3_565 1_665
O3 O1 O2 169.0(6) . 1_665
O3 O1 O2 60.19(15) 4_455 1_665
Ga2 O1 O2 95.8(2) 2_565 1_665
Ga3 O1 O2 40.72(11) 2_565 1_665
Ga3 O1 O2 140.4(4) 1_556 1_665
Ga3 O1 O2 81.45(13) 4_456 1_665
O2 O1 O2 127.5(3) 3_455 1_665
O2 O1 O2 10.60(16) 4 1_665
O2 O1 O2 108.7(2) 1_565 1_665
O3 O1 O2 153.9(5) 2_465 1_665
O3 O1 O2 77.31(14) 5_445 1_665
O3 O1 O2 58.01(17) 6_665 1_665
Ga3 O1 O2 62.38(12) 2_564 1_665
Ga3 O1 O2 133.7(4) . 1_665
Ga3 O1 O2 89.81(17) 4_455 1_665
Ga1 O1 O2 172.0(3) 1_455 1_665
Nb O1 O2 172.0(3) 1_455 1_665
Ga1 O1 O2 56.47(7) . 1_665
Nb O1 O2 56.47(7) . 1_665
Ga1 O1 O2 67.77(9) 1_565 1_665
Nb O1 O2 67.77(9) 1_565 1_665
O2 O1 O2 93.79(13) . 1_665
O2 O1 O2 25.27(11) 3_565 1_665
O2 O1 O2 143.0(2) 4_455 1_665
La O1 O2 90.1(2) 1_556 1_665
La O1 O2 56.09(14) 2_566 1_665
La O1 O2 107.1(3) 4_456 1_665
O3 O1 O2 135.5(4) 2_466 1_665
O3 O1 O2 53.84(15) 6_666 1_665
O3 O1 O2 72.13(17) 5_446 1_665
O3 O1 O2 148.4(3) 6 1_665
O3 O1 O2 88.40(15) 5_455 1_665
O3 O1 O2 46.27(14) 2_565 1_665
Ga2 O1 O2 121.81(18) 1_565 1_665
Ga2 O1 O2 110.96(16) . 1_665
Ga2 O1 O2 12.86(12) 1_665 1_665
O1 O1 O2 125.39(18) 2_465 1_665
O1 O1 O2 114.49(13) 2_455 1_665
O1 O1 O2 28.2(3) 2_565 1_665
O1 O1 O2 95.8(2) 1_554 1_665
O1 O1 O2 84.2(2) 1_556 1_665
Ga3 O1 O2 75.14(11) 4_446 1_665
Ga3 O1 O2 151.6(4) 2_465 1_665
Ga3 O1 O2 44.34(8) 1_666 1_665
O3 O1 O2 134.0(4) 6_556 1_665
O3 O1 O2 82.95(16) 5_456 1_665
O3 O1 O2 42.37(15) 2_566 1_665
O3 O1 O2 38.20(11) 1_655 1_665
O3 O1 O2 156.5(2) 4_345 1_665
O3 O1 O2 81.52(11) 3_575 1_665
O2 O1 O2 118.3(3) 3_454 1_665
O2 O1 O2 58.05(10) 4_554 1_665
O2 O1 O2 107.0(3) 1_564 1_665
O1 O1 O2 115.1(3) 2_466 1_665
O1 O1 O2 106.1(3) 2_456 1_665
O1 O1 O2 29.15(19) 2_566 1_665
O3 O1 O2 78.83(17) 3_564 1_665
O3 O1 O2 129.2(4) 1_554 1_665
O3 O1 O2 79.3(2) 4_454 1_665
O3 O1 O2 65.59(11) 4_445 1_665
O3 O1 O2 169.7(4) 3_465 1_665
O3 O1 O2 54.17(11) 1_665 1_665
La O1 O2 137.75(8) 2_455 1_665
La O1 O2 22.96(9) 4 1_665
La O1 O2 103.22(9) 1_565 1_665
O2 O1 O2 118.99(8) 4_445 1_665
Ga2 O1 O2 84.2(2) 2_566 3_465
La O1 O2 138.1(2) . 3_465
La O1 O2 101.59(9) 2_565 3_465
La O1 O2 33.3(2) 4_455 3_465
O2 O1 O2 94.5(3) 5_455 3_465
O2 O1 O2 123.5(4) 6 3_465
O2 O1 O2 67.9(2) 2_565 3_465
O2 O1 O2 111.8(4) 6_556 3_465
O2 O1 O2 84.7(3) 5_456 3_465
O2 O1 O2 57.5(3) 2_566 3_465
O3 O1 O2 169.0(6) 3_565 3_465
O3 O1 O2 60.19(16) . 3_465
O3 O1 O2 59.21(16) 4_455 3_465
Ga2 O1 O2 95.8(2) 2_565 3_465
Ga3 O1 O2 140.4(4) 2_565 3_465
Ga3 O1 O2 81.45(13) 1_556 3_465
Ga3 O1 O2 40.72(11) 4_456 3_465
O2 O1 O2 108.7(2) 3_455 3_465
O2 O1 O2 127.5(3) 4 3_465
O2 O1 O2 10.60(16) 1_565 3_465
O3 O1 O2 58.02(17) 2_465 3_465
O3 O1 O2 153.9(5) 5_445 3_465
O3 O1 O2 77.31(14) 6_665 3_465
Ga3 O1 O2 133.7(4) 2_564 3_465
Ga3 O1 O2 89.81(17) . 3_465
Ga3 O1 O2 62.38(12) 4_455 3_465
Ga1 O1 O2 67.77(9) 1_455 3_465
Nb O1 O2 67.77(9) 1_455 3_465
Ga1 O1 O2 172.0(3) . 3_465
Nb O1 O2 172.0(3) . 3_465
Ga1 O1 O2 56.47(7) 1_565 3_465
Nb O1 O2 56.47(7) 1_565 3_465
O2 O1 O2 143.0(2) . 3_465
O2 O1 O2 93.79(13) 3_565 3_465
O2 O1 O2 25.27(11) 4_455 3_465
La O1 O2 107.1(3) 1_556 3_465
La O1 O2 90.1(2) 2_566 3_465
La O1 O2 56.09(14) 4_456 3_465
O3 O1 O2 53.84(15) 2_466 3_465
O3 O1 O2 72.13(17) 6_666 3_465
O3 O1 O2 135.5(4) 5_446 3_465
O3 O1 O2 88.40(15) 6 3_465
O3 O1 O2 46.27(14) 5_455 3_465
O3 O1 O2 148.4(3) 2_565 3_465
Ga2 O1 O2 12.86(12) 1_565 3_465
Ga2 O1 O2 121.81(18) . 3_465
Ga2 O1 O2 110.96(16) 1_665 3_465
O1 O1 O2 28.2(3) 2_465 3_465
O1 O1 O2 125.40(18) 2_455 3_465
O1 O1 O2 114.49(13) 2_565 3_465
O1 O1 O2 95.8(2) 1_554 3_465
O1 O1 O2 84.2(2) 1_556 3_465
Ga3 O1 O2 151.6(4) 4_446 3_465
Ga3 O1 O2 44.34(8) 2_465 3_465
Ga3 O1 O2 75.14(11) 1_666 3_465
O3 O1 O2 82.95(16) 6_556 3_465
O3 O1 O2 42.37(15) 5_456 3_465
O3 O1 O2 134.0(4) 2_566 3_465
O3 O1 O2 156.5(2) 1_655 3_465
O3 O1 O2 81.52(11) 4_345 3_465
O3 O1 O2 38.20(11) 3_575 3_465
O2 O1 O2 107.0(3) 3_454 3_465
O2 O1 O2 118.3(3) 4_554 3_465
O2 O1 O2 58.05(10) 1_564 3_465
O1 O1 O2 29.15(19) 2_466 3_465
O1 O1 O2 115.1(3) 2_456 3_465
O1 O1 O2 106.1(3) 2_566 3_465
O3 O1 O2 129.2(4) 3_564 3_465
O3 O1 O2 79.3(2) 1_554 3_465
O3 O1 O2 78.83(17) 4_454 3_465
O3 O1 O2 169.7(4) 4_445 3_465
O3 O1 O2 54.17(11) 3_465 3_465
O3 O1 O2 65.59(11) 1_665 3_465
La O1 O2 103.22(9) 2_455 3_465
La O1 O2 137.75(8) 4 3_465
La O1 O2 22.96(9) 1_565 3_465
O2 O1 O2 118.99(8) 4_445 3_465
O2 O1 O2 118.99(8) 1_665 3_465
Ga2 O1 O3 30.51(13) 2_566 3_566
La O1 O3 87.3(3) . 3_566
La O1 O3 103.0(4) 2_565 3_566
La O1 O3 139.4(5) 4_455 3_566
O2 O1 O3 136.99(18) 5_455 3_566
O2 O1 O3 119.1(2) 6 3_566
O2 O1 O3 163.7(2) 2_565 3_566
O2 O1 O3 14.9(2) 6_556 3_566
O2 O1 O3 43.4(3) 5_456 3_566
O2 O1 O3 59.8(4) 2_566 3_566
O3 O1 O3 54.3(3) 3_565 3_566
O3 O1 O3 100.1(5) . 3_566
O3 O1 O3 100.1(5) 4_455 3_566
Ga2 O1 O3 149.49(13) 2_565 3_566
Ga3 O1 O3 36.3(2) 2_565 3_566
Ga3 O1 O3 70.6(3) 1_556 3_566
Ga3 O1 O3 88.5(4) 4_456 3_566
O2 O1 O3 71.4(3) 3_455 3_566
O2 O1 O3 61.7(3) 4 3_566
O2 O1 O3 109.9(5) 1_565 3_566
O3 O1 O3 136.1(3) 2_465 3_566
O3 O1 O3 89.5(3) 5_445 3_566
O3 O1 O3 123.8(3) 6_665 3_566
Ga3 O1 O3 108.69(11) 2_564 3_566
Ga3 O1 O3 132.75(10) . 3_566
Ga3 O1 O3 155.36(17) 4_455 3_566
Ga1 O1 O3 112.1(3) 1_455 3_566
Nb O1 O3 112.1(3) 1_455 3_566
Ga1 O1 O3 70.95(17) . 3_566
Nb O1 O3 70.95(17) . 3_566
Ga1 O1 O3 117.2(3) 1_565 3_566
Nb O1 O3 117.2(3) 1_565 3_566
O2 O1 O3 58.4(2) . 3_566
O2 O1 O3 81.0(3) 3_565 3_566
O2 O1 O3 110.1(4) 4_455 3_566
La O1 O3 20.24(9) 1_556 3_566
La O1 O3 37.61(17) 2_566 3_566
La O1 O3 59.7(2) 4_456 3_566
O3 O1 O3 75.6(3) 2_466 3_566
O3 O1 O3 66.5(3) 6_666 3_566
O3 O1 O3 23.6(2) 5_446 3_566
O3 O1 O3 114.8(2) 6 3_566
O3 O1 O3 138.7(3) 5_455 3_566
O3 O1 O3 87.9(2) 2_565 3_566
Ga2 O1 O3 103.1(4) 1_565 3_566
Ga2 O1 O3 57.53(17) . 3_566
Ga2 O1 O3 62.8(2) 1_665 3_566
O1 O1 O3 142.1(6) 2_465 3_566
O1 O1 O3 92.7(4) 2_455 3_566
O1 O1 O3 97.1(4) 2_565 3_566
O1 O1 O3 149.49(13) 1_554 3_566
O1 O1 O3 30.51(13) 1_556 3_566
Ga3 O1 O3 43.60(14) 4_446 3_566
Ga3 O1 O3 95.2(3) 2_465 3_566
Ga3 O1 O3 81.4(3) 1_666 3_566
O3 O1 O3 64.1(2) 6_556 3_566
O3 O1 O3 82.6(3) 5_456 3_566
O3 O1 O3 30.8(2) 2_566 3_566
O3 O1 O3 58.80(17) 1_655 3_566
O3 O1 O3 91.8(3) 4_345 3_566
O3 O1 O3 110.5(3) 3_575 3_566
O2 O1 O3 124.70(12) 3_454 3_566
O2 O1 O3 118.16(13) 4_554 3_566
O2 O1 O3 170.3(2) 1_564 3_566
O1 O1 O3 86.0(5) 2_466 3_566
O1 O1 O3 43.1(3) 2_456 3_566
O1 O1 O3 48.6(3) 2_566 3_566
O3 O1 O3 116.08(13) 3_564 3_566
O3 O1 O3 149.20(6) 1_554 3_566
O3 O1 O3 149.20(6) 4_454 3_566
O3 O1 O3 56.88(15) 4_445 3_566
O3 O1 O3 104.9(3) 3_465 3_566
O3 O1 O3 99.3(3) 1_665 3_566
La O1 O3 91.86(16) 2_455 3_566
La O1 O3 76.37(15) 4 3_566
La O1 O3 127.8(3) 1_565 3_566
O2 O1 O3 70.38(18) 4_445 3_566
O2 O1 O3 69.9(2) 1_665 3_566
O2 O1 O3 114.7(3) 3_465 3_566
Ga2 O2 Ga3 120.0(7) . 4_446
Ga2 O2 La 105.8(3) . 4_445
Ga3 O2 La 119.7(3) 4_446 4_445
Ga2 O2 O2 39.7(2) . 4_445
Ga3 O2 O2 144.2(5) 4_446 4_445
La O2 O2 66.0(3) 4_445 4_445
Ga2 O2 O2 39.7(2) . 3_455
Ga3 O2 O2 129.3(4) 4_446 3_455
La O2 O2 111.0(2) 4_445 3_455
O2 O2 O2 60.000(2) 4_445 3_455
Ga2 O2 La 90.9(3) . .
Ga3 O2 La 111.6(4) 4_446 .
La O2 La 104.2(5) 4_445 .
O2 O2 La 99.5(2) 4_445 .
O2 O2 La 51.2(3) 3_455 .
Ga2 O2 O3 117.0(4) . 3_565
Ga3 O2 O3 62.0(3) 4_446 3_565
La O2 O3 127.8(5) 4_445 3_565
O2 O2 O3 146.3(4) 4_445 3_565
O2 O2 O3 87.0(4) 3_455 3_565
La O2 O3 49.7(3) . 3_565
Ga2 O2 O3 158.7(7) . 4_445
Ga3 O2 O3 38.8(3) 4_446 4_445
La O2 O3 91.8(3) 4_445 4_445
O2 O2 O3 155.3(5) 4_445 4_445
O2 O2 O3 143.2(5) 3_455 4_445
La O2 O3 96.4(4) . 4_445
O3 O2 O3 56.4(3) 3_565 4_445
Ga2 O2 O2 102.2(7) . 2_556
Ga3 O2 O2 39.8(3) 4_446 2_556
La O2 O2 96.9(3) 4_445 2_556
O2 O2 O2 107.0(2) 4_445 2_556
O2 O2 O2 136.8(4) 3_455 2_556
La O2 O2 151.19(19) . 2_556
O3 O2 O2 101.7(3) 3_565 2_556
O3 O2 O2 63.0(3) 4_445 2_556
Ga2 O2 O1 84.8(4) . 2_455
Ga3 O2 O1 152.8(6) 4_446 2_455
La O2 O1 56.2(3) 4_445 2_455
O2 O2 O1 62.2(2) 4_445 2_455
O2 O2 O1 62.2(2) 3_455 2_455
La O2 O1 52.7(2) . 2_455
O3 O2 O1 98.2(5) 3_565 2_455
O3 O2 O1 115.6(5) 4_445 2_455
O2 O2 O1 152.9(4) 2_556 2_455
Ga2 O2 O3 89.7(5) . 5_446
Ga3 O2 O3 35.2(2) 4_446 5_446
La O2 O3 153.4(4) 4_445 5_446
O2 O2 O3 126.4(2) 4_445 5_446
O2 O2 O3 94.8(3) 3_455 5_446
La O2 O3 96.9(3) . 5_446
O3 O2 O3 57.6(5) 3_565 5_446
O3 O2 O3 69.6(4) 4_445 5_446
O2 O2 O3 58.1(4) 2_556 5_446
O1 O2 O3 148.9(4) 2_455 5_446
Ga2 O2 O1 30.8(4) . 2_456
Ga3 O2 O1 89.8(5) 4_446 2_456
La O2 O1 122.2(4) 4_445 2_456
O2 O2 O1 62.8(2) 4_445 2_456
O2 O2 O1 62.8(2) 3_455 2_456
La O2 O1 109.0(3) . 2_456
O3 O2 O1 109.8(4) 3_565 2_456
O3 O2 O1 128.5(5) 4_445 2_456
O2 O2 O1 74.5(5) 2_556 2_456
O1 O2 O1 115.6(2) 2_455 2_456
O3 O2 O1 63.6(4) 5_446 2_456
Ga2 O2 O3 133.3(5) . 5_445
Ga3 O2 O3 93.5(4) 4_446 5_445
La O2 O3 79.9(4) 4_445 5_445
O2 O2 O3 121.6(2) 4_445 5_445
O2 O2 O3 94.2(3) 3_455 5_445
La O2 O3 44.2(2) . 5_445
O3 O2 O3 49.3(4) 3_565 5_445
O3 O2 O3 60.8(4) 4_445 5_445
O2 O2 O3 123.6(3) 2_556 5_445
O1 O2 O3 59.5(3) 2_455 5_445
O3 O2 O3 105.4(3) 5_446 5_445
O1 O2 O3 151.8(3) 2_456 5_445
Ga2 O2 O1 128.0(5) . 1_545
Ga3 O2 O1 74.2(3) 4_446 1_545
La O2 O1 46.2(3) 4_445 1_545
O2 O2 O1 97.6(4) 4_445 1_545
O2 O2 O1 155.7(4) 3_455 1_545
La O2 O1 132.9(5) . 1_545
O3 O2 O1 113.4(3) 3_565 1_545
O3 O2 O1 57.9(2) 4_445 1_545
O2 O2 O1 54.8(4) 2_556 1_545
O1 O2 O1 100.2(3) 2_455 1_545
O3 O2 O1 107.2(4) 5_446 1_545
O1 O2 O1 117.8(4) 2_456 1_545
O3 O2 O1 89.9(4) 5_445 1_545
Ga2 O2 Nb 149.0(4) . .
Ga3 O2 Nb 61.0(2) 4_446 .
La O2 Nb 97.7(3) 4_445 .
O2 O2 Nb 154.1(2) 4_445 .
O2 O2 Nb 112.7(4) 3_455 .
La O2 Nb 63.5(2) . .
O3 O2 Nb 33.0(2) 3_565 .
O3 O2 Nb 32.9(2) 4_445 .
O2 O2 Nb 94.58(19) 2_556 .
O1 O2 Nb 92.1(4) 2_455 .
O3 O2 Nb 77.2(3) 5_446 .
O1 O2 Nb 139.3(3) 2_456 .
O3 O2 Nb 32.59(17) 5_445 .
O1 O2 Nb 82.9(2) 1_545 .
Ga2 O2 Ga1 149.0(4) . .
Ga3 O2 Ga1 61.0(2) 4_446 .
La O2 Ga1 97.7(3) 4_445 .
O2 O2 Ga1 154.1(2) 4_445 .
O2 O2 Ga1 112.7(4) 3_455 .
La O2 Ga1 63.5(2) . .
O3 O2 Ga1 33.0(2) 3_565 .
O3 O2 Ga1 32.9(2) 4_445 .
O2 O2 Ga1 94.58(19) 2_556 .
O1 O2 Ga1 92.1(4) 2_455 .
O3 O2 Ga1 77.2(3) 5_446 .
O1 O2 Ga1 139.3(3) 2_456 .
O3 O2 Ga1 32.59(17) 5_445 .
O1 O2 Ga1 82.9(2) 1_545 .
Nb O2 Ga1 0.0 . .
Ga2 O2 Ga2 112.2(5) . 2_556
Ga3 O2 Ga2 59.3(2) 4_446 2_556
La O2 Ga2 68.61(19) 4_445 2_556
O2 O2 Ga2 97.4(4) 4_445 2_556
O2 O2 Ga2 151.8(3) 3_455 2_556
La O2 Ga2 156.8(3) . 2_556
O3 O2 Ga2 116.2(3) 3_565 2_556
O3 O2 Ga2 62.7(2) 4_445 2_556
O2 O2 Ga2 28.4(2) 2_556 2_556
O1 O2 Ga2 124.8(3) 2_455 2_556
O3 O2 Ga2 85.6(3) 5_446 2_556
O1 O2 Ga2 92.8(4) 2_456 2_556
O3 O2 Ga2 112.8(2) 5_445 2_556
O1 O2 Ga2 27.8(4) 1_545 2_556
Nb O2 Ga2 94.86(15) . 2_556
Ga1 O2 Ga2 94.86(15) . 2_556
Ga2 O2 O2 141.2(5) . 2
Ga3 O2 O2 96.8(3) 4_446 2
La O2 O2 39.1(2) 4_445 2
O2 O2 O2 102.84(13) 4_445 2
O2 O2 O2 123.7(3) 3_455 2
La O2 O2 85.9(4) . 2
O3 O2 O2 89.7(3) 3_565 2
O3 O2 O2 59.6(3) 4_445 2
O2 O2 O2 98.8(4) 2_556 2
O1 O2 O2 62.8(4) 2_455 2
O3 O2 O2 129.0(3) 5_446 2
O1 O2 O2 160.3(2) 2_456 2
O3 O2 O2 46.6(3) 5_445 2
O1 O2 O2 47.6(4) 1_545 2
Nb O2 O2 58.67(16) . 2
Ga1 O2 O2 58.67(16) . 2
Ga2 O2 O2 74.9(2) 2_556 2
Ga2 O2 O3 81.1(3) . 1_545
Ga3 O2 O3 113.7(4) 4_446 1_545
La O2 O3 36.3(2) 4_445 1_545
O2 O2 O3 47.5(3) 4_445 1_545
O2 O2 O3 107.2(3) 3_455 1_545
La O2 O3 131.5(4) . 1_545
O3 O2 O3 161.5(5) 3_565 1_545
O3 O2 O3 108.1(3) 4_445 1_545
O2 O2 O3 76.38(19) 2_556 1_545
O1 O2 O3 78.9(3) 2_455 1_545
O3 O2 O3 130.4(4) 5_446 1_545
O1 O2 O3 87.6(3) 2_456 1_545
O3 O2 O3 116.2(4) 5_445 1_545
O1 O2 O3 50.23(17) 1_545 1_545
Nb O2 O3 128.6(3) . 1_545
Ga1 O2 O3 128.6(3) . 1_545
Ga2 O2 O3 54.74(17) 2_556 1_545
O2 O2 O3 72.7(2) 2 1_545
Ga2 O2 La 65.1(4) . 4_446
Ga3 O2 La 68.6(4) 4_446 4_446
La O2 La 102.2(3) 4_445 4_446
O2 O2 La 75.64(19) 4_445 4_446
O2 O2 La 102.66(13) 3_455 4_446
La O2 La 148.3(3) . 4_446
O3 O2 La 121.8(4) 3_565 4_446
O3 O2 La 99.9(4) 4_445 4_446
O2 O2 La 37.3(3) 2_556 4_446
O1 O2 La 137.4(3) 2_455 4_446
O3 O2 La 64.4(3) 5_446 4_446
O1 O2 La 40.5(2) 2_456 4_446
O3 O2 La 160.7(3) 5_445 4_446
O1 O2 La 78.5(4) 1_545 4_446
Nb O2 La 129.3(3) . 4_446
Ga1 O2 La 129.3(3) . 4_446
Ga2 O2 La 52.35(17) 2_556 4_446
O2 O2 La 125.8(3) 2 4_446
O3 O2 La 67.7(3) 1_545 4_446
Ga2 O2 Ga3 44.2(2) . 2_455
Ga3 O2 Ga3 125.0(5) 4_446 2_455
La O2 Ga3 66.65(18) 4_445 2_455
O2 O2 Ga3 20.1(2) 4_445 2_455
O2 O2 Ga3 75.5(2) 3_455 2_455
La O2 Ga3 119.4(2) . 2_455
O3 O2 Ga3 161.1(3) 3_565 2_455
O3 O2 Ga3 141.2(3) 4_445 2_455
O2 O2 Ga3 86.9(2) 2_556 2_455
O1 O2 Ga3 79.9(2) 2_455 2_455
O3 O2 Ga3 116.2(4) 5_446 2_455
O1 O2 Ga3 56.0(2) 2_456 2_455
O3 O2 Ga3 137.6(3) 5_445 2_455
O1 O2 Ga3 85.3(2) 1_545 2_455
Nb O2 Ga3 164.4(3) . 2_455
Ga1 O2 Ga3 164.4(3) . 2_455
Ga2 O2 Ga3 79.09(19) 2_556 2_455
O2 O2 Ga3 105.72(14) 2 2_455
O3 O2 Ga3 36.88(18) 1_545 2_455
La O2 Ga3 57.44(15) 4_446 2_455
Ga2 O2 Ga3 107.6(3) . 2_565
Ga3 O2 Ga3 48.9(2) 4_446 2_565
La O2 Ga3 144.8(4) 4_445 2_565
O2 O2 Ga3 145.8(3) 4_445 2_565
O2 O2 Ga3 88.3(4) 3_455 2_565
La O2 Ga3 64.59(16) . 2_565
O3 O2 Ga3 20.3(3) 3_565 2_565
O3 O2 Ga3 58.8(2) 4_445 2_565
O2 O2 Ga3 86.9(2) 2_556 2_565
O1 O2 Ga3 116.3(3) 2_455 2_565
O3 O2 Ga3 37.4(2) 5_446 2_565
O1 O2 Ga3 92.6(3) 2_456 2_565
O3 O2 Ga3 69.3(2) 5_445 2_565
O1 O2 Ga3 115.51(18) 1_545 2_565
Nb O2 Ga3 47.08(10) . 2_565
Ga1 O2 Ga3 47.08(10) . 2_565
Ga2 O2 Ga3 107.9(2) 2_556 2_565
O2 O2 Ga3 105.74(15) 2 2_565
O3 O2 Ga3 162.6(3) 1_545 2_565
La O2 Ga3 101.7(3) 4_446 2_565
Ga3 O2 Ga3 148.5(3) 2_455 2_565
Ga2 O2 La 57.4(3) . 1_556
Ga3 O2 La 67.8(3) 4_446 1_556
La O2 La 159.2(4) 4_445 1_556
O2 O2 La 96.38(14) 4_445 1_556
O2 O2 La 65.1(2) 3_455 1_556
La O2 La 89.2(2) . 1_556
O3 O2 La 73.0(3) 3_565 1_556
O3 O2 La 102.6(4) 4_445 1_556
O2 O2 La 77.0(4) 2_556 1_556
O1 O2 La 127.0(3) 2_455 1_556
O3 O2 La 33.32(18) 5_446 1_556
O1 O2 La 37.09(16) 2_456 1_556
O3 O2 La 120.3(3) 5_445 1_556
O1 O2 La 131.8(5) 1_545 1_556
Nb O2 La 102.54(19) . 1_556
Ga1 O2 La 102.54(19) . 1_556
Ga2 O2 La 104.7(3) 2_556 1_556
O2 O2 La 160.70(12) 2 1_556
O3 O2 La 123.4(4) 1_545 1_556
La O2 La 60.87(18) 4_446 1_556
Ga3 O2 La 93.0(2) 2_455 1_556
Ga3 O2 La 55.56(12) 2_565 1_556
Ga2 O2 O3 53.4(3) . 2_456
Ga3 O2 O3 100.2(5) 4_446 2_456
La O2 O3 76.6(3) 4_445 2_456
O2 O2 O3 44.6(2) 4_445 2_456
O2 O2 O3 91.9(2) 3_455 2_456
La O2 O3 141.5(2) . 2_456
O3 O2 O3 154.1(4) 3_565 2_456
O3 O2 O3 122.1(4) 4_445 2_456
O2 O2 O3 62.5(2) 2_556 2_456
O1 O2 O3 104.1(3) 2_455 2_456
O3 O2 O3 96.8(5) 5_446 2_456
O1 O2 O3 48.3(2) 2_456 2_456
O3 O2 O3 156.3(4) 5_445 2_456
O1 O2 O3 75.6(3) 1_545 2_456
Nb O2 O3 154.9(3) . 2_456
Ga1 O2 O3 154.9(3) . 2_456
Ga2 O2 O3 60.2(2) 2_556 2_456
O2 O2 O3 112.1(2) 2 2_456
O3 O2 O3 40.3(4) 1_545 2_456
La O2 O3 33.71(17) 4_446 2_456
Ga3 O2 O3 24.84(13) 2_455 2_456
Ga3 O2 O3 133.9(3) 2_565 2_456
La O2 O3 83.0(3) 1_556 2_456
Ga2 O2 La 49.1(3) . 2_455
Ga3 O2 La 168.4(4) 4_446 2_455
La O2 La 70.7(2) 4_445 2_455
O2 O2 La 31.90(15) 4_445 2_455
O2 O2 La 40.90(19) 3_455 2_455
La O2 La 68.10(18) . 2_455
O3 O2 La 117.1(4) 3_565 2_455
O3 O2 La 151.8(5) 4_445 2_455
O2 O2 La 138.8(2) 2_556 2_455
O1 O2 La 36.3(2) 2_455 2_455
O3 O2 La 133.6(3) 5_446 2_455
O1 O2 La 79.7(3) 2_456 2_455
O3 O2 La 93.6(3) 5_445 2_455
O1 O2 La 115.0(3) 1_545 2_455
Nb O2 La 125.3(3) . 2_455
Ga1 O2 La 125.3(3) . 2_455
Ga2 O2 La 125.5(2) 2_556 2_455
O2 O2 La 94.7(4) 2 2_455
O3 O2 La 70.97(18) 1_545 2_455
La O2 La 105.3(2) 4_446 2_455
Ga3 O2 La 51.98(9) 2_455 2_455
Ga3 O2 La 126.2(2) 2_565 2_455
La O2 La 100.71(15) 1_556 2_455
O3 O2 La 76.37(17) 2_456 2_455
Ga2 O2 Ga3 37.12(19) . 1_556
Ga3 O2 Ga3 115.8(4) 4_446 1_556
La O2 Ga3 124.4(3) 4_445 1_556
O2 O2 Ga3 67.2(2) 4_445 1_556
O2 O2 Ga3 14.3(2) 3_455 1_556
La O2 Ga3 56.80(12) . 1_556
O3 O2 Ga3 82.2(2) 3_565 1_556
O3 O2 Ga3 137.5(3) 4_445 1_556
O2 O2 Ga3 124.4(5) 2_556 1_556
O1 O2 Ga3 76.3(2) 2_455 1_556
O3 O2 Ga3 80.9(2) 5_446 1_556
O1 O2 Ga3 53.09(19) 2_456 1_556
O3 O2 Ga3 101.0(3) 5_445 1_556
O1 O2 Ga3 164.4(3) 1_545 1_556
Nb O2 Ga3 112.3(2) . 1_556
Ga1 O2 Ga3 112.3(2) . 1_556
Ga2 O2 Ga3 145.8(3) 2_556 1_556
O2 O2 Ga3 136.7(5) 2 1_556
O3 O2 Ga3 114.3(2) 1_545 1_556
La O2 Ga3 93.6(2) 4_446 1_556
Ga3 O2 Ga3 79.10(13) 2_455 1_556
Ga3 O2 Ga3 79.15(14) 2_565 1_556
La O2 Ga3 50.86(10) 1_556 1_556
O3 O2 Ga3 90.4(2) 2_456 1_556
La O2 Ga3 53.73(8) 2_455 1_556
Ga2 O2 Ga3 138.0(5) . 4_445
Ga3 O2 Ga3 100.3(3) 4_446 4_445
La O2 Ga3 57.8(3) 4_445 4_445
O2 O2 Ga3 110.14(12) 4_445 4_445
O2 O2 Ga3 105.60(17) 3_455 4_445
La O2 Ga3 61.5(2) . 4_445
O3 O2 Ga3 70.3(4) 3_565 4_445
O3 O2 Ga3 62.0(4) 4_445 4_445
O2 O2 Ga3 117.3(4) 2_556 4_445
O1 O2 Ga3 53.5(3) 2_455 4_445
O3 O2 Ga3 122.5(3) 5_446 4_445
O1 O2 Ga3 168.2(3) 2_456 4_445
O3 O2 Ga3 22.53(16) 5_445 4_445
O1 O2 Ga3 71.5(4) 1_545 4_445
Nb O2 Ga3 45.29(14) . 4_445
Ga1 O2 Ga3 45.29(14) . 4_445
Ga2 O2 Ga3 97.69(18) 2_556 4_445
O2 O2 Ga3 24.93(18) 2 4_445
O3 O2 Ga3 94.0(3) 1_545 4_445
La O2 Ga3 149.9(2) 4_446 4_445
Ga3 O2 Ga3 120.7(2) 2_455 4_445
Ga3 O2 Ga3 89.4(2) 2_565 4_445
La O2 Ga3 142.7(2) 1_556 4_445
O3 O2 Ga3 134.3(3) 2_456 4_445
La O2 Ga3 89.7(2) 2_455 4_445
Ga3 O2 Ga3 116.1(3) 1_556 4_445
Ga2 O2 O3 120.7(5) . 6_656
Ga3 O2 O3 1.20(18) 4_446 6_656
La O2 O3 118.5(2) 4_445 6_656
O2 O2 O3 144.0(3) 4_445 6_656
O2 O2 O3 130.5(3) 3_455 6_656
La O2 O3 112.4(2) . 6_656
O3 O2 O3 62.7(3) 3_565 6_656
O3 O2 O3 38.2(4) 4_445 6_656
O2 O2 O3 39.03(16) 2_556 6_656
O1 O2 O3 152.6(4) 2_455 6_656
O3 O2 O3 36.3(2) 5_446 6_656
O1 O2 O3 90.3(4) 2_456 6_656
O3 O2 O3 93.5(2) 5_445 6_656
O1 O2 O3 73.0(3) 1_545 6_656
Nb O2 O3 61.04(17) . 6_656
Ga1 O2 O3 61.04(17) . 6_656
Ga2 O2 O3 58.17(15) 2_556 6_656
O2 O2 O3 95.9(2) 2 6_656
O3 O2 O3 112.7(3) 1_545 6_656
La O2 O3 68.4(2) 4_446 6_656
Ga3 O2 O3 124.6(3) 2_455 6_656
Ga3 O2 O3 49.94(13) 2_565 6_656
La O2 O3 68.8(2) 1_556 6_656
O3 O2 O3 99.8(3) 2_456 6_656
La O2 O3 169.3(3) 2_455 6_656
Ga3 O2 O3 117.0(2) 1_556 6_656
Ga3 O2 O3 99.8(2) 4_445 6_656
Ga2 O2 O3 87.5(3) . 2_455
Ga3 O2 O3 138.7(3) 4_446 2_455
La O2 O3 20.02(15) 4_445 2_455
O2 O2 O3 48.2(3) 4_445 2_455
O2 O2 O3 91.8(2) 3_455 2_455
La O2 O3 96.7(3) . 2_455
O3 O2 O3 135.2(4) 3_565 2_455
O3 O2 O3 111.3(3) 4_445 2_455
O2 O2 O3 109.2(2) 2_556 2_455
O1 O2 O3 44.27(16) 2_455 2_455
O3 O2 O3 166.1(5) 5_446 2_455
O1 O2 O3 109.2(3) 2_456 2_455
O3 O2 O3 86.3(4) 5_445 2_455
O1 O2 O3 64.5(3) 1_545 2_455
Nb O2 O3 111.4(3) . 2_455
Ga1 O2 O3 111.4(3) . 2_455
Ga2 O2 O3 82.83(19) 2_556 2_455
O2 O2 O3 54.7(2) 2 2_455
O3 O2 O3 35.6(3) 1_545 2_455
La O2 O3 102.2(2) 4_446 2_455
Ga3 O2 O3 53.82(16) 2_455 2_455
Ga3 O2 O3 155.5(4) 2_565 2_455
La O2 O3 144.5(2) 1_556 2_455
O3 O2 O3 70.65(17) 2_456 2_455
La O2 O3 51.00(15) 2_455 2_455
Ga3 O2 O3 104.66(19) 1_556 2_455
Ga3 O2 O3 67.0(2) 4_445 2_455
O3 O2 O3 137.5(2) 6_656 2_455
Ga2 O2 Ga2 96.7(4) . 1_554
Ga3 O2 Ga2 141.5(5) 4_446 1_554
La O2 Ga2 52.3(2) 4_445 1_554
O2 O2 Ga2 72.24(8) 4_445 1_554
O2 O2 Ga2 72.24(8) 3_455 1_554
La O2 Ga2 52.6(2) . 1_554
O3 O2 Ga2 92.7(4) 3_565 1_554
O3 O2 Ga2 103.6(4) 4_445 1_554
O2 O2 Ga2 147.5(4) 2_556 1_554
O1 O2 Ga2 12.0(2) 2_455 1_554
O3 O2 Ga2 148.7(4) 5_446 1_554
O1 O2 Ga2 127.6(3) 2_456 1_554
O3 O2 Ga2 49.6(2) 5_445 1_554
O1 O2 Ga2 92.8(4) 1_545 1_554
Nb O2 Ga2 81.8(3) . 1_554
Ga1 O2 Ga2 81.8(3) . 1_554
Ga2 O2 Ga2 119.3(2) 2_556 1_554
O2 O2 Ga2 51.8(3) 2 1_554
O3 O2 Ga2 80.8(3) 1_545 1_554
La O2 Ga2 145.2(2) 4_446 1_554
Ga3 O2 Ga2 88.57(16) 2_455 1_554
Ga3 O2 Ga2 112.3(3) 2_565 1_554
La O2 Ga2 135.4(2) 1_556 1_554
O3 O2 Ga2 111.6(2) 2_456 1_554
La O2 Ga2 48.13(12) 2_455 1_554
Ga3 O2 Ga2 86.01(17) 1_556 1_554
Ga3 O2 Ga2 41.60(12) 4_445 1_554
O3 O2 Ga2 141.2(3) 6_656 1_554
O3 O2 Ga2 45.17(16) 2_455 1_554
Ga2 O2 O2 90.6(5) . 5_446
Ga3 O2 O2 74.6(4) 4_446 5_446
La O2 O2 67.47(15) 4_445 5_446
O2 O2 O2 76.5(4) 4_445 5_446
O2 O2 O2 129.7(4) 3_455 5_446
La O2 O2 171.6(5) . 5_446
O3 O2 O2 135.9(4) 3_565 5_446
O3 O2 O2 85.1(2) 4_445 5_446
O2 O2 O2 35.76(19) 2_556 5_446
O1 O2 O2 119.3(3) 2_455 5_446
O3 O2 O2 91.3(5) 5_446 5_446
O1 O2 O2 76.0(4) 2_456 5_446
O3 O2 O2 131.8(3) 5_445 5_446
O1 O2 O2 41.9(3) 1_545 5_446
Nb O2 O2 117.3(2) . 5_446
Ga1 O2 O2 117.3(2) . 5_446
Ga2 O2 O2 22.46(7) 2_556 5_446
O2 O2 O2 87.80(19) 2 5_446
O3 O2 O2 40.73(19) 1_545 5_446
La O2 O2 38.4(3) 4_446 5_446
Ga3 O2 O2 57.3(2) 2_455 5_446
Ga3 O2 O2 122.6(4) 2_565 5_446
La O2 O2 98.6(4) 1_556 5_446
O3 O2 O2 37.8(2) 2_456 5_446
La O2 O2 107.0(2) 2_455 5_446
Ga3 O2 O2 126.5(4) 1_556 5_446
Ga3 O2 O2 112.6(3) 4_445 5_446
O3 O2 O2 73.7(3) 6_656 5_446
O3 O2 O2 75.1(2) 2_455 5_446
Ga2 O2 O2 119.0(3) 1_554 5_446
Ga2 O2 O2 51.6(2) . 5_456
Ga3 O2 O2 92.0(4) 4_446 5_456
La O2 O2 148.3(4) 4_445 5_456
O2 O2 O2 88.4(2) 4_445 5_456
O2 O2 O2 37.3(3) 3_455 5_456
La O2 O2 60.12(13) . 5_456
O3 O2 O2 65.6(2) 3_565 5_456
O3 O2 O2 116.0(3) 4_445 5_456
O2 O2 O2 108.9(6) 2_556 5_456
O1 O2 O2 96.1(3) 2_455 5_456
O3 O2 O2 57.7(3) 5_446 5_456
O1 O2 O2 51.9(2) 2_456 5_456
O3 O2 O2 100.0(3) 5_445 5_456
O1 O2 O2 163.6(6) 1_545 5_456
Nb O2 O2 98.4(2) . 5_456
Ga1 O2 O2 98.4(2) . 5_456
Ga2 O2 O2 136.4(5) 2_556 5_456
O2 O2 O2 145.7(5) 2 5_456
O3 O2 O2 132.7(4) 1_545 5_456
La O2 O2 88.3(4) 4_446 5_456
Ga3 O2 O2 95.8(3) 2_455 5_456
Ga3 O2 O2 57.44(15) 2_565 5_456
La O2 O2 31.9(2) 1_556 5_456
O3 O2 O2 98.8(3) 2_456 5_456
La O2 O2 77.72(18) 2_455 5_456
Ga3 O2 O2 24.03(10) 1_556 5_456
Ga3 O2 O2 120.8(3) 4_445 5_456
O3 O2 O2 93.2(3) 6_656 5_456
O3 O2 O2 128.7(3) 2_455 5_456
Ga2 O2 O2 103.6(3) 1_554 5_456
O2 O2 O2 126.5(6) 5_446 5_456
Ga2 O2 La 162.0(4) . 2
Ga3 O2 La 59.1(2) 4_446 2
La O2 La 65.23(16) 4_445 2
O2 O2 La 128.9(4) 4_445 2
O2 O2 La 156.8(3) 3_455 2
La O2 La 106.3(3) . 2
O3 O2 La 79.3(2) 3_565 2
O3 O2 La 27.0(2) 4_445 2
O2 O2 La 65.1(3) 2_556 2
O1 O2 La 101.1(3) 2_455 2
O3 O2 La 93.6(2) 5_446 2
O1 O2 La 139.7(4) 2_456 2
O3 O2 La 62.63(18) 5_445 2
O1 O2 La 34.43(14) 1_545 2
Nb O2 La 48.57(9) . 2
Ga1 O2 La 48.57(9) . 2
Ga2 O2 La 50.52(9) 2_556 2
O2 O2 La 38.54(17) 2 2
O3 O2 La 83.3(2) 1_545 2
La O2 La 100.49(19) 4_446 2
Ga3 O2 La 119.49(18) 2_455 2
Ga3 O2 La 85.30(13) 2_565 2
La O2 La 126.7(2) 1_556 2
O3 O2 La 108.6(2) 2_456 2
La O2 La 132.5(3) 2_455 2
Ga3 O2 La 160.8(3) 1_556 2
Ga3 O2 La 52.13(11) 4_445 2
O3 O2 La 58.10(15) 6_656 2
O3 O2 La 85.06(19) 2_455 2
Ga2 O2 La 89.6(2) 1_554 2
O2 O2 La 71.63(13) 5_446 2
O2 O2 La 142.7(3) 5_456 2
Ga2 O2 O3 167.3(5) . 6_655
Ga3 O2 O3 67.7(3) 4_446 6_655
La O2 O3 75.9(3) 4_445 6_655
O2 O2 O3 139.6(2) 4_445 6_655
O2 O2 O3 127.7(3) 3_455 6_655
La O2 O3 76.6(3) . 6_655
O3 O2 O3 56.0(3) 3_565 6_655
O3 O2 O3 29.6(4) 4_445 6_655
O2 O2 O3 90.0(3) 2_556 6_655
O1 O2 O3 86.0(4) 2_455 6_655
O3 O2 O3 93.8(2) 5_446 6_655
O1 O2 O3 156.9(4) 2_456 6_655
O3 O2 O3 34.13(19) 5_445 6_655
O1 O2 O3 62.3(3) 1_545 6_655
Nb O2 O3 23.04(12) . 6_655
Ga1 O2 O3 23.04(12) . 6_655
Ga2 O2 O3 80.23(17) 2_556 6_655
O2 O2 O3 37.29(16) 2 6_655
O3 O2 O3 105.6(2) 1_545 6_655
La O2 O3 127.3(2) 4_446 6_655
Ga3 O2 O3 141.7(2) 2_455 6_655
Ga3 O2 O3 69.11(17) 2_565 6_655
La O2 O3 123.4(2) 1_556 6_655
O3 O2 O3 137.9(2) 2_456 6_655
La O2 O3 122.2(3) 2_455 6_655
Ga3 O2 O3 131.6(3) 1_556 6_655
Ga3 O2 O3 32.59(16) 4_445 6_655
O3 O2 O3 67.25(15) 6_656 6_655
O3 O2 O3 91.9(3) 2_455 6_655
Ga2 O2 O3 74.1(2) 1_554 6_655
O2 O2 O3 101.5(2) 5_446 6_655
O2 O2 O3 121.1(3) 5_456 6_655
La O2 O3 29.89(11) 2 6_655
Ga2 O2 O2 84.4(3) . 6_556
Ga3 O2 O2 62.4(3) 4_446 6_556
La O2 O2 163.8(6) 4_445 6_556
O2 O2 O2 122.9(2) 4_445 6_556
O2 O2 O2 68.8(3) 3_455 6_556
La O2 O2 62.4(2) . 6_556
O3 O2 O2 37.0(3) 3_565 6_556
O3 O2 O2 81.3(2) 4_445 6_556
O2 O2 O2 93.1(5) 2_556 6_556
O1 O2 O2 113.8(4) 2_455 6_556
O3 O2 O2 35.1(2) 5_446 6_556
O1 O2 O2 72.8(3) 2_456 6_556
O3 O2 O2 84.0(3) 5_445 6_556
O1 O2 O2 135.6(2) 1_545 6_556
Nb O2 O2 68.68(19) . 6_556
Ga1 O2 O2 68.68(19) . 6_556
Ga2 O2 O2 119.7(3) 2_556 6_556
O2 O2 O2 126.6(3) 2 6_556
O3 O2 O2 159.8(5) 1_545 6_556
La O2 O2 93.4(4) 4_446 6_556
Ga3 O2 O2 126.8(3) 2_455 6_556
Ga3 O2 O2 23.19(11) 2_565 6_556
La O2 O2 36.49(19) 1_556 6_556
O3 O2 O2 119.5(4) 2_456 6_556
La O2 O2 109.34(14) 2_455 6_556
Ga3 O2 O2 57.67(10) 1_556 6_556
Ga3 O2 O2 106.2(3) 4_445 6_556
O3 O2 O2 63.59(17) 6_656 6_556
O3 O2 O2 157.4(3) 2_455 6_556
Ga2 O2 O2 115.0(4) 1_554 6_556
O2 O2 O2 125.9(6) 5_446 6_556
O2 O2 O2 34.71(19) 5_456 6_556
La O2 O2 108.16(13) 2 6_556
O3 O2 O2 91.4(2) 6_655 6_556
Ga2 O2 O1 82.1(3) . .
Ga3 O2 O1 94.6(3) 4_446 .
La O2 O1 130.5(5) 4_445 .
O2 O2 O1 106.9(3) 4_445 .
O2 O2 O1 47.5(3) 3_455 .
La O2 O1 26.3(3) . .
O3 O2 O1 39.52(19) 3_565 .
O3 O2 O1 95.7(3) 4_445 .
O2 O2 O1 129.9(4) 2_556 .
O1 O2 O1 76.8(3) 2_455 .
O3 O2 O1 72.2(3) 5_446 .
O1 O2 O1 89.7(3) 2_456 .
O3 O2 O1 62.2(3) 5_445 .
O1 O2 O1 149.7(4) 1_545 .
Nb O2 O1 67.20(19) . .
Ga1 O2 O1 67.20(19) . .
Ga2 O2 O1 153.8(2) 2_556 .
O2 O2 O1 108.2(4) 2 .
O3 O2 O1 151.5(3) 1_545 .
La O2 O1 124.3(4) 4_446 .
Ga3 O2 O1 122.96(16) 2_455 .
Ga3 O2 O1 45.89(15) 2_565 .
La O2 O1 63.6(3) 1_556 .
O3 O2 O1 134.7(3) 2_456 .
La O2 O1 80.64(17) 2_455 .
Ga3 O2 O1 45.09(14) 1_556 .
Ga3 O2 O1 83.3(3) 4_445 .
O3 O2 O1 95.7(2) 6_656 .
O3 O2 O1 120.9(4) 2_455 .
Ga2 O2 O1 78.5(3) 1_554 .
O2 O2 O1 161.9(5) 5_446 .
O2 O2 O1 37.8(3) 5_456 .
La O2 O1 115.7(2) 2 .
O3 O2 O1 87.3(3) 6_655 .
O2 O2 O1 37.1(3) 6_556 .
Ga2 O2 Ga1 99.3(4) . 1_556
Ga3 O2 Ga1 23.3(2) 4_446 1_556
La O2 Ga1 141.5(3) 4_445 1_556
O2 O2 Ga1 132.76(12) 4_445 1_556
O2 O2 Ga1 107.0(3) 3_455 1_556
La O2 Ga1 104.1(2) . 1_556
O3 O2 Ga1 59.5(3) 3_565 1_556
O3 O2 Ga1 59.5(3) 4_445 1_556
O2 O2 Ga1 48.8(3) 2_556 1_556
O1 O2 Ga1 156.7(3) 2_455 1_556
O3 O2 Ga1 12.17(14) 5_446 1_556
O1 O2 Ga1 70.9(3) 2_456 1_556
O3 O2 Ga1 103.6(2) 5_445 1_556
O1 O2 Ga1 95.3(3) 1_545 1_556
Nb O2 Ga1 72.61(13) . 1_556
Ga1 O2 Ga1 72.61(13) . 1_556
Ga2 O2 Ga1 75.08(18) 2_556 1_556
O2 O2 Ga1 119.0(2) 2 1_556
O3 O2 Ga1 124.3(3) 1_545 1_556
La O2 Ga1 62.80(17) 4_446 1_556
Ga3 O2 Ga1 118.8(3) 2_455 1_556
Ga3 O2 Ga1 40.57(9) 2_565 1_556
La O2 Ga1 44.61(11) 1_556 1_556
O3 O2 Ga1 96.5(3) 2_456 1_556
La O2 Ga1 145.3(2) 2_455 1_556
Ga3 O2 Ga1 93.03(18) 1_556 1_556
Ga3 O2 Ga1 117.05(16) 4_445 1_556
O3 O2 Ga1 24.34(13) 6_656 1_556
O3 O2 Ga1 157.9(3) 2_455 1_556
Ga2 O2 Ga1 152.0(2) 1_554 1_556
O2 O2 Ga1 83.8(3) 5_446 1_556
O2 O2 Ga1 69.8(3) 5_456 1_556
La O2 Ga1 82.14(12) 2 1_556
O3 O2 Ga1 85.98(19) 6_655 1_556
O2 O2 Ga1 44.70(17) 6_556 1_556
O1 O2 Ga1 81.1(2) . 1_556
Ga2 O2 Nb 99.3(4) . 1_556
Ga3 O2 Nb 23.3(2) 4_446 1_556
La O2 Nb 141.5(3) 4_445 1_556
O2 O2 Nb 132.76(12) 4_445 1_556
O2 O2 Nb 107.0(3) 3_455 1_556
La O2 Nb 104.1(2) . 1_556
O3 O2 Nb 59.5(3) 3_565 1_556
O3 O2 Nb 59.5(3) 4_445 1_556
O2 O2 Nb 48.8(3) 2_556 1_556
O1 O2 Nb 156.7(3) 2_455 1_556
O3 O2 Nb 12.17(14) 5_446 1_556
O1 O2 Nb 70.9(3) 2_456 1_556
O3 O2 Nb 103.6(2) 5_445 1_556
O1 O2 Nb 95.3(3) 1_545 1_556
Nb O2 Nb 72.61(13) . 1_556
Ga1 O2 Nb 72.61(13) . 1_556
Ga2 O2 Nb 75.08(18) 2_556 1_556
O2 O2 Nb 119.0(2) 2 1_556
O3 O2 Nb 124.3(3) 1_545 1_556
La O2 Nb 62.80(17) 4_446 1_556
Ga3 O2 Nb 118.8(3) 2_455 1_556
Ga3 O2 Nb 40.57(9) 2_565 1_556
La O2 Nb 44.61(11) 1_556 1_556
O3 O2 Nb 96.5(3) 2_456 1_556
La O2 Nb 145.3(2) 2_455 1_556
Ga3 O2 Nb 93.03(18) 1_556 1_556
Ga3 O2 Nb 117.05(16) 4_445 1_556
O3 O2 Nb 24.34(13) 6_656 1_556
O3 O2 Nb 157.9(3) 2_455 1_556
Ga2 O2 Nb 152.0(2) 1_554 1_556
O2 O2 Nb 83.8(3) 5_446 1_556
O2 O2 Nb 69.8(3) 5_456 1_556
La O2 Nb 82.14(12) 2 1_556
O3 O2 Nb 85.98(19) 6_655 1_556
O2 O2 Nb 44.70(17) 6_556 1_556
O1 O2 Nb 81.1(2) . 1_556
Ga1 O2 Nb 0.0 1_556 1_556
Ga2 O2 O3 139.6(4) . 1_655
Ga3 O2 O3 41.5(3) 4_446 1_655
La O2 O3 114.2(3) 4_445 1_655
O2 O2 O3 173.9(4) 4_445 1_655
O2 O2 O3 115.3(4) 3_455 1_655
La O2 O3 74.4(2) . 1_655
O3 O2 O3 28.5(2) 3_565 1_655
O3 O2 O3 28.38(18) 4_445 1_655
O2 O2 O3 79.13(16) 2_556 1_655
O1 O2 O3 112.5(4) 2_455 1_655
O3 O2 O3 56.2(4) 5_446 1_655
O1 O2 O3 119.5(3) 2_456 1_655
O3 O2 O3 53.4(3) 5_445 1_655
O1 O2 O3 86.21(18) 1_545 1_655
Nb O2 O3 21.51(16) . 1_655
Ga1 O2 O3 21.51(16) . 1_655
Ga2 O2 O3 88.24(16) 2_556 1_655
O2 O2 O3 76.21(19) 2 1_655
O3 O2 O3 136.4(3) 1_545 1_655
La O2 O3 109.9(3) 4_446 1_655
Ga3 O2 O3 166.0(3) 2_455 1_655
Ga3 O2 O3 32.13(13) 2_565 1_655
La O2 O3 84.5(2) 1_556 1_655
O3 O2 O3 141.4(3) 2_456 1_655
La O2 O3 142.0(3) 2_455 1_655
Ga3 O2 O3 109.3(2) 1_556 1_655
Ga3 O2 O3 66.5(2) 4_445 1_655
O3 O2 O3 41.8(3) 6_656 1_655
O3 O2 O3 130.8(3) 2_455 1_655
Ga2 O2 O3 102.9(3) 1_554 1_655
O2 O2 O3 109.4(2) 5_446 1_655
O2 O2 O3 89.2(2) 5_456 1_655
La O2 O3 53.64(15) 2 1_655
O3 O2 O3 38.9(3) 6_655 1_655
O2 O2 O3 55.32(18) 6_556 1_655
O1 O2 O3 68.00(15) . 1_655
Ga1 O2 O3 51.10(17) 1_556 1_655
Nb O2 O3 51.10(17) 1_556 1_655
Ga2 O2 Ga2 72.6(2) . 2_566
Ga3 O2 Ga2 83.8(3) 4_446 2_566
La O2 Ga2 150.1(4) 4_445 2_566
O2 O2 Ga2 106.6(3) 4_445 2_566
O2 O2 Ga2 48.5(3) 3_455 2_566
La O2 Ga2 46.88(13) . 2_566
O3 O2 Ga2 44.4(2) 3_565 2_566
O3 O2 Ga2 98.0(3) 4_445 2_566
O2 O2 Ga2 112.8(4) 2_556 2_566
O1 O2 Ga2 94.4(2) 2_455 2_566
O3 O2 Ga2 54.9(2) 5_446 2_566
O1 O2 Ga2 71.97(16) 2_456 2_566
O3 O2 Ga2 80.6(2) 5_445 2_566
O1 O2 Ga2 155.5(2) 1_545 2_566
Nb O2 Ga2 76.93(15) . 2_566
Ga1 O2 Ga2 76.93(15) . 2_566
Ga2 O2 Ga2 140.5(3) 2_556 2_566
O2 O2 Ga2 127.1(3) 2 2_566
O3 O2 Ga2 153.4(2) 1_545 2_566
La O2 Ga2 103.7(2) 4_446 2_566
Ga3 O2 Ga2 116.82(17) 2_455 2_566
Ga3 O2 Ga2 39.98(7) 2_565 2_566
La O2 Ga2 42.85(8) 1_556 2_566
O3 O2 Ga2 119.8(3) 2_456 2_566
La O2 Ga2 88.31(14) 2_455 2_566
Ga3 O2 Ga2 39.47(7) 1_556 2_566
Ga3 O2 Ga2 102.7(2) 4_445 2_566
O3 O2 Ga2 85.03(17) 6_656 2_566
O3 O2 Ga2 136.3(2) 2_455 2_566
Ga2 O2 Ga2 97.9(2) 1_554 2_566
O2 O2 Ga2 141.2(5) 5_446 2_566
O2 O2 Ga2 21.58(11) 5_456 2_566
La O2 Ga2 123.30(17) 2 2_566
O3 O2 Ga2 99.52(19) 6_655 2_566
O2 O2 Ga2 21.48(11) 6_556 2_566
O1 O2 Ga2 20.8(3) . 2_566
Ga1 O2 Ga2 65.57(12) 1_556 2_566
Nb O2 Ga2 65.57(12) 1_556 2_566
O3 O2 Ga2 69.97(15) 1_655 2_566
Ga2 O2 Ga3 82.3(3) . 1_546
Ga3 O2 Ga3 96.5(4) 4_446 1_546
La O2 Ga3 51.41(19) 4_445 1_546
O2 O2 Ga3 57.8(3) 4_445 1_546
O2 O2 Ga3 116.5(3) 3_455 1_546
La O2 Ga3 150.5(3) . 1_546
O3 O2 Ga3 155.9(3) 3_565 1_546
O3 O2 Ga3 100.2(2) 4_445 1_546
O2 O2 Ga3 57.83(10) 2_556 1_546
O1 O2 Ga3 98.0(2) 2_455 1_546
O3 O2 Ga3 111.6(4) 5_446 1_546
O1 O2 Ga3 78.9(2) 2_456 1_546
O3 O2 Ga3 128.3(3) 5_445 1_546
O1 O2 Ga3 45.71(19) 1_545 1_546
Nb O2 Ga3 128.59(18) . 1_546
Ga1 O2 Ga3 128.59(18) . 1_546
Ga2 O2 Ga3 39.76(10) 2_556 1_546
O2 O2 Ga3 81.90(14) 2 1_546
O3 O2 Ga3 19.08(17) 1_545 1_546
La O2 Ga3 50.81(12) 4_446 1_546
Ga3 O2 Ga3 41.03(9) 2_455 1_546
Ga3 O2 Ga3 144.7(3) 2_565 1_546
La O2 Ga3 110.4(3) 1_556 1_546
O3 O2 Ga3 31.25(17) 2_456 1_546
La O2 Ga3 86.24(14) 2_455 1_546
Ga3 O2 Ga3 119.11(19) 1_556 1_546
Ga3 O2 Ga3 105.94(18) 4_445 1_546
O3 O2 Ga3 95.5(2) 6_656 1_546
O3 O2 Ga3 54.51(15) 2_455 1_546
Ga2 O2 Ga3 99.58(16) 1_554 1_546
O2 O2 Ga3 22.08(12) 5_446 1_546
O2 O2 Ga3 130.0(4) 5_456 1_546
La O2 Ga3 80.02(12) 2 1_546
O3 O2 Ga3 107.60(16) 6_655 1_546
O2 O2 Ga3 144.1(5) 6_556 1_546
O1 O2 Ga3 163.95(18) . 1_546
Ga1 O2 Ga3 105.3(2) 1_556 1_546
Nb O2 Ga3 105.3(2) 1_556 1_546
O3 O2 Ga3 127.52(18) 1_655 1_546
Ga2 O2 Ga3 150.8(3) 2_566 1_546
Ga2 O2 Ga3 136.8(5) . 1_656
Ga3 O2 Ga3 21.4(2) 4_446 1_656
La O2 Ga3 113.9(2) 4_445 1_656
O2 O2 Ga3 164.7(3) 4_445 1_656
O2 O2 Ga3 129.3(4) 3_455 1_656
La O2 Ga3 95.3(2) . 1_656
O3 O2 Ga3 46.8(2) 3_565 1_656
O3 O2 Ga3 22.6(3) 4_445 1_656
O2 O2 Ga3 57.80(12) 2_556 1_656
O1 O2 Ga3 131.5(4) 2_455 1_656
O3 O2 Ga3 47.14(19) 5_446 1_656
O1 O2 Ga3 108.6(3) 2_456 1_656
O3 O2 Ga3 72.2(2) 5_445 1_656
O1 O2 Ga3 74.69(15) 1_545 1_656
Nb O2 Ga3 39.65(7) . 1_656
Ga1 O2 Ga3 39.65(7) . 1_656
Ga2 O2 Ga3 69.60(12) 2_556 1_656
O2 O2 Ga3 81.90(15) 2 1_656
O3 O2 Ga3 122.8(2) 1_545 1_656
La O2 Ga3 89.8(2) 4_446 1_656
Ga3 O2 Ga3 144.7(3) 2_455 1_656
Ga3 O2 Ga3 41.07(7) 2_565 1_656
La O2 Ga3 79.99(15) 1_556 1_656
O3 O2 Ga3 120.1(3) 2_456 1_656
La O2 Ga3 163.3(3) 2_455 1_656
Ga3 O2 Ga3 119.20(18) 1_556 1_656
Ga3 O2 Ga3 80.31(14) 4_445 1_656
O3 O2 Ga3 21.39(13) 6_656 1_656
O3 O2 Ga3 133.7(2) 2_455 1_656
Ga2 O2 Ga3 120.6(2) 1_554 1_656
O2 O2 Ga3 89.3(2) 5_446 1_656
O2 O2 Ga3 95.8(2) 5_456 1_656
La O2 Ga3 48.65(7) 2 1_656
O3 O2 Ga3 48.29(17) 6_655 1_656
O2 O2 Ga3 61.53(9) 6_556 1_656
O1 O2 Ga3 84.86(14) . 1_656
Ga1 O2 Ga3 37.87(6) 1_556 1_656
Nb O2 Ga3 37.87(6) 1_556 1_656
O3 O2 Ga3 21.34(12) 1_655 1_656
Ga2 O2 Ga3 80.89(12) 2_566 1_656
Ga3 O2 Ga3 109.33(17) 1_546 1_656
Ga2 O2 O2 117.4(4) . 1_554
Ga3 O2 O2 121.5(4) 4_446 1_554
La O2 O2 49.9(3) 4_445 1_554
O2 O2 O2 90.000(1) 4_445 1_554
O2 O2 O2 90.000(1) 3_455 1_554
La O2 O2 56.7(2) . 1_554
O3 O2 O2 83.2(4) 3_565 1_554
O3 O2 O2 83.1(4) 4_445 1_554
O2 O2 O2 132.8(4) 2_556 1_554
O1 O2 O2 32.6(3) 2_455 1_554
O3 O2 O2 140.0(3) 5_446 1_554
O1 O2 O2 148.2(3) 2_456 1_554
O3 O2 O2 34.6(2) 5_445 1_554
O1 O2 O2 79.9(4) 1_545 1_554
Nb O2 O2 64.45(19) . 1_554
Ga1 O2 O2 64.45(19) . 1_554
Ga2 O2 O2 107.69(19) 2_556 1_554
O2 O2 O2 34.0(3) 2 1_554
O3 O2 O2 85.0(3) 1_545 1_554
La O2 O2 152.14(12) 4_446 1_554
Ga3 O2 O2 103.40(17) 2_455 1_554
Ga3 O2 O2 103.42(18) 2_565 1_554
La O2 O2 145.89(15) 1_556 1_554
O3 O2 O2 122.7(2) 2_456 1_554
La O2 O2 68.63(17) 2_455 1_554
Ga3 O2 O2 102.75(17) 1_556 1_554
Ga3 O2 O2 21.22(10) 4_445 1_554
O3 O2 O2 121.1(2) 6_656 1_554
O3 O2 O2 52.0(2) 2_455 1_554
Ga2 O2 O2 20.62(10) 1_554 1_554
O2 O2 O2 115.5(3) 5_446 1_554
O2 O2 O2 115.5(3) 5_456 1_554
La O2 O2 69.94(16) 2 1_554
O3 O2 O2 53.8(2) 6_655 1_554
O2 O2 O2 114.4(3) 6_556 1_554
O1 O2 O2 82.5(3) . 1_554
Ga1 O2 O2 137.06(13) 1_556 1_554
Nb O2 O2 137.06(13) 1_556 1_554
O3 O2 O2 86.0(2) 1_655 1_554
Ga2 O2 O2 103.27(16) 2_566 1_554
Ga3 O2 O2 101.33(15) 1_546 1_554
Ga3 O2 O2 101.34(15) 1_656 1_554
Ga2 O2 O2 62.6(4) . 1_556
Ga3 O2 O2 58.5(4) 4_446 1_556
La O2 O2 130.1(3) 4_445 1_556
O2 O2 O2 90.000(1) 4_445 1_556
O2 O2 O2 90.000(2) 3_455 1_556
La O2 O2 123.3(2) . 1_556
O3 O2 O2 96.8(4) 3_565 1_556
O3 O2 O2 96.9(4) 4_445 1_556
O2 O2 O2 47.2(4) 2_556 1_556
O1 O2 O2 147.4(3) 2_455 1_556
O3 O2 O2 40.0(3) 5_446 1_556
O1 O2 O2 31.8(3) 2_456 1_556
O3 O2 O2 145.4(2) 5_445 1_556
O1 O2 O2 100.1(4) 1_545 1_556
Nb O2 O2 115.55(19) . 1_556
Ga1 O2 O2 115.55(19) . 1_556
Ga2 O2 O2 72.31(19) 2_556 1_556
O2 O2 O2 146.0(3) 2 1_556
O3 O2 O2 95.0(3) 1_545 1_556
La O2 O2 27.86(12) 4_446 1_556
Ga3 O2 O2 76.60(17) 2_455 1_556
Ga3 O2 O2 76.58(18) 2_565 1_556
La O2 O2 34.11(15) 1_556 1_556
O3 O2 O2 57.3(2) 2_456 1_556
La O2 O2 111.37(17) 2_455 1_556
Ga3 O2 O2 77.25(17) 1_556 1_556
Ga3 O2 O2 158.78(10) 4_445 1_556
O3 O2 O2 58.9(2) 6_656 1_556
O3 O2 O2 128.0(2) 2_455 1_556
Ga2 O2 O2 159.38(10) 1_554 1_556
O2 O2 O2 64.5(3) 5_446 1_556
O2 O2 O2 64.5(3) 5_456 1_556
La O2 O2 110.06(16) 2 1_556
O3 O2 O2 126.2(2) 6_655 1_556
O2 O2 O2 65.6(3) 6_556 1_556
O1 O2 O2 97.5(3) . 1_556
Ga1 O2 O2 42.94(13) 1_556 1_556
Nb O2 O2 42.94(13) 1_556 1_556
O3 O2 O2 94.0(2) 1_655 1_556
Ga2 O2 O2 76.73(16) 2_566 1_556
Ga3 O2 O2 78.67(15) 1_546 1_556
Ga3 O2 O2 78.66(15) 1_656 1_556
O2 O2 O2 179.999(3) 1_554 1_556
Ga2 O2 O3 18.55(19) . 6_556
Ga3 O2 O3 114.1(4) 4_446 6_556
La O2 O3 120.5(2) 4_445 6_556
O2 O2 O3 55.5(2) 4_445 6_556
O2 O2 O3 27.90(18) 3_455 6_556
La O2 O3 76.70(19) . 6_556
O3 O2 O3 98.5(3) 3_565 6_556
O3 O2 O3 147.7(3) 4_445 6_556
O2 O2 O3 109.2(5) 2_556 6_556
O1 O2 O3 85.7(3) 2_455 6_556
O3 O2 O3 79.8(3) 5_446 6_556
O1 O2 O3 34.9(2) 2_456 6_556
O3 O2 O3 120.8(3) 5_445 6_556
O1 O2 O3 146.1(3) 1_545 6_556
Nb O2 O3 130.6(2) . 6_556
Ga1 O2 O3 130.6(2) . 6_556
Ga2 O2 O3 126.3(3) 2_556 6_556
O2 O2 O3 148.3(4) 2 6_556
O3 O2 O3 99.5(3) 1_545 6_556
La O2 O3 75.0(2) 4_446 6_556
Ga3 O2 O3 62.69(14) 2_455 6_556
Ga3 O2 O3 90.53(17) 2_565 6_556
La O2 O3 46.58(15) 1_556 6_556
O3 O2 O3 70.6(2) 2_456 6_556
La O2 O3 54.31(16) 2_455 6_556
Ga3 O2 O3 20.16(11) 1_556 6_556
Ga3 O2 O3 133.4(3) 4_445 6_556
O3 O2 O3 115.1(3) 6_656 6_556
O3 O2 O3 100.87(13) 2_455 6_556
Ga2 O2 O3 97.0(2) 1_554 6_556
O2 O2 O3 106.3(4) 5_446 6_556
O2 O2 O3 33.50(15) 5_456 6_556
La O2 O3 173.1(3) 2 6_556
O3 O2 O3 151.5(3) 6_655 6_556
O2 O2 O3 67.40(17) 6_556 6_556
O1 O2 O3 64.25(19) . 6_556
Ga1 O2 O3 91.1(2) 1_556 6_556
Nb O2 O3 91.1(2) 1_556 6_556
O3 O2 O3 122.59(18) 1_655 6_556
Ga2 O2 O3 54.14(11) 2_566 6_556
Ga3 O2 O3 100.50(19) 1_546 6_556
Ga3 O2 O3 125.4(2) 1_656 6_556
O2 O2 O3 116.46(19) 1_554 6_556
O2 O2 O3 63.54(19) 1_556 6_556
Ga2 O2 O2 117.5(4) . 5_445
Ga3 O2 O2 106.4(2) 4_446 5_445
La O2 O2 13.57(9) 4_445 5_445
O2 O2 O2 78.2(4) 4_445 5_445
O2 O2 O2 124.2(3) 3_455 5_445
La O2 O2 109.3(4) . 5_445
O3 O2 O2 121.0(5) 3_565 5_445
O3 O2 O2 78.8(3) 4_445 5_445
O2 O2 O2 87.5(2) 2_556 5_445
O1 O2 O2 66.4(3) 2_455 5_445
O3 O2 O2 140.9(3) 5_446 5_445
O1 O2 O2 128.6(3) 2_456 5_445
O3 O2 O2 77.0(3) 5_445 5_445
O1 O2 O2 34.1(3) 1_545 5_445
Nb O2 O2 88.8(3) . 5_445
Ga1 O2 O2 88.8(3) . 5_445
Ga2 O2 O2 59.07(7) 2_556 5_445
O2 O2 O2 31.63(17) 2 5_445
O3 O2 O2 41.1(2) 1_545 5_445
La O2 O2 100.5(2) 4_446 5_445
Ga3 O2 O2 75.72(17) 2_455 5_445
Ga3 O2 O2 134.7(3) 2_565 5_445
La O2 O2 161.3(4) 1_556 5_445
O3 O2 O2 80.6(2) 2_456 5_445
La O2 O2 84.2(2) 2_455 5_445
Ga3 O2 O2 137.8(3) 1_556 5_445
Ga3 O2 O2 54.5(2) 4_445 5_445
O3 O2 O2 105.18(18) 6_656 5_445
O3 O2 O2 33.57(17) 2_455 5_445
Ga2 O2 O2 60.3(2) 1_554 5_445
O2 O2 O2 62.87(7) 5_446 5_445
O2 O2 O2 161.4(4) 5_456 5_445
La O2 O2 52.00(12) 2 5_445
O3 O2 O2 66.0(2) 6_655 5_445
O2 O2 O2 157.4(4) 6_556 5_445
O1 O2 O2 135.1(5) . 5_445
Ga1 O2 O2 128.8(2) 1_556 5_445
Nb O2 O2 128.8(2) 1_556 5_445
O3 O2 O2 102.9(3) 1_655 5_445
Ga2 O2 O2 155.8(4) 2_566 5_445
Ga3 O2 O2 51.53(11) 1_546 5_445
Ga3 O2 O2 100.55(17) 1_656 5_445
O2 O2 O2 52.6(2) 1_554 5_445
O2 O2 O2 127.4(2) 1_556 5_445
O3 O2 O2 133.4(3) 6_556 5_445
Ga2 O2 O2 84.7(3) . 5_455
Ga3 O2 O2 123.1(4) 4_446 5_455
La O2 O2 96.6(5) 4_445 5_455
O2 O2 O2 88.6(2) 4_445 5_455
O2 O2 O2 45.5(2) 3_455 5_455
La O2 O2 11.54(3) . 5_455
O3 O2 O2 61.2(3) 3_565 5_455
O3 O2 O2 105.6(4) 4_445 5_455
O2 O2 O2 162.7(2) 2_556 5_455
O1 O2 O2 42.5(2) 2_455 5_455
O3 O2 O2 106.5(3) 5_446 5_455
O1 O2 O2 107.2(2) 2_456 5_455
O3 O2 O2 48.8(3) 5_445 5_455
O1 O2 O2 132.2(6) 1_545 5_455
Nb O2 O2 72.7(3) . 5_455
Ga1 O2 O2 72.7(3) . 5_455
Ga2 O2 O2 159.6(4) 2_556 5_455
O2 O2 O2 84.8(5) 2 5_455
O3 O2 O2 120.7(4) 1_545 5_455
La O2 O2 147.7(3) 4_446 5_455
Ga3 O2 O2 108.6(2) 2_455 5_455
Ga3 O2 O2 75.82(14) 2_565 5_455
La O2 O2 93.95(14) 1_556 5_455
O3 O2 O2 131.8(2) 2_456 5_455
La O2 O2 56.87(17) 2_455 5_455
Ga3 O2 O2 54.09(8) 1_556 5_455
Ga3 O2 O2 62.1(3) 4_445 5_455
O3 O2 O2 123.9(2) 6_656 5_455
O3 O2 O2 86.8(3) 2_455 5_455
Ga2 O2 O2 44.3(2) 1_554 5_455
O2 O2 O2 161.4(4) 5_446 5_455
O2 O2 O2 62.87(7) 5_456 5_455
La O2 O2 111.3(4) 2 5_455
O3 O2 O2 82.7(3) 6_655 5_455
O2 O2 O2 71.52(16) 6_556 5_455
O1 O2 O2 34.5(2) . 5_455
Ga1 O2 O2 114.70(18) 1_556 5_455
Nb O2 O2 114.70(18) 1_556 5_455
O3 O2 O2 85.4(2) 1_655 5_455
Ga2 O2 O2 53.67(8) 2_566 5_455
Ga3 O2 O2 139.4(3) 1_546 5_455
Ga3 O2 O2 106.4(2) 1_656 5_455
O2 O2 O2 52.6(2) 1_554 5_455
O2 O2 O2 127.4(2) 1_556 5_455
O3 O2 O2 72.85(18) 6_556 5_455
O2 O2 O2 103.7(5) 5_445 5_455
Ga2 O2 O3 110.0(4) . 2_566
Ga3 O2 O3 30.5(2) 4_446 2_566
La O2 O3 143.2(3) 4_445 2_566
O2 O2 O3 149.1(2) 4_445 2_566
O2 O2 O3 102.0(4) 3_455 2_566
La O2 O3 83.9(2) . 2_566
O3 O2 O3 37.0(4) 3_565 2_566
O3 O2 O3 51.4(4) 4_445 2_566
O2 O2 O3 67.6(2) 2_556 2_566
O1 O2 O3 135.0(3) 2_455 2_566
O3 O2 O3 23.98(16) 5_446 2_566
O1 O2 O3 86.9(3) 2_456 2_566
O3 O2 O3 82.04(18) 5_445 2_566
O1 O2 O3 102.4(3) 1_545 2_566
Nb O2 O3 53.29(17) . 2_566
Ga1 O2 O3 53.29(17) . 2_566
Ga2 O2 O3 89.8(2) 2_556 2_566
O2 O2 O3 108.07(17) 2 2_566
O3 O2 O3 143.7(3) 1_545 2_566
La O2 O3 85.4(2) 4_446 2_566
Ga3 O2 O3 140.1(3) 2_455 2_566
Ga3 O2 O3 19.30(11) 2_565 2_566
La O2 O3 52.77(16) 1_556 2_566
O3 O2 O3 119.0(4) 2_456 2_566
La O2 O3 142.5(2) 2_455 2_566
Ga3 O2 O3 90.35(18) 1_556 2_566
Ga3 O2 O3 98.6(2) 4_445 2_566
O3 O2 O3 31.64(14) 6_656 2_566
O3 O2 O3 162.5(3) 2_455 2_566
Ga2 O2 O3 129.3(3) 1_554 2_566
O2 O2 O3 103.4(3) 5_446 2_566
O2 O2 O3 66.6(2) 5_456 2_566
La O2 O3 78.04(15) 2 2_566
O3 O2 O3 71.21(10) 6_655 2_566
O2 O2 O3 33.22(13) 6_556 2_566
O1 O2 O3 64.27(19) . 2_566
Ga1 O2 O3 22.64(13) 1_556 2_566
Nb O2 O3 22.64(13) 1_556 2_566
O3 O2 O3 32.6(3) 1_655 2_566
Ga2 O2 O3 54.16(13) 2_566 2_566
Ga3 O2 O3 125.4(2) 1_546 2_566
Ga3 O2 O3 29.48(12) 1_656 2_566
O2 O2 O3 116.48(19) 1_554 2_566
O2 O2 O3 63.52(19) 1_556 2_566
O3 O2 O3 96.3(3) 6_556 2_566
O2 O2 O3 130.0(2) 5_445 2_566
O2 O2 O3 95.12(18) 5_455 2_566
Ga2 O2 O2 25.25(13) . 6_446
Ga3 O2 O2 124.7(6) 4_446 6_446
La O2 O2 83.9(2) 4_445 6_446
O2 O2 O2 22.0(3) 4_445 6_446
O2 O2 O2 59.78(14) 3_455 6_446
La O2 O2 108.67(18) . 6_446
O3 O2 O2 142.3(3) 3_565 6_446
O3 O2 O2 154.8(5) 4_445 6_446
O2 O2 O2 92.8(4) 2_556 6_446
O1 O2 O2 82.4(3) 2_455 6_446
O3 O2 O2 104.7(4) 5_446 6_446
O1 O2 O2 41.3(2) 2_456 6_446
O3 O2 O2 141.5(4) 5_445 6_446
O1 O2 O2 103.5(3) 1_545 6_446
Nb O2 O2 172.2(3) . 6_446
Ga1 O2 O2 172.2(3) . 6_446
Ga2 O2 O2 92.8(3) 2_556 6_446
O2 O2 O2 122.6(3) 2 6_446
O3 O2 O2 55.9(2) 1_545 6_446
La O2 O2 57.3(3) 4_446 6_446
Ga3 O2 O2 19.04(10) 2_455 6_446
Ga3 O2 O2 131.1(3) 2_565 6_446
La O2 O2 76.7(3) 1_556 6_446
O3 O2 O2 32.84(19) 2_456 6_446
La O2 O2 48.00(9) 2_455 6_446
Ga3 O2 O2 61.11(9) 1_556 6_446
Ga3 O2 O2 132.2(3) 4_445 6_446
O3 O2 O2 124.8(4) 6_656 6_446
O3 O2 O2 68.3(2) 2_455 6_446
Ga2 O2 O2 93.3(2) 1_554 6_446
O2 O2 O2 70.4(3) 5_446 6_446
O2 O2 O2 76.8(2) 5_456 6_446
La O2 O2 137.9(3) 2 6_446
O3 O2 O2 159.7(3) 6_655 6_446
O2 O2 O2 108.4(3) 6_556 6_446
O1 O2 O2 105.97(17) . 6_446
Ga1 O2 O2 110.8(4) 1_556 6_446
Nb O2 O2 110.8(4) 1_556 6_446
O3 O2 O2 160.8(4) 1_655 6_446
Ga2 O2 O2 97.88(17) 2_566 6_446
Ga3 O2 O2 58.06(19) 1_546 6_446
Ga3 O2 O2 146.0(4) 1_656 6_446
O2 O2 O2 111.8(3) 1_554 6_446
O2 O2 O2 68.2(3) 1_556 6_446
O3 O2 O2 43.76(12) 6_556 6_446
O2 O2 O2 94.1(3) 5_445 6_446
O2 O2 O2 99.55(15) 5_455 6_446
O3 O2 O2 128.1(4) 2_566 6_446
Ga2 O2 O2 117.2(6) . 6_546
Ga3 O2 O2 47.32(18) 4_446 6_546
La O2 O2 78.4(2) 4_445 6_546
O2 O2 O2 108.2(4) 4_445 6_546
O2 O2 O2 156.0(3) 3_455 6_546
La O2 O2 150.3(3) . 6_546
O3 O2 O2 104.9(2) 3_565 6_546
O3 O2 O2 53.87(18) 4_445 6_546
O2 O2 O2 21.20(19) 2_556 6_546
O1 O2 O2 134.0(4) 2_455 6_546
O3 O2 O2 75.2(3) 5_446 6_546
O1 O2 O2 93.3(4) 2_456 6_546
O3 O2 O2 109.4(2) 5_445 6_546
O1 O2 O2 34.0(3) 1_545 6_546
Nb O2 O2 86.73(10) . 6_546
Ga1 O2 O2 86.73(10) . 6_546
Ga2 O2 O2 11.99(9) 2_556 6_546
O2 O2 O2 77.9(2) 2 6_546
O3 O2 O2 66.7(2) 1_545 6_546
La O2 O2 53.3(3) 4_446 6_546
Ga3 O2 O2 89.2(3) 2_455 6_546
Ga3 O2 O2 95.88(18) 2_565 6_546
La O2 O2 97.9(3) 1_556 6_546
O3 O2 O2 68.2(3) 2_456 6_546
La O2 O2 137.4(3) 2_455 6_546
Ga3 O2 O2 145.2(4) 1_556 6_546
Ga3 O2 O2 98.1(2) 4_445 6_546
O3 O2 O2 46.21(14) 6_656 6_546
O3 O2 O2 94.0(2) 2_455 6_546
Ga2 O2 O2 126.7(3) 1_554 6_546
O2 O2 O2 31.86(17) 5_446 6_546
O2 O2 O2 129.6(5) 5_456 6_546
La O2 O2 47.21(9) 2 6_546
O3 O2 O2 75.44(18) 6_655 6_546
O2 O2 O2 108.4(3) 6_556 6_546
O1 O2 O2 141.8(3) . 6_546
Ga1 O2 O2 64.1(2) 1_556 6_546
Nb O2 O2 64.1(2) 1_556 6_546
O3 O2 O2 77.58(13) 1_655 6_546
Ga2 O2 O2 129.7(3) 2_566 6_546
Ga3 O2 O2 51.24(18) 1_546 6_546
Ga3 O2 O2 58.14(8) 1_656 6_546
O2 O2 O2 111.8(3) 1_554 6_546
O2 O2 O2 68.2(3) 1_556 6_546
O3 O2 O2 128.1(4) 6_556 6_546
O2 O2 O2 67.61(9) 5_445 6_546
O2 O2 O2 158.1(4) 5_455 6_546
O3 O2 O2 77.83(19) 2_566 6_546
O2 O2 O2 101.1(4) 6_446 6_546
Ga2 O2 La 14.7(3) . 2_456
Ga3 O2 La 106.9(4) 4_446 2_456
La O2 La 110.3(2) 4_445 2_456
O2 O2 La 46.81(13) 4_445 2_456
O2 O2 La 52.46(12) 3_455 2_456
La O2 La 102.90(18) . 2_456
O3 O2 La 118.8(3) 3_565 2_456
O3 O2 La 145.5(5) 4_445 2_456
O2 O2 La 87.6(4) 2_556 2_456
O1 O2 La 98.9(3) 2_455 2_456
O3 O2 La 79.9(3) 5_446 2_456
O1 O2 La 17.2(2) 2_456 2_456
O3 O2 La 146.7(3) 5_445 2_456
O1 O2 La 120.5(4) 1_545 2_456
Nb O2 La 151.4(2) . 2_456
Ga1 O2 La 151.4(2) . 2_456
Ga2 O2 La 100.3(3) 2_556 2_456
O2 O2 La 149.10(13) 2 2_456
O3 O2 La 79.7(3) 1_545 2_456
La O2 La 50.84(12) 4_446 2_456
Ga3 O2 La 44.13(10) 2_455 2_456
Ga3 O2 La 104.8(2) 2_565 2_456
La O2 La 50.17(11) 1_556 2_456
O3 O2 La 45.13(17) 2_456 2_456
La O2 La 62.72(10) 2_455 2_456
Ga3 O2 La 46.57(9) 1_556 2_456
Ga3 O2 La 152.4(2) 4_445 2_456
O3 O2 La 107.5(3) 6_656 2_456
O3 O2 La 94.57(18) 2_455 2_456
Ga2 O2 La 110.80(14) 1_554 2_456
O2 O2 La 79.9(3) 5_446 2_456
O2 O2 La 54.4(2) 5_456 2_456
La O2 La 150.7(3) 2 2_456
O3 O2 La 173.6(3) 6_655 2_456
O2 O2 La 82.7(2) 6_556 2_456
O1 O2 La 89.6(2) . 2_456
Ga1 O2 La 87.9(2) 1_556 2_456
Nb O2 La 87.9(2) 1_556 2_456
O3 O2 La 134.6(3) 1_655 2_456
Ga2 O2 La 75.95(12) 2_566 2_456
Ga3 O2 La 76.09(15) 1_546 2_456
Ga3 O2 La 125.8(2) 1_656 2_456
O2 O2 La 131.35(12) 1_554 2_456
O2 O2 La 48.65(12) 1_556 2_456
O3 O2 La 26.41(11) 6_556 2_456
O2 O2 La 119.8(2) 5_445 2_456
O2 O2 La 97.97(16) 5_455 2_456
O3 O2 La 102.3(2) 2_566 2_456
O2 O2 La 26.56(14) 6_446 2_456
O2 O2 La 103.8(3) 6_546 2_456
Ga2 O2 Ga2 134.8(4) . 2
Ga3 O2 Ga2 98.3(3) 4_446 2
La O2 Ga2 29.32(14) 4_445 2
O2 O2 Ga2 95.1(3) 4_445 2
O2 O2 Ga2 127.99(12) 3_455 2
La O2 Ga2 96.6(3) . 2
O3 O2 Ga2 101.2(4) 3_565 2
O3 O2 Ga2 64.3(3) 4_445 2
O2 O2 Ga2 92.2(3) 2_556 2
O1 O2 Ga2 65.8(3) 2_455 2
O3 O2 Ga2 132.9(2) 5_446 2
O1 O2 Ga2 148.1(3) 2_456 2
O3 O2 Ga2 58.8(2) 5_445 2
O1 O2 Ga2 38.2(4) 1_545 2
Nb O2 Ga2 69.24(16) . 2
Ga1 O2 Ga2 69.24(16) . 2
Ga2 O2 Ga2 66.00(12) 2_556 2
O2 O2 Ga2 12.29(11) 2 2
O3 O2 Ga2 60.8(2) 1_545 2
La O2 Ga2 114.91(18) 4_446 2
Ga3 O2 Ga2 95.17(16) 2_455 2
Ga3 O2 Ga2 115.90(19) 2_565 2
La O2 Ga2 166.07(19) 1_556 2
O3 O2 Ga2 99.8(2) 2_456 2
La O2 Ga2 93.21(19) 2_455 2
Ga3 O2 Ga2 142.1(3) 1_556 2
Ga3 O2 Ga2 36.83(8) 4_445 2
O3 O2 Ga2 97.26(17) 6_656 2
O3 O2 Ga2 47.40(15) 2_455 2
Ga2 O2 Ga2 56.25(13) 1_554 2
O2 O2 Ga2 76.6(2) 5_446 2
O2 O2 Ga2 156.7(4) 5_456 2
La O2 Ga2 39.40(8) 2 2
O3 O2 Ga2 46.79(14) 6_655 2
O2 O2 Ga2 137.9(3) 6_556 2
O1 O2 Ga2 120.1(4) . 2
Ga1 O2 Ga2 121.48(13) 1_556 2
Nb O2 Ga2 121.48(13) 1_556 2
O3 O2 Ga2 84.9(2) 1_655 2
Ga2 O2 Ga2 139.4(3) 2_566 2
Ga3 O2 Ga2 69.62(11) 1_546 2
Ga3 O2 Ga2 86.86(12) 1_656 2
O2 O2 Ga2 41.69(13) 1_554 2
O2 O2 Ga2 138.31(13) 1_556 2
O3 O2 Ga2 147.2(2) 6_556 2
O2 O2 Ga2 19.79(13) 5_445 2
O2 O2 Ga2 94.2(4) 5_455 2
O3 O2 Ga2 115.13(18) 2_566 2
O2 O2 Ga2 113.0(2) 6_446 2
O2 O2 Ga2 70.96(18) 6_546 2
La O2 Ga2 139.27(16) 2_456 2
Ga2 O2 O2 110.6(3) . 6
Ga3 O2 O2 95.0(3) 4_446 6
La O2 O2 103.8(5) 4_445 6
O2 O2 O2 118.8(2) 4_445 6
O2 O2 O2 71.2(3) 3_455 6
La O2 O2 20.80(15) . 6
O3 O2 O2 34.6(3) 3_565 6
O3 O2 O2 75.6(3) 4_445 6
O2 O2 O2 134.10(5) 2_556 6
O1 O2 O2 63.6(3) 2_455 6
O3 O2 O2 90.2(3) 5_446 6
O1 O2 O2 123.2(3) 2_456 6
O3 O2 O2 28.63(19) 5_445 6
O1 O2 O2 117.9(4) 1_545 6
Nb O2 O2 42.74(15) . 6
Ga1 O2 O2 42.74(15) . 6
Ga2 O2 O2 136.91(18) 2_556 6
O2 O2 O2 74.9(4) 2 6
O3 O2 O2 138.6(5) 1_545 6
La O2 O2 153.7(3) 4_446 6
Ga3 O2 O2 138.9(2) 2_455 6
Ga3 O2 O2 53.46(14) 2_565 6
La O2 O2 94.3(2) 1_556 6
O3 O2 O2 162.24(15) 2_456 6
La O2 O2 86.9(2) 2_455 6
Ga3 O2 O2 74.65(13) 1_556 6
Ga3 O2 O2 50.1(2) 4_445 6
O3 O2 O2 95.55(19) 6_656 6
O3 O2 O2 103.5(4) 2_455 6
Ga2 O2 O2 58.9(2) 1_554 6
O2 O2 O2 158.8(3) 5_446 6
O2 O2 O2 71.34(18) 5_456 6
La O2 O2 87.1(2) 2 6
O3 O2 O2 57.25(19) 6_655 6
O2 O2 O2 60.3(2) 6_556 6
O1 O2 O2 33.6(2) . 6
Ga1 O2 O2 93.82(19) 1_556 6
Nb O2 O2 93.82(19) 1_556 6
O3 O2 O2 55.06(15) 1_655 6
Ga2 O2 O2 52.56(14) 2_566 6
Ga3 O2 O2 155.1(4) 1_546 6
Ga3 O2 O2 76.35(12) 1_656 6
O2 O2 O2 54.0(2) 1_554 6
O2 O2 O2 126.0(2) 1_556 6
O3 O2 O2 94.79(16) 6_556 6
O2 O2 O2 104.0(4) 5_445 6
O2 O2 O2 30.62(17) 5_455 6
O3 O2 O2 71.45(19) 2_566 6
O2 O2 O2 129.5(2) 6_446 6
O2 O2 O2 129.5(2) 6_546 6
La O2 O2 121.17(14) 2_456 6
Ga2 O2 O2 86.9(3) 2 6
Ga2 O2 O3 55.9(2) . 3_455
Ga3 O2 O3 136.0(5) 4_446 3_455
La O2 O3 51.02(18) 4_445 3_455
O2 O2 O3 18.7(3) 4_445 3_455
O2 O2 O3 78.3(3) 3_455 3_455
La O2 O3 112.2(3) . 3_455
O3 O2 O3 161.9(5) 3_565 3_455
O3 O2 O3 136.7(3) 4_445 3_455
O2 O2 O3 96.25(18) 2_556 3_455
O1 O2 O3 65.7(2) 2_455 3_455
O3 O2 O3 133.5(4) 5_446 3_455
O1 O2 O3 72.8(2) 2_456 3_455
O3 O2 O3 120.8(3) 5_445 3_455
O1 O2 O3 78.96(17) 1_545 3_455
Nb O2 O3 147.9(3) . 3_455
Ga1 O2 O3 147.9(3) . 3_455
Ga2 O2 O3 81.08(19) 2_556 3_455
O2 O2 O3 89.82(19) 2 3_455
O3 O2 O3 28.9(2) 1_545 3_455
La O2 O3 72.4(2) 4_446 3_455
Ga3 O2 O3 17.36(14) 2_455 3_455
Ga3 O2 O3 163.5(2) 2_565 3_455
La O2 O3 109.3(2) 1_556 3_455
O3 O2 O3 38.7(3) 2_456 3_455
La O2 O3 44.95(13) 2_455 3_455
Ga3 O2 O3 85.79(14) 1_556 3_455
Ga3 O2 O3 103.4(2) 4_445 3_455
O3 O2 O3 135.3(3) 6_656 3_455
O3 O2 O3 36.6(3) 2_455 3_455
Ga2 O2 O3 72.93(19) 1_554 3_455
O2 O2 O3 62.2(2) 5_446 3_455
O2 O2 O3 106.4(2) 5_456 3_455
La O2 O3 110.74(18) 2 3_455
O3 O2 O3 126.9(2) 6_655 3_455
O2 O2 O3 140.3(2) 6_556 3_455
O1 O2 O3 124.39(19) . 3_455
Ga1 O2 O3 135.0(3) 1_556 3_455
Nb O2 O3 135.0(3) 1_556 3_455
O3 O2 O3 164.3(3) 1_655 3_455
Ga2 O2 O3 125.26(16) 2_566 3_455
Ga3 O2 O3 41.41(13) 1_546 3_455
Ga3 O2 O3 150.7(2) 1_656 3_455
O2 O2 O3 86.3(2) 1_554 3_455
O2 O2 O3 93.7(2) 1_556 3_455
O3 O2 O3 73.13(18) 6_556 3_455
O2 O2 O3 61.72(18) 5_445 3_455
O2 O2 O3 100.7(3) 5_455 3_455
O3 O2 O3 157.1(3) 2_566 3_455
O2 O2 O3 32.84(17) 6_446 3_455
O2 O2 O3 92.6(3) 6_546 3_455
La O2 O3 59.36(15) 2_456 3_455
Ga2 O2 O3 80.24(17) 2 3_455
O2 O2 O3 128.5(3) 6 3_455
Ga2 O2 Ga1 77.3(3) . 1_445
Ga3 O2 Ga1 129.8(3) 4_446 1_445
La O2 Ga1 30.27(13) 4_445 1_445
O2 O2 Ga1 38.7(3) 4_445 1_445
O2 O2 Ga1 95.1(3) 3_455 1_445
La O2 Ga1 114.9(3) . 1_445
O3 O2 Ga1 156.1(5) 3_565 1_445
O3 O2 Ga1 116.9(3) 4_445 1_445
O2 O2 Ga1 93.11(13) 2_556 1_445
O1 O2 Ga1 62.51(15) 2_455 1_445
O3 O2 Ga1 145.4(4) 5_446 1_445
O1 O2 Ga1 92.2(2) 2_456 1_445
O3 O2 Ga1 106.8(3) 5_445 1_445
O1 O2 Ga1 60.84(15) 1_545 1_445
Nb O2 Ga1 128.0(3) . 1_445
Ga1 O2 Ga1 128.0(3) . 1_445
Ga2 O2 Ga1 70.54(13) 2_556 1_445
O2 O2 Ga1 69.35(12) 2 1_445
O3 O2 Ga1 16.73(15) 1_545 1_445
La O2 Ga1 81.14(16) 4_446 1_445
Ga3 O2 Ga1 36.38(7) 2_455 1_445
Ga3 O2 Ga1 175.0(2) 2_565 1_445
La O2 Ga1 129.2(2) 1_556 1_445
O3 O2 Ga1 49.78(18) 2_456 1_445
La O2 Ga1 56.12(9) 2_455 1_445
Ga3 O2 Ga1 104.84(13) 1_556 1_445
Ga3 O2 Ga1 86.24(17) 4_445 1_445
O3 O2 Ga1 128.7(2) 6_656 1_445
O3 O2 Ga1 21.13(14) 2_455 1_445
Ga2 O2 Ga1 65.52(12) 1_554 1_445
O2 O2 Ga1 57.44(16) 5_446 1_445
O2 O2 Ga1 127.0(2) 5_456 1_445
La O2 Ga1 90.20(14) 2 1_445
O3 O2 Ga1 105.9(2) 6_655 1_445
O2 O2 Ga1 161.55(17) 6_556 1_445
O1 O2 Ga1 135.5(3) . 1_445
Ga1 O2 Ga1 140.7(3) 1_556 1_445
Nb O2 Ga1 140.7(3) 1_556 1_445
O3 O2 Ga1 143.1(2) 1_655 1_445
Ga2 O2 Ga1 143.58(15) 2_566 1_445
Ga3 O2 Ga1 35.59(6) 1_546 1_445
Ga3 O2 Ga1 135.52(15) 1_656 1_445
O2 O2 Ga1 73.00(14) 1_554 1_445
O2 O2 Ga1 107.00(14) 1_556 1_445
O3 O2 Ga1 94.15(16) 6_556 1_445
O2 O2 Ga1 40.35(12) 5_445 1_445
O2 O2 Ga1 104.0(3) 5_455 1_445
O3 O2 Ga1 160.2(2) 2_566 1_445
O2 O2 Ga1 53.90(16) 6_446 1_445
O2 O2 Ga1 82.5(2) 6_546 1_445
La O2 Ga1 80.19(12) 2_456 1_445
Ga2 O2 Ga1 59.14(10) 2 1_445
O2 O2 Ga1 124.3(3) 6 1_445
O3 O2 Ga1 21.37(10) 3_455 1_445
Ga2 O2 Nb 77.3(3) . 1_445
Ga3 O2 Nb 129.8(3) 4_446 1_445
La O2 Nb 30.27(13) 4_445 1_445
O2 O2 Nb 38.7(3) 4_445 1_445
O2 O2 Nb 95.1(3) 3_455 1_445
La O2 Nb 114.9(3) . 1_445
O3 O2 Nb 156.1(5) 3_565 1_445
O3 O2 Nb 116.9(3) 4_445 1_445
O2 O2 Nb 93.11(13) 2_556 1_445
O1 O2 Nb 62.51(15) 2_455 1_445
O3 O2 Nb 145.4(4) 5_446 1_445
O1 O2 Nb 92.2(2) 2_456 1_445
O3 O2 Nb 106.8(3) 5_445 1_445
O1 O2 Nb 60.84(15) 1_545 1_445
Nb O2 Nb 128.0(3) . 1_445
Ga1 O2 Nb 128.0(3) . 1_445
Ga2 O2 Nb 70.54(13) 2_556 1_445
O2 O2 Nb 69.35(12) 2 1_445
O3 O2 Nb 16.73(15) 1_545 1_445
La O2 Nb 81.14(16) 4_446 1_445
Ga3 O2 Nb 36.38(7) 2_455 1_445
Ga3 O2 Nb 175.0(2) 2_565 1_445
La O2 Nb 129.2(2) 1_556 1_445
O3 O2 Nb 49.78(18) 2_456 1_445
La O2 Nb 56.12(9) 2_455 1_445
Ga3 O2 Nb 104.84(13) 1_556 1_445
Ga3 O2 Nb 86.24(17) 4_445 1_445
O3 O2 Nb 128.7(2) 6_656 1_445
O3 O2 Nb 21.13(14) 2_455 1_445
Ga2 O2 Nb 65.52(12) 1_554 1_445
O2 O2 Nb 57.44(16) 5_446 1_445
O2 O2 Nb 127.0(2) 5_456 1_445
La O2 Nb 90.20(14) 2 1_445
O3 O2 Nb 105.9(2) 6_655 1_445
O2 O2 Nb 161.55(17) 6_556 1_445
O1 O2 Nb 135.5(3) . 1_445
Ga1 O2 Nb 140.7(3) 1_556 1_445
Nb O2 Nb 140.7(3) 1_556 1_445
O3 O2 Nb 143.1(2) 1_655 1_445
Ga2 O2 Nb 143.58(15) 2_566 1_445
Ga3 O2 Nb 35.59(6) 1_546 1_445
Ga3 O2 Nb 135.52(15) 1_656 1_445
O2 O2 Nb 73.00(14) 1_554 1_445
O2 O2 Nb 107.00(14) 1_556 1_445
O3 O2 Nb 94.15(16) 6_556 1_445
O2 O2 Nb 40.35(12) 5_445 1_445
O2 O2 Nb 104.0(3) 5_455 1_445
O3 O2 Nb 160.2(2) 2_566 1_445
O2 O2 Nb 53.90(16) 6_446 1_445
O2 O2 Nb 82.5(2) 6_546 1_445
La O2 Nb 80.19(12) 2_456 1_445
Ga2 O2 Nb 59.14(10) 2 1_445
O2 O2 Nb 124.3(3) 6 1_445
O3 O2 Nb 21.37(10) 3_455 1_445
Ga1 O2 Nb 0.0 1_445 1_445
Ga2 O2 O3 61.8(3) . 6
Ga3 O2 O3 152.1(4) 4_446 6
La O2 O3 83.0(3) 4_445 6
O2 O2 O3 57.27(18) 4_445 6
O2 O2 O3 32.37(17) 3_455 6
La O2 O3 42.45(14) . 6
O3 O2 O3 91.7(3) 3_565 6
O3 O2 O3 134.0(4) 4_445 6
O2 O2 O3 162.9(3) 2_556 6
O1 O2 O3 29.9(2) 2_455 6
O3 O2 O3 123.7(2) 5_446 6
O1 O2 O3 91.0(3) 2_456 6
O3 O2 O3 73.3(3) 5_445 6
O1 O2 O3 128.9(4) 1_545 6
Nb O2 O3 102.4(3) . 6
Ga1 O2 O3 102.4(3) . 6
Ga2 O2 O3 148.5(2) 2_556 6
O2 O2 O3 91.8(4) 2 6
O3 O2 O3 94.2(2) 1_545 6
La O2 O3 125.9(2) 4_446 6
Ga3 O2 O3 77.30(14) 2_455 6
Ga3 O2 O3 103.2(2) 2_565 6
La O2 O3 97.14(17) 1_556 6
O3 O2 O3 101.09(13) 2_456 6
La O2 O3 25.65(10) 2_455 6
Ga3 O2 O3 46.45(14) 1_556 6
Ga3 O2 O3 77.2(2) 4_445 6
O3 O2 O3 153.1(2) 6_656 6
O3 O2 O3 66.42(19) 2_455 6
Ga2 O2 O3 39.99(14) 1_554 6
O2 O2 O3 132.4(3) 5_446 6
O2 O2 O3 67.0(2) 5_456 6
La O2 O3 128.7(3) 2 6
O3 O2 O3 106.4(3) 6_655 6
O2 O2 O3 91.3(2) 6_556 6
O1 O2 O3 57.4(2) . 6
Ga1 O2 O3 135.20(19) 1_556 6
Nb O2 O3 135.20(19) 1_556 6
O3 O2 O3 116.6(2) 1_655 6
Ga2 O2 O3 69.92(14) 2_566 6
Ga3 O2 O3 111.08(16) 1_546 6
Ga3 O2 O3 137.7(2) 1_656 6
O2 O2 O3 58.83(16) 1_554 6
O2 O2 O3 121.17(16) 1_556 6
O3 O2 O3 57.64(11) 6_556 6
O2 O2 O3 94.8(3) 5_445 6
O2 O2 O3 31.29(13) 5_455 6
O3 O2 O3 121.7(2) 2_566 6
O2 O2 O3 70.17(16) 6_446 6
O2 O2 O3 160.3(3) 6_546 6
La O2 O3 76.55(13) 2_456 6
Ga2 O2 O3 95.7(2) 2 6
O2 O2 O3 61.69(17) 6 6
O3 O2 O3 70.27(16) 3_455 6
Ga1 O2 O3 78.07(14) 1_445 6
Nb O2 O3 78.07(14) 1_445 6
Ga2 O2 O3 33.5(3) . 4_345
Ga3 O2 O3 143.4(4) 4_446 4_345
La O2 O3 96.2(2) 4_445 4_345
O2 O2 O3 43.4(2) 4_445 4_345
O2 O2 O3 17.1(2) 3_455 4_345
La O2 O3 61.66(15) . 4_345
O3 O2 O3 103.1(2) 3_565 4_345
O3 O2 O3 157.9(4) 4_445 4_345
O2 O2 O3 135.7(5) 2_556 4_345
O1 O2 O3 54.8(3) 2_455 4_345
O3 O2 O3 108.2(2) 5_446 4_345
O1 O2 O3 62.7(3) 2_456 4_345
O3 O2 O3 100.4(3) 5_445 4_345
O1 O2 O3 138.8(3) 1_545 4_345
Nb O2 O3 125.2(3) . 4_345
Ga1 O2 O3 125.2(3) . 4_345
Ga2 O2 O3 139.3(2) 2_556 4_345
O2 O2 O3 117.4(4) 2 4_345
O3 O2 O3 90.20(14) 1_545 4_345
La O2 O3 98.4(2) 4_446 4_345
Ga3 O2 O3 60.36(12) 2_455 4_345
Ga3 O2 O3 105.40(17) 2_565 4_345
La O2 O3 75.95(18) 1_556 4_345
O3 O2 O3 79.9(2) 2_456 4_345
La O2 O3 25.61(13) 2_455 4_345
Ga3 O2 O3 28.33(12) 1_556 4_345
Ga3 O2 O3 105.5(3) 4_445 4_345
O3 O2 O3 144.5(3) 6_656 4_345
O3 O2 O3 76.4(2) 2_455 4_345
Ga2 O2 O3 66.34(18) 1_554 4_345
O2 O2 O3 117.0(3) 5_446 4_345
O2 O2 O3 52.36(18) 5_456 4_345
La O2 O3 155.9(3) 2 4_345
O3 O2 O3 134.3(3) 6_655 4_345
O2 O2 O3 85.42(14) 6_556 4_345
O1 O2 O3 63.60(12) . 4_345
Ga1 O2 O3 120.1(2) 1_556 4_345
Nb O2 O3 120.1(2) 1_556 4_345
O3 O2 O3 131.6(2) 1_655 4_345
Ga2 O2 O3 65.55(13) 2_566 4_345
Ga3 O2 O3 100.86(16) 1_546 4_345
Ga3 O2 O3 146.4(2) 1_656 4_345
O2 O2 O3 86.4(2) 1_554 4_345
O2 O2 O3 93.6(2) 1_556 4_345
O3 O2 O3 31.0(3) 6_556 4_345
O2 O2 O3 109.7(3) 5_445 4_345
O2 O2 O3 53.13(14) 5_455 4_345
O3 O2 O3 118.48(17) 2_566 4_345
O2 O2 O3 47.02(12) 6_446 4_345
O2 O2 O3 148.1(3) 6_546 4_345
La O2 O3 48.19(15) 2_456 4_345
Ga2 O2 O3 117.9(2) 2 4_345
O2 O2 O3 82.46(15) 6 4_345
O3 O2 O3 61.43(19) 3_455 4_345
Ga1 O2 O3 78.03(14) 1_445 4_345
Nb O2 O3 78.03(14) 1_445 4_345
O3 O2 O3 28.5(2) 6 4_345
Ga2 O2 O3 139.5(4) . 2_565
Ga3 O2 O3 70.7(3) 4_446 2_565
La O2 O3 99.1(3) 4_445 2_565
O2 O2 O3 145.1(2) 4_445 2_565
O2 O2 O3 101.4(3) 3_455 2_565
La O2 O3 51.67(18) . 2_565
O3 O2 O3 28.8(4) 3_565 2_565
O3 O2 O3 44.9(3) 4_445 2_565
O2 O2 O3 106.10(19) 2_556 2_565
O1 O2 O3 83.1(3) 2_455 2_565
O3 O2 O3 81.4(2) 5_446 2_565
O1 O2 O3 138.6(3) 2_456 2_565
O3 O2 O3 24.57(14) 5_445 2_565
O1 O2 O3 92.2(3) 1_545 2_565
Nb O2 O3 11.93(11) . 2_565
Ga1 O2 O3 11.93(11) . 2_565
Ga2 O2 O3 106.44(17) 2_556 2_565
O2 O2 O3 60.90(18) 2 2_565
O3 O2 O3 133.4(3) 1_545 2_565
La O2 O3 139.3(2) 4_446 2_565
Ga3 O2 O3 162.2(3) 2_455 2_565
Ga3 O2 O3 46.93(17) 2_565 2_565
La O2 O3 101.7(2) 1_556 2_565
O3 O2 O3 166.6(3) 2_456 2_565
La O2 O3 114.4(3) 2_455 2_565
Ga3 O2 O3 102.4(2) 1_556 2_565
Ga3 O2 O3 42.46(15) 4_445 2_565
O3 O2 O3 70.93(11) 6_656 2_565
O3 O2 O3 109.3(3) 2_455 2_565
Ga2 O2 O3 73.9(2) 1_554 2_565
O2 O2 O3 128.8(2) 5_446 2_565
O2 O2 O3 91.5(3) 5_456 2_565
La O2 O3 58.55(14) 2 2_565
O3 O2 O3 30.09(15) 6_655 2_565
O2 O2 O3 65.8(3) 6_556 2_565
O1 O2 O3 57.5(2) . 2_565
Ga1 O2 O3 78.99(16) 1_556 2_565
Nb O2 O3 78.99(16) 1_556 2_565
O3 O2 O3 29.4(3) 1_655 2_565
Ga2 O2 O3 69.94(17) 2_566 2_565
Ga3 O2 O3 137.69(19) 1_546 2_565
Ga3 O2 O3 49.74(13) 1_656 2_565
O2 O2 O3 58.81(17) 1_554 2_565
O2 O2 O3 121.19(17) 1_556 2_565
O3 O2 O3 121.7(2) 6_556 2_565
O2 O2 O3 92.4(3) 5_445 2_565
O2 O2 O3 60.8(2) 5_455 2_565
O3 O2 O3 57.67(11) 2_566 2_565
O2 O2 O3 160.3(3) 6_446 2_565
O2 O2 O3 98.61(17) 6_546 2_565
La O2 O3 145.9(2) 2_456 2_565
Ga2 O2 O3 72.60(18) 2 2_565
O2 O2 O3 30.87(13) 6 2_565
O3 O2 O3 145.1(3) 3_455 2_565
Ga1 O2 O3 128.6(3) 1_445 2_565
Nb O2 O3 128.6(3) 1_445 2_565
O3 O2 O3 90.8(3) 6 2_565
O3 O2 O3 113.3(2) 4_345 2_565
Ga2 O2 O3 51.0(3) . .
Ga3 O2 O3 122.1(3) 4_446 .
La O2 O3 116.8(3) 4_445 .
O2 O2 O3 72.1(3) 4_445 .
O2 O2 O3 12.5(2) 3_455 .
La O2 O3 40.47(15) . .
O3 O2 O3 74.6(3) 3_565 .
O3 O2 O3 130.7(3) 4_445 .
O2 O2 O3 140.4(5) 2_556 .
O1 O2 O3 63.1(2) 2_455 .
O3 O2 O3 89.8(3) 5_446 .
O1 O2 O3 70.2(3) 2_456 .
O3 O2 O3 84.5(3) 5_445 .
O1 O2 O3 163.0(4) 1_545 .
Nb O2 O3 100.4(2) . .
Ga1 O2 O3 100.4(2) . .
Ga2 O2 O3 162.7(3) 2_556 .
O2 O2 O3 120.2(5) 2 .
O3 O2 O3 118.7(2) 1_545 .
La O2 O3 110.8(2) 4_446 .
Ga3 O2 O3 88.03(14) 2_455 .
Ga3 O2 O3 77.47(15) 2_565 .
La O2 O3 64.14(17) 1_556 .
O3 O2 O3 103.91(19) 2_456 .
La O2 O3 49.65(11) 2_455 .
Ga3 O2 O3 17.19(14) 1_556 .
Ga3 O2 O3 98.9(3) 4_445 .
O3 O2 O3 123.34(18) 6_656 .
O3 O2 O3 99.0(2) 2_455 .
Ga2 O2 O3 71.38(19) 1_554 .
O2 O2 O3 141.5(4) 5_446 .
O2 O2 O3 33.01(19) 5_456 .
La O2 O3 146.7(3) 2 .
O3 O2 O3 116.8(2) 6_655 .
O2 O2 O3 59.89(14) 6_556 .
O1 O2 O3 35.12(10) . .
Ga1 O2 O3 101.67(19) 1_556 .
Nb O2 O3 101.67(19) 1_556 .
O3 O2 O3 103.1(2) 1_655 .
Ga2 O2 O3 38.67(11) 2_566 .
Ga3 O2 O3 129.02(17) 1_546 .
Ga3 O2 O3 118.40(17) 1_656 .
O2 O2 O3 86.4(2) 1_554 .
O2 O2 O3 93.6(2) 1_556 .
O3 O2 O3 36.4(2) 6_556 .
O2 O2 O3 128.9(3) 5_445 .
O2 O2 O3 36.92(16) 5_455 .
O3 O2 O3 92.82(19) 2_566 .
O2 O2 O3 72.17(12) 6_446 .
O2 O2 O3 161.6(4) 6_546 .
La O2 O3 62.44(15) 2_456 .
Ga2 O2 O3 127.4(3) 2 .
O2 O2 O3 59.67(15) 6 .
O3 O2 O3 90.09(11) 3_455 .
Ga1 O2 O3 105.44(14) 1_445 .
Nb O2 O3 105.44(14) 1_445 .
O3 O2 O3 34.1(2) 6 .
O3 O2 O3 28.70(15) 4_345 .
O3 O2 O3 89.3(2) 2_565 .
Ga2 O2 O3 79.2(4) . 3_566
Ga3 O2 O3 43.6(3) 4_446 3_566
La O2 O3 155.4(4) 4_445 3_566
O2 O2 O3 115.51(13) 4_445 3_566
O2 O2 O3 88.4(2) 3_455 3_566
La O2 O3 99.8(2) . 3_566
O3 O2 O3 65.9(3) 3_565 3_566
O3 O2 O3 79.8(3) 4_445 3_566
O2 O2 O3 58.7(4) 2_556 3_566
O1 O2 O3 148.0(3) 2_455 3_566
O3 O2 O3 10.9(2) 5_446 3_566
O1 O2 O3 52.7(3) 2_456 3_566
O3 O2 O3 114.8(3) 5_445 3_566
O1 O2 O3 111.5(4) 1_545 3_566
Nb O2 O3 87.84(19) . 3_566
Ga1 O2 O3 87.84(19) . 3_566
Ga2 O2 O3 87.1(2) 2_556 3_566
O2 O2 O3 139.4(2) 2 3_566
O3 O2 O3 124.9(4) 1_545 3_566
La O2 O3 57.28(19) 4_446 3_566
Ga3 O2 O3 106.1(3) 2_455 3_566
Ga3 O2 O3 45.67(15) 2_565 3_566
La O2 O3 24.18(9) 1_556 3_566
O3 O2 O3 88.2(2) 2_456 3_566
La O2 O3 124.8(2) 2_455 3_566
Ga3 O2 O3 74.16(16) 1_556 3_566
Ga3 O2 O3 133.1(2) 4_445 3_566
O3 O2 O3 44.7(2) 6_656 3_566
O3 O2 O3 158.9(3) 2_455 3_566
Ga2 O2 O3 152.2(2) 1_554 3_566
O2 O2 O3 88.6(4) 5_446 3_566
O2 O2 O3 52.4(3) 5_456 3_566
La O2 O3 102.69(17) 2 3_566
O3 O2 O3 104.7(3) 6_655 3_566
O2 O2 O3 37.6(2) 6_556 3_566
O1 O2 O3 73.8(3) . 3_566
Ga1 O2 O3 20.63(9) 1_556 3_566
Nb O2 O3 20.63(9) 1_556 3_566
O3 O2 O3 67.03(15) 1_655 3_566
Ga2 O2 O3 54.48(15) 2_566 3_566
Ga3 O2 O3 107.0(3) 1_546 3_566
Ga3 O2 O3 57.65(13) 1_656 3_566
O2 O2 O3 149.08(16) 1_554 3_566
O2 O2 O3 30.92(16) 1_556 3_566
O3 O2 O3 70.54(19) 6_556 3_566
O2 O2 O3 145.5(3) 5_445 3_566
O2 O2 O3 108.0(2) 5_455 3_566
O3 O2 O3 34.6(2) 2_566 3_566
O2 O2 O3 93.9(3) 6_446 3_566
O2 O2 O3 77.9(3) 6_546 3_566
La O2 O3 68.99(17) 2_456 3_566
Ga2 O2 O3 141.90(17) 2 3_566
O2 O2 O3 96.5(2) 6 3_566
O3 O2 O3 123.4(3) 3_455 3_566
Ga1 O2 O3 137.9(3) 1_445 3_566
Nb O2 O3 137.9(3) 1_445 3_566
O3 O2 O3 119.41(19) 6 3_566
O3 O2 O3 100.1(2) 4_345 3_566
O3 O2 O3 91.3(2) 2_565 3_566
O3 O2 O3 85.39(19) . 3_566
Ga2 O2 O3 93.3(5) . 4_446
Ga3 O2 O3 27.9(3) 4_446 4_446
La O2 O3 127.5(3) 4_445 4_446
O2 O2 O3 117.98(18) 4_445 4_446
O2 O2 O3 114.43(18) 3_455 4_446
La O2 O3 124.3(2) . 4_446
O3 O2 O3 79.9(3) 3_565 4_446
O3 O2 O3 66.0(3) 4_445 4_446
O2 O2 O3 30.7(3) 2_556 4_446
O1 O2 O3 176.3(3) 2_455 4_446
O3 O2 O3 27.7(2) 5_446 4_446
O1 O2 O3 62.6(3) 2_456 4_446
O3 O2 O3 120.4(3) 5_445 4_446
O1 O2 O3 83.5(4) 1_545 4_446
Nb O2 O3 87.91(18) . 4_446
Ga1 O2 O3 87.91(18) . 4_446
Ga2 O2 O3 58.92(18) 2_556 4_446
O2 O2 O3 120.1(3) 2 4_446
O3 O2 O3 104.0(3) 1_545 4_446
La O2 O3 43.56(14) 4_446 4_446
Ga3 O2 O3 100.9(3) 2_455 4_446
Ga3 O2 O3 61.23(16) 2_565 4_446
La O2 O3 49.50(15) 1_556 4_446
O3 O2 O3 77.1(2) 2_456 4_446
La O2 O3 142.2(3) 2_455 4_446
Ga3 O2 O3 100.2(2) 1_556 4_446
Ga3 O2 O3 128.01(17) 4_445 4_446
O3 O2 O3 28.3(2) 6_656 4_446
O3 O2 O3 138.9(2) 2_455 4_446
Ga2 O2 O3 169.4(2) 1_554 4_446
O2 O2 O3 63.9(3) 5_446 4_446
O2 O2 O3 80.2(3) 5_456 4_446
La O2 O3 81.69(15) 2 4_446
O3 O2 O3 95.4(2) 6_655 4_446
O2 O2 O3 62.8(3) 6_556 4_446
O1 O2 O3 99.9(3) . 4_446
Ga1 O2 O3 20.66(10) 1_556 4_446
Nb O2 O3 20.66(10) 1_556 4_446
O3 O2 O3 67.07(16) 1_655 4_446
Ga2 O2 O3 82.02(17) 2_566 4_446
Ga3 O2 O3 84.89(19) 1_546 4_446
Ga3 O2 O3 48.88(13) 1_656 4_446
O2 O2 O3 149.16(13) 1_554 4_446
O2 O2 O3 30.84(13) 1_556 4_446
O3 O2 O3 91.5(2) 6_556 4_446
O2 O2 O3 117.3(2) 5_445 4_446
O2 O2 O3 134.2(2) 5_455 4_446
O3 O2 O3 42.9(2) 2_566 4_446
O2 O2 O3 97.2(4) 6_446 4_446
O2 O2 O3 49.7(2) 6_546 4_446
La O2 O3 79.5(2) 2_456 4_446
Ga2 O2 O3 117.57(16) 2 4_446
O2 O2 O3 114.4(2) 6 4_446
O3 O2 O3 115.8(3) 3_455 4_446
Ga1 O2 O3 120.2(2) 1_445 4_446
Nb O2 O3 120.2(2) 1_445 4_446
O3 O2 O3 146.6(2) 6 4_446
O3 O2 O3 122.5(3) 4_345 4_446
O3 O2 O3 96.3(2) 2_565 4_446
O3 O2 O3 113.2(2) . 4_446
O3 O2 O3 28.29(17) 3_566 4_446
Ga2 O2 La 111.2(5) . 2_556
Ga3 O2 La 25.6(2) 4_446 2_556
La O2 La 104.2(2) 4_445 2_556
O2 O2 La 121.1(3) 4_445 2_556
O2 O2 La 139.13(14) 3_455 2_556
La O2 La 137.2(2) . 2_556
O3 O2 La 87.5(3) 3_565 2_556
O3 O2 La 51.4(3) 4_445 2_556
O2 O2 La 14.34(9) 2_556 2_556
O1 O2 La 158.5(3) 2_455 2_556
O3 O2 La 49.3(2) 5_446 2_556
O1 O2 La 81.3(3) 2_456 2_556
O3 O2 La 112.1(2) 5_445 2_556
O1 O2 La 58.8(3) 1_545 2_556
Nb O2 La 81.43(14) . 2_556
Ga1 O2 La 81.43(14) . 2_556
Ga2 O2 La 36.71(10) 2_556 2_556
O2 O2 La 96.7(3) 2 2_556
O3 O2 La 89.1(2) 1_545 2_556
La O2 La 48.66(12) 4_446 2_556
Ga3 O2 La 101.1(2) 2_455 2_556
Ga3 O2 La 73.73(14) 2_565 2_556
La O2 La 74.52(18) 1_556 2_556
O3 O2 La 76.5(2) 2_456 2_556
La O2 La 152.9(3) 2_455 2_556
Ga3 O2 La 125.1(2) 1_556 2_556
Ga3 O2 La 110.45(13) 4_445 2_556
O3 O2 La 24.81(11) 6_656 2_556
O3 O2 La 119.5(2) 2_455 2_556
Ga2 O2 La 148.50(19) 1_554 2_556
O2 O2 La 49.2(2) 5_446 2_556
O2 O2 La 105.1(3) 5_456 2_556
La O2 La 59.44(10) 2 2_556
O3 O2 La 80.09(18) 6_655 2_556
O2 O2 La 83.0(2) 6_556 2_556
O1 O2 La 118.5(2) . 2_556
Ga1 O2 La 38.40(8) 1_556 2_556
Nb O2 La 38.40(8) 1_556 2_556
O3 O2 La 64.96(15) 1_655 2_556
Ga2 O2 La 103.97(17) 2_566 2_556
Ga3 O2 La 71.17(14) 1_546 2_556
Ga3 O2 La 43.63(8) 1_656 2_556
O2 O2 La 129.38(11) 1_554 2_556
O2 O2 La 50.62(11) 1_556 2_556
O3 O2 La 114.1(3) 6_556 2_556
O2 O2 La 92.86(15) 5_445 2_556
O2 O2 La 148.7(2) 5_455 2_556
O3 O2 La 54.61(13) 2_566 2_556
O2 O2 La 105.6(3) 6_446 2_556
O2 O2 La 25.84(14) 6_546 2_556
La O2 La 96.4(2) 2_456 2_556
Ga2 O2 La 92.79(11) 2 2_556
O2 O2 La 119.81(13) 6 2_556
O3 O2 La 110.5(2) 3_455 2_556
Ga1 O2 La 105.72(16) 1_445 2_556
Nb O2 La 105.72(16) 1_445 2_556
O3 O2 La 171.5(2) 6 2_556
O3 O2 La 144.0(3) 4_345 2_556
O3 O2 La 92.60(14) 2_565 2_556
O3 O2 La 138.1(2) . 2_556
O3 O2 La 52.73(14) 3_566 2_556
O3 O2 La 25.04(9) 4_446 2_556
Ga2 O2 O1 88.7(5) . 1_546
Ga3 O2 O1 50.3(3) 4_446 1_546
La O2 O1 98.0(3) 4_445 1_546
O2 O2 O1 94.8(2) 4_445 1_546
O2 O2 O1 125.05(17) 3_455 1_546
La O2 O1 157.0(3) . 1_546
O3 O2 O1 110.9(4) 3_565 1_546
O3 O2 O1 76.8(3) 4_445 1_546
O2 O2 O1 13.8(2) 2_556 1_546
O1 O2 O1 149.9(3) 2_455 1_546
O3 O2 O1 60.1(3) 5_446 1_546
O1 O2 O1 62.2(2) 2_456 1_546
O3 O2 O1 137.3(2) 5_445 1_546
O1 O2 O1 61.7(3) 1_545 1_546
Nb O2 O1 107.94(18) . 1_546
Ga1 O2 O1 107.94(18) . 1_546
Ga2 O2 O1 33.95(19) 2_556 1_546
O2 O2 O1 108.5(3) 2 1_546
O3 O2 O1 71.1(3) 1_545 1_546
La O2 O1 23.63(11) 4_446 1_546
Ga3 O2 O1 74.98(18) 2_455 1_546
Ga3 O2 O1 93.7(2) 2_565 1_546
La O2 O1 71.3(2) 1_556 1_546
O3 O2 O1 50.19(17) 2_456 1_546
La O2 O1 126.3(2) 2_455 1_546
Ga3 O2 O1 114.2(3) 1_556 1_546
Ga3 O2 O1 129.32(19) 4_445 1_546
O3 O2 O1 49.77(16) 6_656 1_546
O3 O2 O1 106.2(2) 2_455 1_546
Ga2 O2 O1 150.2(2) 1_554 1_546
O2 O2 O1 31.3(2) 5_446 1_546
O2 O2 O1 102.7(4) 5_456 1_546
La O2 O1 77.70(17) 2 1_546
O3 O2 O1 103.6(2) 6_655 1_546
O2 O2 O1 94.6(3) 6_556 1_546
O1 O2 O1 131.4(4) . 1_546
Ga1 O2 O1 53.35(15) 1_556 1_546
Nb O2 O1 53.35(15) 1_556 1_546
O3 O2 O1 91.22(19) 1_655 1_546
Ga2 O2 O1 111.6(2) 2_566 1_546
Ga3 O2 O1 51.98(14) 1_546 1_546
Ga3 O2 O1 69.98(13) 1_656 1_546
O2 O2 O1 141.64(17) 1_554 1_546
O2 O2 O1 38.36(17) 1_556 1_546
O3 O2 O1 97.1(3) 6_556 1_546
O2 O2 O1 91.2(2) 5_445 1_546
O2 O2 O1 165.1(3) 5_455 1_546
O3 O2 O1 74.69(19) 2_566 1_546
O2 O2 O1 79.3(3) 6_446 1_546
O2 O2 O1 31.2(2) 6_546 1_546
La O2 O1 74.3(2) 2_456 1_546
Ga2 O2 O1 99.95(19) 2 1_546
O2 O2 O1 145.1(2) 6 1_546
O3 O2 O1 86.4(2) 3_455 1_546
Ga1 O2 O1 87.39(16) 1_445 1_546
Nb O2 O1 87.39(16) 1_445 1_546
O3 O2 O1 149.2(2) 6 1_546
O3 O2 O1 122.1(3) 4_345 1_546
O3 O2 O1 119.20(17) 2_565 1_546
O3 O2 O1 131.2(3) . 1_546
O3 O2 O1 57.6(2) 3_566 1_546
O3 O2 O1 32.90(13) 4_446 1_546
La O2 O1 26.60(6) 2_556 1_546
Ga2 O2 O2 152.3(4) . 3
Ga3 O2 O2 32.3(3) 4_446 3
La O2 O2 95.1(2) 4_445 3
O2 O2 O2 154.6(4) 4_445 3
O2 O2 O2 145.4(4) 3_455 3
La O2 O2 101.61(17) . 3
O3 O2 O2 58.68(17) 3_565 3
O3 O2 O2 7.0(4) 4_445 3
O2 O2 O2 56.5(3) 2_556 3
O1 O2 O2 122.5(3) 2_455 3
O3 O2 O2 64.5(2) 5_446 3
O1 O2 O2 121.7(3) 2_456 3
O3 O2 O2 67.61(17) 5_445 3
O1 O2 O2 57.49(16) 1_545 3
Nb O2 O2 38.62(11) . 3
Ga1 O2 O2 38.62(11) . 3
Ga2 O2 O2 58.66(15) 2_556 3
O2 O2 O2 65.1(3) 2 3
O3 O2 O2 107.3(2) 1_545 3
La O2 O2 93.12(14) 4_446 3
Ga3 O2 O2 137.7(2) 2_455 3
Ga3 O2 O2 58.13(8) 2_565 3
La O2 O2 97.76(10) 1_556 3
O3 O2 O2 116.8(2) 2_456 3
La O2 O2 158.60(16) 2_455 3
Ga3 O2 O2 137.2(2) 1_556 3
Ga3 O2 O2 68.96(10) 4_445 3
O3 O2 O2 31.58(19) 6_656 3
O3 O2 O2 115.0(2) 2_455 3
Ga2 O2 O2 110.55(10) 1_554 3
O2 O2 O2 80.6(2) 5_446 3
O2 O2 O2 114.4(2) 5_456 3
La O2 O2 29.93(14) 2 3
O3 O2 O2 36.6(2) 6_655 3
O2 O2 O2 79.80(14) 6_556 3
O1 O2 O2 98.20(15) . 3
Ga1 O2 O2 53.85(10) 1_556 3
Nb O2 O2 53.85(10) 1_556 3
O3 O2 O2 30.19(10) 1_655 3
Ga2 O2 O2 98.04(14) 2_566 3
Ga3 O2 O2 97.39(19) 1_546 3
Ga3 O2 O2 18.79(10) 1_656 3
O2 O2 O2 90.0 1_554 3
O2 O2 O2 90.0 1_556 3
O3 O2 O2 143.94(19) 6_556 3
O2 O2 O2 81.76(19) 5_445 3
O2 O2 O2 111.3(2) 5_455 3
O3 O2 O2 48.27(14) 2_566 3
O2 O2 O2 149.0(3) 6_446 3
O2 O2 O2 48.93(12) 6_546 3
La O2 O2 138.64(12) 2_456 3
Ga2 O2 O2 68.71(13) 2 3
O2 O2 O2 80.95(12) 6 3
O3 O2 O2 136.2(2) 3_455 3
Ga1 O2 O2 117.92(19) 1_445 3
Nb O2 O2 117.92(19) 1_445 3
O3 O2 O2 140.59(19) 6 3
O3 O2 O2 161.7(2) 4_345 3
O3 O2 O2 50.49(11) 2_565 3
O3 O2 O2 133.2(2) . 3
O3 O2 O2 74.39(11) 3_566 3
O3 O2 O2 59.17(13) 4_446 3
La O2 O2 44.51(11) 2_556 3
O1 O2 O2 70.20(13) 1_546 3
Ga2 O2 O2 112.4(4) . 4
Ga3 O2 O2 58.8(2) 4_446 4
La O2 O2 134.6(2) 4_445 4
O2 O2 O2 145.4(4) 4_445 4
O2 O2 O2 85.4(4) 3_455 4
La O2 O2 53.0(2) . 4
O3 O2 O2 7.0(4) 3_565 4
O3 O2 O2 58.68(17) 4_445 4
O2 O2 O2 98.20(10) 2_556 4
O1 O2 O2 103.3(2) 2_455 4
O3 O2 O2 51.1(3) 5_446 4
O1 O2 O2 103.1(2) 2_456 4
O3 O2 O2 56.3(2) 5_445 4
O1 O2 O2 116.46(16) 1_545 4
Nb O2 O2 38.62(11) . 4
Ga1 O2 O2 38.62(11) . 4
Ga2 O2 O2 115.54(15) 2_556 4
O2 O2 O2 96.24(5) 2 4
O3 O2 O2 166.4(3) 1_545 4
La O2 O2 115.41(11) 4_446 4
Ga3 O2 O2 156.5(2) 2_455 4
Ga3 O2 O2 13.72(17) 2_565 4
La O2 O2 66.18(17) 1_556 4
O3 O2 O2 147.2(2) 2_456 4
La O2 O2 118.8(2) 2_455 4
Ga3 O2 O2 79.1(2) 1_556 4
Ga3 O2 O2 77.30(9) 4_445 4
O3 O2 O2 59.70(12) 6_656 4
O3 O2 O2 142.0(2) 2_455 4
Ga2 O2 O2 98.68(15) 1_554 4
O2 O2 O2 133.4(2) 5_446 4
O2 O2 O2 60.7(2) 5_456 4
La O2 O2 83.13(9) 2 4
O3 O2 O2 61.62(12) 6_655 4
O2 O2 O2 30.4(3) 6_556 4
O1 O2 O2 38.88(15) . 4
Ga1 O2 O2 53.85(10) 1_556 4
Nb O2 O2 53.85(10) 1_556 4
O3 O2 O2 30.30(11) 1_655 4
Ga2 O2 O2 40.17(16) 2_566 4
Ga3 O2 O2 154.97(19) 1_546 4
Ga3 O2 O2 46.03(5) 1_656 4
O2 O2 O2 90.000(1) 1_554 4
O2 O2 O2 90.000(1) 1_556 4
O3 O2 O2 94.1(2) 6_556 4
O2 O2 O2 127.2(2) 5_445 4
O2 O2 O2 64.49(18) 5_455 4
O3 O2 O2 31.67(15) 2_566 4
O2 O2 O2 137.4(3) 6_446 4
O2 O2 O2 103.85(9) 6_546 4
La O2 O2 112.82(17) 2_456 4
Ga2 O2 O2 107.52(9) 2 4
O2 O2 O2 40.0(2) 6 4
O3 O2 O2 163.3(2) 3_455 4
Ga1 O2 O2 162.98(14) 1_445 4
Nb O2 O2 162.98(14) 1_445 4
O3 O2 O2 93.9(2) 6 4
O3 O2 O2 102.1(2) 4_345 4
O3 O2 O2 35.57(16) 2_565 4
O3 O2 O2 73.4(2) . 4
O3 O2 O2 59.09(16) 3_566 4
O3 O2 O2 74.43(11) 4_446 4
La O2 O2 84.35(8) 2_556 4
O1 O2 O2 106.31(10) 1_546 4
O2 O2 O2 60.000(1) 3 4
Ga2 O2 O2 92.0(4) . 4_444
Ga3 O2 O2 147.9(4) 4_446 4_444
La O2 O2 40.6(2) 4_445 4_444
O2 O2 O2 61.39(10) 4_445 4_444
O2 O2 O2 76.15(5) 3_455 4_444
La O2 O2 66.3(2) . 4_444
O3 O2 O2 107.1(4) 3_565 4_444
O3 O2 O2 109.3(4) 4_445 4_444
O2 O2 O2 137.4(3) 2_556 4_444
O1 O2 O2 15.64(13) 2_455 4_444
O3 O2 O2 163.1(4) 5_446 4_444
O1 O2 O2 121.8(3) 2_456 4_444
O3 O2 O2 61.87(19) 5_445 4_444
O1 O2 O2 84.8(4) 1_545 4_444
Nb O2 O2 92.99(19) . 4_444
Ga1 O2 O2 92.99(19) . 4_444
Ga2 O2 O2 109.2(2) 2_556 4_444
O2 O2 O2 51.56(19) 2 4_444
O3 O2 O2 66.4(3) 1_545 4_444
La O2 O2 131.1(2) 4_446 4_444
Ga3 O2 O2 75.7(2) 2_455 4_444
Ga3 O2 O2 126.9(2) 2_565 4_444
La O2 O2 141.3(2) 1_556 4_444
O3 O2 O2 97.7(3) 2_456 4_444
La O2 O2 43.40(19) 2_455 4_444
Ga3 O2 O2 90.4(2) 1_556 4_444
Ga3 O2 O2 49.20(8) 4_445 4_444
O3 O2 O2 147.1(2) 6_656 4_444
O3 O2 O2 30.76(18) 2_455 4_444
Ga2 O2 O2 14.60(5) 1_554 4_444
O2 O2 O2 105.4(3) 5_446 4_444
O2 O2 O2 111.4(3) 5_456 4_444
La O2 O2 89.98(17) 2 4_444
O3 O2 O2 81.2(2) 6_655 4_444
O2 O2 O2 128.5(4) 6_556 4_444
O1 O2 O2 91.4(3) . 4_444
Ga1 O2 O2 165.4(2) 1_556 4_444
Nb O2 O2 165.4(2) 1_556 4_444
O3 O2 O2 114.5(2) 1_655 4_444
Ga2 O2 O2 109.8(2) 2_566 4_444
Ga3 O2 O2 85.3(2) 1_546 4_444
Ga3 O2 O2 129.40(18) 1_656 4_444
O2 O2 O2 28.62(10) 1_554 4_444
O2 O2 O2 151.39(10) 1_556 4_444
O3 O2 O2 96.9(2) 6_556 4_444
O2 O2 O2 50.9(2) 5_445 4_444
O2 O2 O2 57.0(2) 5_455 4_444
O3 O2 O2 143.3(2) 2_566 4_444
O2 O2 O2 83.3(3) 6_446 4_444
O2 O2 O2 118.4(3) 6_546 4_444
La O2 O2 104.60(18) 2_456 4_444
Ga2 O2 O2 52.22(12) 2 4_444
O2 O2 O2 73.5(2) 6 4_444
O3 O2 O2 59.3(2) 3_455 4_444
Ga1 O2 O2 50.92(16) 1_445 4_444
Nb O2 O2 50.92(16) 1_445 4_444
O3 O2 O2 44.49(18) 6 4_444
O3 O2 O2 66.2(2) 4_345 4_444
O3 O2 O2 86.45(17) 2_565 4_444
O3 O2 O2 78.3(2) . 4_444
O3 O2 O2 163.6(2) 3_566 4_444
O3 O2 O2 168.1(2) 4_446 4_444
La O2 O2 143.6(2) 2_556 4_444
O1 O2 O2 136.7(2) 1_546 4_444
O2 O2 O2 115.64(14) 3 4_444
O2 O2 O2 113.21(14) 4 4_444
Ga2 O2 O2 92.0(4) . 3_454
Ga3 O2 O2 139.6(5) 4_446 3_454
La O2 O2 66.8(2) 4_445 3_454
O2 O2 O2 76.15(5) 4_445 3_454
O2 O2 O2 61.38(10) 3_455 3_454
La O2 O2 38.6(2) . 3_454
O3 O2 O2 82.5(4) 3_565 3_454
O3 O2 O2 106.2(4) 4_445 3_454
O2 O2 O2 161.0(4) 2_556 3_454
O1 O2 O2 15.64(13) 2_455 3_454
O3 O2 O2 135.5(4) 5_446 3_454
O1 O2 O2 121.8(3) 2_456 3_454
O3 O2 O2 46.6(2) 5_445 3_454
O1 O2 O2 106.4(4) 1_545 3_454
Nb O2 O2 78.8(2) . 3_454
Ga1 O2 O2 78.8(2) . 3_454
Ga2 O2 O2 133.6(2) 2_556 3_454
O2 O2 O2 62.5(3) 2 3_454
O3 O2 O2 93.7(3) 1_545 3_454
La O2 O2 151.8(2) 4_446 3_454
Ga3 O2 O2 94.80(19) 2_455 3_454
Ga3 O2 O2 100.9(3) 2_565 3_454
La O2 O2 121.7(2) 1_556 3_454
O3 O2 O2 119.3(2) 2_456 3_454
La O2 O2 47.00(16) 2_455 3_454
Ga3 O2 O2 74.3(2) 1_556 3_454
Ga3 O2 O2 46.41(11) 4_445 3_454
O3 O2 O2 139.8(3) 6_656 3_454
O3 O2 O2 58.32(16) 2_455 3_454
Ga2 O2 O2 14.61(5) 1_554 3_454
O2 O2 O2 133.1(3) 5_446 3_454
O2 O2 O2 89.8(3) 5_456 3_454
La O2 O2 97.99(19) 2 3_454
O3 O2 O2 77.0(2) 6_655 3_454
O2 O2 O2 100.9(4) 6_556 3_454
O1 O2 O2 64.0(3) . 3_454
Ga1 O2 O2 141.5(3) 1_556 3_454
Nb O2 O2 141.5(3) 1_556 3_454
O3 O2 O2 98.2(3) 1_655 3_454
Ga2 O2 O2 83.3(2) 2_566 3_454
Ga3 O2 O2 112.73(18) 1_546 3_454
Ga3 O2 O2 118.4(2) 1_656 3_454
O2 O2 O2 28.62(10) 1_554 3_454
O2 O2 O2 151.38(10) 1_556 3_454
O3 O2 O2 88.2(2) 6_556 3_454
O2 O2 O2 74.7(2) 5_445 3_454
O2 O2 O2 29.7(3) 5_455 3_454
O3 O2 O2 119.4(3) 2_566 3_454
O2 O2 O2 94.9(3) 6_446 3_454
O2 O2 O2 139.8(3) 6_546 3_454
La O2 O2 106.74(18) 2_456 3_454
Ga2 O2 O2 68.86(11) 2 3_454
O2 O2 O2 48.0(2) 6 3_454
O3 O2 O2 81.2(2) 3_455 3_454
Ga1 O2 O2 77.63(14) 1_445 3_454
Nb O2 O2 77.63(14) 1_445 3_454
O3 O2 O2 30.80(17) 6 3_454
O3 O2 O2 59.1(2) 4_345 3_454
O3 O2 O2 68.9(2) 2_565 3_454
O3 O2 O2 58.5(2) . 3_454
O3 O2 O2 137.7(3) 3_566 3_454
O3 O2 O2 162.1(2) 4_446 3_454
La O2 O2 156.80(19) 2_556 3_454
O1 O2 O2 164.5(2) 1_546 3_454
O2 O2 O2 113.21(14) 3 3_454
O2 O2 O2 87.8(2) 4 3_454
O2 O2 O2 27.71(9) 4_444 3_454
Ga2 O2 O2 39.5(4) . 4_446
Ga3 O2 O2 86.0(4) 4_446 4_446
La O2 O2 111.8(4) 4_445 4_446
O2 O2 O2 61.38(10) 4_445 4_446
O2 O2 O2 76.15(5) 3_455 4_446
La O2 O2 124.1(2) . 4_446
O3 O2 O2 120.2(4) 3_565 4_446
O3 O2 O2 122.7(4) 4_445 4_446
O2 O2 O2 62.8(3) 2_556 4_446
O1 O2 O2 121.1(3) 2_455 4_446
O3 O2 O2 67.1(3) 5_446 4_446
O1 O2 O2 15.29(12) 2_456 4_446
O3 O2 O2 166.9(3) 5_445 4_446
O1 O2 O2 102.5(4) 1_545 4_446
Nb O2 O2 144.0(2) . 4_446
Ga1 O2 O2 144.0(2) . 4_446
Ga2 O2 O2 78.1(3) 2_556 4_446
O2 O2 O2 146.6(3) 2 4_446
O3 O2 O2 75.7(3) 1_545 4_446
La O2 O2 26.51(10) 4_446 4_446
Ga3 O2 O2 49.2(2) 2_455 4_446
Ga3 O2 O2 101.09(18) 2_565 4_446
La O2 O2 47.65(8) 1_556 4_446
O3 O2 O2 35.4(2) 2_456 4_446
La O2 O2 85.03(19) 2_455 4_446
Ga3 O2 O2 67.69(15) 1_556 4_446
Ga3 O2 O2 169.5(2) 4_445 4_446
O3 O2 O2 86.2(2) 6_656 4_446
O3 O2 O2 102.7(3) 2_455 4_446
Ga2 O2 O2 132.49(18) 1_554 4_446
O2 O2 O2 60.7(4) 5_446 4_446
O2 O2 O2 67.0(3) 5_456 4_446
La O2 O2 127.0(3) 2 4_446
O3 O2 O2 152.0(3) 6_655 4_446
O2 O2 O2 84.1(3) 6_556 4_446
O1 O2 O2 104.7(3) . 4_446
Ga1 O2 O2 71.49(13) 1_556 4_446
Nb O2 O2 71.49(13) 1_556 4_446
O3 O2 O2 122.5(2) 1_655 4_446
Ga2 O2 O2 86.31(15) 2_566 4_446
Ga3 O2 O2 64.7(2) 1_546 4_446
Ga3 O2 O2 106.82(19) 1_656 4_446
O2 O2 O2 151.39(10) 1_554 4_446
O2 O2 O2 28.62(10) 1_556 4_446
O3 O2 O2 48.54(17) 6_556 4_446
O2 O2 O2 115.8(3) 5_445 4_446
O2 O2 O2 121.4(2) 5_455 4_446
O3 O2 O2 91.1(2) 2_566 4_446
O2 O2 O2 39.6(3) 6_446 4_446
O2 O2 O2 79.8(3) 6_546 4_446
La O2 O2 24.81(11) 2_456 4_446
Ga2 O2 O2 134.3(2) 2 4_446
O2 O2 O2 138.3(3) 6 4_446
O3 O2 O2 66.6(2) 3_455 4_446
Ga1 O2 O2 83.3(2) 1_445 4_446
Nb O2 O2 83.3(2) 1_445 4_446
O3 O2 O2 101.27(19) 6 4_446
O3 O2 O2 73.0(2) 4_345 4_446
O3 O2 O2 147.9(2) 2_565 4_446
O3 O2 O2 84.7(2) . 4_446
O3 O2 O2 56.85(13) 3_566 4_446
O3 O2 O2 58.06(14) 4_446 4_446
La O2 O2 71.97(16) 2_556 4_446
O1 O2 O2 49.58(18) 1_546 4_446
O2 O2 O2 115.64(14) 3 4_446
O2 O2 O2 113.21(14) 4 4_446
O2 O2 O2 122.8(2) 4_444 4_446
O2 O2 O2 130.99(17) 3_454 4_446
Ga2 O2 O2 39.5(4) . 3_456
Ga3 O2 O2 81.1(3) 4_446 3_456
La O2 O2 137.5(4) 4_445 3_456
O2 O2 O2 76.14(5) 4_445 3_456
O2 O2 O2 61.38(10) 3_455 3_456
La O2 O2 100.5(3) . 3_456
O3 O2 O2 94.5(4) 3_565 3_456
O3 O2 O2 119.2(4) 4_445 3_456
O2 O2 O2 75.7(4) 2_556 3_456
O1 O2 O2 121.1(3) 2_455 3_456
O3 O2 O2 50.8(2) 5_446 3_456
O1 O2 O2 15.29(12) 2_456 3_456
O3 O2 O2 139.3(3) 5_445 3_456
O1 O2 O2 126.2(4) 1_545 3_456
Nb O2 O2 124.3(3) . 3_456
Ga1 O2 O2 124.3(3) . 3_456
Ga2 O2 O2 98.9(2) 2_556 3_456
O2 O2 O2 173.7(4) 2 3_456
O3 O2 O2 102.6(3) 1_545 3_456
La O2 O2 47.84(8) 4_446 3_456
Ga3 O2 O2 71.1(2) 2_455 3_456
Ga3 O2 O2 77.41(19) 2_565 3_456
La O2 O2 21.84(9) 1_556 3_456
O3 O2 O2 62.7(2) 2_456 3_456
La O2 O2 87.6(2) 2_455 3_456
Ga3 O2 O2 48.87(19) 1_556 3_456
Ga3 O2 O2 161.3(2) 4_445 3_456
O3 O2 O2 81.8(2) 6_656 3_456
O3 O2 O2 123.7(3) 2_455 3_456
Ga2 O2 O2 132.49(18) 1_554 3_456
O2 O2 O2 85.9(3) 5_446 3_456
O2 O2 O2 40.6(3) 5_456 3_456
La O2 O2 137.8(2) 2 3_456
O3 O2 O2 144.2(3) 6_655 3_456
O2 O2 O2 57.6(2) 6_556 3_456
O1 O2 O2 77.9(3) . 3_456
Ga1 O2 O2 59.81(13) 1_556 3_456
Nb O2 O2 59.81(13) 1_556 3_456
O3 O2 O2 105.5(3) 1_655 3_456
Ga2 O2 O2 58.75(16) 2_566 3_456
Ga3 O2 O2 92.37(19) 1_546 3_456
Ga3 O2 O2 97.53(18) 1_656 3_456
O2 O2 O2 151.38(10) 1_554 3_456
O2 O2 O2 28.62(10) 1_556 3_456
O3 O2 O2 35.5(2) 6_556 3_456
O2 O2 O2 143.3(3) 5_445 3_456
O2 O2 O2 101.4(3) 5_455 3_456
O3 O2 O2 73.0(2) 2_566 3_456
O2 O2 O2 55.4(2) 6_446 3_456
O2 O2 O2 96.4(3) 6_546 3_456
La O2 O2 29.34(13) 2_456 3_456
Ga2 O2 O2 161.9(2) 2 3_456
O2 O2 O2 111.2(3) 6 3_456
O3 O2 O2 87.7(2) 3_455 3_456
Ga1 O2 O2 107.4(2) 1_445 3_456
Nb O2 O2 107.4(2) 1_445 3_456
O3 O2 O2 92.9(2) 6 3_456
O3 O2 O2 66.3(2) 4_345 3_456
O3 O2 O2 123.3(2) 2_565 3_456
O3 O2 O2 65.6(2) . 3_456
O3 O2 O2 39.98(13) 3_566 3_456
O3 O2 O2 56.25(13) 4_446 3_456
La O2 O2 78.76(12) 2_556 3_456
O1 O2 O2 65.58(17) 1_546 3_456
O2 O2 O2 113.21(14) 3 3_456
O2 O2 O2 87.8(2) 4 3_456
O2 O2 O2 130.99(17) 4_444 3_456
O2 O2 O2 122.8(2) 3_454 3_456
O2 O2 O2 27.71(9) 4_446 3_456
Ga2 O2 O2 65.4(2) . 6_445
Ga3 O2 O2 167.1(4) 4_446 6_445
La O2 O2 48.5(2) 4_445 6_445
O2 O2 O2 32.8(2) 4_445 6_445
O2 O2 O2 62.85(16) 3_455 6_445
La O2 O2 79.0(3) . 6_445
O3 O2 O2 127.8(5) 3_565 6_445
O3 O2 O2 135.7(5) 4_445 6_445
O2 O2 O2 129.82(19) 2_556 6_445
O1 O2 O2 30.8(2) 2_455 6_445
O3 O2 O2 154.5(3) 5_446 6_445
O1 O2 O2 93.7(3) 2_456 6_445
O3 O2 O2 89.3(4) 5_445 6_445
O1 O2 O2 93.3(3) 1_545 6_445
Nb O2 O2 121.3(4) . 6_445
Ga1 O2 O2 121.3(4) . 6_445
Ga2 O2 O2 108.1(2) 2_556 6_445
O2 O2 O2 76.1(4) 2 6_445
O3 O2 O2 54.2(2) 1_545 6_445
La O2 O2 106.6(3) 4_446 6_445
Ga3 O2 O2 49.19(12) 2_455 6_445
Ga3 O2 O2 143.0(3) 2_565 6_445
La O2 O2 121.19(16) 1_556 6_445
O3 O2 O2 73.3(2) 2_456 6_445
La O2 O2 22.12(4) 2_455 6_445
Ga3 O2 O2 75.85(6) 1_556 6_445
Ga3 O2 O2 77.9(3) 4_445 6_445
O3 O2 O2 166.0(3) 6_656 6_445
O3 O2 O2 28.92(16) 2_455 6_445
Ga2 O2 O2 39.70(18) 1_554 6_445
O2 O2 O2 94.2(3) 5_446 6_445
O2 O2 O2 99.84(15) 5_456 6_445
La O2 O2 111.8(3) 2 6_445
O3 O2 O2 109.4(4) 6_655 6_445
O2 O2 O2 130.4(2) 6_556 6_445
O1 O2 O2 97.8(3) . 6_445
Ga1 O2 O2 164.6(3) 1_556 6_445
Nb O2 O2 164.6(3) 1_556 6_445
O3 O2 O2 142.6(4) 1_655 6_445
Ga2 O2 O2 109.01(17) 2_566 6_445
Ga3 O2 O2 72.12(18) 1_546 6_445
Ga3 O2 O2 157.6(3) 1_656 6_445
O2 O2 O2 57.3(2) 1_554 6_445
O2 O2 O2 122.7(2) 1_556 6_445
O3 O2 O2 74.71(15) 6_556 6_445
O2 O2 O2 62.1(3) 5_445 6_445
O2 O2 O2 67.5(3) 5_455 6_445
O3 O2 O2 162.0(3) 2_566 6_445
O2 O2 O2 54.55(9) 6_446 6_445
O2 O2 O2 120.0(3) 6_546 6_445
La O2 O2 76.64(13) 2_456 6_445
Ga2 O2 O2 72.5(2) 2 6_445
O2 O2 O2 93.5(3) 6 6_445
O3 O2 O2 35.14(17) 3_455 6_445
Ga1 O2 O2 37.74(12) 1_445 6_445
Nb O2 O2 37.74(12) 1_445 6_445
O3 O2 O2 40.38(13) 6 6_445
O3 O2 O2 47.67(12) 4_345 6_445
O3 O2 O2 113.5(4) 2_565 6_445
O3 O2 O2 70.61(13) . 6_445
O3 O2 O2 144.5(2) 3_566 6_445
O3 O2 O2 150.1(3) 4_446 6_445
La O2 O2 143.2(3) 2_556 6_445
O1 O2 O2 121.3(3) 1_546 6_445
O2 O2 O2 141.01(18) 3 6_445
O2 O2 O2 131.9(3) 4 6_445
O2 O2 O2 28.7(3) 4_444 6_445
O2 O2 O2 46.14(18) 3_454 6_445
O2 O2 O2 94.1(3) 4_446 6_445
O2 O2 O2 104.8(3) 3_456 6_445
Ga2 O2 O2 144.9(4) . 6_545
Ga3 O2 O2 81.02(16) 4_446 6_545
La O2 O2 41.70(19) 4_445 6_545
O2 O2 O2 106.5(4) 4_445 6_545
O2 O2 O2 145.9(2) 3_455 6_545
La O2 O2 107.8(4) . 6_545
O3 O2 O2 97.4(3) 3_565 6_545
O3 O2 O2 50.3(2) 4_445 6_545
O2 O2 O2 75.6(3) 2_556 6_545
O1 O2 O2 83.7(4) 2_455 6_545
O3 O2 O2 116.1(2) 5_446 6_545
O1 O2 O2 142.9(4) 2_456 6_545
O3 O2 O2 65.1(3) 5_445 6_545
O1 O2 O2 25.2(3) 1_545 6_545
Nb O2 O2 64.52(16) . 6_545
Ga1 O2 O2 64.52(16) . 6_545
Ga2 O2 O2 51.68(11) 2_556 6_545
O2 O2 O2 23.47(15) 2 6_545
O3 O2 O2 64.2(2) 1_545 6_545
La O2 O2 103.5(3) 4_446 6_545
Ga3 O2 O2 101.0(2) 2_455 6_545
Ga3 O2 O2 107.25(16) 2_565 6_545
La O2 O2 148.4(3) 1_556 6_545
O3 O2 O2 97.9(3) 2_456 6_545
La O2 O2 110.3(3) 2_455 6_545
Ga3 O2 O2 159.7(4) 1_556 6_545
Ga3 O2 O2 46.39(19) 4_445 6_545
O3 O2 O2 79.94(14) 6_656 6_545
O3 O2 O2 61.5(2) 2_455 6_545
Ga2 O2 O2 73.8(3) 1_554 6_545
O2 O2 O2 66.91(11) 5_446 6_545
O2 O2 O2 162.8(4) 5_456 6_545
La O2 O2 23.53(4) 2 6_545
O3 O2 O2 41.74(14) 6_655 6_545
O2 O2 O2 130.4(2) 6_556 6_545
O1 O2 O2 126.7(4) . 6_545
Ga1 O2 O2 104.28(13) 1_556 6_545
Nb O2 O2 104.28(13) 1_556 6_545
O3 O2 O2 75.12(18) 1_655 6_545
Ga2 O2 O2 141.3(3) 2_566 6_545
Ga3 O2 O2 66.73(17) 1_546 6_545
Ga3 O2 O2 72.19(5) 1_656 6_545
O2 O2 O2 57.3(2) 1_554 6_545
O2 O2 O2 122.7(2) 1_556 6_545
O3 O2 O2 162.0(2) 6_556 6_545
O2 O2 O2 28.60(14) 5_445 6_545
O2 O2 O2 108.0(5) 5_455 6_545
O3 O2 O2 101.55(15) 2_566 6_545
O2 O2 O2 120.0(3) 6_446 6_545
O2 O2 O2 54.55(9) 6_546 6_545
La O2 O2 142.7(3) 2_456 6_545
Ga2 O2 O2 18.01(13) 2 6_545
O2 O2 O2 93.5(3) 6 6_545
O3 O2 O2 89.2(2) 3_455 6_545
Ga1 O2 O2 67.99(17) 1_445 6_545
Nb O2 O2 67.99(17) 1_445 6_545
O3 O2 O2 113.5(3) 6 6_545
O3 O2 O2 135.5(3) 4_345 6_545
O3 O2 O2 71.4(2) 2_565 6_545
O3 O2 O2 143.7(4) . 6_545
O3 O2 O2 124.3(2) 3_566 6_545
O3 O2 O2 99.62(19) 4_446 6_545
La O2 O2 74.98(14) 2_556 6_545
O1 O2 O2 85.0(2) 1_546 6_545
O2 O2 O2 53.45(12) 3 6_545
O2 O2 O2 102.53(9) 4 6_545
O2 O2 O2 70.2(2) 4_444 6_545
O2 O2 O2 85.5(2) 3_454 6_545
O2 O2 O2 127.6(4) 4_446 6_545
O2 O2 O2 150.6(3) 3_456 6_545
O2 O2 O2 88.8(3) 6_445 6_545
Ga2 O2 La 119.3(3) . 1_545
Ga3 O2 La 86.9(2) 4_446 1_545
La O2 La 34.48(14) 4_445 1_545
O2 O2 La 85.6(3) 4_445 1_545
O2 O2 La 142.6(3) 3_455 1_545
La O2 La 131.0(3) . 1_545
O3 O2 La 123.6(3) 3_565 1_545
O3 O2 La 69.7(2) 4_445 1_545
O2 O2 La 63.5(3) 2_556 1_545
O1 O2 La 90.1(2) 2_455 1_545
O3 O2 La 118.9(3) 5_446 1_545
O1 O2 La 116.2(3) 2_456 1_545
O3 O2 La 91.9(2) 5_445 1_545
O1 O2 La 13.05(16) 1_545 1_545
Nb O2 La 91.47(15) . 1_545
Ga1 O2 La 91.47(15) . 1_545
Ga2 O2 La 35.11(9) 2_556 1_545
O2 O2 La 46.03(16) 2 1_545
O3 O2 La 38.87(16) 1_545 1_545
La O2 La 80.37(15) 4_446 1_545
Ga3 O2 La 75.24(12) 2_455 1_545
Ga3 O2 La 128.09(14) 2_565 1_545
La O2 La 139.0(3) 1_556 1_545
O3 O2 La 69.86(19) 2_456 1_545
La O2 La 101.94(16) 2_455 1_545
Ga3 O2 La 152.72(17) 1_556 1_545
Ga3 O2 La 70.96(12) 4_445 1_545
O3 O2 La 85.74(15) 6_656 1_545
O3 O2 La 51.86(13) 2_455 1_545
Ga2 O2 La 84.24(15) 1_554 1_545
O2 O2 La 41.99(17) 5_446 1_545
O2 O2 La 168.2(4) 5_456 1_545
La O2 La 44.44(7) 2 1_545
O3 O2 La 69.31(13) 6_655 1_545
O2 O2 La 148.62(12) 6_556 1_545
O1 O2 La 154.1(4) . 1_545
Ga1 O2 La 107.32(15) 1_556 1_545
Nb O2 La 107.32(15) 1_556 1_545
O3 O2 La 97.73(16) 1_655 1_545
Ga2 O2 La 167.69(16) 2_566 1_545
Ga3 O2 La 38.66(6) 1_546 1_545
Ga3 O2 La 87.56(10) 1_656 1_545
O2 O2 La 74.74(13) 1_554 1_545
O2 O2 La 105.26(13) 1_556 1_545
O3 O2 La 137.82(19) 6_556 1_545
O2 O2 La 23.96(10) 5_445 1_545
O2 O2 La 127.0(4) 5_455 1_545
O3 O2 La 115.40(16) 2_566 1_545
O2 O2 La 94.1(2) 6_446 1_545
O2 O2 La 44.06(15) 6_546 1_545
La O2 La 114.71(17) 2_456 1_545
Ga2 O2 La 34.56(5) 2 1_545
O2 O2 La 120.5(3) 6 1_545
O3 O2 La 66.99(13) 3_455 1_545
Ga1 O2 La 48.05(7) 1_445 1_545
Nb O2 La 48.05(7) 1_445 1_545
O3 O2 La 117.4(2) 6 1_545
O3 O2 La 125.83(18) 4_345 1_545
O3 O2 La 99.29(17) 2_565 1_545
O3 O2 La 150.8(2) . 1_545
O3 O2 La 121.9(2) 3_566 1_545
O3 O2 La 93.62(15) 4_446 1_545
La O2 La 69.74(10) 2_556 1_545
O1 O2 La 67.76(17) 1_546 1_545
O2 O2 La 69.96(15) 3 1_545
O2 O2 La 127.57(14) 4 1_545
O2 O2 La 74.47(16) 4_444 1_545
O2 O2 La 98.60(13) 3_454 1_545
O2 O2 La 101.2(2) 4_446 1_545
O2 O2 La 127.7(2) 3_456 1_545
O2 O2 La 80.41(18) 6_445 1_545
O2 O2 La 28.07(12) 6_545 1_545
Ga2 O2 O3 61.3(4) . 1_546
Ga3 O2 O3 79.7(4) 4_446 1_546
La O2 O3 91.4(3) 4_445 1_546
O2 O2 O3 64.6(2) 4_445 1_546
O2 O2 O3 100.8(2) 3_455 1_546
La O2 O3 151.2(3) . 1_546
O3 O2 O3 134.4(5) 3_565 1_546
O3 O2 O3 107.2(4) 4_445 1_546
O2 O2 O3 44.4(2) 2_556 1_546
O1 O2 O3 125.3(3) 2_455 1_546
O3 O2 O3 77.0(3) 5_446 1_546
O1 O2 O3 42.9(2) 2_456 1_546
O3 O2 O3 164.6(3) 5_445 1_546
O1 O2 O3 74.9(4) 1_545 1_546
Nb O2 O3 138.9(2) . 1_546
Ga1 O2 O3 138.9(2) . 1_546
Ga2 O2 O3 51.79(18) 2_556 1_546
O2 O2 O3 120.0(3) 2 1_546
O3 O2 O3 55.9(2) 1_545 1_546
La O2 O3 12.71(10) 4_446 1_546
Ga3 O2 O3 45.59(14) 2_455 1_546
Ga3 O2 O3 114.3(3) 2_565 1_546
La O2 O3 70.2(2) 1_556 1_546
O3 O2 O3 21.2(2) 2_456 1_546
La O2 O3 95.52(18) 2_455 1_546
Ga3 O2 O3 94.4(2) 1_556 1_546
Ga3 O2 O3 144.9(2) 4_445 1_546
O3 O2 O3 79.4(2) 6_656 1_546
O3 O2 O3 89.8(3) 2_455 1_546
Ga2 O2 O3 132.58(18) 1_554 1_546
O2 O2 O3 33.1(3) 5_446 1_546
O2 O2 O3 94.2(4) 5_456 1_546
La O2 O3 102.18(19) 2 1_546
O3 O2 O3 131.4(2) 6_655 1_546
O2 O2 O3 104.6(4) 6_556 1_546
O1 O2 O3 131.7(4) . 1_546
Ga1 O2 O3 75.5(2) 1_556 1_546
Nb O2 O3 75.5(2) 1_556 1_546
O3 O2 O3 121.2(3) 1_655 1_546
Ga2 O2 O3 112.1(2) 2_566 1_546
Ga3 O2 O3 40.32(13) 1_546 1_546
Ga3 O2 O3 100.4(2) 1_656 1_546
O2 O2 O3 140.84(13) 1_554 1_546
O2 O2 O3 39.16(13) 1_556 1_546
O3 O2 O3 74.56(18) 6_556 1_546
O2 O2 O3 91.5(2) 5_445 1_546
O2 O2 O3 145.9(3) 5_455 1_546
O3 O2 O3 98.1(2) 2_566 1_546
O2 O2 O3 48.4(2) 6_446 1_546
O2 O2 O3 56.0(3) 6_546 1_546
La O2 O3 48.51(14) 2_456 1_546
Ga2 O2 O3 108.16(18) 2 1_546
O2 O2 O3 164.5(3) 6 1_546
O3 O2 O3 59.87(17) 3_455 1_546
Ga1 O2 O3 68.65(14) 1_445 1_546
Nb O2 O3 68.65(14) 1_445 1_546
O3 O2 O3 118.5(2) 6 1_546
O3 O2 O3 93.14(19) 4_345 1_546
O3 O2 O3 150.02(19) 2_565 1_546
O3 O2 O3 110.9(3) . 1_546
O3 O2 O3 69.5(2) 3_566 1_546
O3 O2 O3 55.9(2) 4_446 1_546
La O2 O3 57.51(14) 2_556 1_546
O1 O2 O3 30.97(10) 1_546 1_546
O2 O2 O3 100.87(15) 3 1_546
O2 O2 O3 128.04(12) 4 1_546
O2 O2 O3 118.4(2) 4_444 1_546
O2 O2 O3 140.4(2) 3_454 1_546
O2 O2 O3 27.63(16) 4_446 1_546
O2 O2 O3 53.78(14) 3_456 1_546
O2 O2 O3 94.5(2) 6_445 1_546
O2 O2 O3 100.0(3) 6_545 1_546
La O2 O3 74.05(15) 1_545 1_546
Ga2 O2 O3 126.4(4) . 3_564
Ga3 O2 O3 102.4(4) 4_446 3_564
La O2 O3 75.6(3) 4_445 3_564
O2 O2 O3 112.88(12) 4_445 3_564
O2 O2 O3 88.6(2) 3_455 3_564
La O2 O3 40.70(19) . 3_564
O3 O2 O3 55.5(3) 3_565 3_564
O3 O2 O3 69.0(3) 4_445 3_564
O2 O2 O3 131.2(3) 2_556 3_564
O1 O2 O3 50.7(3) 2_455 3_564
O3 O2 O3 112.7(3) 5_446 3_564
O1 O2 O3 149.7(3) 2_456 3_564
O3 O2 O3 8.82(17) 5_445 3_564
O1 O2 O3 92.3(4) 1_545 3_564
Nb O2 O3 41.40(16) . 3_564
Ga1 O2 O3 41.40(16) . 3_564
Ga2 O2 O3 117.3(2) 2_556 3_564
O2 O2 O3 46.3(2) 2 3_564
O3 O2 O3 111.7(3) 1_545 3_564
La O2 O3 168.48(18) 4_446 3_564
Ga3 O2 O3 129.4(2) 2_455 3_564
Ga3 O2 O3 75.78(18) 2_565 3_564
La O2 O3 123.4(2) 1_556 3_564
O3 O2 O3 150.3(3) 2_456 3_564
La O2 O3 84.9(2) 2_455 3_564
Ga3 O2 O3 96.9(2) 1_556 3_564
Ga3 O2 O3 21.35(10) 4_445 3_564
O3 O2 O3 102.4(2) 6_656 3_564
O3 O2 O3 79.7(2) 2_455 3_564
Ga2 O2 O3 40.97(13) 1_554 3_564
O2 O2 O3 133.8(3) 5_446 3_564
O2 O2 O3 99.4(3) 5_456 3_564
La O2 O3 68.22(16) 2 3_564
O3 O2 O3 41.2(2) 6_655 3_564
O2 O2 O3 88.2(3) 6_556 3_564
O1 O2 O3 62.0(3) . 3_564
Ga1 O2 O3 111.75(17) 1_556 3_564
Nb O2 O3 111.75(17) 1_556 3_564
O3 O2 O3 62.02(18) 1_655 3_564
Ga2 O2 O3 81.75(18) 2_566 3_564
Ga3 O2 O3 126.1(2) 1_546 3_564
Ga3 O2 O3 80.99(15) 1_656 3_564
O2 O2 O3 27.64(11) 1_554 3_564
O2 O2 O3 152.36(11) 1_556 3_564
O3 O2 O3 116.0(2) 6_556 3_564
O2 O2 O3 74.7(3) 5_445 3_564
O2 O2 O3 43.2(2) 5_455 3_564
O3 O2 O3 89.8(2) 2_566 3_564
O2 O2 O3 132.7(3) 6_446 3_564
O2 O2 O3 115.4(2) 6_546 3_564
La O2 O3 140.64(19) 2_456 3_564
Ga2 O2 O3 58.03(15) 2 3_564
O2 O2 O3 29.27(18) 6 3_564
O3 O2 O3 113.0(3) 3_455 3_564
Ga1 O2 O3 100.6(2) 1_445 3_564
Nb O2 O3 100.6(2) 1_445 3_564
O3 O2 O3 65.41(18) 6 3_564
O3 O2 O3 93.1(2) 4_345 3_564
O3 O2 O3 32.93(19) 2_565 3_564
O3 O2 O3 79.9(2) . 3_564
O3 O2 O3 121.4(2) 3_566 3_564
O3 O2 O3 129.09(16) 4_446 3_564
La O2 O3 120.45(15) 2_556 3_564
O1 O2 O3 144.87(17) 1_546 3_564
O2 O2 O3 75.94(9) 3 3_564
O2 O2 O3 62.37(11) 4 3_564
O2 O2 O3 53.74(11) 4_444 3_564
O2 O2 O3 37.86(13) 3_454 3_564
O2 O2 O3 164.6(2) 4_446 3_564
O2 O2 O3 140.0(2) 3_456 3_564
O2 O2 O3 80.7(3) 6_445 3_564
O2 O2 O3 67.2(2) 6_545 3_564
La O2 O3 92.30(17) 1_545 3_564
O3 O2 O3 166.1(2) 1_546 3_564
Ga2 O2 O2 96.9(4) . 3_445
Ga3 O2 O2 93.7(2) 4_446 3_445
La O2 O2 41.1(3) 4_445 3_445
O2 O2 O2 67.7(4) 4_445 3_445
O2 O2 O2 127.7(4) 3_455 3_445
La O2 O2 145.2(2) . 3_445
O3 O2 O2 144.8(3) 3_565 3_445
O3 O2 O2 88.50(19) 4_445 3_445
O2 O2 O2 59.2(2) 2_556 3_445
O1 O2 O2 94.2(2) 2_455 3_445
O3 O2 O2 116.9(3) 5_446 3_445
O1 O2 O2 94.1(2) 2_456 3_445
O3 O2 O2 113.58(18) 5_445 3_445
O1 O2 O2 31.50(12) 1_545 3_445
Nb O2 O2 114.10(13) . 3_445
Ga1 O2 O2 114.10(13) . 3_445
Ga2 O2 O2 34.40(9) 2_556 3_445
O2 O2 O2 67.0(2) 2 3_445
O3 O2 O2 21.05(17) 1_545 3_445
La O2 O2 62.58(13) 4_446 3_445
Ga3 O2 O2 53.81(16) 2_455 3_445
Ga3 O2 O2 141.93(17) 2_565 3_445
La O2 O2 123.42(16) 1_556 3_445
O3 O2 O2 46.7(2) 2_456 3_445
La O2 O2 91.9(2) 2_455 3_445
Ga3 O2 O2 132.9(2) 1_556 3_445
Ga3 O2 O2 91.56(9) 4_445 3_445
O3 O2 O2 92.56(12) 6_656 3_445
O3 O2 O2 50.1(2) 2_455 3_445
Ga2 O2 O2 92.71(14) 1_554 3_445
O2 O2 O2 26.4(3) 5_446 3_445
O2 O2 O2 145.5(3) 5_456 3_445
La O2 O2 65.89(7) 2 3_445
O3 O2 O2 92.42(11) 6_655 3_445
O2 O2 O2 152.0(3) 6_556 3_445
O1 O2 O2 170.9(3) . 3_445
Ga1 O2 O2 107.96(10) 1_556 3_445
Nb O2 O2 107.96(10) 1_556 3_445
O3 O2 O2 116.79(16) 1_655 3_445
Ga2 O2 O2 165.78(17) 2_566 3_445
Ga3 O2 O2 15.49(12) 1_546 3_445
Ga3 O2 O2 101.75(11) 1_656 3_445
O2 O2 O2 90.0 1_554 3_445
O2 O2 O2 90.0 1_556 3_445
O3 O2 O2 115.3(2) 6_556 3_445
O2 O2 O2 38.0(2) 5_445 3_445
O2 O2 O2 136.5(2) 5_455 3_445
O3 O2 O2 124.17(16) 2_566 3_445
O2 O2 O2 72.0(3) 6_446 3_445
O2 O2 O2 46.35(13) 6_546 3_445
La O2 O2 91.49(17) 2_456 3_445
Ga2 O2 O2 54.83(10) 2 3_445
O2 O2 O2 141.7(2) 6 3_445
O3 O2 O2 49.53(18) 3_455 3_445
Ga1 O2 O2 36.17(15) 1_445 3_445
Nb O2 O2 36.17(15) 1_445 3_445
O3 O2 O2 114.1(2) 6 3_445
O3 O2 O2 110.9(2) 4_345 3_445
O3 O2 O2 122.47(15) 2_565 3_445
O3 O2 O2 139.6(2) . 3_445
O3 O2 O2 115.00(15) 3_566 3_445
O3 O2 O2 89.22(10) 4_446 3_445
La O2 O2 70.36(6) 2_556 3_445
O1 O2 O2 57.49(14) 1_546 3_445
O2 O2 O2 86.91(16) 3 3_445
O2 O2 O2 146.91(16) 4 3_445
O2 O2 O2 79.54(19) 4_444 3_445
O2 O2 O2 107.04(16) 3_454 3_445
O2 O2 O2 79.54(19) 4_446 3_445
O2 O2 O2 107.04(16) 3_456 3_445
O2 O2 O2 73.7(2) 6_445 3_445
O2 O2 O2 51.27(17) 6_545 3_445
La O2 O2 23.22(8) 1_545 3_445
O3 O2 O2 53.73(14) 1_546 3_445
O3 O2 O2 112.43(11) 3_564 3_445
Ga2 O2 O2 145.3(4) . 4_545
Ga3 O2 O2 45.2(3) 4_446 4_545
La O2 O2 74.66(15) 4_445 4_545
O2 O2 O2 127.7(4) 4_445 4_545
O2 O2 O2 172.3(4) 3_455 4_545
La O2 O2 123.1(2) . 4_545
O3 O2 O2 85.4(3) 3_565 4_545
O3 O2 O2 29.2(2) 4_445 4_545
O2 O2 O2 44.7(4) 2_556 4_545
O1 O2 O2 119.9(3) 2_455 4_545
O3 O2 O2 80.3(2) 5_446 4_545
O1 O2 O2 119.2(3) 2_456 4_545
O3 O2 O2 81.4(2) 5_445 4_545
O1 O2 O2 31.50(12) 1_545 4_545
Nb O2 O2 60.49(16) . 4_545
Ga1 O2 O2 60.49(16) . 4_545
Ga2 O2 O2 34.40(9) 2_556 4_545
O2 O2 O2 57.2(3) 2 4_545
O3 O2 O2 80.51(17) 1_545 4_545
La O2 O2 80.70(9) 4_446 4_545
Ga3 O2 O2 111.98(17) 2_455 4_545
Ga3 O2 O2 84.20(17) 2_565 4_545
La O2 O2 111.51(14) 1_556 4_545
O3 O2 O2 94.61(17) 2_456 4_545
La O2 O2 145.30(17) 2_455 4_545
Ga3 O2 O2 160.96(19) 1_556 4_545
Ga3 O2 O2 72.60(11) 4_445 4_545
O3 O2 O2 44.07(16) 6_656 4_545
O3 O2 O2 94.32(16) 2_455 4_545
Ga2 O2 O2 109.02(9) 1_554 4_545
O2 O2 O2 56.84(12) 5_446 4_545
O2 O2 O2 137.0(3) 5_456 4_545
La O2 O2 20.48(16) 2 4_545
O3 O2 O2 47.40(18) 6_655 4_545
O2 O2 O2 104.27(11) 6_556 4_545
O1 O2 O2 124.8(2) . 4_545
Ga1 O2 O2 68.17(12) 1_556 4_545
Nb O2 O2 68.17(12) 1_556 4_545
O3 O2 O2 56.95(16) 1_655 4_545
Ga2 O2 O2 124.11(19) 2_566 4_545
Ga3 O2 O2 71.02(9) 1_546 4_545
Ga3 O2 O2 43.22(11) 1_656 4_545
O2 O2 O2 90.0 1_554 4_545
O2 O2 O2 90.000(1) 1_556 4_545
O3 O2 O2 153.50(19) 6_556 4_545
O2 O2 O2 61.21(11) 5_445 4_545
O2 O2 O2 130.1(3) 5_455 4_545
O3 O2 O2 71.17(17) 2_566 4_545
O2 O2 O2 127.1(3) 6_446 4_545
O2 O2 O2 28.0(2) 6_546 4_545
La O2 O2 131.51(14) 2_456 4_545
Ga2 O2 O2 54.83(10) 2 4_545
O2 O2 O2 102.65(10) 6 4_545
O3 O2 O2 109.39(18) 3_455 4_545
Ga1 O2 O2 92.31(12) 1_445 4_545
Nb O2 O2 92.31(12) 1_445 4_545
O3 O2 O2 148.79(16) 6 4_545
O3 O2 O2 170.3(2) 4_345 4_545
O3 O2 O2 72.03(16) 2_565 4_545
O3 O2 O2 159.9(2) . 4_545
O3 O2 O2 87.61(13) 3_566 4_545
O3 O2 O2 63.22(13) 4_446 4_545
La O2 O2 39.57(11) 2_556 4_545
O1 O2 O2 57.49(14) 1_546 4_545
O2 O2 O2 26.91(16) 3 4_545
O2 O2 O2 86.91(16) 4 4_545
O2 O2 O2 107.04(16) 4_444 4_545
O2 O2 O2 118.33(11) 3_454 4_545
O2 O2 O2 107.04(16) 4_446 4_545
O2 O2 O2 118.33(11) 3_456 4_545
O2 O2 O2 123.18(19) 6_445 4_545
O2 O2 O2 36.86(19) 6_545 4_545
La O2 O2 44.46(7) 1_545 4_545
O3 O2 O2 84.00(11) 1_546 4_545
O3 O2 O2 87.84(12) 3_564 4_545
O2 O2 O2 60.0 3_445 4_545
Ga2 O2 O3 144.7(5) . 4_444
Ga3 O2 O3 94.0(3) 4_446 4_444
La O2 O3 58.7(3) 4_445 4_444
O2 O2 O3 115.05(15) 4_445 4_444
O2 O2 O3 111.93(18) 3_455 4_444
La O2 O3 66.2(2) . 4_444
O3 O2 O3 69.1(3) 3_565 4_444
O3 O2 O3 55.6(3) 4_445 4_444
O2 O2 O3 110.7(4) 2_556 4_444
O1 O2 O3 60.1(3) 2_455 4_444
O3 O2 O3 118.3(3) 5_446 4_444
O1 O2 O3 174.8(3) 2_456 4_444
O3 O2 O3 24.32(17) 5_445 4_444
O1 O2 O3 66.8(4) 1_545 4_444
Nb O2 O3 41.45(16) . 4_444
Ga1 O2 O3 41.45(16) . 4_444
Ga2 O2 O3 92.23(17) 2_556 4_444
O2 O2 O3 22.34(17) 2 4_444
O3 O2 O3 94.1(3) 1_545 4_444
La O2 O3 144.56(18) 4_446 4_444
Ga3 O2 O3 123.8(2) 2_455 4_444
Ga3 O2 O3 87.20(19) 2_565 4_444
La O2 O3 142.1(2) 1_556 4_444
O3 O2 O3 134.1(2) 2_456 4_444
La O2 O3 96.2(2) 2_455 4_444
Ga3 O2 O3 121.8(3) 1_556 4_444
Ga3 O2 O3 6.78(10) 4_445 4_444
O3 O2 O3 93.6(2) 6_656 4_444
O3 O2 O3 70.04(19) 2_455 4_444
Ga2 O2 O3 48.12(16) 1_554 4_444
O2 O2 O3 108.5(3) 5_446 4_444
O2 O2 O3 124.2(3) 5_456 4_444
La O2 O3 45.54(13) 2 4_444
O3 O2 O3 26.4(3) 6_655 4_444
O2 O2 O3 105.8(3) 6_556 4_444
O1 O2 O3 86.4(3) . 4_444
Ga1 O2 O3 111.82(16) 1_556 4_444
Nb O2 O3 111.82(16) 1_556 4_444
O3 O2 O3 62.06(16) 1_655 4_444
Ga2 O2 O3 104.8(2) 2_566 4_444
Ga3 O2 O3 104.24(16) 1_546 4_444
Ga3 O2 O3 74.52(15) 1_656 4_444
O2 O2 O3 27.57(13) 1_554 4_444
O2 O2 O3 152.43(13) 1_556 4_444
O3 O2 O3 139.8(2) 6_556 4_444
O2 O2 O3 53.5(2) 5_445 4_444
O2 O2 O3 67.7(3) 5_455 4_444
O3 O2 O3 94.6(2) 2_566 4_444
O2 O2 O3 137.0(3) 6_446 4_444
O2 O2 O3 92.0(2) 6_546 4_444
La O2 O3 158.9(2) 2_456 4_444
Ga2 O2 O3 34.63(10) 2 4_444
O2 O2 O3 52.9(2) 6 4_444
O3 O2 O3 106.6(3) 3_455 4_444
Ga1 O2 O3 88.17(18) 1_445 4_444
Nb O2 O3 88.17(18) 1_445 4_444
O3 O2 O3 83.9(2) 6 4_444
O3 O2 O3 112.3(3) 4_345 4_444
O3 O2 O3 40.5(2) 2_565 4_444
O3 O2 O3 104.6(3) . 4_444
O3 O2 O3 129.08(16) 3_566 4_444
O3 O2 O3 121.59(18) 4_446 4_444
La O2 O3 103.67(13) 2_556 4_444
O1 O2 O3 123.03(18) 1_546 4_444
O2 O2 O3 62.44(13) 3 4_444
O2 O2 O3 75.98(10) 4 4_444
O2 O2 O3 54.87(13) 4_444 4_444
O2 O2 O3 53.18(14) 3_454 4_444
O2 O2 O3 168.8(2) 4_446 4_444
O2 O2 O3 163.1(2) 3_456 4_444
O2 O2 O3 83.4(3) 6_445 4_444
O2 O2 O3 41.7(2) 6_545 4_444
La O2 O3 67.64(12) 1_545 4_444
O3 O2 O3 141.47(17) 1_546 4_444
O3 O2 O3 25.49(13) 3_564 4_444
O2 O2 O3 89.30(9) 3_445 4_444
O2 O2 O3 66.00(12) 4_545 4_444
Ga2 O2 O1 37.2(3) . 1_445
Ga3 O2 O1 153.8(5) 4_446 1_445
La O2 O1 71.3(2) 4_445 1_445
O2 O2 O1 13.7(2) 4_445 1_445
O2 O2 O1 47.8(2) 3_455 1_445
La O2 O1 85.9(2) . 1_445
O3 O2 O1 132.8(3) 3_565 1_445
O3 O2 O1 163.0(4) 4_445 1_445
O2 O2 O1 119.8(3) 2_556 1_445
O1 O2 O1 53.4(4) 2_455 1_445
O3 O2 O1 126.9(3) 5_446 1_445
O1 O2 O1 65.5(4) 2_456 1_445
O3 O2 O1 112.3(3) 5_445 1_445
O1 O2 O1 108.7(2) 1_545 1_445
Nb O2 O1 144.5(4) . 1_445
Ga1 O2 O1 144.5(4) . 1_445
Ga2 O2 O1 110.99(19) 2_556 1_445
O2 O2 O1 104.0(3) 2 1_445
O3 O2 O1 59.45(15) 1_545 1_445
La O2 O1 86.2(2) 4_446 1_445
Ga3 O2 O1 33.45(13) 2_455 1_445
Ga3 O2 O1 135.78(16) 2_565 1_445
La O2 O1 94.2(2) 1_556 1_445
O3 O2 O1 57.29(19) 2_456 1_445
La O2 O1 19.31(17) 2_455 1_445
Ga3 O2 O1 56.82(10) 1_556 1_445
Ga3 O2 O1 105.3(3) 4_445 1_445
O3 O2 O1 154.0(4) 6_656 1_445
O3 O2 O1 51.7(2) 2_455 1_445
Ga2 O2 O1 64.6(2) 1_554 1_445
O2 O2 O1 90.3(2) 5_446 1_445
O2 O2 O1 79.7(2) 5_456 1_445
La O2 O1 136.5(2) 2 1_445
O3 O2 O1 137.5(3) 6_655 1_445
O2 O2 O1 114.30(12) 6_556 1_445
O1 O2 O1 93.79(13) . 1_445
Ga1 O2 O1 136.2(3) 1_556 1_445
Nb O2 O1 136.2(3) 1_556 1_445
O3 O2 O1 160.3(3) 1_655 1_445
Ga2 O2 O1 95.80(12) 2_566 1_445
Ga3 O2 O1 71.31(11) 1_546 1_445
Ga3 O2 O1 174.0(3) 1_656 1_445
O2 O2 O1 84.2(2) 1_554 1_445
O2 O2 O1 95.8(2) 1_556 1_445
O3 O2 O1 49.2(2) 6_556 1_445
O2 O2 O1 84.5(2) 5_445 1_445
O2 O2 O1 75.1(2) 5_455 1_445
O3 O2 O1 145.4(2) 2_566 1_445
O2 O2 O1 29.2(2) 6_446 1_445
O2 O2 O1 122.0(3) 6_546 1_445
La O2 O1 48.4(2) 2_456 1_445
Ga2 O2 O1 98.8(2) 2 1_445
O2 O2 O1 105.6(2) 6 1_445
O3 O2 O1 30.75(9) 3_455 1_445
Ga1 O2 O1 48.04(9) 1_445 1_445
Nb O2 O1 48.04(9) 1_445 1_445
O3 O2 O1 43.94(15) 6 1_445
O3 O2 O1 30.75(9) 4_345 1_445
O3 O2 O1 133.8(3) 2_565 1_445
O3 O2 O1 59.36(9) . 1_445
O3 O2 O1 116.4(3) 3_566 1_445
O3 O2 O1 125.9(3) 4_446 1_445
La O2 O1 133.6(3) 2_556 1_445
O1 O2 O1 107.0(3) 1_546 1_445
O2 O2 O1 165.9(2) 3 1_445
O2 O2 O1 132.6(2) 4 1_445
O2 O2 O1 56.4(3) 4_444 1_445
O2 O2 O1 65.8(2) 3_454 1_445
O2 O2 O1 67.9(3) 4_446 1_445
O2 O2 O1 76.5(3) 3_456 1_445
O2 O2 O1 28.4(2) 6_445 1_445
O2 O2 O1 113.0(2) 6_545 1_445
La O2 O1 96.07(13) 1_545 1_445
O3 O2 O1 76.2(2) 1_546 1_445
O3 O2 O1 103.5(3) 3_564 1_445
O2 O2 O1 80.26(18) 3_445 1_445
O2 O2 O1 139.86(17) 4_545 1_445
O3 O2 O1 111.2(3) 4_444 1_445
Ga2 O2 O3 71.4(3) . 6_546
Ga3 O2 O3 96.7(4) 4_446 6_546
La O2 O3 61.8(3) 4_445 6_546
O2 O2 O3 52.7(3) 4_445 6_546
O2 O2 O3 108.0(3) 3_455 6_546
La O2 O3 151.5(2) . 6_546
O3 O2 O3 158.6(3) 3_565 6_546
O3 O2 O3 108.1(3) 4_445 6_546
O2 O2 O3 56.93(13) 2_556 6_546
O1 O2 O3 102.3(2) 2_455 6_546
O3 O2 O3 104.9(4) 5_446 6_546
O1 O2 O3 66.5(2) 2_456 6_546
O3 O2 O3 140.4(3) 5_445 6_546
O1 O2 O3 56.9(2) 1_545 6_546
Nb O2 O3 138.88(18) . 6_546
Ga1 O2 O3 138.88(18) . 6_546
Ga2 O2 O3 45.54(13) 2_556 6_546
O2 O2 O3 94.15(17) 2 6_546
O3 O2 O3 26.4(3) 1_545 6_546
La O2 O3 41.32(14) 4_446 6_546
Ga3 O2 O3 33.59(12) 2_455 6_546
Ga3 O2 O3 141.3(3) 2_565 6_546
La O2 O3 99.0(2) 1_556 6_546
O3 O2 O3 19.05(17) 2_456 6_546
La O2 O3 83.56(16) 2_455 6_546
Ga3 O2 O3 108.52(19) 1_556 6_546
Ga3 O2 O3 117.88(19) 4_445 6_546
O3 O2 O3 95.9(2) 6_656 6_546
O3 O2 O3 61.36(14) 2_455 6_546
Ga2 O2 O3 106.18(19) 1_554 6_546
O2 O2 O3 23.87(16) 5_446 6_546
O2 O2 O3 117.7(3) 5_456 6_546
La O2 O3 90.62(15) 2 6_546
O3 O2 O3 119.18(18) 6_655 6_546
O2 O2 O3 134.2(4) 6_556 6_546
O1 O2 O3 153.5(2) . 6_546
Ga1 O2 O3 100.7(2) 1_556 6_546
Nb O2 O3 100.7(2) 1_556 6_546
O3 O2 O3 133.2(2) 1_655 6_546
Ga2 O2 O3 138.5(2) 2_566 6_546
Ga3 O2 O3 12.36(10) 1_546 6_546
Ga3 O2 O3 113.0(2) 1_656 6_546
O2 O2 O3 111.24(15) 1_554 6_546
O2 O2 O3 68.76(15) 1_556 6_546
O3 O2 O3 89.22(19) 6_556 6_546
O2 O2 O3 63.40(19) 5_445 6_546
O2 O2 O3 140.1(2) 5_455 6_546
O3 O2 O3 122.7(3) 2_566 6_546
O2 O2 O3 48.35(19) 6_446 6_546
O2 O2 O3 55.7(2) 6_546 6_546
La O2 O3 64.14(14) 2_456 6_546
Ga2 O2 O3 81.86(14) 2 6_546
O2 O2 O3 164.9(3) 6 6_546
O3 O2 O3 39.3(2) 3_455 6_546
Ga1 O2 O3 40.66(14) 1_445 6_546
Nb O2 O3 40.66(14) 1_445 6_546
O3 O2 O3 109.19(19) 6 6_546
O3 O2 O3 93.79(14) 4_345 6_546
O3 O2 O3 149.07(16) 2_565 6_546
O3 O2 O3 120.5(2) . 6_546
O3 O2 O3 98.6(2) 3_566 6_546
O3 O2 O3 80.0(2) 4_446 6_546
La O2 O3 71.14(16) 2_556 6_546
O1 O2 O3 48.04(15) 1_546 6_546
O2 O2 O3 104.18(19) 3 6_546
O2 O2 O3 154.33(18) 4 6_546
O2 O2 O3 91.6(2) 4_444 6_546
O2 O2 O3 117.8(2) 3_454 6_546
O2 O2 O3 52.51(19) 4_446 6_546
O2 O2 O3 80.22(19) 3_456 6_546
O2 O2 O3 73.5(2) 6_445 6_546
O2 O2 O3 78.9(2) 6_545 6_546
La O2 O3 50.82(11) 1_545 6_546
O3 O2 O3 29.6(2) 1_546 6_546
O3 O2 O3 137.39(19) 3_564 6_546
O2 O2 O3 27.78(13) 3_445 6_546
O2 O2 O3 79.13(12) 4_545 6_546
O3 O2 O3 116.49(18) 4_444 6_546
O1 O2 O3 66.39(16) 1_445 6_546
Ga3 O3 Nb 113.2(3) 1_556 1_455
Ga3 O3 Ga1 113.2(3) 1_556 1_455
Nb O3 Ga1 0.0 1_455 1_455
Ga3 O3 La 137.8(4) 1_556 4_455
Nb O3 La 104.6(5) 1_455 4_455
Ga1 O3 La 104.6(5) 1_455 4_455
Ga3 O3 Ga3 95.5(5) 1_556 2_465
Nb O3 Ga3 87.2(3) 1_455 2_465
Ga1 O3 Ga3 87.2(3) 1_455 2_465
La O3 Ga3 104.7(3) 4_455 2_465
Ga3 O3 O3 155.3(6) 1_556 2_465
Nb O3 O3 48.1(3) 1_455 2_465
Ga1 O3 O3 48.1(3) 1_455 2_465
La O3 O3 56.5(2) 4_455 2_465
Ga3 O3 O3 98.8(4) 2_465 2_465
Ga3 O3 O3 66.3(3) 1_556 4_345
Nb O3 O3 47.1(2) 1_455 4_345
Ga1 O3 O3 47.1(2) 1_455 4_345
La O3 O3 149.2(3) 4_455 4_345
Ga3 O3 O3 87.8(2) 2_465 4_345
O3 O3 O3 94.20(6) 2_465 4_345
Ga3 O3 O3 106.5(2) 1_556 3_465
Nb O3 O3 47.1(2) 1_455 3_465
Ga1 O3 O3 47.1(2) 1_455 3_465
La O3 O3 112.9(4) 4_455 3_465
Ga3 O3 O3 40.3(3) 2_465 3_465
O3 O3 O3 73.2(4) 2_465 3_465
O3 O3 O3 60.000(1) 4_345 3_465
Ga3 O3 O2 126.6(7) 1_556 4_455
Nb O3 O2 95.3(3) 1_455 4_455
Ga1 O3 O2 95.3(3) 1_455 4_455
La O3 O2 64.9(3) 4_455 4_455
Ga3 O3 O2 39.8(3) 2_465 4_455
O3 O3 O2 75.8(4) 2_465 4_455
O3 O3 O2 121.2(4) 4_345 4_455
O3 O3 O2 61.6(4) 3_465 4_455
Ga3 O3 O3 63.2(4) 1_556 2_466
Nb O3 O3 119.0(4) 1_455 2_466
Ga1 O3 O3 119.0(4) 1_455 2_466
La O3 O3 113.6(3) 4_455 2_466
Ga3 O3 O3 39.1(2) 2_465 2_466
O3 O3 O3 136.5(7) 2_465 2_466
O3 O3 O3 93.94(7) 4_345 2_466
O3 O3 O3 74.3(3) 3_465 2_466
O2 O3 O3 63.6(4) 4_455 2_466
Ga3 O3 O2 40.0(3) 1_556 3_455
Nb O3 O2 95.6(4) 1_455 3_455
Ga1 O3 O2 95.6(4) 1_455 3_455
La O3 O2 120.4(4) 4_455 3_455
Ga3 O3 O2 132.2(5) 2_465 3_455
O3 O3 O2 118.2(7) 2_465 3_455
O3 O3 O2 62.0(3) 4_345 3_455
O3 O3 O2 121.5(3) 3_465 3_455
O2 O3 O2 165.9(7) 4_455 3_455
O3 O3 O2 103.2(5) 2_466 3_455
Ga3 O3 O2 36.3(2) 1_556 5_456
Nb O3 O2 149.3(4) 1_455 5_456
Ga1 O3 O2 149.3(4) 1_455 5_456
La O3 O2 103.4(3) 4_455 5_456
Ga3 O3 O2 97.8(5) 2_465 5_456
O3 O3 O2 156.8(4) 2_465 5_456
O3 O3 O2 102.6(3) 4_345 5_456
O3 O3 O2 129.2(3) 3_465 5_456
O2 O3 O2 107.9(4) 4_455 5_456
O3 O3 O2 58.8(4) 2_466 5_456
O2 O3 O2 58.8(5) 3_455 5_456
Ga3 O3 O3 101.2(3) 1_556 6
Nb O3 O3 36.4(3) 1_455 6
Ga1 O3 O3 36.4(3) 1_455 6
La O3 O3 98.0(5) 4_455 6
Ga3 O3 O3 123.17(18) 2_465 6
O3 O3 O3 54.1(5) 2_465 6
O3 O3 O3 52.6(3) 4_345 6
O3 O3 O3 82.9(2) 3_465 6
O2 O3 O3 125.6(5) 4_455 6
O3 O3 O3 146.2(3) 2_466 6
O2 O3 O3 67.9(3) 3_455 6
O2 O3 O3 126.5(3) 5_456 6
Ga3 O3 O1 86.4(4) 1_556 .
Nb O3 O1 134.1(6) 1_455 .
Ga1 O3 O1 134.1(6) 1_455 .
La O3 O1 53.1(3) 4_455 .
Ga3 O3 O1 133.9(4) 2_465 .
O3 O3 O1 97.9(5) 2_465 .
O3 O3 O1 133.3(4) 4_345 .
O3 O3 O1 165.5(4) 3_465 .
O2 O3 O1 105.5(3) 4_455 .
O3 O3 O1 106.9(5) 2_466 .
O2 O3 O1 72.7(3) 3_455 .
O2 O3 O1 58.9(5) 5_456 .
O3 O3 O1 101.3(4) 6 .
Ga3 O3 O2 112.0(4) 1_556 5_455
Nb O3 O2 80.4(4) 1_455 5_455
Ga1 O3 O2 80.4(4) 1_455 5_455
La O3 O2 55.9(3) 4_455 5_455
Ga3 O3 O2 152.5(4) 2_465 5_455
O3 O3 O2 54.9(4) 2_465 5_455
O3 O3 O2 101.1(3) 4_345 5_455
O3 O3 O2 124.0(2) 3_465 5_455
O2 O3 O2 116.8(4) 4_455 5_455
O3 O3 O2 160.6(3) 2_466 5_455
O2 O3 O2 73.9(4) 3_455 5_455
O2 O3 O2 105.4(3) 5_456 5_455
O3 O3 O2 51.3(3) 6 5_455
O1 O3 O2 53.7(4) . 5_455
Ga3 O3 O3 23.5(3) 1_556 6_556
Nb O3 O3 99.8(3) 1_455 6_556
Ga1 O3 O3 99.8(3) 1_455 6_556
La O3 O3 155.6(5) 4_455 6_556
Ga3 O3 O3 75.2(3) 2_465 6_556
O3 O3 O3 147.9(3) 2_465 6_556
O3 O3 O3 54.5(4) 4_345 6_556
O3 O3 O3 83.2(2) 3_465 6_556
O2 O3 O3 112.0(5) 4_455 6_556
O3 O3 O3 51.2(4) 2_466 6_556
O2 O3 O3 57.2(3) 3_455 6_556
O2 O3 O3 53.2(3) 5_456 6_556
O3 O3 O3 102.2(4) 6 6_556
O1 O3 O3 109.0(4) . 6_556
O2 O3 O3 131.0(3) 5_455 6_556
Ga3 O3 Ga2 65.1(2) 1_556 2_566
Nb O3 Ga2 160.7(5) 1_455 2_566
Ga1 O3 Ga2 160.7(5) 1_455 2_566
La O3 Ga2 73.07(18) 4_455 2_566
Ga3 O3 Ga2 112.0(4) 2_465 2_566
O3 O3 Ga2 126.1(3) 2_465 2_566
O3 O3 Ga2 128.7(3) 4_345 2_566
O3 O3 Ga2 151.9(3) 3_465 2_566
O2 O3 Ga2 100.6(3) 4_455 2_566
O3 O3 Ga2 78.2(3) 2_466 2_566
O2 O3 Ga2 70.6(3) 3_455 2_566
O2 O3 Ga2 31.13(19) 5_456 2_566
O3 O3 Ga2 124.4(2) 6 2_566
O1 O3 Ga2 30.0(4) . 2_566
O2 O3 Ga2 82.8(3) 5_455 2_566
O3 O3 Ga2 84.2(3) 6_556 2_566
Ga3 O3 Ga3 64.0(2) 1_556 4_346
Nb O3 Ga3 60.0(2) 1_455 4_346
Ga1 O3 Ga3 60.0(2) 1_455 4_346
La O3 Ga3 157.5(3) 4_455 4_346
Ga3 O3 Ga3 60.88(19) 2_465 4_346
O3 O3 Ga3 106.24(17) 2_465 4_346
O3 O3 Ga3 28.47(15) 4_345 4_346
O3 O3 Ga3 44.75(17) 3_465 4_346
O2 O3 Ga3 98.5(3) 4_455 4_346
O3 O3 Ga3 67.32(19) 2_466 4_346
O2 O3 Ga3 79.5(2) 3_455 4_346
O2 O3 Ga3 96.0(3) 5_456 4_346
O3 O3 Ga3 78.9(2) 6 4_346
O1 O3 Ga3 149.4(4) . 4_346
O2 O3 Ga3 129.3(3) 5_455 4_346
O3 O3 Ga3 42.94(14) 6_556 4_346
Ga2 O3 Ga3 127.1(3) 2_566 4_346
Ga3 O3 La 73.7(3) 1_556 .
Nb O3 La 101.6(4) 1_455 .
Ga1 O3 La 101.6(4) 1_455 .
La O3 La 81.1(3) 4_455 .
Ga3 O3 La 168.0(4) 2_465 .
O3 O3 La 93.1(5) 2_465 .
O3 O3 La 92.3(3) 4_345 .
O3 O3 La 147.1(3) 3_465 .
O2 O3 La 145.0(3) 4_455 .
O3 O3 La 129.1(4) 2_466 .
O2 O3 La 39.7(2) 3_455 .
O2 O3 La 70.5(3) 5_456 .
O3 O3 La 65.21(15) 6 .
O1 O3 La 42.29(18) . .
O2 O3 La 38.95(19) 5_455 .
O3 O3 La 95.10(14) 6_556 .
Ga2 O3 La 59.17(14) 2_566 .
Ga3 O3 La 116.55(18) 4_346 .
Ga3 O3 O2 116.8(4) 1_556 1_565
Nb O3 O2 129.0(4) 1_455 1_565
Ga1 O3 O2 129.0(4) 1_455 1_565
La O3 O2 36.9(2) 4_455 1_565
Ga3 O3 O2 78.7(2) 2_465 1_565
O3 O3 O2 85.8(3) 2_465 1_565
O3 O3 O2 166.3(4) 4_345 1_565
O3 O3 O2 107.1(4) 3_465 1_565
O2 O3 O2 45.6(3) 4_455 1_565
O3 O3 O2 76.9(3) 2_466 1_565
O2 O3 O2 129.7(3) 3_455 1_565
O2 O3 O2 81.6(3) 5_456 1_565
O3 O3 O2 134.7(5) 6 1_565
O1 O3 O2 60.05(16) . 1_565
O2 O3 O2 90.2(3) 5_455 1_565
O3 O3 O2 122.6(6) 6_556 1_565
Ga2 O3 O2 60.06(17) 2_566 1_565
Ga3 O3 O2 138.9(4) 4_346 1_565
La O3 O2 101.4(2) . 1_565
Ga3 O3 O3 120.2(3) 1_556 5_345
Nb O3 O3 8.7(2) 1_455 5_345
Ga1 O3 O3 8.7(2) 1_455 5_345
La O3 O3 99.4(4) 4_455 5_345
Ga3 O3 O3 81.7(2) 2_465 5_345
O3 O3 O3 43.4(2) 2_465 5_345
O3 O3 O3 53.9(3) 4_345 5_345
O3 O3 O3 42.4(3) 3_465 5_345
O2 O3 O3 86.8(3) 4_455 5_345
O3 O3 O3 116.3(4) 2_466 5_345
O2 O3 O3 104.3(3) 3_455 5_345
O2 O3 O3 156.5(3) 5_456 5_345
O3 O3 O3 43.1(2) 6 5_345
O1 O3 O3 135.9(7) . 5_345
O2 O3 O3 82.7(4) 5_455 5_345
O3 O3 O3 104.7(2) 6_556 5_345
Ga2 O3 O3 165.5(5) 2_566 5_345
Ga3 O3 O3 63.1(2) 4_346 5_345
La O3 O3 107.9(4) . 5_345
O2 O3 O3 120.9(3) 1_565 5_345
Ga3 O3 Ga3 117.9(4) 1_556 .
Nb O3 Ga3 52.4(3) 1_455 .
Ga1 O3 Ga3 52.4(3) 1_455 .
La O3 Ga3 71.7(3) 4_455 .
Ga3 O3 Ga3 134.3(3) 2_465 .
O3 O3 Ga3 39.9(4) 2_465 .
O3 O3 Ga3 79.37(14) 4_345 .
O3 O3 Ga3 97.49(9) 3_465 .
O2 O3 Ga3 115.2(4) 4_455 .
O3 O3 Ga3 171.4(2) 2_466 .
O2 O3 Ga3 78.6(4) 3_455 .
O2 O3 Ga3 127.7(4) 5_456 .
O3 O3 Ga3 26.7(2) 6 .
O1 O3 Ga3 81.7(4) . .
O2 O3 Ga3 28.05(18) 5_455 .
O3 O3 Ga3 126.2(4) 6_556 .
Ga2 O3 Ga3 110.2(3) 2_566 .
Ga3 O3 Ga3 105.0(2) 4_346 .
La O3 Ga3 57.27(18) . .
O2 O3 Ga3 108.6(3) 1_565 .
O3 O3 Ga3 55.3(3) 5_345 .
Ga3 O3 Ga2 114.7(5) 1_556 1_565
Nb O3 Ga2 118.5(3) 1_455 1_565
Ga1 O3 Ga2 118.5(3) 1_455 1_565
La O3 Ga2 57.55(17) 4_455 1_565
Ga3 O3 Ga2 52.35(15) 2_465 1_565
O3 O3 Ga2 89.9(3) 2_465 1_565
O3 O3 Ga2 140.0(3) 4_345 1_565
O3 O3 Ga2 83.5(4) 3_465 1_565
O2 O3 Ga2 23.58(19) 4_455 1_565
O3 O3 Ga2 58.2(2) 2_466 1_565
O2 O3 Ga2 145.7(4) 3_455 1_565
O2 O3 Ga2 87.5(3) 5_456 1_565
O3 O3 Ga2 143.9(4) 6 1_565
O1 O3 Ga2 85.08(19) . 1_565
O2 O3 Ga2 113.4(2) 5_455 1_565
O3 O3 Ga2 109.2(5) 6_556 1_565
Ga2 O3 Ga2 77.02(16) 2_566 1_565
Ga3 O3 Ga2 112.9(3) 4_346 1_565
La O3 Ga2 127.19(19) . 1_565
O2 O3 Ga2 26.34(14) 1_565 1_565
O3 O3 Ga2 109.85(12) 5_345 1_565
Ga3 O3 Ga2 124.4(2) . 1_565
Ga3 O3 O3 65.0(4) 1_556 5_346
Nb O3 O3 79.5(3) 1_455 5_346
Ga1 O3 O3 79.5(3) 1_455 5_346
La O3 O3 143.1(3) 4_455 5_346
Ga3 O3 O3 38.47(17) 2_465 5_346
O3 O3 O3 117.3(3) 2_465 5_346
O3 O3 O3 55.1(2) 4_345 5_346
O3 O3 O3 44.2(3) 3_465 5_346
O2 O3 O3 78.2(3) 4_455 5_346
O3 O3 O3 41.8(2) 2_466 5_346
O2 O3 O3 95.1(3) 3_455 5_346
O2 O3 O3 85.7(4) 5_456 5_346
O3 O3 O3 104.9(2) 6 5_346
O1 O3 O3 144.1(6) . 5_346
O2 O3 O3 155.9(3) 5_455 5_346
O3 O3 O3 41.6(2) 6_556 5_346
Ga2 O3 O3 114.2(5) 2_566 5_346
Ga3 O3 O3 26.78(13) 4_346 5_346
La O3 O3 134.73(19) . 5_346
O2 O3 O3 112.8(3) 1_565 5_346
O3 O3 O3 79.4(3) 5_345 5_346
Ga3 O3 O3 129.9(3) . 5_346
Ga2 O3 O3 87.9(2) 1_565 5_346
Ga3 O3 Nb 45.8(3) 1_556 1_456
Nb O3 Nb 106.1(3) 1_455 1_456
Ga1 O3 Nb 106.1(3) 1_455 1_456
La O3 Nb 138.0(4) 4_455 1_456
Ga3 O3 Nb 49.7(2) 2_465 1_456
O3 O3 Nb 144.1(4) 2_465 1_456
O3 O3 Nb 71.07(9) 4_345 1_456
O3 O3 Nb 71.07(9) 3_465 1_456
O2 O3 Nb 84.2(4) 4_455 1_456
O3 O3 Nb 24.61(17) 2_466 1_456
O2 O3 Nb 84.3(4) 3_455 1_456
O2 O3 Nb 58.2(3) 5_456 1_456
O3 O3 Nb 123.6(3) 6 1_456
O1 O3 Nb 116.2(5) . 1_456
O2 O3 Nb 157.8(3) 5_455 1_456
O3 O3 Nb 28.0(2) 6_556 1_456
Ga2 O3 Nb 86.3(3) 2_566 1_456
Ga3 O3 Nb 47.36(14) 4_346 1_456
La O3 Nb 119.2(2) . 1_456
O2 O3 Nb 101.1(3) 1_565 1_456
O3 O3 Nb 107.0(4) 5_345 1_456
Ga3 O3 Nb 150.21(18) . 1_456
Ga2 O3 Nb 82.6(2) 1_565 1_456
O3 O3 Nb 27.9(2) 5_346 1_456
Ga3 O3 Ga1 45.8(3) 1_556 1_456
Nb O3 Ga1 106.1(3) 1_455 1_456
Ga1 O3 Ga1 106.1(3) 1_455 1_456
La O3 Ga1 138.0(4) 4_455 1_456
Ga3 O3 Ga1 49.7(2) 2_465 1_456
O3 O3 Ga1 144.1(4) 2_465 1_456
O3 O3 Ga1 71.07(9) 4_345 1_456
O3 O3 Ga1 71.07(9) 3_465 1_456
O2 O3 Ga1 84.2(4) 4_455 1_456
O3 O3 Ga1 24.61(17) 2_466 1_456
O2 O3 Ga1 84.3(4) 3_455 1_456
O2 O3 Ga1 58.2(3) 5_456 1_456
O3 O3 Ga1 123.6(3) 6 1_456
O1 O3 Ga1 116.2(5) . 1_456
O2 O3 Ga1 157.8(3) 5_455 1_456
O3 O3 Ga1 28.0(2) 6_556 1_456
Ga2 O3 Ga1 86.3(3) 2_566 1_456
Ga3 O3 Ga1 47.36(14) 4_346 1_456
La O3 Ga1 119.2(2) . 1_456
O2 O3 Ga1 101.1(3) 1_565 1_456
O3 O3 Ga1 107.0(4) 5_345 1_456
Ga3 O3 Ga1 150.21(18) . 1_456
Ga2 O3 Ga1 82.6(2) 1_565 1_456
O3 O3 Ga1 27.9(2) 5_346 1_456
Nb O3 Ga1 0.0 1_456 1_456
Ga3 O3 O2 76.5(3) 1_556 2_566
Nb O3 O2 170.1(3) 1_455 2_566
Ga1 O3 O2 170.1(3) 1_455 2_566
La O3 O2 67.0(2) 4_455 2_566
Ga3 O3 O2 90.0(3) 2_465 2_566
O3 O3 O2 123.26(19) 2_465 2_566
O3 O3 O2 142.3(2) 4_345 2_566
O3 O3 O2 130.0(3) 3_465 2_566
O2 O3 O2 76.6(2) 4_455 2_566
O3 O3 O2 62.7(2) 2_466 2_566
O2 O3 O2 93.3(3) 3_455 2_566
O2 O3 O2 40.6(3) 5_456 2_566
O3 O3 O2 146.6(2) 6 2_566
O1 O3 O2 45.5(4) . 2_566
O2 O3 O2 98.0(2) 5_455 2_566
O3 O3 O2 88.6(4) 6_556 2_566
Ga2 O3 O2 24.52(12) 2_566 2_566
Ga3 O3 O2 126.2(4) 4_346 2_566
La O3 O2 82.59(18) . 2_566
O2 O3 O2 41.1(3) 1_565 2_566
O3 O3 O2 161.84(18) 5_345 2_566
Ga3 O3 O2 125.8(3) . 2_566
Ga2 O3 O2 53.13(14) 1_565 2_566
O3 O3 O2 104.0(4) 5_346 2_566
Nb O3 O2 79.0(3) 1_456 2_566
Ga1 O3 O2 79.0(3) 1_456 2_566
Ga3 O3 La 67.8(2) 1_556 2_455
Nb O3 La 53.89(18) 1_455 2_455
Ga1 O3 La 53.89(18) 1_455 2_455
La O3 La 127.4(4) 4_455 2_455
Ga3 O3 La 119.1(2) 2_465 2_455
O3 O3 La 87.7(4) 2_465 2_455
O3 O3 La 31.3(2) 4_345 2_455
O3 O3 La 87.0(2) 3_465 2_455
O2 O3 La 147.5(3) 4_455 2_455
O3 O3 La 118.7(3) 2_466 2_455
O2 O3 La 41.8(3) 3_455 2_455
O2 O3 La 98.4(2) 5_456 2_455
O3 O3 La 33.97(19) 6 2_455
O1 O3 La 104.3(3) . 2_455
O2 O3 La 72.3(2) 5_455 2_455
O3 O3 La 69.2(2) 6_556 2_455
Ga2 O3 La 111.7(2) 2_566 2_455
Ga3 O3 La 59.21(10) 4_346 2_455
La O3 La 62.12(14) . 2_455
O2 O3 La 161.9(4) 1_565 2_455
O3 O3 La 62.56(12) 5_345 2_455
Ga3 O3 La 57.19(14) . 2_455
Ga2 O3 La 170.5(2) 1_565 2_455
O3 O3 La 85.13(14) 5_346 2_455
Nb O3 La 94.07(16) 1_456 2_455
Ga1 O3 La 94.07(16) 1_456 2_455
O2 O3 La 135.1(2) 2_566 2_455
Ga3 O3 Ga3 154.0(3) 1_556 2_464
Nb O3 Ga3 41.7(2) 1_455 2_464
Ga1 O3 Ga3 41.7(2) 1_455 2_464
La O3 Ga3 63.7(2) 4_455 2_464
Ga3 O3 Ga3 90.2(2) 2_465 2_464
O3 O3 Ga3 10.0(2) 2_465 2_464
O3 O3 Ga3 88.68(14) 4_345 2_464
O3 O3 Ga3 63.23(19) 3_465 2_464
O2 O3 Ga3 71.6(3) 4_455 2_464
O3 O3 Ga3 128.9(4) 2_466 2_464
O2 O3 Ga3 122.4(5) 3_455 2_464
O2 O3 Ga3 166.3(3) 5_456 2_464
O3 O3 Ga3 55.3(3) 6 2_464
O1 O3 Ga3 107.7(5) . 2_464
O2 O3 Ga3 64.3(2) 5_455 2_464
O3 O3 Ga3 140.2(2) 6_556 2_464
Ga2 O3 Ga3 135.2(3) 2_566 2_464
Ga3 O3 Ga3 97.56(18) 4_346 2_464
La O3 Ga3 101.7(3) . 2_464
O2 O3 Ga3 89.2(3) 1_565 2_464
O3 O3 Ga3 35.7(2) 5_345 2_464
Ga3 O3 Ga3 46.25(14) . 2_464
Ga2 O3 Ga3 88.76(16) 1_565 2_464
O3 O3 Ga3 107.3(3) 5_346 2_464
Nb O3 Ga3 134.2(2) 1_456 2_464
Ga1 O3 Ga3 134.2(2) 1_456 2_464
O2 O3 Ga3 128.9(2) 2_566 2_464
La O3 Ga3 87.2(2) 2_455 2_464
Ga3 O3 O1 158.2(5) 1_556 2_465
Nb O3 O1 88.1(3) 1_455 2_465
Ga1 O3 O1 88.1(3) 1_455 2_465
La O3 O1 29.03(11) 4_455 2_465
Ga3 O3 O1 80.2(3) 2_465 2_465
O3 O3 O1 45.6(3) 2_465 2_465
O3 O3 O1 134.3(3) 4_345 2_465
O3 O3 O1 84.1(3) 3_465 2_465
O2 O3 O1 41.9(3) 4_455 2_465
O3 O3 O1 103.1(4) 2_466 2_465
O2 O3 O1 147.5(5) 3_455 2_465
O2 O3 O1 122.6(3) 5_456 2_465
O3 O3 O1 99.0(5) 6 2_465
O1 O3 O1 81.6(3) . 2_465
O2 O3 O1 74.9(3) 5_455 2_465
O3 O3 O1 153.7(5) 6_556 2_465
Ga2 O3 O1 96.49(18) 2_566 2_465
Ga3 O3 O1 128.8(2) 4_346 2_465
La O3 O1 107.9(3) . 2_465
O2 O3 O1 41.4(3) 1_565 2_465
O3 O3 O1 80.6(3) 5_345 2_465
Ga3 O3 O1 78.3(3) . 2_465
Ga2 O3 O1 46.3(3) 1_565 2_465
O3 O3 O1 117.3(2) 5_346 2_465
Nb O3 O1 125.7(4) 1_456 2_465
Ga1 O3 O1 125.7(4) 1_456 2_465
O2 O3 O1 82.0(3) 2_566 2_465
La O3 O1 132.9(4) 2_455 2_465
Ga3 O3 O1 47.9(2) 2_464 2_465
Ga3 O3 La 64.3(3) 1_556 4_456
Nb O3 La 148.8(5) 1_455 4_456
Ga1 O3 La 148.8(5) 1_455 4_456
La O3 La 92.5(2) 4_455 4_456
Ga3 O3 La 63.0(2) 2_465 4_456
O3 O3 La 140.4(3) 2_465 4_456
O3 O3 La 118.09(11) 4_345 4_456
O3 O3 La 102.3(2) 3_465 4_456
O2 O3 La 68.2(3) 4_455 4_456
O3 O3 La 30.16(15) 2_466 4_456
O2 O3 La 98.0(4) 3_455 4_456
O2 O3 La 40.3(3) 5_456 4_456
O3 O3 La 165.4(4) 6 4_456
O1 O3 La 77.0(4) . 4_456
O2 O3 La 130.5(3) 5_455 4_456
O3 O3 La 65.3(4) 6_556 4_456
Ga2 O3 La 49.62(15) 2_566 4_456
Ga3 O3 La 95.1(3) 4_346 4_456
La O3 La 106.80(19) . 4_456
O2 O3 La 57.3(2) 1_565 4_456
O3 O3 La 144.6(4) 5_345 4_456
Ga3 O3 La 158.4(2) . 4_456
Ga2 O3 La 50.76(13) 1_565 4_456
O3 O3 La 71.4(3) 5_346 4_456
Nb O3 La 47.95(14) 1_456 4_456
Ga1 O3 La 47.95(14) 1_456 4_456
O2 O3 La 32.70(16) 2_566 4_456
La O3 La 131.9(2) 2_455 4_456
Ga3 O3 La 139.25(19) 2_464 4_456
O1 O3 La 95.2(3) 2_465 4_456
Ga3 O3 O2 95.5(5) 1_556 6_456
Nb O3 O2 88.0(3) 1_455 6_456
Ga1 O3 O2 88.0(3) 1_455 6_456
La O3 O2 104.1(3) 4_455 6_456
Ga3 O3 O2 0.87(13) 2_465 6_456
O3 O3 O2 99.0(4) 2_465 6_456
O3 O3 O2 88.6(2) 4_345 6_456
O3 O3 O2 41.1(2) 3_465 6_456
O2 O3 O2 39.3(4) 4_455 6_456
O3 O3 O2 38.6(3) 2_466 6_456
O2 O3 O2 132.5(4) 3_455 6_456
O2 O3 O2 97.3(5) 5_456 6_456
O3 O3 O2 123.99(15) 6 6_456
O1 O3 O2 133.0(4) . 6_456
O2 O3 O2 152.5(3) 5_455 6_456
O3 O3 O2 75.5(3) 6_556 6_456
Ga2 O3 O2 111.2(3) 2_566 6_456
Ga3 O3 O2 61.64(19) 4_346 6_456
La O3 O2 167.7(3) . 6_456
O2 O3 O2 77.9(2) 1_565 6_456
O3 O3 O2 82.4(3) 5_345 6_456
Ga3 O3 O2 134.8(3) . 6_456
Ga2 O3 O2 51.56(17) 1_565 6_456
O3 O3 O2 39.03(17) 5_346 6_456
Nb O3 O2 49.7(2) 1_456 6_456
Ga1 O3 O2 49.7(2) 1_456 6_456
O2 O3 O2 89.2(3) 2_566 6_456
La O3 O2 119.9(2) 2_455 6_456
Ga3 O3 O2 90.6(2) 2_464 6_456
O1 O3 O2 79.8(3) 2_465 6_456
La O3 O2 62.3(2) 4_456 6_456
Ga3 O3 O2 126.4(4) 1_556 2_565
Nb O3 O2 103.3(4) 1_455 2_565
Ga1 O3 O2 103.3(4) 1_455 2_565
La O3 O2 20.29(17) 4_455 2_565
Ga3 O3 O2 125.0(2) 2_465 2_565
O3 O3 O2 58.5(3) 2_465 2_565
O3 O3 O2 137.9(2) 4_345 2_565
O3 O3 O2 127.1(3) 3_465 2_565
O2 O3 O2 85.2(3) 4_455 2_565
O3 O3 O2 128.13(19) 2_466 2_565
O2 O3 O2 100.8(3) 3_455 2_565
O2 O3 O2 98.5(2) 5_456 2_565
O3 O3 O2 85.5(4) 6 2_565
O1 O3 O2 40.7(4) . 2_565
O2 O3 O2 37.6(2) 5_455 2_565
O3 O3 O2 149.6(2) 6_556 2_565
Ga2 O3 O2 67.6(2) 2_566 2_565
Ga3 O3 O2 163.1(3) 4_346 2_565
La O3 O2 61.23(18) . 2_565
O2 O3 O2 52.6(3) 1_565 2_565
O3 O3 O2 100.9(4) 5_345 2_565
Ga3 O3 O2 59.0(2) . 2_565
Ga2 O3 O2 76.38(16) 1_565 2_565
O3 O3 O2 163.43(14) 5_346 2_565
Nb O3 O2 149.4(3) 1_456 2_565
Ga1 O3 O2 149.4(3) 1_456 2_565
O2 O3 O2 70.65(17) 2_566 2_565
La O3 O2 109.9(3) 2_455 2_565
Ga3 O3 O2 67.8(2) 2_464 2_565
O1 O3 O2 47.20(17) 2_465 2_565
La O3 O2 101.5(2) 4_456 2_565
O2 O3 O2 124.4(2) 6_456 2_565
Ga3 O3 Ga2 31.9(2) 1_556 .
Nb O3 Ga2 98.7(2) 1_455 .
Ga1 O3 Ga2 98.7(2) 1_455 .
La O3 Ga2 126.2(3) 4_455 .
Ga3 O3 Ga2 124.5(3) 2_465 .
O3 O3 Ga2 125.8(5) 2_465 .
O3 O3 Ga2 60.6(3) 4_345 .
O3 O3 Ga2 118.4(3) 3_465 .
O2 O3 Ga2 158.3(5) 4_455 .
O3 O3 Ga2 95.1(4) 2_466 .
O2 O3 Ga2 8.2(3) 3_455 .
O2 O3 Ga2 53.7(2) 5_456 .
O3 O3 Ga2 74.01(19) 6 .
O1 O3 Ga2 76.0(2) . .
O2 O3 Ga2 82.0(2) 5_455 .
O3 O3 Ga2 49.27(13) 6_556 .
Ga2 O3 Ga2 69.60(14) 2_566 .
Ga3 O3 Ga2 74.75(13) 4_346 .
La O3 Ga2 46.68(9) . .
O2 O3 Ga2 129.6(2) 1_565 .
O3 O3 Ga2 107.32(10) 5_345 .
Ga3 O3 Ga2 86.43(18) . .
Ga2 O3 Ga2 141.1(3) 1_565 .
O3 O3 Ga2 88.1(2) 5_346 .
Nb O3 Ga2 76.11(16) 1_456 .
Ga1 O3 Ga2 76.11(16) 1_456 .
O2 O3 Ga2 90.7(2) 2_566 .
La O3 Ga2 45.06(7) 2_455 .
Ga3 O3 Ga2 129.1(3) 2_464 .
O1 O3 Ga2 154.5(3) 2_465 .
La O3 Ga2 91.57(19) 4_456 .
O2 O3 Ga2 124.7(3) 6_456 .
O2 O3 Ga2 107.3(2) 2_565 .
Ga3 O3 O2 150.5(4) 1_556 6_455
Nb O3 O2 45.7(2) 1_455 6_455
Ga1 O3 O2 45.7(2) 1_455 6_455
La O3 O2 71.4(2) 4_455 6_455
Ga3 O3 O2 66.9(2) 2_465 6_455
O3 O3 O2 32.2(3) 2_465 6_455
O3 O3 O2 88.7(2) 4_345 6_455
O3 O3 O2 44.7(3) 3_465 6_455
O2 O3 O2 53.0(3) 4_455 6_455
O3 O3 O2 105.6(4) 2_466 6_455
O2 O3 O2 139.9(4) 3_455 6_455
O2 O3 O2 160.9(4) 5_456 6_455
O3 O3 O2 72.6(3) 6 6_455
O1 O3 O2 123.0(4) . 6_455
O2 O3 O2 87.1(3) 5_455 6_455
O3 O3 O2 127.85(16) 6_556 6_455
Ga2 O3 O2 142.5(2) 2_566 6_455
Ga3 O3 O2 86.56(19) 4_346 6_455
La O3 O2 125.0(3) . 6_455
O2 O3 O2 84.1(2) 1_565 6_455
O3 O3 O2 37.22(16) 5_345 6_455
Ga3 O3 O2 69.1(2) . 6_455
Ga2 O3 O2 74.21(17) 1_565 6_455
O3 O3 O2 88.3(2) 5_346 6_455
Nb O3 O2 112.9(2) 1_456 6_455
Ga1 O3 O2 112.9(2) 1_456 6_455
O2 O3 O2 124.6(2) 2_566 6_455
La O3 O2 99.2(2) 2_455 6_455
Ga3 O3 O2 23.32(14) 2_464 6_455
O1 O3 O2 46.03(17) 2_465 6_455
La O3 O2 120.7(2) 4_456 6_455
O2 O3 O2 67.25(15) 6_456 6_455
O2 O3 O2 82.5(3) 2_565 6_455
Ga2 O3 O2 144.2(2) . 6_455
Ga3 O3 La 146.4(5) 1_556 2_465
Nb O3 La 74.3(2) 1_455 2_465
Ga1 O3 La 74.3(2) 1_455 2_465
La O3 La 61.36(16) 4_455 2_465
Ga3 O3 La 51.23(14) 2_465 2_465
O3 O3 La 53.1(3) 2_465 2_465
O3 O3 La 110.8(3) 4_345 2_465
O3 O3 La 53.1(3) 3_465 2_465
O2 O3 La 23.8(3) 4_455 2_465
O3 O3 La 84.2(3) 2_466 2_465
O2 O3 La 169.6(4) 3_455 2_465
O2 O3 La 131.5(3) 5_456 2_465
O3 O3 La 101.9(3) 6 2_465
O1 O3 La 112.4(2) . 2_465
O2 O3 La 101.5(3) 5_455 2_465
O3 O3 La 126.1(3) 6_556 2_465
Ga2 O3 La 118.48(17) 2_566 2_465
Ga3 O3 La 97.15(18) 4_346 2_465
La O3 La 138.8(3) . 2_465
O2 O3 La 58.60(16) 1_565 2_465
O3 O3 La 65.67(11) 5_345 2_465
Ga3 O3 La 93.0(2) . 2_465
Ga2 O3 La 44.59(9) 1_565 2_465
O3 O3 La 85.65(12) 5_346 2_465
Nb O3 La 100.7(2) 1_456 2_465
Ga1 O3 La 100.7(2) 1_456 2_465
O2 O3 La 96.57(17) 2_566 2_465
La O3 La 128.2(2) 2_455 2_465
Ga3 O3 La 48.01(9) 2_464 2_465
O1 O3 La 32.51(11) 2_465 2_465
La O3 La 92.07(17) 4_456 2_465
O2 O3 La 51.11(19) 6_456 2_465
O2 O3 La 79.55(17) 2_565 2_465
Ga2 O3 La 171.39(17) . 2_465
O2 O3 La 29.72(12) 6_455 2_465
Ga3 O3 Ga2 117.4(4) 1_556 2_565
Nb O3 Ga2 91.8(4) 1_455 2_565
Ga1 O3 Ga2 91.8(4) 1_455 2_565
La O3 Ga2 41.3(2) 4_455 2_565
Ga3 O3 Ga2 144.3(3) 2_465 2_565
O3 O3 Ga2 56.7(4) 2_465 2_565
O3 O3 Ga2 117.0(2) 4_345 2_565
O3 O3 Ga2 129.80(14) 3_465 2_565
O2 O3 Ga2 105.0(3) 4_455 2_565
O3 O3 Ga2 147.08(13) 2_466 2_565
O2 O3 Ga2 83.4(3) 3_455 2_565
O2 O3 Ga2 100.9(3) 5_456 2_565
O3 O3 Ga2 66.3(3) 6 2_565
O1 O3 Ga2 43.6(4) . 2_565
O2 O3 Ga2 15.85(14) 5_455 2_565
O3 O3 Ga2 139.68(16) 6_556 2_565
Ga2 O3 Ga2 73.68(17) 2_566 2_565
Ga3 O3 Ga2 145.0(3) 4_346 2_565
La O3 Ga2 44.61(12) . 2_565
O2 O3 Ga2 74.4(2) 1_565 2_565
O3 O3 Ga2 92.4(4) 5_345 2_565
Ga3 O3 Ga2 41.14(12) . 2_565
Ga2 O3 Ga2 98.35(16) 1_565 2_565
O3 O3 Ga2 171.0(4) 5_346 2_565
Nb O3 Ga2 159.1(2) 1_456 2_565
Ga1 O3 Ga2 159.1(2) 1_456 2_565
O2 O3 Ga2 84.9(2) 2_566 2_565
La O3 Ga2 87.9(2) 2_455 2_565
Ga3 O3 Ga2 66.65(18) 2_464 2_565
O1 O3 Ga2 64.1(2) 2_465 2_565
La O3 Ga2 117.56(15) 4_456 2_565
O2 O3 Ga2 143.9(2) 6_456 2_565
O2 O3 Ga2 22.01(12) 2_565 2_565
Ga2 O3 Ga2 90.99(18) . 2_565
O2 O3 Ga2 87.2(2) 6_455 2_565
La O3 Ga2 94.23(18) 2_465 2_565
Ga3 O3 O1 94.9(5) 1_556 2_466
Nb O3 O1 128.4(3) 1_455 2_466
Ga1 O3 O1 128.4(3) 1_455 2_466
La O3 O1 74.9(3) 4_455 2_466
Ga3 O3 O1 46.08(16) 2_465 2_466
O3 O3 O1 109.5(4) 2_465 2_466
O3 O3 O1 129.6(3) 4_345 2_466
O3 O3 O1 84.6(3) 3_465 2_466
O2 O3 O1 36.3(3) 4_455 2_466
O3 O3 O1 39.0(3) 2_466 2_466
O2 O3 O1 130.1(5) 3_455 2_466
O2 O3 O1 71.6(3) 5_456 2_466
O3 O3 O1 161.9(3) 6 2_466
O1 O3 O1 87.8(3) . 2_466
O2 O3 O1 129.0(3) 5_455 2_466
O3 O3 O1 89.2(5) 6_556 2_466
Ga2 O3 O1 70.16(19) 2_566 2_466
Ga3 O3 O1 101.2(3) 4_346 2_466
La O3 O1 128.29(19) . 2_466
O2 O3 O1 39.0(2) 1_565 2_466
O3 O3 O1 120.62(19) 5_345 2_466
Ga3 O3 O1 144.5(3) . 2_466
Ga2 O3 O1 20.3(2) 1_565 2_466
O3 O3 O1 74.5(3) 5_346 2_466
Nb O3 O1 63.7(3) 1_456 2_466
Ga1 O3 O1 63.7(3) 1_456 2_466
O2 O3 O1 45.95(14) 2_566 2_466
La O3 O1 157.7(3) 2_455 2_466
Ga3 O3 O1 107.2(2) 2_464 2_466
O1 O3 O1 66.63(12) 2_465 2_466
La O3 O1 32.2(2) 4_456 2_466
O2 O3 O1 45.21(15) 6_456 2_466
O2 O3 O1 91.6(2) 2_565 2_466
Ga2 O3 O1 123.7(3) . 2_466
O2 O3 O1 89.3(2) 6_455 2_466
La O3 O1 60.07(18) 2_465 2_466
Ga2 O3 O1 113.21(19) 2_565 2_466
Ga3 O3 O2 83.1(3) 1_556 1_455
Nb O3 O2 42.2(3) 1_455 1_455
Ga1 O3 O2 42.2(3) 1_455 1_455
La O3 O2 139.0(3) 4_455 1_455
Ga3 O3 O2 60.23(18) 2_465 1_455
O3 O3 O2 86.7(2) 2_465 1_455
O3 O3 O2 30.1(2) 4_345 1_455
O3 O3 O2 30.4(2) 3_465 1_455
O2 O3 O2 91.0(2) 4_455 1_455
O3 O3 O2 79.6(2) 2_466 1_455
O2 O3 O2 91.13(18) 3_455 1_455
O2 O3 O2 115.8(3) 5_456 1_455
O3 O3 O2 68.5(2) 6 1_455
O1 O3 O2 163.4(2) . 1_455
O2 O3 O2 119.4(3) 5_455 1_455
O3 O3 O2 62.7(2) 6_556 1_455
Ga2 O3 O2 146.9(3) 2_566 1_455
Ga3 O3 O2 19.79(16) 4_346 1_455
La O3 O2 121.9(2) . 1_455
O2 O3 O2 136.4(3) 1_565 1_455
O3 O3 O2 43.9(3) 5_345 1_455
Ga3 O3 O2 92.0(2) . 1_455
Ga2 O3 O2 110.9(2) 1_565 1_455
O3 O3 O2 38.0(2) 5_346 1_455
Nb O3 O2 64.0(2) 1_456 1_455
Ga1 O3 O2 64.0(2) 1_456 1_455
O2 O3 O2 142.1(3) 2_566 1_455
La O3 O2 59.78(13) 2_455 1_455
Ga3 O3 O2 77.8(2) 2_464 1_455
O1 O3 O2 112.3(2) 2_465 1_455
La O3 O2 109.4(3) 4_456 1_455
O2 O3 O2 61.1(2) 6_456 1_455
O2 O3 O2 144.9(3) 2_565 1_455
Ga2 O3 O2 88.38(16) . 1_455
O2 O3 O2 67.7(3) 6_455 1_455
La O3 O2 83.06(16) 2_465 1_455
Ga2 O3 O2 133.0(3) 2_565 1_455
O1 O3 O2 105.8(3) 2_466 1_455
Ga3 O3 O1 72.6(3) 1_556 2_455
Nb O3 O1 73.9(3) 1_455 2_455
Ga1 O3 O1 73.9(3) 1_455 2_455
La O3 O1 101.8(4) 4_455 2_455
Ga3 O3 O1 150.6(2) 2_465 2_455
O3 O3 O1 85.3(6) 2_465 2_455
O3 O3 O1 62.9(2) 4_345 2_455
O3 O3 O1 116.3(3) 3_465 2_455
O2 O3 O1 160.8(5) 4_455 2_455
O3 O3 O1 135.5(4) 2_466 2_455
O2 O3 O1 33.0(4) 3_455 2_455
O2 O3 O1 88.2(3) 5_456 2_455
O3 O3 O1 39.2(2) 6 2_455
O1 O3 O1 73.4(2) . 2_455
O2 O3 O1 46.6(3) 5_455 2_455
O3 O3 O1 85.8(3) 6_556 2_455
Ga2 O3 O1 87.72(19) 2_566 2_455
Ga3 O3 O1 89.94(16) 4_346 2_455
La O3 O1 31.23(8) . 2_455
O2 O3 O1 130.7(3) 1_565 2_455
O3 O3 O1 81.6(3) 5_345 2_455
Ga3 O3 O1 45.6(3) . 2_455
Ga2 O3 O1 157.0(2) 1_565 2_455
O3 O3 O1 114.26(17) 5_346 2_455
Nb O3 O1 113.8(2) 1_456 2_455
Ga1 O3 O1 113.8(2) 1_456 2_455
O2 O3 O1 112.1(2) 2_566 2_455
La O3 O1 31.66(8) 2_455 2_455
Ga3 O3 O1 90.2(3) 2_464 2_455
O1 O3 O1 120.5(5) 2_465 2_455
La O3 O1 128.4(3) 4_456 2_455
O2 O3 O1 151.4(2) 6_456 2_455
O2 O3 O1 82.0(3) 2_565 2_455
Ga2 O3 O1 40.8(2) . 2_455
O2 O3 O1 110.8(3) 6_455 2_455
La O3 O1 138.2(4) 2_465 2_455
Ga2 O3 O1 60.5(2) 2_565 2_455
O1 O3 O1 157.7(3) 2_466 2_455
O2 O3 O1 91.22(16) 1_455 2_455
Ga3 O3 La 116.2(3) 1_556 1_455
Nb O3 La 34.68(19) 1_455 1_455
Ga1 O3 La 34.68(19) 1_455 1_455
La O3 La 105.5(3) 4_455 1_455
Ga3 O3 La 52.94(14) 2_465 1_455
O3 O3 La 59.8(2) 2_465 1_455
O3 O3 La 59.7(2) 4_345 1_455
O3 O3 La 14.48(15) 3_465 1_455
O2 O3 La 65.8(2) 4_455 1_455
O3 O3 La 88.6(3) 2_466 1_455
O2 O3 La 121.1(3) 3_455 1_455
O2 O3 La 143.2(4) 5_456 1_455
O3 O3 La 71.06(14) 6 1_455
O1 O3 La 157.0(5) . 1_455
O2 O3 La 109.5(3) 5_455 1_455
O3 O3 La 93.95(11) 6_556 1_455
Ga2 O3 La 164.5(3) 2_566 1_455
Ga3 O3 La 52.26(10) 4_346 1_455
La O3 La 136.3(3) . 1_455
O2 O3 La 109.2(2) 1_565 1_455
O3 O3 La 28.78(15) 5_345 1_455
Ga3 O3 La 83.31(17) . 1_455
Ga2 O3 La 89.15(16) 1_565 1_455
O3 O3 La 57.51(18) 5_346 1_455
Nb O3 La 84.97(17) 1_456 1_455
Ga1 O3 La 84.97(17) 1_456 1_455
O2 O3 La 140.4(3) 2_566 1_455
La O3 La 81.71(12) 2_455 1_455
Ga3 O3 La 49.82(9) 2_464 1_455
O1 O3 La 78.37(13) 2_465 1_455
La O3 La 115.8(2) 4_456 1_455
O2 O3 La 53.68(16) 6_456 1_455
O2 O3 La 116.3(3) 2_565 1_455
Ga2 O3 La 120.33(14) . 1_455
O2 O3 La 34.33(13) 6_455 1_455
La O3 La 51.11(8) 2_465 1_455
Ga2 O3 La 115.8(2) 2_565 1_455
O1 O3 La 94.48(16) 2_466 1_455
O2 O3 La 33.95(14) 1_455 1_455
O1 O3 La 107.5(2) 2_455 1_455
Ga3 O3 Ga3 98.4(3) 1_556 4_456
Nb O3 Ga3 148.4(3) 1_455 4_456
Ga1 O3 Ga3 148.4(3) 1_455 4_456
La O3 Ga3 46.81(15) 4_455 4_456
Ga3 O3 Ga3 88.4(2) 2_465 4_456
O3 O3 Ga3 101.97(12) 2_465 4_456
O3 O3 Ga3 163.77(16) 4_345 4_456
O3 O3 Ga3 123.5(4) 3_465 4_456
O2 O3 Ga3 62.7(2) 4_455 4_456
O3 O3 Ga3 73.38(15) 2_466 4_456
O2 O3 Ga3 110.3(3) 3_455 4_456
O2 O3 Ga3 62.3(2) 5_456 4_456
O3 O3 Ga3 140.4(4) 6 4_456
O1 O3 Ga3 46.0(2) . 4_456
O2 O3 Ga3 89.4(2) 5_455 4_456
O3 O3 Ga3 109.3(4) 6_556 4_456
Ga2 O3 Ga3 39.93(7) 2_566 4_456
Ga3 O3 Ga3 140.7(3) 4_346 4_456
La O3 Ga3 88.20(14) . 4_456
O2 O3 Ga3 20.30(15) 1_565 4_456
O3 O3 Ga3 140.8(2) 5_345 4_456
Ga3 O3 Ga3 114.1(2) . 4_456
Ga2 O3 Ga3 40.01(7) 1_565 4_456
O3 O3 Ga3 114.6(3) 5_346 4_456
Nb O3 Ga3 94.6(2) 1_456 4_456
Ga1 O3 Ga3 94.6(2) 1_456 4_456
O2 O3 Ga3 21.89(14) 2_566 4_456
La O3 Ga3 149.4(2) 2_455 4_456
Ga3 O3 Ga3 107.11(16) 2_464 4_456
O1 O3 Ga3 60.26(19) 2_465 4_456
La O3 Ga3 46.74(9) 4_456 4_456
O2 O3 Ga3 87.54(19) 6_456 4_456
O2 O3 Ga3 55.25(17) 2_565 4_456
Ga2 O3 Ga3 109.51(17) . 4_456
O2 O3 Ga3 104.30(17) 6_455 4_456
La O3 Ga3 78.57(10) 2_465 4_456
Ga2 O3 Ga3 74.10(11) 2_565 4_456
O1 O3 Ga3 42.76(10) 2_466 4_456
O2 O3 Ga3 148.5(3) 1_455 4_456
O1 O3 Ga3 119.40(18) 2_455 4_456
La O3 Ga3 128.25(17) 1_455 4_456
Ga3 O3 Ga3 114.1(3) 1_556 4_345
Nb O3 Ga3 12.3(2) 1_455 4_345
Ga1 O3 Ga3 12.3(2) 1_455 4_345
La O3 Ga3 98.9(3) 4_455 4_345
Ga3 O3 Ga3 99.2(2) 2_465 4_345
O3 O3 Ga3 43.74(17) 2_465 4_345
O3 O3 Ga3 50.73(12) 4_345 4_345
O3 O3 Ga3 59.24(10) 3_465 4_345
O2 O3 Ga3 103.0(3) 4_455 4_345
O3 O3 Ga3 131.0(2) 2_466 4_345
O2 O3 Ga3 89.3(3) 3_455 4_345
O2 O3 Ga3 147.3(3) 5_456 4_345
O3 O3 Ga3 25.13(13) 6 4_345
O1 O3 Ga3 122.0(5) . 4_345
O2 O3 Ga3 68.4(2) 5_455 4_345
O3 O3 Ga3 105.2(3) 6_556 4_345
Ga2 O3 Ga3 148.8(3) 2_566 4_345
Ga3 O3 Ga3 68.89(13) 4_346 4_345
La O3 Ga3 90.0(2) . 4_345
O2 O3 Ga3 129.1(3) 1_565 4_345
O3 O3 Ga3 18.03(15) 5_345 4_345
Ga3 O3 Ga3 40.40(10) . 4_345
Ga2 O3 Ga3 124.9(2) 1_565 4_345
O3 O3 Ga3 90.5(2) 5_346 4_345
Nb O3 Ga3 116.06(16) 1_456 4_345
Ga1 O3 Ga3 116.06(16) 1_456 4_345
O2 O3 Ga3 164.9(3) 2_566 4_345
La O3 Ga3 48.97(10) 2_455 4_345
Ga3 O3 Ga3 39.92(9) 2_464 4_345
O1 O3 Ga3 87.8(3) 2_465 4_345
La O3 Ga3 161.0(2) 4_456 4_345
O2 O3 Ga3 100.00(19) 6_456 4_345
O2 O3 Ga3 94.2(3) 2_565 4_345
Ga2 O3 Ga3 93.79(15) . 4_345
O2 O3 Ga3 50.67(14) 6_455 4_345
La O3 Ga3 80.34(14) 2_465 4_345
Ga2 O3 Ga3 80.6(2) 2_565 4_345
O1 O3 Ga3 138.14(19) 2_466 4_345
O2 O3 Ga3 52.61(17) 1_455 4_345
O1 O3 Ga3 63.9(2) 2_455 4_345
La O3 Ga3 46.40(8) 1_455 4_345
Ga3 O3 Ga3 145.5(2) 4_456 4_345
Ga3 O3 O3 43.6(4) 1_556 1_556
Nb O3 O3 128.1(3) 1_455 1_556
Ga1 O3 O3 128.1(3) 1_455 1_556
La O3 O3 120.7(3) 4_455 1_556
Ga3 O3 O3 59.3(2) 2_465 1_556
O3 O3 O3 157.5(4) 2_465 1_556
O3 O3 O3 90.000(1) 4_345 1_556
O3 O3 O3 90.0 3_465 1_556
O2 O3 O3 83.2(4) 4_455 1_556
O3 O3 O3 21.0(3) 2_466 1_556
O2 O3 O3 83.1(4) 3_455 1_556
O2 O3 O3 40.0(3) 5_456 1_556
O3 O3 O3 140.1(3) 6 1_556
O1 O3 O3 95.2(5) . 1_556
O2 O3 O3 145.4(2) 5_455 1_556
O3 O3 O3 37.8(3) 6_556 1_556
Ga2 O3 O3 65.1(2) 2_566 1_556
Ga3 O3 O3 68.90(19) 4_346 1_556
La O3 O3 108.76(18) . 1_556
O2 O3 O3 85.0(3) 1_565 1_556
O3 O3 O3 128.7(3) 5_345 1_556
Ga3 O3 O3 161.56(11) . 1_556
Ga2 O3 O3 73.06(17) 1_565 1_556
O3 O3 O3 49.3(3) 5_346 1_556
Nb O3 O3 22.00(11) 1_456 1_556
Ga1 O3 O3 22.00(11) 1_456 1_556
O2 O3 O3 57.3(2) 2_566 1_556
La O3 O3 106.73(16) 2_455 1_556
Ga3 O3 O3 149.51(14) 2_464 1_556
O1 O3 O3 119.4(3) 2_465 1_556
La O3 O3 28.13(11) 4_456 1_556
O2 O3 O3 58.9(2) 6_456 1_556
O2 O3 O3 128.0(2) 2_565 1_556
Ga2 O3 O3 75.20(16) . 1_556
O2 O3 O3 126.2(2) 6_455 1_556
La O3 O3 104.92(16) 2_465 1_556
Ga2 O3 O3 138.82(11) 2_565 1_556
O1 O3 O3 52.7(2) 2_466 1_556
O2 O3 O3 86.0(2) 1_455 1_556
O1 O3 O3 116.0(3) 2_455 1_556
La O3 O3 104.41(15) 1_455 1_556
Ga3 O3 O3 74.52(15) 4_456 1_556
Ga3 O3 O3 137.79(12) 4_345 1_556
Ga3 O3 O3 136.4(4) 1_556 1_554
Nb O3 O3 51.9(3) 1_455 1_554
Ga1 O3 O3 51.9(3) 1_455 1_554
La O3 O3 59.3(3) 4_455 1_554
Ga3 O3 O3 120.7(2) 2_465 1_554
O3 O3 O3 22.5(4) 2_465 1_554
O3 O3 O3 90.000(2) 4_345 1_554
O3 O3 O3 90.0 3_465 1_554
O2 O3 O3 96.8(4) 4_455 1_554
O3 O3 O3 159.0(3) 2_466 1_554
O2 O3 O3 96.9(4) 3_455 1_554
O2 O3 O3 140.0(3) 5_456 1_554
O3 O3 O3 39.9(3) 6 1_554
O1 O3 O3 84.8(5) . 1_554
O2 O3 O3 34.6(2) 5_455 1_554
O3 O3 O3 142.2(3) 6_556 1_554
Ga2 O3 O3 114.9(2) 2_566 1_554
Ga3 O3 O3 111.10(19) 4_346 1_554
La O3 O3 71.24(18) . 1_554
O2 O3 O3 95.0(3) 1_565 1_554
O3 O3 O3 51.3(3) 5_345 1_554
Ga3 O3 O3 18.44(11) . 1_554
Ga2 O3 O3 106.94(17) 1_565 1_554
O3 O3 O3 130.7(3) 5_346 1_554
Nb O3 O3 158.00(11) 1_456 1_554
Ga1 O3 O3 158.00(11) 1_456 1_554
O2 O3 O3 122.7(2) 2_566 1_554
La O3 O3 73.27(16) 2_455 1_554
Ga3 O3 O3 30.49(14) 2_464 1_554
O1 O3 O3 60.6(3) 2_465 1_554
La O3 O3 151.86(11) 4_456 1_554
O2 O3 O3 121.0(2) 6_456 1_554
O2 O3 O3 52.0(2) 2_565 1_554
Ga2 O3 O3 104.80(16) . 1_554
O2 O3 O3 53.8(2) 6_455 1_554
La O3 O3 75.08(16) 2_465 1_554
Ga2 O3 O3 41.18(11) 2_565 1_554
O1 O3 O3 127.3(2) 2_466 1_554
O2 O3 O3 94.0(2) 1_455 1_554
O1 O3 O3 64.0(3) 2_455 1_554
La O3 O3 75.59(15) 1_455 1_554
Ga3 O3 O3 105.48(15) 4_456 1_554
Ga3 O3 O3 42.21(12) 4_345 1_554
O3 O3 O3 179.999(3) 1_556 1_554
Ga3 O3 O2 56.9(3) 1_556 6_556
Nb O3 O2 154.6(4) 1_455 6_556
Ga1 O3 O2 154.6(4) 1_455 6_556
La O3 O2 80.9(2) 4_455 6_556
Ga3 O3 O2 115.8(3) 2_465 6_556
O3 O3 O2 131.1(4) 2_465 6_556
O3 O3 O2 119.3(3) 4_345 6_556
O3 O3 O2 153.4(2) 3_465 6_556
O2 O3 O2 109.2(3) 4_455 6_556
O3 O3 O2 79.3(3) 2_466 6_556
O2 O3 O2 61.4(2) 3_455 6_556
O2 O3 O2 25.69(15) 5_456 6_556
O3 O3 O2 118.88(15) 6 6_556
O1 O3 O2 33.2(4) . 6_556
O2 O3 O2 82.65(18) 5_455 6_556
O3 O3 O2 77.5(3) 6_556 6_556
Ga2 O3 O2 9.47(11) 2_566 6_556
Ga3 O3 O2 120.3(3) 4_346 6_556
La O3 O2 54.17(15) . 6_556
O2 O3 O2 69.5(2) 1_565 6_556
O3 O3 O2 162.0(3) 5_345 6_556
Ga3 O3 O2 108.7(2) . 6_556
Ga2 O3 O2 85.64(17) 1_565 6_556
O3 O3 O2 111.2(4) 5_346 6_556
Nb O3 O2 83.5(2) 1_456 6_556
Ga1 O3 O2 83.5(2) 1_456 6_556
O2 O3 O2 32.57(14) 2_566 6_556
La O3 O2 102.85(18) 2_455 6_556
Ga3 O3 O2 140.8(3) 2_464 6_556
O1 O3 O2 105.51(19) 2_465 6_556
La O3 O2 52.83(16) 4_456 6_556
O2 O3 O2 115.1(3) 6_456 6_556
O2 O3 O2 73.14(11) 2_565 6_556
Ga2 O3 O2 60.16(14) . 6_556
O2 O3 O2 151.5(3) 6_455 6_556
La O3 O2 127.85(18) 2_465 6_556
Ga2 O3 O2 75.85(18) 2_565 6_556
O1 O3 O2 76.99(19) 2_466 6_556
O2 O3 O2 139.9(2) 1_455 6_556
O1 O3 O2 80.73(19) 2_455 6_556
La O3 O2 167.8(3) 1_455 6_556
Ga3 O3 O2 49.34(12) 4_456 6_556
Ga3 O3 O2 144.0(2) 4_345 6_556
O3 O3 O2 63.54(19) 1_556 6_556
O3 O3 O2 116.5(2) 1_554 6_556
Ga3 O3 O2 49.8(2) 1_556 2_456
Nb O3 O2 69.0(3) 1_455 2_456
Ga1 O3 O2 69.0(3) 1_455 2_456
La O3 O2 172.3(3) 4_455 2_456
Ga3 O3 O2 71.4(2) 2_465 2_456
O3 O3 O2 116.92(18) 2_465 2_456
O3 O3 O2 26.79(18) 4_345 2_456
O3 O3 O2 59.8(2) 3_465 2_456
O2 O3 O2 110.7(4) 4_455 2_456
O3 O3 O2 67.8(2) 2_466 2_456
O2 O3 O2 65.5(3) 3_455 2_456
O2 O3 O2 83.9(3) 5_456 2_456
O3 O3 O2 79.3(3) 6 2_456
O1 O3 O2 134.4(3) . 2_456
O2 O3 O2 125.1(3) 5_455 2_456
O3 O3 O2 31.0(2) 6_556 2_456
Ga2 O3 O2 114.4(3) 2_566 2_456
Ga3 O3 O2 15.03(11) 4_346 2_456
La O3 O2 103.99(16) . 2_456
O2 O3 O2 144.4(3) 1_565 2_456
O3 O3 O2 73.7(3) 5_345 2_456
Ga3 O3 O2 106.0(2) . 2_456
Ga2 O3 O2 121.1(3) 1_565 2_456
O3 O3 O2 33.51(14) 5_346 2_456
Nb O3 O2 44.33(16) 1_456 2_456
Ga1 O3 O2 44.33(16) 1_456 2_456
O2 O3 O2 119.0(4) 2_566 2_456
La O3 O2 52.72(14) 2_455 2_456
Ga3 O3 O2 109.3(2) 2_464 2_456
O1 O3 O2 143.8(2) 2_465 2_456
La O3 O2 91.5(2) 4_456 2_456
O2 O3 O2 72.0(2) 6_456 2_456
O2 O3 O2 162.5(3) 2_565 2_456
Ga2 O3 O2 60.19(12) . 2_456
O2 O3 O2 100.92(14) 6_455 2_456
La O3 O2 111.9(2) 2_465 2_456
Ga2 O3 O2 140.5(2) 2_565 2_456
O1 O3 O2 105.5(3) 2_466 2_456
O2 O3 O2 33.3(3) 1_455 2_456
O1 O3 O2 80.76(18) 2_455 2_456
La O3 O2 66.83(16) 1_455 2_456
Ga3 O3 O2 138.0(3) 4_456 2_456
Ga3 O3 O2 75.54(17) 4_345 2_456
O3 O3 O2 63.52(19) 1_556 2_456
O3 O3 O2 116.48(19) 1_554 2_456
O2 O3 O2 106.7(3) 6_556 2_456
Ga3 O3 La 25.90(17) 1_556 1_556
Nb O3 La 137.7(3) 1_455 1_556
Ga1 O3 La 137.7(3) 1_455 1_556
La O3 La 112.3(2) 4_455 1_556
Ga3 O3 La 102.3(3) 2_465 1_556
O3 O3 La 158.3(5) 2_465 1_556
O3 O3 La 91.7(2) 4_345 1_556
O3 O3 La 127.24(12) 3_465 1_556
O2 O3 La 118.4(4) 4_455 1_556
O3 O3 La 63.6(3) 2_466 1_556
O2 O3 La 47.9(3) 3_455 1_556
O2 O3 La 11.91(16) 5_456 1_556
O3 O3 La 115.9(2) 6 1_556
O1 O3 La 63.5(4) . 1_556
O2 O3 La 103.4(2) 5_455 1_556
O3 O3 La 45.9(2) 6_556 1_556
Ga2 O3 La 39.29(11) 2_566 1_556
Ga3 O3 La 88.61(19) 4_346 1_556
La O3 La 65.71(12) . 1_556
O2 O3 La 93.3(2) 1_565 1_556
O3 O3 La 145.43(19) 5_345 1_556
Ga3 O3 La 121.6(2) . 1_556
Ga2 O3 La 98.9(2) 1_565 1_556
O3 O3 La 83.1(3) 5_346 1_556
Nb O3 La 57.29(13) 1_456 1_556
Ga1 O3 La 57.29(13) 1_456 1_556
O2 O3 La 52.20(17) 2_566 1_556
La O3 La 86.56(13) 2_455 1_556
Ga3 O3 La 167.4(3) 2_464 1_556
O1 O3 La 133.9(2) 2_465 1_556
La O3 La 50.17(11) 4_456 1_556
O2 O3 La 102.0(3) 6_456 1_556
O2 O3 La 104.2(2) 2_565 1_556
Ga2 O3 La 42.23(8) . 1_556
O2 O3 La 169.2(3) 6_455 1_556
La O3 La 142.2(2) 2_465 1_556
Ga2 O3 La 102.20(15) 2_565 1_556
O1 O3 La 82.2(2) 2_466 1_556
O2 O3 La 108.2(2) 1_455 1_556
O1 O3 La 78.8(2) 2_455 1_556
La O3 La 139.5(2) 1_455 1_556
Ga3 O3 La 73.76(12) 4_456 1_556
Ga3 O3 La 135.50(15) 4_345 1_556
O3 O3 La 43.04(13) 1_556 1_556
O3 O3 La 136.96(13) 1_554 1_556
O2 O3 La 31.69(15) 6_556 1_556
O2 O3 La 75.23(18) 2_456 1_556
Ga3 O3 O2 43.7(3) 1_556 4_445
Nb O3 O2 79.7(2) 1_455 4_445
Ga1 O3 O2 79.7(2) 1_455 4_445
La O3 O2 133.1(4) 4_455 4_445
Ga3 O3 O2 122.2(3) 2_465 4_445
O3 O3 O2 111.8(5) 2_465 4_445
O3 O3 O2 43.9(3) 4_345 4_445
O3 O3 O2 103.8(3) 3_465 4_445
O2 O3 O2 161.9(5) 4_455 4_445
O3 O3 O2 103.5(4) 2_466 4_445
O2 O3 O2 18.1(2) 3_455 4_445
O2 O3 O2 72.0(2) 5_456 4_445
O3 O3 O2 57.9(2) 6 4_445
O1 O3 O2 90.0(2) . 4_445
O2 O3 O2 79.8(2) 5_455 4_445
O3 O3 O2 52.7(2) 6_556 4_445
Ga2 O3 O2 88.20(18) 2_566 4_445
Ga3 O3 O2 63.91(14) 4_346 4_445
La O3 O2 52.83(14) . 4_445
O2 O3 O2 147.8(2) 1_565 4_445
O3 O3 O2 88.30(14) 5_345 4_445
Ga3 O3 O2 75.5(2) . 4_445
Ga2 O3 O2 158.3(3) 1_565 4_445
O3 O3 O2 83.73(18) 5_346 4_445
Nb O3 O2 80.6(2) 1_456 4_445
Ga1 O3 O2 80.6(2) 1_456 4_445
O2 O3 O2 109.7(2) 2_566 4_445
La O3 O2 26.38(12) 2_455 4_445
Ga3 O3 O2 112.9(3) 2_464 4_445
O1 O3 O2 153.4(4) 2_465 4_445
La O3 O2 107.5(2) 4_456 4_445
O2 O3 O2 122.8(2) 6_456 4_445
O2 O3 O2 112.8(3) 2_565 4_445
Ga2 O3 O2 19.04(10) . 4_445
O2 O3 O2 125.3(2) 6_455 4_445
La O3 O2 153.3(2) 2_465 4_445
Ga2 O3 O2 92.6(2) 2_565 4_445
O1 O3 O2 138.6(4) 2_466 4_445
O2 O3 O2 73.5(2) 1_455 4_445
O1 O3 O2 33.3(2) 2_455 4_445
La O3 O2 102.97(15) 1_455 4_445
Ga3 O3 O2 128.09(19) 4_456 4_445
Ga3 O3 O2 75.35(17) 4_345 4_445
O3 O3 O2 86.3(2) 1_556 4_445
O3 O3 O2 93.7(2) 1_554 4_445
O2 O3 O2 78.84(18) 6_556 4_445
O2 O3 O2 51.27(13) 2_456 4_445
La O3 O2 60.20(15) 1_556 4_445
Ga3 O3 O1 13.5(3) 1_556 2_456
Nb O3 O1 109.5(3) 1_455 2_456
Ga1 O3 O1 109.5(3) 1_455 2_456
La O3 O1 132.8(3) 4_455 2_456
Ga3 O3 O1 108.6(4) 2_465 2_456
O3 O3 O1 144.1(6) 2_465 2_456
O3 O3 O1 64.9(3) 4_345 2_456
O3 O3 O1 114.3(2) 3_465 2_456
O2 O3 O1 139.7(5) 4_455 2_456
O3 O3 O1 76.6(4) 2_466 2_456
O2 O3 O1 26.6(4) 3_455 2_456
O2 O3 O1 40.2(2) 5_456 2_456
O3 O3 O1 90.9(3) 6 2_456
O1 O3 O1 79.7(3) . 2_456
O2 O3 O1 98.7(3) 5_455 2_456
O3 O3 O1 34.50(17) 6_556 2_456
Ga2 O3 O1 63.91(14) 2_566 2_456
Ga3 O3 O1 69.76(14) 4_346 2_456
La O3 O1 60.9(2) . 2_456
O2 O3 O1 121.4(3) 1_565 2_456
O3 O3 O1 117.60(16) 5_345 2_456
Ga3 O3 O1 105.0(3) . 2_456
Ga2 O3 O1 125.2(3) 1_565 2_456
O3 O3 O1 75.9(3) 5_346 2_456
Nb O3 O1 59.1(2) 1_456 2_456
Ga1 O3 O1 59.1(2) 1_456 2_456
O2 O3 O1 80.3(2) 2_566 2_456
La O3 O1 59.02(19) 2_455 2_456
Ga3 O3 O1 146.0(3) 2_464 2_456
O1 O3 O1 160.23(19) 2_465 2_456
La O3 O1 74.5(2) 4_456 2_456
O2 O3 O1 108.7(3) 6_456 2_456
O2 O3 O1 117.4(2) 2_565 2_456
Ga2 O3 O1 18.6(2) . 2_456
O2 O3 O1 153.57(19) 6_455 2_456
La O3 O1 159.8(4) 2_465 2_456
Ga2 O3 O1 105.3(2) 2_565 2_456
O1 O3 O1 106.2(4) 2_466 2_456
O2 O3 O1 87.27(18) 1_455 2_456
O1 O3 O1 59.45(8) 2_455 2_456
La O3 O1 121.21(15) 1_455 2_456
Ga3 O3 O1 101.54(18) 4_456 2_456
Ga3 O3 O1 107.6(2) 4_345 2_456
O3 O3 O1 56.6(3) 1_556 2_456
O3 O3 O1 123.4(3) 1_554 2_456
O2 O3 O1 54.78(15) 6_556 2_456
O2 O3 O1 54.80(14) 2_456 2_456
La O3 O1 28.29(13) 1_556 2_456
O2 O3 O1 33.2(2) 4_445 2_456
Ga3 O3 O2 99.3(4) 1_556 6
Nb O3 O2 106.3(4) 1_455 6
Ga1 O3 O2 106.3(4) 1_455 6
La O3 O2 50.8(2) 4_455 6
Ga3 O3 O2 153.9(2) 2_465 6
O3 O3 O2 75.9(4) 2_465 6
O3 O3 O2 117.9(3) 4_345 6
O3 O3 O2 148.68(16) 3_465 6
O2 O3 O2 115.2(3) 4_455 6
O3 O3 O2 134.7(3) 2_466 6
O2 O3 O2 69.9(3) 3_455 6
O2 O3 O2 82.1(2) 5_456 6
O3 O3 O2 74.8(3) 6 6
O1 O3 O2 27.8(4) . 6
O2 O3 O2 25.99(14) 5_455 6
O3 O3 O2 122.53(15) 6_556 6
Ga2 O3 O2 56.9(2) 2_566 6
Ga3 O3 O2 145.3(2) 4_346 6
La O3 O2 30.36(13) . 6
O2 O3 O2 75.4(2) 1_565 6
O3 O3 O2 108.6(4) 5_345 6
Ga3 O3 O2 53.93(17) . 6
Ga2 O3 O2 101.66(17) 1_565 6
O3 O3 O2 164.1(2) 5_346 6
Nb O3 O2 140.0(2) 1_456 6
Ga1 O3 O2 140.0(2) 1_456 6
O2 O3 O2 72.79(12) 2_566 6
La O3 O2 86.6(2) 2_455 6
Ga3 O3 O2 85.8(2) 2_464 6
O1 O3 O2 78.0(2) 2_465 6
La O3 O2 104.75(18) 4_456 6
O2 O3 O2 153.1(2) 6_456 6
O2 O3 O2 30.96(14) 2_565 6
Ga2 O3 O2 76.44(18) . 6
O2 O3 O2 106.4(3) 6_455 6
La O3 O2 110.1(2) 2_465 6
Ga2 O3 O2 19.31(13) 2_565 6
O1 O3 O2 110.86(18) 2_466 6
O2 O3 O2 142.9(2) 1_455 6
O1 O3 O2 55.39(18) 2_455 6
La O3 O2 134.4(3) 1_455 6
Ga3 O3 O2 68.24(14) 4_456 6
Ga3 O3 O2 94.3(2) 4_345 6
O3 O3 O2 121.17(16) 1_556 6
O3 O3 O2 58.83(16) 1_554 6
O2 O3 O2 57.64(11) 6_556 6
O2 O3 O2 134.1(2) 2_456 6
La O3 O2 82.90(17) 1_556 6
O2 O3 O2 82.8(2) 4_445 6
O1 O3 O2 88.2(2) 2_456 6
Ga3 O3 O2 128.9(5) 1_556 3_465
Nb O3 O2 106.2(3) 1_455 3_465
Ga1 O3 O2 106.2(3) 1_455 3_465
La O3 O2 50.67(19) 4_455 3_465
Ga3 O3 O2 54.56(16) 2_465 3_465
O3 O3 O2 75.7(3) 2_465 3_465
O3 O3 O2 137.6(4) 4_345 3_465
O3 O3 O2 77.8(3) 3_465 3_465
O2 O3 O2 16.6(2) 4_455 3_465
O3 O3 O2 69.8(3) 2_466 3_465
O2 O3 O2 157.9(4) 3_455 3_465
O2 O3 O2 101.3(3) 5_456 3_465
O3 O3 O2 129.5(4) 6 3_465
O1 O3 O2 89.07(16) . 3_465
O2 O3 O2 105.5(2) 5_455 3_465
O3 O3 O2 120.8(4) 6_556 3_465
Ga2 O3 O2 87.33(18) 2_566 3_465
Ga3 O3 O2 114.6(2) 4_346 3_465
La O3 O2 128.7(2) . 3_465
O2 O3 O2 29.43(15) 1_565 3_465
O3 O3 O2 97.48(16) 5_345 3_465
Ga3 O3 O2 111.6(3) . 3_465
Ga2 O3 O2 14.36(15) 1_565 3_465
O3 O3 O2 92.68(18) 5_346 3_465
Nb O3 O2 93.2(2) 1_456 3_465
Ga1 O3 O2 93.2(2) 1_456 3_465
O2 O3 O2 64.7(2) 2_566 3_465
La O3 O2 160.0(3) 2_455 3_465
Ga3 O3 O2 74.41(18) 2_464 3_465
O1 O3 O2 33.4(3) 2_465 3_465
La O3 O2 65.11(19) 4_456 3_465
O2 O3 O2 53.91(18) 6_456 3_465
O2 O3 O2 70.79(19) 2_565 3_465
Ga2 O3 O2 154.9(3) . 3_465
O2 O3 O2 60.86(18) 6_455 3_465
La O3 O2 31.84(13) 2_465 3_465
Ga2 O3 O2 91.89(17) 2_565 3_465
O1 O3 O2 34.0(2) 2_466 3_465
O2 O3 O2 107.5(2) 1_455 3_465
O1 O3 O2 152.2(3) 2_455 3_465
La O3 O2 80.39(15) 1_455 3_465
Ga3 O3 O2 47.91(12) 4_456 3_465
Ga3 O3 O2 111.3(2) 4_345 3_465
O3 O3 O2 86.4(2) 1_556 3_465
O3 O3 O2 93.6(2) 1_554 3_465
O2 O3 O2 96.5(2) 6_556 3_465
O2 O3 O2 125.9(2) 2_456 3_465
La O3 O2 113.0(2) 1_556 3_465
O2 O3 O2 172.5(4) 4_445 3_465
O1 O3 O2 139.5(3) 2_456 3_465
O2 O3 O2 99.6(2) 6 3_465
Ga3 O3 O2 93.8(3) 1_556 2_455
Nb O3 O2 22.23(17) 1_455 2_455
Ga1 O3 O2 22.23(17) 1_455 2_455
La O3 O2 117.7(4) 4_455 2_455
Ga3 O3 O2 100.2(2) 2_465 2_455
O3 O3 O2 63.9(2) 2_465 2_455
O3 O3 O2 31.45(17) 4_345 2_455
O3 O3 O2 61.25(18) 3_465 2_455
O2 O3 O2 116.7(3) 4_455 2_455
O3 O3 O2 121.33(17) 2_466 2_455
O2 O3 O2 73.5(4) 3_455 2_455
O2 O3 O2 128.4(2) 5_456 2_455
O3 O3 O2 25.60(18) 6 2_455
O1 O3 O2 125.7(4) . 2_455
O2 O3 O2 76.8(3) 5_455 2_455
O3 O3 O2 85.8(3) 6_556 2_455
Ga2 O3 O2 142.4(2) 2_566 2_455
Ga3 O3 O2 54.32(16) 4_346 2_455
La O3 O2 85.8(2) . 2_455
O2 O3 O2 149.4(3) 1_565 2_455
O3 O3 O2 30.89(13) 5_345 2_455
Ga3 O3 O2 50.77(15) . 2_455
Ga2 O3 O2 140.2(2) 1_565 2_455
O3 O3 O2 79.6(2) 5_346 2_455
Nb O3 O2 101.05(18) 1_456 2_455
Ga1 O3 O2 101.05(18) 1_456 2_455
O2 O3 O2 166.6(3) 2_566 2_455
La O3 O2 31.72(11) 2_455 2_455
Ga3 O3 O2 60.15(17) 2_464 2_455
O1 O3 O2 108.0(3) 2_465 2_455
La O3 O2 149.0(3) 4_456 2_455
O2 O3 O2 101.08(14) 6_456 2_455
O2 O3 O2 109.3(3) 2_565 2_455
Ga2 O3 O2 76.47(14) . 2_455
O2 O3 O2 67.88(18) 6_455 2_455
La O3 O2 96.52(18) 2_465 2_455
Ga2 O3 O2 91.6(2) 2_565 2_455
O1 O3 O2 145.8(2) 2_466 2_455
O2 O3 O2 42.9(2) 1_455 2_455
O1 O3 O2 55.41(15) 2_455 2_455
La O3 O2 52.34(12) 1_455 2_455
Ga3 O3 O2 164.3(3) 4_456 2_455
Ga3 O3 O2 20.32(12) 4_345 2_455
O3 O3 O2 121.19(17) 1_556 2_455
O3 O3 O2 58.81(17) 1_554 2_455
O2 O3 O2 134.1(2) 6_556 2_455
O2 O3 O2 57.67(11) 2_456 2_455
La O3 O2 116.50(16) 1_556 2_455
O2 O3 O2 57.47(17) 4_445 2_455
O1 O3 O2 88.2(2) 2_456 2_455
O2 O3 O2 100.2(3) 6 2_455
O2 O3 O2 128.36(19) 3_465 2_455
Ga3 O3 O1 124.2(5) 1_556 1_455
Nb O3 O1 61.2(3) 1_455 1_455
Ga1 O3 O1 61.2(3) 1_455 1_455
La O3 O1 89.9(3) 4_455 1_455
Ga3 O3 O1 33.8(3) 2_465 1_455
O3 O3 O1 65.4(4) 2_465 1_455
O3 O3 O1 85.2(3) 4_345 1_455
O3 O3 O1 25.3(3) 3_465 1_455
O2 O3 O1 37.49(19) 4_455 1_455
O3 O3 O1 72.8(3) 2_466 1_455
O2 O3 O1 146.8(3) 3_455 1_455
O2 O3 O1 131.3(4) 5_456 1_455
O3 O3 O1 96.6(2) 6 1_455
O1 O3 O1 140.5(2) . 1_455
O2 O3 O1 120.3(4) 5_455 1_455
O3 O3 O1 101.0(2) 6_556 1_455
Ga2 O3 O1 136.8(3) 2_566 1_455
Ga3 O3 O1 68.55(15) 4_346 1_455
La O3 O1 158.1(4) . 1_455
O2 O3 O1 82.35(17) 1_565 1_455
O3 O3 O1 53.6(2) 5_345 1_455
Ga3 O3 O1 100.9(3) . 1_455
Ga2 O3 O1 60.65(13) 1_565 1_455
O3 O3 O1 59.4(2) 5_346 1_455
Nb O3 O1 80.5(3) 1_456 1_455
Ga1 O3 O1 80.5(3) 1_456 1_455
O2 O3 O1 112.3(2) 2_566 1_455
La O3 O1 110.11(17) 2_455 1_455
Ga3 O3 O1 56.5(3) 2_464 1_455
O1 O3 O1 60.9(2) 2_465 1_455
La O3 O1 93.5(3) 4_456 1_455
O2 O3 O1 34.2(3) 6_456 1_455
O2 O3 O1 107.2(3) 2_565 1_455
Ga2 O3 O1 143.25(19) . 1_455
O2 O3 O1 33.3(3) 6_455 1_455
La O3 O1 28.62(12) 2_465 1_455
Ga2 O3 O1 118.2(3) 2_565 1_455
O1 O3 O1 67.1(2) 2_466 1_455
O2 O3 O1 55.70(13) 1_455 1_455
O1 O3 O1 135.14(19) 2_455 1_455
La O3 O1 28.55(12) 1_455 1_455
Ga3 O3 O1 100.21(14) 4_456 1_455
Ga3 O3 O1 71.6(2) 4_345 1_455
O3 O3 O1 93.0(3) 1_556 1_455
O3 O3 O1 87.0(3) 1_554 1_455
O2 O3 O1 144.1(3) 6_556 1_455
O2 O3 O1 83.30(18) 2_456 1_455
La O3 O1 136.0(3) 1_556 1_455
O2 O3 O1 129.10(16) 4_445 1_455
O1 O3 O1 135.2(2) 2_456 1_455
O2 O3 O1 136.4(3) 6 1_455
O2 O3 O1 52.95(12) 3_465 1_455
O2 O3 O1 80.70(19) 2_455 1_455
Ga3 O3 Ga2 167.8(3) 1_556 1_564
Nb O3 Ga2 77.1(3) 1_455 1_564
Ga1 O3 Ga2 77.1(3) 1_455 1_564
La O3 Ga2 30.03(15) 4_455 1_564
Ga3 O3 Ga2 91.51(19) 2_465 1_564
O3 O3 Ga2 30.92(15) 2_465 1_564
O3 O3 Ga2 124.13(16) 4_345 1_564
O3 O3 Ga2 85.3(3) 3_465 1_564
O2 O3 Ga2 55.9(3) 4_455 1_564
O3 O3 Ga2 118.7(3) 2_466 1_564
O2 O3 Ga2 135.7(4) 3_455 1_564
O2 O3 Ga2 132.7(2) 5_456 1_564
O3 O3 Ga2 83.1(4) 6 1_564
O1 O3 Ga2 81.6(3) . 1_564
O2 O3 Ga2 61.9(2) 5_455 1_564
O3 O3 Ga2 166.6(2) 6_556 1_564
Ga2 O3 Ga2 103.01(17) 2_566 1_564
Ga3 O3 Ga2 128.2(2) 4_346 1_564
La O3 Ga2 98.3(2) . 1_564
O2 O3 Ga2 54.9(2) 1_565 1_564
O3 O3 Ga2 70.7(3) 5_345 1_564
Ga3 O3 Ga2 62.24(15) . 1_564
Ga2 O3 Ga2 62.47(11) 1_565 1_564
O3 O3 Ga2 125.28(17) 5_346 1_564
Nb O3 Ga2 139.9(2) 1_456 1_564
Ga1 O3 Ga2 139.9(2) 1_456 1_564
O2 O3 Ga2 93.52(18) 2_566 1_564
La O3 Ga2 117.1(3) 2_455 1_564
Ga3 O3 Ga2 35.45(7) 2_464 1_564
O1 O3 Ga2 16.2(3) 2_465 1_564
La O3 Ga2 110.75(13) 4_456 1_564
O2 O3 Ga2 91.3(2) 6_456 1_564
O2 O3 Ga2 42.04(15) 2_565 1_564
Ga2 O3 Ga2 143.8(3) . 1_564
O2 O3 Ga2 41.70(15) 6_455 1_564
La O3 Ga2 40.53(7) 2_465 1_564
Ga2 O3 Ga2 53.74(11) 2_565 1_564
O1 O3 Ga2 82.8(2) 2_466 1_564
O2 O3 Ga2 109.1(2) 1_455 1_564
O1 O3 Ga2 105.5(3) 2_455 1_564
La O3 Ga2 76.02(12) 1_455 1_564
Ga3 O3 Ga2 71.74(9) 4_456 1_564
Ga3 O3 Ga2 74.46(15) 4_345 1_564
O3 O3 Ga2 135.54(12) 1_556 1_564
O3 O3 Ga2 44.46(12) 1_554 1_564
O2 O3 Ga2 110.94(18) 6_556 1_564
O2 O3 Ga2 142.3(2) 2_456 1_564
La O3 Ga2 142.30(14) 1_556 1_564
O2 O3 Ga2 137.7(3) 4_445 1_564
O1 O3 Ga2 158.8(3) 2_456 1_564
O2 O3 Ga2 70.62(17) 6 1_564
O2 O3 Ga2 49.40(16) 3_465 1_564
O2 O3 Ga2 94.7(2) 2_455 1_564
O1 O3 Ga2 65.9(2) 1_455 1_564
Ga3 O3 O3 63.2(4) 1_556 3_565
Nb O3 O3 122.8(4) 1_455 3_565
Ga1 O3 O3 122.8(4) 1_455 3_565
La O3 O3 81.09(14) 4_455 3_565
Ga3 O3 O3 147.6(2) 2_465 3_565
O3 O3 O3 110.3(4) 2_465 3_565
O3 O3 O3 103.5(4) 4_345 3_565
O3 O3 O3 163.5(4) 3_465 3_565
O2 O3 O3 134.7(2) 4_455 3_565
O3 O3 O3 109.0(3) 2_466 3_565
O2 O3 O3 42.3(3) 3_455 3_565
O2 O3 O3 50.3(3) 5_456 3_565
O3 O3 O3 86.53(9) 6 3_565
O1 O3 O3 30.40(7) . 3_565
O2 O3 O3 55.6(2) 5_455 3_565
O3 O3 O3 86.68(10) 6_556 3_565
Ga2 O3 O3 38.20(13) 2_566 3_565
Ga3 O3 O3 120.6(2) 4_346 3_565
La O3 O3 21.69(16) . 3_565
O2 O3 O3 89.26(14) 1_565 3_565
O3 O3 O3 129.5(3) 5_345 3_565
Ga3 O3 O3 78.07(14) . 3_565
Ga2 O3 O3 112.18(14) 1_565 3_565
O3 O3 O3 128.1(2) 5_346 3_565
Nb O3 O3 104.95(14) 1_456 3_565
Ga1 O3 O3 104.95(14) 1_456 3_565
O2 O3 O3 62.40(13) 2_566 3_565
La O3 O3 77.2(2) 2_455 3_565
Ga3 O3 O3 119.88(13) 2_464 3_565
O1 O3 O3 110.12(13) 2_465 3_565
La O3 O3 85.13(9) 4_456 3_565
O2 O3 O3 146.97(19) 6_456 3_565
O2 O3 O3 64.28(14) 2_565 3_565
Ga2 O3 O3 45.97(17) . 3_565
O2 O3 O3 142.16(19) 6_455 3_565
La O3 O3 142.21(15) 2_465 3_565
Ga2 O3 O3 55.24(9) 2_565 3_565
O1 O3 O3 108.31(12) 2_466 3_565
O2 O3 O3 133.3(2) 1_455 3_565
O1 O3 O3 49.76(16) 2_455 3_565
La O3 O3 157.2(2) 1_455 3_565
Ga3 O3 O3 72.22(8) 4_456 3_565
Ga3 O3 O3 111.53(18) 4_345 3_565
O3 O3 O3 90.000(1) 1_556 3_565
O3 O3 O3 90.0 1_554 3_565
O2 O3 O3 32.53(15) 6_556 3_565
O2 O3 O3 105.8(2) 2_456 3_565
La O3 O3 47.95(14) 1_556 3_565
O2 O3 O3 59.8(2) 4_445 3_565
O1 O3 O3 53.1(2) 2_456 3_565
O2 O3 O3 36.31(15) 6 3_565
O2 O3 O3 118.67(16) 3_465 3_565
O2 O3 O3 105.1(2) 2_455 3_565
O1 O3 O3 170.8(2) 1_455 3_565
Ga2 O3 O3 106.05(9) 1_564 3_565
Ga3 O3 O3 103.1(2) 1_556 4_455
Nb O3 O3 139.9(3) 1_455 4_455
Ga1 O3 O3 139.9(3) 1_455 4_455
La O3 O3 35.9(2) 4_455 4_455
Ga3 O3 O3 106.3(2) 2_465 4_455
O3 O3 O3 92.07(3) 2_465 4_455
O3 O3 O3 163.5(4) 4_345 4_455
O3 O3 O3 136.5(4) 3_465 4_455
O2 O3 O3 75.2(2) 4_455 4_455
O3 O3 O3 91.94(3) 2_466 4_455
O2 O3 O3 101.7(3) 3_455 4_455
O2 O3 O3 67.63(19) 5_456 4_455
O3 O3 O3 121.5(2) 6 4_455
O1 O3 O3 30.40(7) . 4_455
O2 O3 O3 70.34(17) 5_455 4_455
O3 O3 O3 120.0(2) 6_556 4_455
Ga2 O3 O3 38.20(13) 2_566 4_455
Ga3 O3 O3 158.7(2) 4_346 4_455
La O3 O3 72.12(10) . 4_455
O2 O3 O3 29.65(15) 1_565 4_455
O3 O3 O3 135.2(3) 5_345 4_455
Ga3 O3 O3 95.97(10) . 4_455
Ga2 O3 O3 55.08(14) 1_565 4_455
O3 O3 O3 133.6(2) 5_346 4_455
Nb O3 O3 111.36(11) 1_456 4_455
Ga1 O3 O3 111.36(11) 1_456 4_455
O2 O3 O3 32.8(2) 2_566 4_455
La O3 O3 134.1(2) 2_455 4_455
Ga3 O3 O3 99.54(13) 2_464 4_455
O1 O3 O3 58.57(17) 2_465 4_455
La O3 O3 63.63(12) 4_456 4_455
O2 O3 O3 105.5(2) 6_456 4_455
O2 O3 O3 38.1(2) 2_565 4_455
Ga2 O3 O3 103.56(15) . 4_455
O2 O3 O3 104.54(19) 6_455 4_455
La O3 O3 85.04(17) 2_465 4_455
Ga2 O3 O3 55.24(9) 2_565 4_455
O1 O3 O3 61.56(15) 2_466 4_455
O2 O3 O3 166.0(2) 1_455 4_455
O1 O3 O3 102.59(15) 2_455 4_455
La O3 O3 135.88(19) 1_455 4_455
Ga3 O3 O3 19.22(13) 4_456 4_455
Ga3 O3 O3 132.13(12) 4_345 4_455
O3 O3 O3 90.0 1_556 4_455
O3 O3 O3 90.0 1_554 4_455
O2 O3 O3 46.98(14) 6_556 4_455
O2 O3 O3 151.01(19) 2_456 4_455
La O3 O3 77.22(9) 1_556 4_455
O2 O3 O3 119.64(19) 4_445 4_455
O1 O3 O3 101.68(12) 2_456 4_455
O2 O3 O3 49.31(11) 6 4_455
O2 O3 O3 58.80(16) 3_465 4_455
O2 O3 O3 146.72(18) 2_455 4_455
O1 O3 O3 111.26(19) 1_455 4_455
Ga2 O3 O3 65.22(12) 1_564 4_455
O3 O3 O3 60.000(1) 3_565 4_455
Ga3 O3 O2 45.9(3) 1_556 .
Nb O3 O2 102.8(3) 1_455 .
Ga1 O3 O2 102.8(3) 1_455 .
La O3 O2 108.7(3) 4_455 .
Ga3 O3 O2 141.2(4) 2_465 .
O3 O3 O2 115.9(6) 2_465 .
O3 O3 O2 73.5(3) 4_345 .
O3 O3 O2 133.4(3) 3_465 .
O2 O3 O2 161.8(4) 4_455 .
O3 O3 O2 107.4(4) 2_466 .
O2 O3 O2 12.2(2) 3_455 .
O2 O3 O2 55.7(3) 5_456 .
O3 O3 O2 71.11(17) 6 .
O1 O3 O2 60.59(17) . .
O2 O3 O2 66.1(3) 5_455 .
O3 O3 O2 66.16(17) 6_556 .
Ga2 O3 O2 61.41(15) 2_566 .
Ga3 O3 O2 91.59(17) 4_346 .
La O3 O2 29.08(14) . .
O2 O3 O2 118.7(2) 1_565 .
O3 O3 O2 111.26(19) 5_345 .
Ga3 O3 O2 76.1(2) . .
Ga2 O3 O2 138.3(2) 1_565 .
O3 O3 O2 105.9(2) 5_346 .
Nb O3 O2 91.7(2) 1_456 .
Ga1 O3 O2 91.7(2) 1_456 .
O2 O3 O2 85.24(19) 2_566 .
La O3 O2 50.31(12) 2_455 .
Ga3 O3 O2 122.1(3) 2_464 .
O1 O3 O2 136.7(3) 2_465 .
La O3 O2 95.9(2) 4_456 .
O2 O3 O2 141.3(2) 6_456 .
O2 O3 O2 89.5(2) 2_565 .
Ga2 O3 O2 17.81(12) . .
O2 O3 O2 143.3(3) 6_455 .
La O3 O2 167.6(3) 2_465 .
Ga2 O3 O2 73.65(19) 2_565 .
O1 O3 O2 126.8(3) 2_466 .
O2 O3 O2 103.1(2) 1_455 .
O1 O3 O2 32.5(2) 2_455 .
La O3 O2 131.61(16) 1_455 .
Ga3 O3 O2 100.14(16) 4_456 .
Ga3 O3 O2 94.70(19) 4_345 .
O3 O3 O2 86.4(2) 1_556 .
O3 O3 O2 93.6(2) 1_554 .
O2 O3 O2 52.71(19) 6_556 .
O2 O3 O2 77.43(15) 2_456 .
La O3 O2 46.40(15) 1_556 .
O2 O3 O2 29.62(11) 4_445 .
O1 O3 O2 32.6(2) 2_456 .
O2 O3 O2 58.6(2) 6 .
O2 O3 O2 147.96(16) 3_465 .
O2 O3 O2 81.41(18) 2_455 .
O1 O3 O2 158.71(16) 1_455 .
Ga2 O3 O2 127.2(3) 1_564 .
O3 O3 O2 30.22(16) 3_565 .
O3 O3 O2 90.03(16) 4_455 .
Ga3 O3 O2 167.0(5) 1_556 4_454
Nb O3 O2 58.7(3) 1_455 4_454
Ga1 O3 O2 58.7(3) 1_455 4_454
La O3 O2 46.5(2) 4_455 4_454
Ga3 O3 O2 94.1(2) 2_465 4_454
O3 O3 O2 12.3(2) 2_465 4_454
O3 O3 O2 105.53(15) 4_345 4_454
O3 O3 O2 75.8(2) 3_465 4_454
O2 O3 O2 65.9(3) 4_455 4_454
O3 O3 O2 128.9(4) 2_466 4_454
O2 O3 O2 127.7(5) 3_455 4_454
O2 O3 O2 149.8(3) 5_456 4_454
O3 O3 O2 66.2(4) 6 4_454
O1 O3 O2 93.2(4) . 4_454
O2 O3 O2 58.4(3) 5_455 4_454
O3 O3 O2 157.0(2) 6_556 4_454
Ga2 O3 O2 118.8(2) 2_566 4_454
Ga3 O3 O2 114.0(2) 4_346 4_454
La O3 O2 97.4(3) . 4_454
O2 O3 O2 73.7(2) 1_565 4_454
O3 O3 O2 52.9(3) 5_345 4_454
Ga3 O3 O2 49.33(17) . 4_454
Ga2 O3 O2 78.09(17) 1_565 4_454
O3 O3 O2 119.6(3) 5_346 4_454
Nb O3 O2 143.1(2) 1_456 4_454
Ga1 O3 O2 143.1(2) 1_456 4_454
O2 O3 O2 112.1(2) 2_566 4_454
La O3 O2 99.9(2) 2_455 4_454
Ga3 O3 O2 17.18(8) 2_464 4_454
O1 O3 O2 33.2(3) 2_465 4_454
La O3 O2 128.25(18) 4_456 4_454
O2 O3 O2 94.2(3) 6_456 4_454
O2 O3 O2 52.50(14) 2_565 4_454
Ga2 O3 O2 135.7(3) . 4_454
O2 O3 O2 31.3(2) 6_455 4_454
La O3 O2 44.76(14) 2_465 4_454
Ga2 O3 O2 56.09(16) 2_565 4_454
O1 O3 O2 98.0(2) 2_466 4_454
O2 O3 O2 94.2(2) 1_455 4_454
O1 O3 O2 94.9(3) 2_455 4_454
La O3 O2 63.82(14) 1_455 4_454
Ga3 O3 O2 90.48(14) 4_456 4_454
Ga3 O3 O2 55.62(15) 4_345 4_454
O3 O3 O2 149.08(16) 1_556 4_454
O3 O3 O2 30.92(16) 1_554 4_454
O2 O3 O2 125.4(2) 6_556 4_454
O2 O3 O2 126.3(2) 2_456 4_454
La O3 O2 156.7(2) 1_556 4_454
O2 O3 O2 123.4(3) 4_445 4_454
O1 O3 O2 154.3(4) 2_456 4_454
O2 O3 O2 75.20(18) 6 4_454
O2 O3 O2 64.03(12) 3_465 4_454
O2 O3 O2 75.9(2) 2_455 4_454
O1 O3 O2 62.6(3) 1_455 4_454
Ga2 O3 O2 18.84(9) 1_564 4_454
O3 O3 O2 111.33(14) 3_565 4_454
O3 O3 O2 82.39(13) 4_455 4_454
O2 O3 O2 123.3(3) . 4_454
Ga3 O3 O2 105.7(4) 1_556 3_454
Nb O3 O2 58.8(3) 1_455 3_454
Ga1 O3 O2 58.8(3) 1_455 3_454
La O3 O2 78.0(3) 4_455 3_454
Ga3 O3 O2 144.8(3) 2_465 3_454
O3 O3 O2 52.7(4) 2_465 3_454
O3 O3 O2 75.95(18) 4_345 3_454
O3 O3 O2 105.65(15) 3_465 3_454
O2 O3 O2 127.6(5) 4_455 3_454
O3 O3 O2 167.7(3) 2_466 3_454
O2 O3 O2 66.0(3) 3_455 3_454
O2 O3 O2 116.0(4) 5_456 3_454
O3 O3 O2 25.8(2) 6 3_454
O1 O3 O2 76.3(4) . 3_454
O2 O3 O2 25.7(2) 5_455 3_454
O3 O3 O2 116.6(3) 6_556 3_454
Ga2 O3 O2 102.4(3) 2_566 3_454
Ga3 O3 O2 103.7(2) 4_346 3_454
La O3 O2 46.10(16) . 3_454
O2 O3 O2 114.3(3) 1_565 3_454
O3 O3 O2 63.4(3) 5_345 3_454
Ga3 O3 O2 12.75(11) . 3_454
Ga2 O3 O2 134.0(3) 1_565 3_454
O3 O3 O2 130.3(2) 5_346 3_454
Nb O3 O2 143.31(17) 1_456 3_454
Ga1 O3 O2 143.31(17) 1_456 3_454
O2 O3 O2 121.8(2) 2_566 3_454
La O3 O2 49.46(14) 2_455 3_454
Ga3 O3 O2 58.90(19) 2_464 3_454
O1 O3 O2 89.1(3) 2_465 3_454
La O3 O2 152.0(2) 4_456 3_454
O2 O3 O2 145.4(2) 6_456 3_454
O2 O3 O2 62.0(2) 2_565 3_454
Ga2 O3 O2 73.98(16) . 3_454
O2 O3 O2 81.5(2) 6_455 3_454
La O3 O2 105.7(2) 2_465 3_454
Ga2 O3 O2 41.26(14) 2_565 3_454
O1 O3 O2 152.8(3) 2_466 3_454
O2 O3 O2 94.3(2) 1_455 3_454
O1 O3 O2 33.2(3) 2_455 3_454
La O3 O2 92.1(2) 1_455 3_454
Ga3 O3 O2 115.1(2) 4_456 3_454
Ga3 O3 O2 46.53(15) 4_345 3_454
O3 O3 O2 149.16(13) 1_556 3_454
O3 O3 O2 30.84(13) 1_554 3_454
O2 O3 O2 99.4(2) 6_556 3_454
O2 O3 O2 101.3(2) 2_456 3_454
La O3 O2 109.06(18) 1_556 3_454
O2 O3 O2 64.40(16) 4_445 3_454
O1 O3 O2 92.6(3) 2_456 3_454
O2 O3 O2 49.15(15) 6 3_454
O2 O3 O2 122.5(3) 3_465 3_454
O2 O3 O2 51.44(19) 2_455 3_454
O1 O3 O2 112.5(3) 1_455 3_454
Ga2 O3 O2 73.31(19) 1_564 3_454
O3 O3 O2 67.53(15) 3_565 3_454
O3 O3 O2 96.02(12) 4_455 3_454
O2 O3 O2 63.41(15) . 3_454
O2 O3 O2 61.7(2) 4_454 3_454
Ga3 O3 Ga2 108.5(4) 1_556 2_466
Nb O3 Ga2 74.2(3) 1_455 2_466
Ga1 O3 Ga2 74.2(3) 1_455 2_466
La O3 Ga2 99.1(2) 4_455 2_466
Ga3 O3 Ga2 15.65(13) 2_465 2_466
O3 O3 Ga2 83.5(4) 2_465 2_466
O3 O3 Ga2 85.3(3) 4_345 2_466
O3 O3 Ga2 29.2(2) 3_465 2_466
O2 O3 Ga2 36.5(2) 4_455 2_466
O3 O3 Ga2 54.7(3) 2_466 2_466
O2 O3 Ga2 140.5(3) 3_455 2_466
O2 O3 Ga2 113.4(4) 5_456 2_466
O3 O3 Ga2 110.63(11) 6 2_466
O1 O3 Ga2 140.7(2) . 2_466
O2 O3 Ga2 138.2(3) 5_455 2_466
O3 O3 Ga2 86.4(2) 6_556 2_466
Ga2 O3 Ga2 125.0(3) 2_566 2_466
Ga3 O3 Ga2 62.21(14) 4_346 2_466
La O3 Ga2 175.8(3) . 2_466
O2 O3 Ga2 81.01(19) 1_565 2_466
O3 O3 Ga2 67.85(18) 5_345 2_466
Ga3 O3 Ga2 118.75(19) . 2_466
Ga2 O3 Ga2 55.60(12) 1_565 2_466
O3 O3 Ga2 45.89(9) 5_346 2_466
Nb O3 Ga2 63.28(15) 1_456 2_466
Ga1 O3 Ga2 63.28(15) 1_456 2_466
O2 O3 Ga2 101.4(2) 2_566 2_466
La O3 Ga2 115.00(15) 2_455 2_466
Ga3 O3 Ga2 74.74(12) 2_464 2_466
O1 O3 Ga2 71.55(18) 2_465 2_466
La O3 Ga2 77.41(18) 4_456 2_466
O2 O3 Ga2 16.11(16) 6_456 2_466
O2 O3 Ga2 118.63(17) 2_565 2_466
Ga2 O3 Ga2 134.0(2) . 2_466
O2 O3 Ga2 51.49(16) 6_455 2_466
La O3 Ga2 39.86(7) 2_465 2_466
Ga2 O3 Ga2 133.88(18) 2_565 2_466
O1 O3 Ga2 55.58(11) 2_466 2_466
O2 O3 Ga2 55.49(13) 1_455 2_466
O1 O3 Ga2 145.34(16) 2_455 2_466
La O3 Ga2 39.57(7) 1_455 2_466
Ga3 O3 Ga2 95.03(15) 4_456 2_466
Ga3 O3 Ga2 85.78(12) 4_345 2_466
O3 O3 Ga2 74.79(13) 1_556 2_466
O3 O3 Ga2 105.20(13) 1_554 2_466
O2 O3 Ga2 130.0(3) 6_556 2_466
O2 O3 Ga2 75.37(15) 2_456 2_466
La O3 Ga2 117.8(2) 1_556 2_466
O2 O3 Ga2 126.11(19) 4_445 2_466
O1 O3 Ga2 120.8(3) 2_456 2_466
O2 O3 Ga2 149.58(19) 6 2_466
O2 O3 Ga2 52.98(12) 3_465 2_466
O2 O3 Ga2 90.35(14) 2_455 2_466
O1 O3 Ga2 18.2(2) 1_455 2_466
Ga2 O3 Ga2 80.18(11) 1_564 2_466
O3 O3 Ga2 162.53(15) 3_565 2_466
O3 O3 Ga2 110.51(18) 4_455 2_466
O2 O3 Ga2 151.8(2) . 2_466
O2 O3 Ga2 79.92(16) 4_454 2_466
O2 O3 Ga2 129.8(2) 3_454 2_466
Ga3 O3 La 97.4(3) 1_556 2_565
Nb O3 La 128.7(5) 1_455 2_565
Ga1 O3 La 128.7(5) 1_455 2_565
La O3 La 42.13(14) 4_455 2_565
Ga3 O3 La 131.2(2) 2_465 2_565
O3 O3 La 88.2(3) 2_465 2_565
O3 O3 La 140.2(4) 4_345 2_565
O3 O3 La 154.9(3) 3_465 2_565
O2 O3 La 98.0(2) 4_455 2_565
O3 O3 La 111.24(19) 2_466 2_565
O2 O3 La 81.9(2) 3_455 2_565
O2 O3 La 68.6(2) 5_456 2_565
O3 O3 La 100.0(3) 6 2_565
O1 O3 La 11.0(3) . 2_565
O2 O3 La 49.54(18) 5_455 2_565
O3 O3 La 119.80(19) 6_556 2_565
Ga2 O3 La 38.28(11) 2_566 2_565
Ga3 O3 La 160.3(2) 4_346 2_565
La O3 La 47.84(9) . 2_565
O2 O3 La 53.57(14) 1_565 2_565
O3 O3 La 128.7(5) 5_345 2_565
Ga3 O3 La 77.32(17) . 2_565
Ga2 O3 La 79.64(11) 1_565 2_565
O3 O3 La 151.7(4) 5_346 2_565
Nb O3 La 124.3(2) 1_456 2_565
Ga1 O3 La 124.3(2) 1_456 2_565
O2 O3 La 48.49(16) 2_566 2_565
La O3 La 109.4(2) 2_455 2_565
Ga3 O3 La 97.8(2) 2_464 2_565
O1 O3 La 70.85(11) 2_465 2_565
La O3 La 81.13(11) 4_456 2_565
O2 O3 La 130.34(19) 6_456 2_565
O2 O3 La 30.17(16) 2_565 2_565
Ga2 O3 La 86.00(13) . 2_565
O2 O3 La 112.1(2) 6_455 2_565
La O3 La 102.27(13) 2_465 2_565
Ga2 O3 La 36.92(6) 2_565 2_565
O1 O3 La 85.95(12) 2_466 2_565
O2 O3 La 168.2(3) 1_455 2_565
O1 O3 La 77.77(15) 2_455 2_565
La O3 La 146.2(2) 1_455 2_565
Ga3 O3 La 43.19(6) 4_456 2_565
Ga3 O3 La 117.4(2) 4_345 2_565
O3 O3 La 102.55(13) 1_556 2_565
O3 O3 La 77.45(13) 1_554 2_565
O2 O3 La 43.03(15) 6_556 2_565
O2 O3 La 145.3(2) 2_456 2_565
La O3 La 74.06(10) 1_556 2_565
O2 O3 La 98.63(17) 4_445 2_565
O1 O3 La 90.66(14) 2_456 2_565
O2 O3 La 25.36(11) 6 2_565
O2 O3 La 81.45(12) 3_465 2_565
O2 O3 La 125.5(2) 2_455 2_565
O1 O3 La 130.74(16) 1_455 2_565
Ga2 O3 La 70.54(11) 1_564 2_565
O3 O3 La 40.03(7) 3_565 2_565
O3 O3 La 24.89(7) 4_455 2_565
O2 O3 La 69.77(14) . 2_565
O2 O3 La 82.67(16) 4_454 2_565
O2 O3 La 74.19(17) 3_454 2_565
Ga2 O3 La 134.34(13) 2_466 2_565
Ga3 O3 La 19.56(17) 1_556 2_456
Nb O3 La 96.5(2) 1_455 2_456
Ga1 O3 La 96.5(2) 1_455 2_456
La O3 La 157.3(3) 4_455 2_456
Ga3 O3 La 84.6(3) 2_465 2_456
O3 O3 La 143.72(18) 2_465 2_456
O3 O3 La 49.65(17) 4_345 2_456
O3 O3 La 87.74(16) 3_465 2_456
O2 O3 La 122.1(4) 4_455 2_456
O3 O3 La 61.2(3) 2_466 2_456
O2 O3 La 47.7(3) 3_455 2_456
O2 O3 La 54.26(19) 5_456 2_456
O3 O3 La 93.8(3) 6 2_456
O1 O3 La 105.6(4) . 2_456
O2 O3 La 121.1(2) 5_455 2_456
O3 O3 La 10.18(18) 6_556 2_456
Ga2 O3 La 84.24(19) 2_566 2_456
Ga3 O3 La 44.43(10) 4_346 2_456
La O3 La 86.38(14) . 2_456
O2 O3 La 129.9(3) 1_565 2_456
O3 O3 La 102.5(2) 5_345 2_456
Ga3 O3 La 116.66(16) . 2_456
Ga2 O3 La 118.9(3) 1_565 2_456
O3 O3 La 49.04(18) 5_346 2_456
Nb O3 La 38.16(8) 1_456 2_456
Ga1 O3 La 38.16(8) 1_456 2_456
O2 O3 La 92.7(2) 2_566 2_456
La O3 La 60.19(9) 2_455 2_456
Ga3 O3 La 138.09(15) 2_464 2_456
O1 O3 La 163.8(4) 2_465 2_456
La O3 La 72.95(17) 4_456 2_456
O2 O3 La 84.8(2) 6_456 2_456
O2 O3 La 144.6(2) 2_565 2_456
Ga2 O3 La 39.93(8) . 2_456
O2 O3 La 130.99(19) 6_455 2_456
La O3 La 134.6(2) 2_465 2_456
Ga2 O3 La 130.90(17) 2_565 2_456
O1 O3 La 98.8(3) 2_466 2_456
O2 O3 La 63.57(18) 1_455 2_456
O1 O3 La 75.7(2) 2_455 2_456
La O3 La 96.68(14) 1_455 2_456
Ga3 O3 La 114.3(2) 4_456 2_456
Ga3 O3 La 100.00(11) 4_345 2_456
O3 O3 La 46.54(11) 1_556 2_456
O3 O3 La 133.46(11) 1_554 2_456
O2 O3 La 76.40(18) 6_556 2_456
O2 O3 La 30.34(14) 2_456 2_456
La O3 La 44.96(8) 1_556 2_456
O2 O3 La 42.54(16) 4_445 2_456
O1 O3 La 27.23(11) 2_456 2_456
O2 O3 La 115.10(18) 6 2_456
O2 O3 La 130.9(3) 3_465 2_456
O2 O3 La 79.90(15) 2_455 2_456
O1 O3 La 108.0(2) 1_455 2_456
Ga2 O3 La 172.65(16) 1_564 2_456
O3 O3 La 80.35(16) 3_565 2_456
O3 O3 La 121.86(11) 4_455 2_456
O2 O3 La 57.30(15) . 2_456
O2 O3 La 155.15(18) 4_454 2_456
O2 O3 La 106.57(15) 3_454 2_456
Ga2 O3 La 94.74(18) 2_466 2_456
La O3 La 116.66(14) 2_565 2_456
Ga3 O3 O1 47.5(2) 1_556 1_556
Nb O3 O1 158.6(4) 1_455 1_556
Ga1 O3 O1 158.6(4) 1_455 1_556
La O3 O1 96.8(2) 4_455 1_556
Ga3 O3 O1 86.1(3) 2_465 1_556
O3 O3 O1 153.29(12) 2_465 1_556
O3 O3 O1 112.29(19) 4_345 1_556
O3 O3 O1 122.37(17) 3_465 1_556
O2 O3 O1 92.4(4) 4_455 1_556
O3 O3 O1 48.3(3) 2_466 1_556
O2 O3 O1 74.3(3) 3_455 1_556
O2 O3 O1 15.5(2) 5_456 1_556
O3 O3 O1 141.9(2) 6 1_556
O1 O3 O1 61.8(3) . 1_556
O2 O3 O1 113.6(3) 5_455 1_556
O3 O3 O1 58.8(3) 6_556 1_556
Ga2 O3 O1 31.74(19) 2_566 1_556
Ga3 O3 O1 99.1(3) 4_346 1_556
La O3 O1 82.84(17) . 1_556
O2 O3 O1 69.3(2) 1_565 1_556
O3 O3 O1 161.7(4) 5_345 1_556
Ga3 O3 O1 139.4(2) . 1_556
Ga2 O3 O1 72.23(16) 1_565 1_556
O3 O3 O1 82.6(4) 5_346 1_556
Nb O3 O1 54.82(18) 1_456 1_556
Ga1 O3 O1 54.82(18) 1_456 1_556
O2 O3 O1 30.09(18) 2_566 1_556
La O3 O1 113.04(17) 2_455 1_556
Ga3 O3 O1 158.49(16) 2_464 1_556
O1 O3 O1 110.7(3) 2_465 1_556
La O3 O1 25.27(9) 4_456 1_556
O2 O3 O1 85.5(2) 6_456 1_556
O2 O3 O1 97.2(2) 2_565 1_556
Ga2 O3 O1 68.92(13) . 1_556
O2 O3 O1 145.5(2) 6_455 1_556
La O3 O1 116.02(19) 2_465 1_556
Ga2 O3 O1 105.41(17) 2_565 1_556
O1 O3 O1 56.16(17) 2_466 1_556
O2 O3 O1 117.9(3) 1_455 1_556
O1 O3 O1 103.3(3) 2_455 1_556
La O3 O1 136.8(3) 1_455 1_556
Ga3 O3 O1 51.67(12) 4_456 1_556
Ga3 O3 O1 161.48(16) 4_345 1_556
O3 O3 O1 33.41(15) 1_556 1_556
O3 O3 O1 146.59(15) 1_554 1_556
O2 O3 O1 31.03(18) 6_556 1_556
O2 O3 O1 89.6(2) 2_456 1_556
La O3 O1 26.70(5) 1_556 1_556
O2 O3 O1 86.78(18) 4_445 1_556
O1 O3 O1 54.11(16) 2_456 1_556
O2 O3 O1 88.20(19) 6 1_556
O2 O3 O1 86.3(2) 3_465 1_556
O2 O3 O1 141.4(2) 2_455 1_556
O1 O3 O1 118.3(4) 1_455 1_556
Ga2 O3 O1 123.39(14) 1_564 1_556
O3 O3 O1 61.52(13) 3_565 1_556
O3 O3 O1 61.52(13) 4_455 1_556
O2 O3 O1 70.95(17) . 1_556
O2 O3 O1 142.15(17) 4_454 1_556
O2 O3 O1 128.94(19) 3_454 1_556
Ga2 O3 O1 101.3(2) 2_466 1_556
La O3 O1 69.49(15) 2_565 1_556
La O3 O1 62.64(14) 2_456 1_556
Ga3 O3 O3 116.8(4) 1_556 4_344
Nb O3 O3 30.1(3) 1_455 4_344
Ga1 O3 O3 30.1(3) 1_455 4_344
La O3 O3 87.3(3) 4_455 4_344
Ga3 O3 O3 115.7(3) 2_465 4_344
O3 O3 O3 38.6(3) 2_465 4_344
O3 O3 O3 62.02(11) 4_345 4_344
O3 O3 O3 76.43(5) 3_465 4_344
O2 O3 O3 110.4(3) 4_455 4_344
O3 O3 O3 148.9(3) 2_466 4_344
O2 O3 O3 83.4(4) 3_455 4_344
O2 O3 O3 141.2(4) 5_456 4_344
O3 O3 O3 15.8(2) 6 4_344
O1 O3 O3 104.0(4) . 4_344
O2 O3 O3 50.5(2) 5_455 4_344
O3 O3 O3 115.2(4) 6_556 4_344
Ga2 O3 O3 131.6(3) 2_566 4_344
Ga3 O3 O3 84.6(2) 4_346 4_344
La O3 O3 74.6(2) . 4_344
O2 O3 O3 122.2(3) 1_565 4_344
O3 O3 O3 34.1(3) 5_345 4_344
Ga3 O3 O3 22.44(7) . 4_344
Ga2 O3 O3 128.1(2) 1_565 4_344
O3 O3 O3 107.9(3) 5_346 4_344
Nb O3 O3 131.8(2) 1_456 4_344
Ga1 O3 O3 131.8(2) 1_456 4_344
O2 O3 O3 148.0(3) 2_566 4_344
La O3 O3 49.08(18) 2_455 4_344
Ga3 O3 O3 39.48(7) 2_464 4_344
O1 O3 O3 83.9(3) 2_465 4_344
La O3 O3 178.5(2) 4_456 4_344
O2 O3 O3 116.4(2) 6_456 4_344
O2 O3 O3 78.7(2) 2_565 4_344
Ga2 O3 O3 89.7(2) . 4_344
O2 O3 O3 57.83(16) 6_455 4_344
La O3 O3 86.53(14) 2_465 4_344
Ga2 O3 O3 63.13(16) 2_565 4_344
O1 O3 O3 146.5(2) 2_466 4_344
O2 O3 O3 69.9(2) 1_455 4_344
O1 O3 O3 53.0(3) 2_455 4_344
La O3 O3 62.85(14) 1_455 4_344
Ga3 O3 O3 133.3(2) 4_456 4_344
Ga3 O3 O3 17.99(10) 4_345 4_344
O3 O3 O3 152.02(11) 1_556 4_344
O3 O3 O3 27.98(11) 1_554 4_344
O2 O3 O3 128.6(3) 6_556 4_344
O2 O3 O3 88.6(2) 2_456 4_344
La O3 O3 131.2(2) 1_556 4_344
O2 O3 O3 73.7(2) 4_445 4_344
O1 O3 O3 106.7(3) 2_456 4_344
O2 O3 O3 76.3(2) 6 4_344
O2 O3 O3 113.7(2) 3_465 4_344
O2 O3 O3 30.95(17) 2_455 4_344
O1 O3 O3 85.1(3) 1_455 4_344
Ga2 O3 O3 68.46(11) 1_564 4_344
O3 O3 O3 96.3(2) 3_565 4_344
O3 O3 O3 116.74(13) 4_455 4_344
O2 O3 O3 85.5(2) . 4_344
O2 O3 O3 50.80(13) 4_454 4_344
O2 O3 O3 29.29(15) 3_454 4_344
Ga2 O3 O3 101.16(17) 2_466 4_344
La O3 O3 99.7(2) 2_565 4_344
La O3 O3 107.68(17) 2_456 4_344
O1 O3 O3 156.2(2) 1_556 4_344
Ga3 O3 O3 34.1(3) 1_556 4_346
Nb O3 O3 103.0(4) 1_455 4_346
Ga1 O3 O3 103.0(4) 1_455 4_346
La O3 O3 148.6(3) 4_455 4_346
Ga3 O3 O3 62.0(2) 2_465 4_346
O3 O3 O3 148.3(3) 2_465 4_346
O3 O3 O3 62.02(11) 4_345 4_346
O3 O3 O3 76.43(5) 3_465 4_346
O2 O3 O3 97.9(4) 4_455 4_346
O3 O3 O3 37.6(2) 2_466 4_346
O2 O3 O3 71.0(4) 3_455 4_346
O2 O3 O3 54.9(2) 5_456 4_346
O3 O3 O3 113.1(4) 6 4_346
O1 O3 O3 113.7(5) . 4_346
O2 O3 O3 144.8(3) 5_455 4_346
O3 O3 O3 14.2(2) 6_556 4_346
Ga2 O3 O3 85.5(2) 2_566 4_346
Ga3 O3 O3 43.1(2) 4_346 4_346
La O3 O3 107.6(2) . 4_346
O2 O3 O3 112.2(3) 1_565 4_346
O3 O3 O3 106.0(4) 5_345 4_346
Ga3 O3 O3 138.70(19) . 4_346
Ga2 O3 O3 95.87(19) 1_565 4_346
O3 O3 O3 32.4(3) 5_346 4_346
Nb O3 O3 13.83(5) 1_456 4_346
Ga1 O3 O3 13.83(5) 1_456 4_346
O2 O3 O3 83.9(2) 2_566 4_346
La O3 O3 81.6(2) 2_455 4_346
Ga3 O3 O3 138.6(2) 2_464 4_346
O1 O3 O3 139.5(3) 2_465 4_346
La O3 O3 56.09(9) 4_456 4_346
O2 O3 O3 62.2(2) 6_456 4_346
O2 O3 O3 153.0(3) 2_565 4_346
Ga2 O3 O3 62.88(17) . 4_346
O2 O3 O3 120.7(3) 6_455 4_346
La O3 O3 113.2(2) 2_465 4_346
Ga2 O3 O3 151.3(2) 2_565 4_346
O1 O3 O3 76.4(2) 2_466 4_346
O2 O3 O3 62.1(3) 1_455 4_346
O1 O3 O3 100.0(3) 2_455 4_346
La O3 O3 89.0(2) 1_455 4_346
Ga3 O3 O3 102.40(16) 4_456 4_346
Ga3 O3 O3 110.9(2) 4_345 4_346
O3 O3 O3 27.98(11) 1_556 4_346
O3 O3 O3 152.02(11) 1_554 4_346
O2 O3 O3 80.6(2) 6_556 4_346
O2 O3 O3 35.7(2) 2_456 4_346
La O3 O3 50.82(11) 1_556 4_346
O2 O3 O3 66.8(2) 4_445 4_346
O1 O3 O3 46.7(2) 2_456 4_346
O2 O3 O3 132.6(2) 6 4_346
O2 O3 O3 106.9(2) 3_465 4_346
O2 O3 O3 93.3(2) 2_455 4_346
O1 O3 O3 90.4(3) 1_455 4_346
Ga2 O3 O3 153.3(2) 1_564 4_346
O3 O3 O3 96.3(2) 3_565 4_346
O3 O3 O3 116.74(13) 4_455 4_346
O2 O3 O3 79.2(2) . 4_346
O2 O3 O3 152.0(3) 4_454 4_346
O2 O3 O3 130.12(19) 3_454 4_346
Ga2 O3 O3 74.36(17) 2_466 4_346
La O3 O3 123.51(18) 2_565 4_346
La O3 O3 24.33(11) 2_456 4_346
O1 O3 O3 56.00(16) 1_556 4_346
O3 O3 O3 124.0(2) 4_344 4_346
Ga3 O3 O3 140.6(4) 1_556 3_464
Nb O3 O3 30.1(3) 1_455 3_464
Ga1 O3 O3 30.1(3) 1_455 3_464
La O3 O3 74.4(2) 4_455 3_464
Ga3 O3 O3 95.3(3) 2_465 3_464
O3 O3 O3 17.96(11) 2_465 3_464
O3 O3 O3 76.43(5) 4_345 3_464
O3 O3 O3 62.02(11) 3_465 3_464
O2 O3 O3 83.2(4) 4_455 3_464
O3 O3 O3 134.2(4) 2_466 3_464
O2 O3 O3 110.5(4) 3_455 3_464
O2 O3 O3 166.8(4) 5_456 3_464
O3 O3 O3 42.7(3) 6 3_464
O1 O3 O3 112.0(5) . 3_464
O2 O3 O3 62.31(19) 5_455 3_464
O3 O3 O3 130.0(4) 6_556 3_464
Ga2 O3 O3 141.7(3) 2_566 3_464
Ga3 O3 O3 89.1(2) 4_346 3_464
La O3 O3 96.3(2) . 3_464
O2 O3 O3 102.5(3) 1_565 3_464
O3 O3 O3 26.1(3) 5_345 3_464
Ga3 O3 O3 39.05(6) . 3_464
Ga2 O3 O3 101.8(2) 1_565 3_464
O3 O3 O3 103.9(3) 5_346 3_464
Nb O3 O3 131.8(2) 1_456 3_464
Ga1 O3 O3 131.8(2) 1_456 3_464
O2 O3 O3 141.2(2) 2_566 3_464
La O3 O3 73.82(18) 2_455 3_464
Ga3 O3 O3 13.51(9) 2_464 3_464
O1 O3 O3 61.2(2) 2_465 3_464
La O3 O3 151.5(2) 4_456 3_464
O2 O3 O3 95.8(2) 6_456 3_464
O2 O3 O3 74.9(2) 2_565 3_464
Ga2 O3 O3 116.7(2) . 3_464
O2 O3 O3 31.27(18) 6_455 3_464
La O3 O3 59.41(17) 2_465 3_464
Ga2 O3 O3 68.63(12) 2_565 3_464
O1 O3 O3 119.4(3) 2_466 3_464
O2 O3 O3 70.0(2) 1_455 3_464
O1 O3 O3 79.6(3) 2_455 3_464
La O3 O3 47.62(16) 1_455 3_464
Ga3 O3 O3 119.65(19) 4_456 3_464
Ga3 O3 O3 26.61(11) 4_345 3_464
O3 O3 O3 152.02(11) 1_556 3_464
O3 O3 O3 27.98(11) 1_554 3_464
O2 O3 O3 144.4(2) 6_556 3_464
O2 O3 O3 99.1(2) 2_456 3_464
La O3 O3 158.3(2) 1_556 3_464
O2 O3 O3 99.7(2) 4_445 3_464
O1 O3 O3 132.8(3) 2_456 3_464
O2 O3 O3 86.77(18) 6 3_464
O2 O3 O3 87.5(2) 3_465 3_464
O2 O3 O3 46.92(18) 2_455 3_464
O1 O3 O3 61.9(3) 1_455 3_464
Ga2 O3 O3 48.01(12) 1_564 3_464
O3 O3 O3 116.74(13) 3_565 3_464
O3 O3 O3 109.88(15) 4_455 3_464
O2 O3 O3 112.2(2) . 3_464
O2 O3 O3 29.19(12) 4_454 3_464
O2 O3 O3 50.82(14) 3_454 3_464
Ga2 O3 O3 79.74(18) 2_466 3_464
La O3 O3 103.48(16) 2_565 3_464
La O3 O3 126.08(18) 2_456 3_464
O1 O3 O3 171.2(2) 1_556 3_464
O3 O3 O3 27.13(10) 4_344 3_464
O3 O3 O3 132.06(19) 4_346 3_464
Ga3 O3 O3 59.6(3) 1_556 3_466
Nb O3 O3 103.0(4) 1_455 3_466
Ga1 O3 O3 103.0(4) 1_455 3_466
La O3 O3 129.3(4) 4_455 3_466
Ga3 O3 O3 36.0(3) 2_465 3_466
O3 O3 O3 132.9(5) 2_465 3_466
O3 O3 O3 76.43(5) 4_345 3_466
O3 O3 O3 62.02(11) 3_465 3_466
O2 O3 O3 70.8(4) 4_455 3_466
O3 O3 O3 17.96(12) 2_466 3_466
O2 O3 O3 98.0(3) 3_455 3_466
O2 O3 O3 67.7(3) 5_456 3_466
O3 O3 O3 128.3(3) 6 3_466
O1 O3 O3 122.3(5) . 3_466
O2 O3 O3 171.6(3) 5_455 3_466
O3 O3 O3 41.2(2) 6_556 3_466
Ga2 O3 O3 92.5(2) 2_566 3_466
Ga3 O3 O3 49.38(17) 4_346 3_466
La O3 O3 132.7(2) . 3_466
O2 O3 O3 93.5(3) 1_565 3_466
O3 O3 O3 101.8(4) 5_345 3_466
Ga3 O3 O3 154.02(19) . 3_466
Ga2 O3 O3 71.9(2) 1_565 3_466
O3 O3 O3 24.1(3) 5_346 3_466
Nb O3 O3 13.83(5) 1_456 3_466
Ga1 O3 O3 13.83(5) 1_456 3_466
O2 O3 O3 79.9(2) 2_566 3_466
La O3 O3 103.28(18) 2_455 3_466
Ga3 O3 O3 123.3(2) 2_464 3_466
O1 O3 O3 112.6(4) 2_465 3_466
La O3 O3 47.25(12) 4_456 3_466
O2 O3 O3 36.0(2) 6_456 3_466
O2 O3 O3 145.7(3) 2_565 3_466
Ga2 O3 O3 89.87(16) . 3_466
O2 O3 O3 100.9(3) 6_455 3_466
La O3 O3 86.9(3) 2_465 3_466
Ga2 O3 O3 164.80(19) 2_565 3_466
O1 O3 O3 54.6(3) 2_466 3_466
O2 O3 O3 62.2(2) 1_455 3_466
O1 O3 O3 126.5(2) 2_455 3_466
La O3 O3 76.4(2) 1_455 3_466
Ga3 O3 O3 91.3(2) 4_456 3_466
Ga3 O3 O3 114.47(18) 4_345 3_466
O3 O3 O3 27.98(11) 1_556 3_466
O3 O3 O3 152.02(11) 1_554 3_466
O2 O3 O3 91.5(2) 6_556 3_466
O2 O3 O3 50.96(16) 2_456 3_466
La O3 O3 68.81(10) 1_556 3_466
O2 O3 O3 93.2(2) 4_445 3_466
O1 O3 O3 72.9(2) 2_456 3_466
O2 O3 O3 149.1(2) 6 3_466
O2 O3 O3 81.1(3) 3_465 3_466
O2 O3 O3 103.4(2) 2_455 3_466
O1 O3 O3 67.8(3) 1_455 3_466
Ga2 O3 O3 126.3(2) 1_564 3_466
O3 O3 O3 116.74(13) 3_565 3_466
O3 O3 O3 109.88(15) 4_455 3_466
O2 O3 O3 105.5(2) . 3_466
O2 O3 O3 130.0(3) 4_454 3_466
O2 O3 O3 152.22(19) 3_454 3_466
Ga2 O3 O3 50.11(19) 2_466 3_466
La O3 O3 128.09(18) 2_565 3_466
La O3 O3 51.25(9) 2_456 3_466
O1 O3 O3 60.92(15) 1_556 3_466
O3 O3 O3 132.06(18) 4_344 3_466
O3 O3 O3 27.13(10) 4_346 3_466
O3 O3 O3 124.0(2) 3_464 3_466
Ga3 O3 O1 64.3(3) 1_556 1_445
Nb O3 O1 49.1(2) 1_455 1_445
Ga1 O3 O1 49.1(2) 1_455 1_445
La O3 O1 146.3(4) 4_455 1_445
Ga3 O3 O1 95.5(2) 2_465 1_445
O3 O3 O1 94.3(3) 2_465 1_445
O3 O3 O1 7.8(2) 4_345 1_445
O3 O3 O1 67.3(2) 3_465 1_445
O2 O3 O1 128.8(3) 4_455 1_445
O3 O3 O1 99.1(3) 2_466 1_445
O2 O3 O1 55.2(2) 3_455 1_445
O2 O3 O1 100.2(3) 5_456 1_445
O3 O3 O1 48.3(3) 6 1_445
O1 O3 O1 125.7(2) . 1_445
O2 O3 O1 94.8(3) 5_455 1_445
O3 O3 O1 55.8(3) 6_556 1_445
Ga2 O3 O1 123.8(2) 2_566 1_445
Ga3 O3 O1 35.56(17) 4_346 1_445
La O3 O1 84.50(14) . 1_445
O2 O3 O1 174.1(3) 1_565 1_445
O3 O3 O1 56.7(2) 5_345 1_445
Ga3 O3 O1 74.8(2) . 1_445
Ga2 O3 O1 147.8(2) 1_565 1_445
O3 O3 O1 61.91(19) 5_346 1_445
Nb O3 O1 75.4(2) 1_456 1_445
Ga1 O3 O1 75.4(2) 1_456 1_445
O2 O3 O1 140.7(3) 2_566 1_445
La O3 O1 23.74(14) 2_455 1_445
Ga3 O3 O1 90.0(2) 2_464 1_445
O1 O3 O1 137.2(2) 2_465 1_445
La O3 O1 120.9(3) 4_456 1_445
O2 O3 O1 96.3(2) 6_456 1_445
O2 O3 O1 132.1(3) 2_565 1_445
Ga2 O3 O1 54.59(11) . 1_445
O2 O3 O1 92.9(2) 6_455 1_445
La O3 O1 116.99(17) 2_465 1_445
Ga2 O3 O1 110.6(3) 2_565 1_445
O1 O3 O1 136.2(2) 2_466 1_445
O2 O3 O1 37.80(11) 1_455 1_445
O1 O3 O1 55.13(18) 2_455 1_445
La O3 O1 66.01(10) 1_455 1_445
Ga3 O3 O1 162.5(3) 4_456 1_445
Ga3 O3 O1 50.6(2) 4_345 1_445
O3 O3 O1 92.8(2) 1_556 1_445
O3 O3 O1 87.2(2) 1_554 1_445
O2 O3 O1 114.3(2) 6_556 1_445
O2 O3 O1 31.3(2) 2_456 1_445
La O3 O1 88.8(2) 1_556 1_445
O2 O3 O1 37.07(10) 4_445 1_445
O1 O3 O1 61.1(2) 2_456 1_445
O2 O3 O1 110.3(2) 6 1_445
O2 O3 O1 145.09(18) 3_465 1_445
O2 O3 O1 30.4(2) 2_455 1_445
O1 O3 O1 92.33(11) 1_455 1_445
Ga2 O3 O1 125.0(3) 1_564 1_445
O3 O3 O1 96.2(2) 3_565 1_445
O3 O3 O1 156.1(2) 4_455 1_445
O2 O3 O1 66.47(12) . 1_445
O2 O3 O1 106.2(3) 4_454 1_445
O2 O3 O1 70.1(2) 3_454 1_445
Ga2 O3 O1 93.13(12) 2_466 1_445
La O3 O1 132.33(18) 2_565 1_445
La O3 O1 49.5(2) 2_456 1_445
O1 O3 O1 111.5(3) 1_556 1_445
O3 O3 O1 59.5(3) 4_344 1_445
O3 O3 O1 65.1(3) 4_346 1_445
O3 O3 O1 77.0(2) 3_464 1_445
O3 O3 O1 82.1(3) 3_466 1_445
Ga3 O3 La 92.7(4) 1_556 2_466
Nb O3 La 108.0(3) 1_455 2_466
Ga1 O3 La 108.0(3) 1_455 2_466
La O3 La 93.0(2) 4_455 2_466
Ga3 O3 La 21.72(13) 2_465 2_466
O3 O3 La 107.9(4) 2_465 2_466
O3 O3 La 106.4(2) 4_345 2_466
O3 O3 La 61.6(2) 3_465 2_466
O2 O3 La 34.3(3) 4_455 2_466
O3 O3 La 29.5(3) 2_466 2_466
O2 O3 La 132.7(4) 3_455 2_466
O2 O3 La 82.9(3) 5_456 2_466
O3 O3 La 144.36(7) 6 2_466
O1 O3 La 112.3(3) . 2_466
O2 O3 La 148.8(2) 5_455 2_466
O3 O3 La 78.3(3) 6_556 2_466
Ga2 O3 La 91.3(2) 2_566 2_466
Ga3 O3 La 78.1(2) 4_346 2_466
La O3 La 150.3(2) . 2_466
O2 O3 La 60.8(2) 1_565 2_466
O3 O3 La 101.7(2) 5_345 2_466
Ga3 O3 La 147.68(19) . 2_466
Ga2 O3 La 35.80(11) 1_565 2_466
O3 O3 La 52.20(15) 5_346 2_466
Nb O3 La 50.34(13) 1_456 2_466
Ga1 O3 La 50.34(13) 1_456 2_466
O2 O3 La 68.48(18) 2_566 2_466
La O3 La 137.2(2) 2_455 2_466
Ga3 O3 La 101.53(14) 2_464 2_466
O1 O3 La 75.4(3) 2_465 2_466
La O3 La 44.08(11) 4_456 2_466
O2 O3 La 20.86(12) 6_456 2_466
O2 O3 La 112.17(16) 2_565 2_466
Ga2 O3 La 124.6(2) . 2_466
O2 O3 La 79.17(18) 6_455 2_466
La O3 La 54.94(10) 2_465 2_466
Ga2 O3 La 134.11(13) 2_565 2_466
O1 O3 La 24.73(9) 2_466 2_466
O2 O3 La 81.06(19) 1_455 2_466
O1 O3 La 164.2(3) 2_455 2_466
La O3 La 73.34(13) 1_455 2_466
Ga3 O3 La 67.46(12) 4_456 2_466
Ga3 O3 La 119.64(15) 4_345 2_466
O3 O3 La 49.97(9) 1_556 2_466
O3 O3 La 130.03(9) 1_554 2_466
O2 O3 La 96.2(2) 6_556 2_466
O2 O3 La 85.30(19) 2_456 2_466
La O3 La 90.42(19) 1_556 2_466
O2 O3 La 130.8(3) 4_445 2_466
O1 O3 La 106.1(3) 2_456 2_466
O2 O3 La 135.30(15) 6 2_466
O2 O3 La 43.39(15) 3_465 2_466
O2 O3 La 121.92(18) 2_455 2_466
O1 O3 La 49.4(2) 1_455 2_466
Ga2 O3 La 90.13(11) 1_564 2_466
O3 O3 La 128.78(10) 3_565 2_466
O3 O3 La 86.07(13) 4_455 2_466
O2 O3 La 136.2(3) . 2_466
O2 O3 La 99.44(17) 4_454 2_466
O2 O3 La 160.4(2) 3_454 2_466
Ga2 O3 La 33.85(7) 2_466 2_466
La O3 La 110.64(13) 2_565 2_466
La O3 La 88.50(18) 2_456 2_466
O1 O3 La 68.93(15) 1_556 2_466
O3 O3 La 134.44(18) 4_344 2_466
O3 O3 La 64.17(11) 4_346 2_466
O3 O3 La 110.17(19) 3_464 2_466
O3 O3 La 37.71(16) 3_466 2_466
O1 O3 La 113.7(2) 1_445 2_466
Ga3 O3 O2 152.5(4) 1_556 1_564
Nb O3 O2 83.4(3) 1_455 1_564
Ga1 O3 O2 83.4(3) 1_455 1_564
La O3 O2 21.4(2) 4_455 1_564
Ga3 O3 O2 107.5(2) 2_465 1_564
O3 O3 O2 35.51(13) 2_465 1_564
O3 O3 O2 128.01(12) 4_345 1_564
O3 O3 O2 100.8(2) 3_465 1_564
O2 O3 O2 69.8(3) 4_455 1_564
O3 O3 O2 129.2(3) 2_466 1_564
O2 O3 O2 120.3(4) 3_455 1_564
O2 O3 O2 123.0(2) 5_456 1_564
O3 O3 O2 78.9(4) 6 1_564
O1 O3 O2 67.0(4) . 1_564
O2 O3 O2 46.97(14) 5_455 1_564
O3 O3 O2 175.94(14) 6_556 1_564
Ga2 O3 O2 91.89(19) 2_566 1_564
Ga3 O3 O2 141.0(2) 4_346 1_564
La O3 O2 81.8(2) . 1_564
O2 O3 O2 55.9(2) 1_565 1_564
O3 O3 O2 78.9(3) 5_345 1_564
Ga3 O3 O2 54.12(16) . 1_564
Ga2 O3 O2 70.97(15) 1_565 1_564
O3 O3 O2 142.03(19) 5_346 1_564
Nb O3 O2 153.2(2) 1_456 1_564
Ga1 O3 O2 153.2(2) 1_456 1_564
O2 O3 O2 88.4(3) 2_566 1_564
La O3 O2 111.3(3) 2_455 1_564
Ga3 O3 O2 43.54(12) 2_464 1_564
O1 O3 O2 28.0(2) 2_465 1_564
La O3 O2 112.97(15) 4_456 1_564
O2 O3 O2 107.2(2) 6_456 1_564
O2 O3 O2 26.35(19) 2_565 1_564
Ga2 O3 O2 128.1(2) . 1_564
O2 O3 O2 56.20(15) 6_455 1_564
La O3 O2 57.03(12) 2_465 1_564
Ga2 O3 O2 37.23(10) 2_565 1_564
O1 O3 O2 90.6(2) 2_466 1_564
O2 O3 O2 121.2(3) 1_455 1_564
O1 O3 O2 92.8(3) 2_455 1_564
La O3 O2 90.11(16) 1_455 1_564
Ga3 O3 O2 68.12(13) 4_456 1_564
Ga3 O3 O2 77.53(18) 4_345 1_564
O3 O3 O2 140.84(13) 1_556 1_564
O3 O3 O2 39.16(13) 1_554 1_564
O2 O3 O2 98.5(2) 6_556 1_564
O2 O3 O2 152.4(2) 2_456 1_564
La O3 O2 130.09(16) 1_556 1_564
O2 O3 O2 126.1(3) 4_445 1_564
O1 O3 O2 142.0(3) 2_456 1_564
O2 O3 O2 53.87(15) 6 1_564
O2 O3 O2 60.02(12) 3_465 1_564
O2 O3 O2 96.60(19) 2_455 1_564
O1 O3 O2 82.6(2) 1_455 1_564
Ga2 O3 O2 16.76(7) 1_564 1_564
O3 O3 O2 89.53(9) 3_565 1_564
O3 O3 O2 56.57(13) 4_455 1_564
O2 O3 O2 110.9(3) . 1_564
O2 O3 O2 26.95(14) 4_454 1_564
O2 O3 O2 63.1(2) 3_454 1_564
Ga2 O3 O2 96.83(13) 2_466 1_564
La O3 O2 56.15(11) 2_565 1_564
La O3 O2 167.9(2) 2_456 1_564
O1 O3 O2 118.00(17) 1_556 1_564
O3 O3 O2 66.68(14) 4_344 1_564
O3 O3 O2 166.8(2) 4_346 1_564
O3 O3 O2 53.34(13) 3_464 1_564
O3 O3 O2 140.6(2) 3_466 1_564
O1 O3 O2 126.1(3) 1_445 1_564
La O3 O2 103.04(13) 2_466 1_564
Ga3 O3 La 137.0(4) 1_556 1_565
Nb O3 La 108.9(3) 1_455 1_565
Ga1 O3 La 108.9(3) 1_455 1_565
La O3 La 27.65(16) 4_455 1_565
Ga3 O3 La 77.61(15) 2_465 1_565
O3 O3 La 66.27(18) 2_465 1_565
O3 O3 La 153.0(3) 4_345 1_565
O3 O3 La 95.2(3) 3_465 1_565
O2 O3 La 38.4(2) 4_455 1_565
O3 O3 La 88.9(2) 2_466 1_565
O2 O3 La 143.1(3) 3_455 1_565
O2 O3 La 101.8(2) 5_456 1_565
O3 O3 La 118.2(4) 6 1_565
O1 O3 La 70.49(14) . 1_565
O2 O3 La 83.3(2) 5_455 1_565
O3 O3 La 139.1(5) 6_556 1_565
Ga2 O3 La 78.21(11) 2_566 1_565
Ga3 O3 La 136.6(2) 4_346 1_565
La O3 La 106.65(17) . 1_565
O2 O3 La 20.30(19) 1_565 1_565
O3 O3 La 101.0(2) 5_345 1_565
Ga3 O3 La 94.62(18) . 1_565
Ga2 O3 La 30.85(7) 1_565 1_565
O3 O3 La 115.82(13) 5_346 1_565
Nb O3 La 113.4(2) 1_456 1_565
Ga1 O3 La 113.4(2) 1_456 1_565
O2 O3 La 61.27(15) 2_566 1_565
La O3 La 151.7(3) 2_455 1_565
Ga3 O3 La 69.01(10) 2_464 1_565
O1 O3 La 21.2(2) 2_465 1_565
La O3 La 75.26(10) 4_456 1_565
O2 O3 La 76.98(17) 6_456 1_565
O2 O3 La 47.66(11) 2_565 1_565
Ga2 O3 La 145.93(16) . 1_565
O2 O3 La 64.76(14) 6_455 1_565
La O3 La 42.68(6) 2_465 1_565
Ga2 O3 La 68.98(10) 2_565 1_565
O1 O3 La 50.1(2) 2_466 1_565
O2 O3 La 125.54(18) 1_455 1_565
O1 O3 La 129.4(3) 2_455 1_565
La O3 La 93.53(12) 1_455 1_565
Ga3 O3 La 39.81(5) 4_456 1_565
Ga3 O3 La 108.93(17) 4_345 1_565
O3 O3 La 101.48(12) 1_556 1_565
O3 O3 La 78.52(12) 1_554 1_565
O2 O3 La 87.62(14) 6_556 1_565
O2 O3 La 149.0(2) 2_456 1_565
La O3 La 113.46(14) 1_556 1_565
O2 O3 La 159.5(2) 4_445 1_565
O1 O3 La 141.34(18) 2_456 1_565
O2 O3 La 76.85(14) 6 1_565
O2 O3 La 23.14(11) 3_465 1_565
O2 O3 La 129.1(2) 2_455 1_565
O1 O3 La 69.98(10) 1_455 1_565
Ga2 O3 La 35.59(5) 1_564 1_565
O3 O3 La 100.88(11) 3_565 1_565
O3 O3 La 42.41(12) 4_455 1_565
O2 O3 La 130.98(18) . 1_565
O2 O3 La 53.95(11) 4_454 1_565
O2 O3 La 103.3(2) 3_454 1_565
Ga2 O3 La 74.43(9) 2_466 1_565
La O3 La 61.26(7) 2_565 1_565
La O3 La 148.0(2) 2_456 1_565
O1 O3 La 89.51(12) 1_556 1_565
O3 O3 La 104.01(14) 4_344 1_565
O3 O3 La 126.42(16) 4_346 1_565
O3 O3 La 82.37(16) 3_464 1_565
O3 O3 La 102.6(2) 3_466 1_565
O1 O3 La 157.6(2) 1_445 1_565
La O3 La 65.54(9) 2_466 1_565
O2 O3 La 40.54(10) 1_564 1_565
Ga3 O3 O2 71.2(4) 1_556 4_456
Nb O3 O2 123.8(4) 1_455 4_456
Ga1 O3 O2 123.8(4) 1_455 4_456
La O3 O2 103.0(3) 4_455 4_456
Ga3 O3 O2 38.4(2) 2_465 4_456
O3 O3 O2 130.7(5) 2_465 4_456
O3 O3 O2 103.99(15) 4_345 4_456
O3 O3 O2 77.17(19) 3_465 4_456
O2 O3 O2 55.5(3) 4_455 4_456
O3 O3 O2 10.60(16) 2_466 4_456
O2 O3 O2 110.7(5) 3_455 4_456
O2 O3 O2 60.5(3) 5_456 4_456
O3 O3 O2 155.3(3) 6 4_456
O1 O3 O2 101.5(4) . 4_456
O2 O3 O2 153.4(3) 5_455 4_456
O3 O3 O2 61.3(3) 6_556 4_456
Ga2 O3 O2 74.8(2) 2_566 4_456
Ga3 O3 O2 76.7(2) 4_346 4_456
La O3 O2 130.5(2) . 4_456
O2 O3 O2 66.4(3) 1_565 4_456
O3 O3 O2 119.5(3) 5_345 4_456
Ga3 O3 O2 170.7(2) . 4_456
Ga2 O3 O2 47.93(16) 1_565 4_456
O3 O3 O2 50.4(2) 5_346 4_456
Nb O3 O2 35.20(12) 1_456 4_456
Ga1 O3 O2 35.20(12) 1_456 4_456
O2 O3 O2 56.18(18) 2_566 4_456
La O3 O2 129.3(2) 2_455 4_456
Ga3 O3 O2 124.63(19) 2_464 4_456
O1 O3 O2 93.4(3) 2_465 4_456
La O3 O2 25.14(10) 4_456 4_456
O2 O3 O2 37.8(2) 6_456 4_456
O2 O3 O2 118.1(2) 2_565 4_456
Ga2 O3 O2 102.8(2) . 4_456
O2 O3 O2 102.1(2) 6_455 4_456
La O3 O2 77.66(17) 2_465 4_456
Ga2 O3 O2 138.26(16) 2_565 4_456
O1 O3 O2 28.5(2) 2_466 4_456
O2 O3 O2 87.1(2) 1_455 4_456
O1 O3 O2 143.7(3) 2_455 4_456
La O3 O2 90.86(18) 1_455 4_456
Ga3 O3 O2 64.16(15) 4_456 4_456
Ga3 O3 O2 136.06(19) 4_345 4_456
O3 O3 O2 27.64(11) 1_556 4_456
O3 O3 O2 152.36(11) 1_554 4_456
O2 O3 O2 77.5(2) 6_556 4_456
O2 O3 O2 78.2(2) 2_456 4_456
La O3 O2 67.39(16) 1_556 4_456
O2 O3 O2 113.0(3) 4_445 4_456
O1 O3 O2 84.2(3) 2_456 4_456
O2 O3 O2 128.97(18) 6 4_456
O2 O3 O2 59.98(16) 3_465 4_456
O2 O3 O2 129.8(2) 2_455 4_456
O1 O3 O2 70.9(3) 1_455 4_456
Ga2 O3 O2 109.30(15) 1_564 4_456
O3 O3 O2 109.17(10) 3_565 4_456
O3 O3 O2 83.13(12) 4_455 4_456
O2 O3 O2 113.1(3) . 4_456
O2 O3 O2 121.4(2) 4_454 4_456
O2 O3 O2 176.5(2) 3_454 4_456
Ga2 O3 O2 53.60(13) 2_466 4_456
La O3 O2 104.22(16) 2_565 4_456
La O3 O2 71.16(17) 2_456 4_456
O1 O3 O2 47.69(15) 1_556 4_456
O3 O3 O2 153.6(2) 4_344 4_456
O3 O3 O2 48.02(10) 4_346 4_456
O3 O3 O2 132.7(2) 3_464 4_456
O3 O3 O2 27.56(12) 3_466 4_456
O1 O3 O2 109.5(3) 1_445 4_456
La O3 O2 23.10(9) 2_466 4_456
O2 O3 O2 118.86(14) 1_564 4_456
La O3 O2 78.42(13) 1_565 4_456
Ga3 O3 La 75.7(4) 1_556 1_456
Nb O3 La 81.5(3) 1_455 1_456
Ga1 O3 La 81.5(3) 1_455 1_456
La O3 La 129.6(3) 4_455 1_456
Ga3 O3 La 24.89(12) 2_465 1_456
O3 O3 La 111.3(4) 2_465 1_456
O3 O3 La 66.15(17) 4_345 1_456
O3 O3 La 39.04(9) 3_465 1_456
O2 O3 La 64.7(3) 4_455 1_456
O3 O3 La 37.49(15) 2_466 1_456
O2 O3 La 108.3(3) 3_455 1_456
O2 O3 La 90.4(3) 5_456 1_456
O3 O3 La 112.07(17) 6 1_456
O1 O3 La 144.4(5) . 1_456
O2 O3 La 161.9(3) 5_455 1_456
O3 O3 La 53.16(15) 6_556 1_456
Ga2 O3 La 115.1(3) 2_566 1_456
Ga3 O3 La 37.87(12) 4_346 1_456
La O3 La 147.8(2) . 1_456
O2 O3 La 101.0(3) 1_565 1_456
O3 O3 La 79.3(3) 5_345 1_456
Ga3 O3 La 133.88(17) . 1_456
Ga2 O3 La 75.32(17) 1_565 1_456
O3 O3 La 13.58(6) 5_346 1_456
Nb O3 La 32.95(8) 1_456 1_456
Ga1 O3 La 32.95(8) 1_456 1_456
O2 O3 La 99.8(3) 2_566 1_456
La O3 La 97.07(14) 2_455 1_456
Ga3 O3 La 101.36(14) 2_464 1_456
O1 O3 La 104.2(2) 2_465 1_456
La O3 La 67.54(16) 4_456 1_456
O2 O3 La 25.47(15) 6_456 1_456
O2 O3 La 149.87(18) 2_565 1_456
Ga2 O3 La 101.15(17) . 1_456
O2 O3 La 80.05(18) 6_455 1_456
La O3 La 73.13(13) 2_465 1_456
Ga2 O3 La 166.88(18) 2_565 1_456
O1 O3 La 63.93(19) 2_466 1_456
O2 O3 La 43.63(16) 1_455 1_456
O1 O3 La 127.26(17) 2_455 1_456
La O3 La 53.43(10) 1_455 1_456
Ga3 O3 La 106.0(2) 4_456 1_456
Ga3 O3 La 93.50(12) 4_345 1_456
O3 O3 La 50.98(10) 1_556 1_456
O3 O3 La 129.02(10) 1_554 1_456
O2 O3 La 114.5(3) 6_556 1_456
O2 O3 La 46.74(12) 2_456 1_456
La O3 La 90.23(18) 1_556 1_456
O2 O3 La 97.30(19) 4_445 1_456
O1 O3 La 87.6(2) 2_456 1_456
O2 O3 La 172.0(2) 6 1_456
O2 O3 La 79.26(17) 3_465 1_456
O2 O3 La 86.52(15) 2_455 1_456
O1 O3 La 48.7(2) 1_455 1_456
Ga2 O3 La 113.46(14) 1_564 1_456
O3 O3 La 137.70(11) 3_565 1_456
O3 O3 La 125.16(15) 4_455 1_456
O2 O3 La 118.8(2) . 1_456
O2 O3 La 110.94(17) 4_454 1_456
O2 O3 La 137.90(16) 3_454 1_456
Ga2 O3 La 33.30(7) 2_466 1_456
La O3 La 147.9(2) 2_565 1_456
La O3 La 61.50(11) 2_456 1_456
O1 O3 La 83.8(2) 1_556 1_456
O3 O3 La 111.49(17) 4_344 1_456
O3 O3 La 41.78(12) 4_346 1_456
O3 O3 La 101.05(17) 3_464 1_456
O3 O3 La 23.02(12) 3_466 1_456
O1 O3 La 73.41(17) 1_445 1_456
La O3 La 40.25(8) 2_466 1_456
O2 O3 La 130.13(15) 1_564 1_456
La O3 La 102.38(14) 1_565 1_456
O2 O3 La 43.73(11) 4_456 1_456
Ga3 O3 O3 134.2(4) 1_556 5_455
Nb O3 O3 110.4(4) 1_455 5_455
Ga1 O3 O3 110.4(4) 1_455 5_455
La O3 O3 7.42(10) 4_455 5_455
Ga3 O3 O3 100.07(13) 2_465 5_455
O3 O3 O3 62.53(19) 2_465 5_455
O3 O3 O3 156.2(2) 4_345 5_455
O3 O3 O3 113.2(3) 3_465 5_455
O2 O3 O3 60.7(2) 4_455 5_455
O3 O3 O3 106.3(2) 2_466 5_455
O2 O3 O3 122.8(3) 3_455 5_455
O2 O3 O3 98.6(3) 5_456 5_455
O3 O3 O3 105.5(5) 6 5_455
O1 O3 O3 52.4(2) . 5_455
O2 O3 O3 62.4(2) 5_455 5_455
O3 O3 O3 149.2(5) 6_556 5_455
Ga2 O3 O3 69.11(15) 2_566 5_455
Ga3 O3 O3 157.5(2) 4_346 5_455
La O3 O3 84.6(2) . 5_455
O2 O3 O3 29.51(19) 1_565 5_455
O3 O3 O3 104.7(4) 5_345 5_455
Ga3 O3 O3 79.1(3) . 5_455
Ga2 O3 O3 51.10(5) 1_565 5_455
O3 O3 O3 138.15(19) 5_346 5_455
Nb O3 O3 130.6(3) 1_456 5_455
Ga1 O3 O3 130.6(3) 1_456 5_455
O2 O3 O3 60.73(19) 2_566 5_455
La O3 O3 134.4(4) 2_455 5_455
Ga3 O3 O3 69.0(2) 2_464 5_455
O1 O3 O3 29.34(7) 2_465 5_455
La O3 O3 85.24(17) 4_456 5_455
O2 O3 O3 99.43(17) 6_456 5_455
O2 O3 O3 25.49(15) 2_565 5_455
Ga2 O3 O3 127.7(2) . 5_455
O2 O3 O3 74.19(19) 6_455 5_455
La O3 O3 60.40(7) 2_465 5_455
Ga2 O3 O3 47.30(16) 2_565 5_455
O1 O3 O3 67.8(2) 2_466 5_455
O2 O3 O3 141.5(2) 1_455 5_455
O1 O3 O3 107.5(3) 2_455 5_455
La O3 O3 107.55(18) 1_455 5_455
Ga3 O3 O3 39.96(10) 4_456 5_455
Ga3 O3 O3 105.6(3) 4_345 5_455
O3 O3 O3 113.4(2) 1_556 5_455
O3 O3 O3 66.6(2) 1_554 5_455
O2 O3 O3 77.51(19) 6_556 5_455
O2 O3 O3 171.4(2) 2_456 5_455
La O3 O3 108.27(19) 1_556 5_455
O2 O3 O3 137.3(3) 4_445 5_455
O1 O3 O3 131.24(19) 2_456 5_455
O2 O3 O3 54.49(17) 6 5_455
O2 O3 O3 45.55(10) 3_465 5_455
O2 O3 O3 124.8(3) 2_455 5_455
O1 O3 O3 88.98(14) 1_455 5_455
Ga2 O3 O3 34.17(12) 1_564 5_455
O3 O3 O3 81.82(15) 3_565 5_455
O3 O3 O3 31.1(2) 4_455 5_455
O2 O3 O3 110.8(2) . 5_455
O2 O3 O3 51.86(17) 4_454 5_455
O2 O3 O3 85.1(3) 3_454 5_455
Ga2 O3 O3 96.15(8) 2_466 5_455
La O3 O3 41.91(10) 2_565 5_455
La O3 O3 152.8(3) 2_456 5_455
O1 O3 O3 90.8(2) 1_556 5_455
O3 O3 O3 94.5(2) 4_344 5_455
O3 O3 O3 141.2(2) 4_346 5_455
O3 O3 O3 80.5(2) 3_464 5_455
O3 O3 O3 122.3(3) 3_466 5_455
O1 O3 O3 153.7(4) 1_445 5_455
La O3 O3 86.82(12) 2_466 5_455
O2 O3 O3 28.20(16) 1_564 5_455
La O3 O3 22.46(5) 1_565 5_455
O2 O3 O3 95.8(2) 4_456 5_455
La O3 O3 124.80(16) 1_456 5_455
Ga3 O3 O3 78.1(2) 1_556 5_445
Nb O3 O3 98.7(4) 1_455 5_445
Ga1 O3 O3 98.7(4) 1_455 5_445
La O3 O3 78.2(4) 4_455 5_445
Ga3 O3 O3 172.6(5) 2_465 5_445
O3 O3 O3 88.5(6) 2_465 5_445
O3 O3 O3 93.0(2) 4_345 5_445
O3 O3 O3 145.1(3) 3_465 5_445
O2 O3 O3 142.8(4) 4_455 5_445
O3 O3 O3 133.6(4) 2_466 5_445
O2 O3 O3 43.2(2) 3_455 5_445
O2 O3 O3 74.8(3) 5_456 5_445
O3 O3 O3 62.40(18) 6 5_445
O1 O3 O3 42.8(2) . 5_445
O2 O3 O3 34.3(2) 5_455 5_445
O3 O3 O3 99.27(11) 6_556 5_445
Ga2 O3 O3 62.02(18) 2_566 5_445
Ga3 O3 O3 118.39(11) 4_346 5_445
La O3 O3 4.67(6) . 5_445
O2 O3 O3 100.7(3) 1_565 5_445
O3 O3 O3 104.7(4) 5_345 5_445
Ga3 O3 O3 53.0(2) . 5_445
Ga2 O3 O3 126.9(2) 1_565 5_445
O3 O3 O3 138.15(19) 5_346 5_445
Nb O3 O3 123.8(2) 1_456 5_445
Ga1 O3 O3 123.8(2) 1_456 5_445
O2 O3 O3 84.9(2) 2_566 5_445
La O3 O3 62.22(9) 2_455 5_445
Ga3 O3 O3 97.1(3) 2_464 5_445
O1 O3 O3 104.3(4) 2_465 5_445
La O3 O3 110.4(2) 4_456 5_445
O2 O3 O3 172.2(4) 6_456 5_445
O2 O3 O3 58.1(2) 2_565 5_445
Ga2 O3 O3 50.48(5) . 5_445
O2 O3 O3 120.4(4) 6_455 5_445
La O3 O3 134.6(3) 2_465 5_445
Ga2 O3 O3 40.55(19) 2_565 5_445
O1 O3 O3 130.0(2) 2_466 5_445
O2 O3 O3 121.94(18) 1_455 5_445
O1 O3 O3 30.73(5) 2_455 5_445
La O3 O3 133.3(3) 1_455 5_445
Ga3 O3 O3 88.82(19) 4_456 5_445
Ga3 O3 O3 86.9(2) 4_345 5_445
O3 O3 O3 113.4(2) 1_556 5_445
O3 O3 O3 66.6(2) 1_554 5_445
O2 O3 O3 57.60(18) 6_556 5_445
O2 O3 O3 106.50(11) 2_456 5_445
La O3 O3 70.32(14) 1_556 5_445
O2 O3 O3 55.24(11) 4_445 5_445
O1 O3 O3 65.27(19) 2_456 5_445
O2 O3 O3 27.60(18) 6 5_445
O2 O3 O3 127.0(2) 3_465 5_445
O2 O3 O3 84.10(19) 2_455 5_445
O1 O3 O3 153.6(4) 1_455 5_445
Ga2 O3 O3 94.1(3) 1_564 5_445
O3 O3 O3 25.4(2) 3_565 5_445
O3 O3 O3 71.93(17) 4_455 5_445
O2 O3 O3 33.11(14) . 5_445
O2 O3 O3 92.7(3) 4_454 5_445
O2 O3 O3 42.14(19) 3_454 5_445
Ga2 O3 O3 171.7(3) 2_466 5_445
La O3 O3 47.23(15) 2_565 5_445
La O3 O3 90.35(11) 2_456 5_445
O1 O3 O3 86.9(2) 1_556 5_445
O3 O3 O3 71.0(2) 4_344 5_445
O3 O3 O3 112.0(2) 4_346 5_445
O3 O3 O3 92.0(2) 3_464 5_445
O3 O3 O3 137.3(2) 3_466 5_445
O1 O3 O3 85.20(11) 1_445 5_445
La O3 O3 153.2(2) 2_466 5_445
O2 O3 O3 77.8(3) 1_564 5_445
La O3 O3 104.4(2) 1_565 5_445
O2 O3 O3 134.5(3) 4_456 5_445
La O3 O3 151.52(19) 1_456 5_445
O3 O3 O3 82.1(2) 5_455 5_445
Ga3 O3 O2 16.6(3) 1_556 3_456
Nb O3 O2 123.9(3) 1_455 3_456
Ga1 O3 O2 123.9(3) 1_455 3_456
La O3 O2 131.3(3) 4_455 3_456
Ga3 O3 O2 83.6(3) 2_465 3_456
O3 O3 O2 171.2(3) 2_465 3_456
O3 O3 O2 77.34(18) 4_345 3_456
O3 O3 O2 104.09(12) 3_465 3_456
O2 O3 O2 110.7(5) 4_455 3_456
O3 O3 O2 48.0(3) 2_466 3_456
O2 O3 O2 55.6(3) 3_455 3_456
O2 O3 O2 28.6(2) 5_456 3_456
O3 O3 O2 117.5(3) 6 3_456
O1 O3 O2 86.3(4) . 3_456
O2 O3 O2 123.7(3) 5_455 3_456
O3 O3 O2 24.7(2) 6_556 3_456
Ga2 O3 O2 59.75(18) 2_566 3_456
Ga3 O3 O2 67.40(18) 4_346 3_456
La O3 O2 84.74(17) . 3_456
O2 O3 O2 103.0(3) 1_565 3_456
O3 O3 O2 129.3(3) 5_345 3_456
Ga3 O3 O2 134.09(19) . 3_456
Ga2 O3 O2 98.2(2) 1_565 3_456
O3 O3 O2 59.9(3) 5_346 3_456
Nb O3 O2 35.25(11) 1_456 3_456
Ga1 O3 O2 35.25(11) 1_456 3_456
O2 O3 O2 65.04(19) 2_566 3_456
La O3 O2 83.77(16) 2_455 3_456
Ga3 O3 O2 164.90(18) 2_464 3_456
O1 O3 O2 143.2(3) 2_465 3_456
La O3 O2 48.09(14) 4_456 3_456
O2 O3 O2 83.5(2) 6_456 3_456
O2 O3 O2 126.8(2) 2_565 3_456
Ga2 O3 O2 47.66(13) . 3_456
O2 O3 O2 147.9(3) 6_455 3_456
La O3 O2 132.2(3) 2_465 3_456
Ga2 O3 O2 124.89(17) 2_565 3_456
O1 O3 O2 78.3(3) 2_466 3_456
O2 O3 O2 87.2(2) 1_455 3_456
O1 O3 O2 88.5(3) 2_455 3_456
La O3 O2 116.6(2) 1_455 3_456
Ga3 O3 O2 86.56(18) 4_456 3_456
Ga3 O3 O2 127.56(15) 4_345 3_456
O3 O3 O2 27.57(13) 1_556 3_456
O3 O3 O2 152.43(13) 1_554 3_456
O2 O3 O2 53.63(16) 6_556 3_456
O2 O3 O2 55.7(2) 2_456 3_456
La O3 O2 23.16(9) 1_556 3_456
O2 O3 O2 60.26(14) 4_445 3_456
O1 O3 O2 29.0(2) 2_456 3_456
O2 O3 O2 105.64(19) 6 3_456
O2 O3 O2 112.3(3) 3_465 3_456
O2 O3 O2 107.3(2) 2_455 3_456
O1 O3 O2 115.7(3) 1_455 3_456
Ga2 O3 O2 157.90(18) 1_564 3_456
O3 O3 O2 69.82(14) 3_565 3_456
O3 O3 O2 95.43(11) 4_455 3_456
O2 O3 O2 59.52(14) . 3_456
O2 O3 O2 176.3(2) 4_454 3_456
O2 O3 O2 121.59(18) 3_454 3_456
Ga2 O3 O2 98.1(2) 2_466 3_456
La O3 O2 96.62(15) 2_565 3_456
La O3 O2 27.70(10) 2_456 3_456
O1 O3 O2 34.96(13) 1_556 3_456
O3 O3 O2 132.85(19) 4_344 3_456
O3 O3 O2 27.67(12) 4_346 3_456
O3 O3 O2 153.78(19) 3_464 3_456
O3 O3 O2 48.04(10) 3_466 3_456
O1 O3 O2 77.0(2) 1_445 3_456
La O3 O2 77.40(17) 2_466 3_456
O2 O3 O2 151.55(16) 1_564 3_456
La O3 O2 122.56(19) 1_565 3_456
O2 O3 O2 55.19(19) 4_456 3_456
La O3 O2 67.89(15) 1_456 3_456
O3 O3 O2 125.6(2) 5_455 3_456
O3 O3 O2 89.40(18) 5_445 3_456
Ga3 O3 O1 123.9(4) 1_556 1_554
Nb O3 O1 81.4(4) 1_455 1_554
Ga1 O3 O1 81.4(4) 1_455 1_554
La O3 O1 43.7(2) 4_455 1_554
Ga3 O3 O1 140.3(3) 2_465 1_554
O3 O3 O1 46.9(4) 2_465 1_554
O3 O3 O1 110.47(17) 4_345 1_554
O3 O3 O1 119.58(15) 3_465 1_554
O2 O3 O1 103.5(4) 4_455 1_554
O3 O3 O1 155.47(10) 2_466 1_554
O2 O3 O1 86.9(4) 3_455 1_554
O2 O3 O1 111.2(3) 5_456 1_554
O3 O3 O1 58.3(3) 6 1_554
O1 O3 O1 54.3(3) . 1_554
O2 O3 O1 13.29(14) 5_455 1_554
O3 O3 O1 144.1(3) 6_556 1_554
Ga2 O3 O1 84.3(2) 2_566 1_554
Ga3 O3 O1 137.1(3) 4_346 1_554
La O3 O1 50.25(16) . 1_554
O2 O3 O1 79.5(3) 1_565 1_554
O3 O3 O1 81.8(4) 5_345 1_554
Ga3 O3 O1 32.07(12) . 1_554
Ga2 O3 O1 101.18(17) 1_565 1_554
O3 O3 O1 160.9(4) 5_346 1_554
Nb O3 O1 168.9(2) 1_456 1_554
Ga1 O3 O1 168.9(2) 1_456 1_554
O2 O3 O1 94.8(2) 2_566 1_554
La O3 O1 83.8(2) 2_455 1_554
Ga3 O3 O1 56.78(17) 2_464 1_554
O1 O3 O1 61.7(2) 2_465 1_554
La O3 O1 127.20(18) 4_456 1_554
O2 O3 O1 140.2(2) 6_456 1_554
O2 O3 O1 27.40(17) 2_565 1_554
Ga2 O3 O1 94.88(19) . 1_554
O2 O3 O1 78.2(2) 6_455 1_554
La O3 O1 89.11(17) 2_465 1_554
Ga2 O3 O1 10.67(12) 2_565 1_554
O1 O3 O1 118.3(3) 2_466 1_554
O2 O3 O1 123.1(3) 1_455 1_554
O1 O3 O1 59.8(2) 2_455 1_554
La O3 O1 105.4(2) 1_455 1_554
Ga3 O3 O1 82.17(16) 4_456 1_554
Ga3 O3 O1 70.49(18) 4_345 1_554
O3 O3 O1 149.49(13) 1_556 1_554
O3 O3 O1 30.51(13) 1_554 1_554
O2 O3 O1 86.4(2) 6_556 1_554
O2 O3 O1 136.1(2) 2_456 1_554
La O3 O1 111.62(19) 1_556 1_554
O2 O3 O1 93.0(2) 4_445 1_554
O1 O3 O1 111.0(3) 2_456 1_554
O2 O3 O1 29.16(17) 6 1_554
O2 O3 O1 92.48(18) 3_465 1_554
O2 O3 O1 82.8(2) 2_455 1_554
O1 O3 O1 110.5(3) 1_455 1_554
Ga2 O3 O1 48.95(11) 1_564 1_554
O3 O3 O1 63.92(11) 3_565 1_554
O3 O3 O1 63.92(11) 4_455 1_554
O2 O3 O1 78.5(2) . 1_554
O2 O3 O1 47.83(16) 4_454 1_554
O2 O3 O1 34.81(12) 3_454 1_554
Ga2 O3 O1 127.46(18) 2_466 1_554
La O3 O1 47.35(14) 2_565 1_554
La O3 O1 134.28(17) 2_456 1_554
O1 O3 O1 116.08(13) 1_556 1_554
O3 O3 O1 53.36(14) 4_344 1_554
O3 O3 O1 157.7(2) 4_346 1_554
O3 O3 O1 58.04(13) 3_464 1_554
O3 O3 O1 172.94(19) 3_466 1_554
O1 O3 O1 104.9(3) 1_445 1_554
La O3 O1 135.85(12) 2_466 1_554
O2 O3 O1 33.70(10) 1_564 1_554
La O3 O1 70.57(11) 1_565 1_554
O2 O3 O1 145.53(15) 4_456 1_554
La O3 O1 158.1(2) 1_456 1_554
O3 O3 O1 50.62(18) 5_455 1_554
O3 O3 O1 45.8(2) 5_445 1_554
O2 O3 O1 133.66(19) 3_456 1_554
Ga3 O3 La 84.9(2) 1_556 4_345
Nb O3 La 29.69(19) 1_455 4_345
Ga1 O3 La 29.69(19) 1_455 4_345
La O3 La 134.3(3) 4_455 4_345
Ga3 O3 La 80.46(16) 2_465 4_345
O3 O3 La 77.76(10) 2_465 4_345
O3 O3 La 19.3(2) 4_345 4_345
O3 O3 La 45.3(2) 3_465 4_345
O2 O3 La 106.6(2) 4_455 4_345
O3 O3 La 98.85(13) 2_466 4_345
O2 O3 La 79.2(2) 3_455 4_345
O2 O3 La 121.2(2) 5_456 4_345
O3 O3 La 48.14(15) 6 4_345
O1 O3 La 145.3(3) . 4_345
O2 O3 La 99.4(3) 5_455 4_345
O3 O3 La 70.1(2) 6_556 4_345
Ga2 O3 La 147.95(18) 2_566 4_345
Ga3 O3 La 32.61(9) 4_346 4_345
La O3 La 103.16(17) . 4_345
O2 O3 La 151.1(2) 1_565 4_345
O3 O3 La 35.42(18) 5_345 4_345
Ga3 O3 La 73.06(12) . 4_345
Ga2 O3 La 128.85(19) 1_565 4_345
O3 O3 La 57.03(18) 5_346 4_345
Nb O3 La 79.95(12) 1_456 4_345
Ga1 O3 La 79.95(12) 1_456 4_345
O2 O3 La 158.3(3) 2_566 4_345
La O3 La 41.68(6) 2_455 4_345
Ga3 O3 La 70.99(11) 2_464 4_345
O1 O3 La 115.0(2) 2_465 4_345
La O3 La 127.6(2) 4_456 4_345
O2 O3 La 81.33(15) 6_456 4_345
O2 O3 La 130.6(3) 2_565 4_345
Ga2 O3 La 79.00(9) . 4_345
O2 O3 La 69.33(14) 6_455 4_345
La O3 La 92.61(12) 2_465 4_345
Ga2 O3 La 114.1(2) 2_565 4_345
O1 O3 La 126.4(2) 2_466 4_345
O2 O3 La 20.78(13) 1_455 4_345
O1 O3 La 71.95(10) 2_455 4_345
La O3 La 41.83(5) 1_455 4_345
Ga3 O3 La 168.6(2) 4_456 4_345
Ga3 O3 La 36.63(5) 4_345 4_345
O3 O3 La 101.30(12) 1_556 4_345
O3 O3 La 78.70(12) 1_554 4_345
O2 O3 La 138.55(17) 6_556 4_345
O2 O3 La 39.41(15) 2_456 4_345
La O3 La 110.65(13) 1_556 4_345
O2 O3 La 61.15(11) 4_445 4_345
O1 O3 La 84.26(11) 2_456 4_345
O2 O3 La 122.1(2) 6 4_345
O2 O3 La 122.02(17) 3_465 4_345
O2 O3 La 22.59(11) 2_455 4_345
O1 O3 La 69.20(10) 1_455 4_345
Ga2 O3 La 106.12(16) 1_564 4_345
O3 O3 La 118.7(2) 3_565 4_345
O3 O3 La 168.68(12) 4_455 4_345
O2 O3 La 90.01(13) . 4_345
O2 O3 La 88.14(16) 4_454 4_345
O2 O3 La 73.93(14) 3_454 4_345
Ga2 O3 La 73.64(9) 2_466 4_345
La O3 La 147.4(2) 2_565 4_345
La O3 La 67.13(7) 2_456 4_345
O1 O3 La 128.9(2) 1_556 4_345
O3 O3 La 52.00(14) 4_344 4_345
O3 O3 La 74.35(18) 4_346 4_345
O3 O3 La 59.82(15) 3_464 4_345
O3 O3 La 80.98(15) 3_466 4_345
O1 O3 La 24.41(8) 1_445 4_345
La O3 La 101.65(14) 2_466 4_345
O2 O3 La 113.07(19) 1_564 4_345
La O3 La 133.83(14) 1_565 4_345
O2 O3 La 107.22(17) 4_456 4_345
La O3 La 64.20(8) 1_456 4_345
O3 O3 La 140.0(3) 5_455 4_345
O3 O3 La 102.50(14) 5_445 4_345
O2 O3 La 94.34(14) 3_456 4_345
O1 O3 La 105.03(19) 1_554 4_345
Ga3 O3 O3 95.7(4) 1_556 5_456
Nb O3 O3 147.9(3) 1_455 5_456
Ga1 O3 O3 147.9(3) 1_455 5_456
La O3 O3 55.63(12) 4_455 5_456
Ga3 O3 O3 75.9(2) 2_465 5_456
O3 O3 O3 107.22(15) 2_465 5_456
O3 O3 O3 154.7(3) 4_345 5_456
O3 O3 O3 112.9(3) 3_465 5_456
O2 O3 O3 54.57(19) 4_455 5_456
O3 O3 O3 61.2(2) 2_466 5_456
O2 O3 O3 116.0(4) 3_455 5_456
O2 O3 O3 61.6(3) 5_456 5_456
O3 O3 O3 152.5(5) 6 5_456
O1 O3 O3 58.0(3) . 5_456
O2 O3 O3 102.2(3) 5_455 5_456
O3 O3 O3 101.9(5) 6_556 5_456
Ga2 O3 O3 46.05(16) 2_566 5_456
Ga3 O3 O3 128.3(4) 4_346 5_456
La O3 O3 99.68(19) . 5_456
O2 O3 O3 21.4(2) 1_565 5_456
O3 O3 O3 139.31(14) 5_345 5_456
Ga3 O3 O3 125.8(3) . 5_456
Ga2 O3 O3 31.00(4) 1_565 5_456
O3 O3 O3 101.8(4) 5_346 5_456
Nb O3 O3 83.6(3) 1_456 5_456
Ga1 O3 O3 83.6(3) 1_456 5_456
O2 O3 O3 22.74(15) 2_566 5_456
La O3 O3 157.7(2) 2_455 5_456
Ga3 O3 O3 110.31(17) 2_464 5_456
O1 O3 O3 62.5(2) 2_465 5_456
La O3 O3 36.94(16) 4_456 5_456
O2 O3 O3 75.1(2) 6_456 5_456
O2 O3 O3 67.0(2) 2_565 5_456
Ga2 O3 O3 113.4(2) . 5_456
O2 O3 O3 102.19(14) 6_455 5_456
La O3 O3 73.83(4) 2_465 5_456
Ga2 O3 O3 86.70(18) 2_565 5_456
O1 O3 O3 29.98(10) 2_466 5_456
O2 O3 O3 135.7(3) 1_455 5_456
O1 O3 O3 130.8(2) 2_455 5_456
La O3 O3 120.02(14) 1_455 5_456
Ga3 O3 O3 13.02(7) 4_456 5_456
Ga3 O3 O3 150.2(2) 4_345 5_456
O3 O3 O3 65.1(2) 1_556 5_456
O3 O3 O3 114.9(2) 1_554 5_456
O2 O3 O3 54.83(17) 6_556 5_456
O2 O3 O3 127.9(4) 2_456 5_456
La O3 O3 73.5(2) 1_556 5_456
O2 O3 O3 132.4(2) 4_445 5_456
O1 O3 O3 101.7(3) 2_456 5_456
O2 O3 O3 81.22(19) 6 5_456
O2 O3 O3 42.00(12) 3_465 5_456
O2 O3 O3 170.0(2) 2_455 5_456
O1 O3 O3 91.47(13) 1_455 5_456
Ga2 O3 O3 76.31(13) 1_564 5_456
O3 O3 O3 81.92(14) 3_565 5_456
O3 O3 O3 32.2(2) 4_455 5_456
O2 O3 O3 107.45(19) . 5_456
O2 O3 O3 95.03(17) 4_454 5_456
O2 O3 O3 127.9(3) 3_454 5_456
Ga2 O3 O3 83.83(15) 2_466 5_456
La O3 O3 56.06(12) 2_565 5_456
La O3 O3 108.6(3) 2_456 5_456
O1 O3 O3 48.27(18) 1_556 5_456
O3 O3 O3 142.8(3) 4_344 5_456
O3 O3 O3 93.0(2) 4_346 5_456
O3 O3 O3 123.7(2) 3_464 5_456
O3 O3 O3 79.0(3) 3_466 5_456
O1 O3 O3 157.7(4) 1_445 5_456
La O3 O3 54.70(14) 2_466 5_456
O2 O3 O3 76.12(18) 1_564 5_456
La O3 O3 41.33(9) 1_565 5_456
O2 O3 O3 51.6(2) 4_456 5_456
La O3 O3 93.0(2) 1_456 5_456
O3 O3 O3 48.30(8) 5_455 5_456
O3 O3 O3 100.8(2) 5_445 5_456
O2 O3 O3 81.6(3) 3_456 5_456
O1 O3 O3 94.2(2) 1_554 5_456
La O3 O3 156.3(3) 4_345 5_456
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La O3 2.393(8) 3_565
La O3 2.393(8) 5_445
La O2 2.424(9) 3_455
La O2 2.424(9) 5_455
La O1 2.579(8) 2_455
La O1 2.579(8) .
La O2 2.843(11) .
La O2 2.843(11) 6
La Ga2 3.388(2) .
La Ga2 3.388(2) 2_565
La Ga1 3.4654(7) .
La Nb 3.4654(7) .
Ga1 O3 1.977(9) 4_445
Ga1 O3 1.977(9) 5_445
Ga1 O3 1.977(9) 1_655
Ga1 O3 1.977(9) 2_565
Ga1 O3 1.977(9) 6_655
Ga1 O3 1.977(9) 3_565
Ga1 La 3.4654(7) 2
Ga1 La 3.4654(7) 4
Ga1 O2 3.618(9) 2
Ga1 O2 3.618(9) 3
Ga1 O2 3.618(9) 5
Ga2 O2 1.798(9) 4_445
Ga2 O2 1.798(9) .
Ga2 O2 1.798(9) 3_455
Ga2 O1 1.75(2) 2_456
Ga2 O1 3.32(2) 2_455
Ga2 La 3.388(2) 4_445
Ga2 La 3.388(2) 2_455
Ga2 O3 3.477(8) 6_556
Ga2 O3 3.477(8) 2_456
Ga2 O3 3.478(8) 5_446
Ga2 La 3.602(2) 4_446
Ga3 O3 1.815(10) 6
Ga3 O3 1.815(10) 1_554
Ga3 O2 1.865(9) 3_454
Ga3 O2 1.865(9) 5_455
Ga3 O3 2.572(11) 2_465
Ga3 O3 2.572(11) 4_344
Ga3 Nb 3.1662(9) 1_454
Ga3 Nb 3.1662(9) 1_455
Ga3 O1 3.550(10) 1_554
Ga3 O1 3.550(10) 2_455
Ga3 O3 3.650(8) 5_345
Ga3 O3 3.650(8) 3_464
Nb O3 1.977(9) 4_445
Nb O3 1.977(9) 5_445
Nb O3 1.977(9) 1_655
Nb O3 1.977(9) 2_565
Nb O3 1.977(9) 6_655
Nb O3 1.977(9) 3_565
Nb Ga3 3.1662(9) 4_445
Nb Ga3 3.1662(9) 4_446
Nb Ga3 3.1662(9) 1_656
Nb Ga3 3.1662(9) 1_655
Nb Ga3 3.1662(9) 2_565
Nb Ga3 3.1662(9) 2_564
O1 Ga2 1.75(2) 2_566
O1 La 2.579(8) 2_565
O1 La 2.579(8) 4_455
O1 O2 2.96(2) 5_455
O1 O2 2.96(2) 6
O1 O2 2.96(2) 2_565
O1 O2 3.03(2) 6_556
O1 O2 3.03(2) 5_456
O1 O2 3.03(2) 2_566
O1 O3 3.168(8) 3_565
O1 O3 3.168(8) .
O1 O3 3.168(8) 4_455
O1 Ga2 3.32(2) 2_565
O1 Ga3 3.550(10) 2_565
O1 Ga3 3.550(10) 1_556
O1 Ga3 3.550(10) 4_456
O1 O2 3.571(9) 3_455
O1 O2 3.571(9) 4
O1 O2 3.571(9) 1_565
O1 O3 4.395(13) 2_465
O1 O3 4.395(13) 5_445
O1 O3 4.395(13) 6_665
O1 Ga3 4.699(16) 2_564
O1 Ga3 4.699(16) 4_455
O1 Ga1 4.760(4) 1_455
O1 Nb 4.760(4) 1_455
O1 Ga1 4.760(4) 1_565
O1 Nb 4.760(4) 1_565
O1 O2 4.798(9) .
O1 O2 4.798(9) 3_565
O1 O2 4.798(9) 4_455
O1 La 4.782(19) 1_556
O1 La 4.782(19) 2_566
O1 La 4.782(19) 4_456
O1 O3 4.812(18) 2_466
O1 O3 4.812(18) 6_666
O1 O3 4.812(18) 5_446
O1 O3 4.913(15) 6
O1 O3 4.913(15) 5_455
O1 O3 4.913(15) 2_565
O1 Ga2 4.888(6) 1_565
O1 Ga2 4.888(6) 1_665
O1 O1 5.028(16) 2_465
O1 O1 5.028(16) 2_455
O1 O1 5.028(16) 2_565
O1 O1 5.0690 1_554
O1 O1 5.0690 1_556
O1 Ga3 5.286(7) 4_446
O1 Ga3 5.286(7) 2_465
O1 Ga3 5.286(7) 1_666
O1 O3 5.289(14) 6_556
O1 O3 5.289(14) 5_456
O1 O3 5.289(14) 2_566
O1 O3 5.385(9) 1_655
O1 O3 5.385(9) 4_345
O1 O3 5.385(9) 3_575
O1 O2 5.67(2) 3_454
O1 O2 5.67(2) 4_554
O1 O2 5.67(2) 1_564
O1 O1 5.66(2) 2_466
O1 O1 5.66(2) 2_456
O1 O1 5.66(2) 2_566
O1 O3 5.73(2) 3_564
O1 O3 5.73(2) 1_554
O1 O3 5.73(2) 4_454
O1 O3 5.815(7) 4_445
O1 O3 5.815(7) 3_465
O1 O3 5.815(7) 1_665
O1 La 5.888(4) 2_455
O1 La 5.888(4) 4
O1 La 5.888(4) 1_565
O1 O2 6.197(7) 4_445
O1 O2 6.197(7) 1_665
O1 O2 6.197(7) 3_465
O1 O3 6.22(2) 3_566
O2 Ga3 1.865(9) 4_446
O2 La 2.424(9) 4_445
O2 O2 2.765(12) 4_445
O2 O2 2.765(12) 3_455
O2 O3 2.853(12) 3_565
O2 O3 2.844(10) 4_445
O2 O2 2.87(2) 2_556
O2 O1 2.96(2) 2_455
O2 O3 2.986(14) 5_446
O2 O1 3.03(2) 2_456
O2 O3 3.379(17) 5_445
O2 O1 3.571(9) 1_545
O2 Ga2 3.691(9) 2_556
O2 O2 3.76(2) 2
O2 O3 3.866(11) 1_545
O2 La 3.969(13) 4_446
O2 Ga3 4.202(9) 2_455
O2 Ga3 4.197(8) 2_565
O2 La 4.237(11) 1_556
O2 O3 4.236(14) 2_456
O2 La 4.282(8) 2_455
O2 Ga3 4.415(7) 1_556
O2 Ga3 4.393(13) 4_445
O2 O3 4.436(14) 6_656
O2 O3 4.522(13) 2_455
O2 Ga2 4.533(13) 1_554
O2 O2 4.526(12) 5_446
O2 O2 4.526(12) 5_456
O2 La 4.550(7) 2
O2 O3 4.709(13) 6_655
O2 O2 4.722(17) 6_556
O2 Ga1 4.792(10) 1_556
O2 Nb 4.792(10) 1_556
O2 O3 4.831(11) 1_655
O2 Ga2 4.887(8) 2_566
O2 Ga3 4.957(9) 1_546
O2 Ga3 4.953(7) 1_656
O2 O2 5.0690 1_554
O2 O2 5.0690 1_556
O2 O3 5.135(11) 6_556
O2 O2 5.141(16) 5_445
O2 O2 5.141(16) 5_455
O2 O3 5.132(12) 2_566
O2 O2 5.236(15) 6_446
O2 O2 5.236(15) 6_546
O2 La 5.311(10) 2_456
O2 Ga2 5.286(10) 2
O2 O2 5.31(2) 6
O2 O3 5.323(11) 3_455
O2 Ga1 5.336(8) 1_445
O2 Nb 5.336(8) 1_445
O2 O3 5.372(14) 6
O2 O3 5.377(10) 4_345
O2 O3 5.370(13) 2_565
O2 O3 5.480(11) .
O2 O3 5.513(16) 3_566
O2 O3 5.508(18) 4_446
O2 La 5.530(10) 2_556
O2 O1 5.67(2) 1_546
O2 O2 5.654(13) 3
O2 O2 5.654(13) 4
O2 O2 5.774(6) 4_444
O2 O2 5.774(6) 3_454
O2 O2 5.774(6) 4_446
O2 O2 5.774(6) 3_456
O2 O2 5.776(15) 6_445
O2 O2 5.776(15) 6_545
O2 La 5.929(8) 1_545
O2 O3 6.099(17) 1_546
O2 O3 6.106(19) 3_564
O2 O2 6.090(14) 3_445
O2 O2 6.090(14) 4_545
O2 O3 6.102(17) 4_444
O2 O1 6.197(7) 1_445
O2 O3 6.315(12) 6_546
O3 Ga3 1.815(10) 1_556
O3 Nb 1.977(9) 1_455
O3 Ga1 1.977(9) 1_455
O3 La 2.393(8) 4_455
O3 Ga3 2.572(11) 2_465
O3 O3 2.64(2) 2_465
O3 O3 2.693(13) 4_345
O3 O3 2.693(13) 3_465
O3 O2 2.853(12) 4_455
O3 O3 2.82(3) 2_466
O3 O2 2.844(10) 3_455
O3 O2 2.986(14) 5_456
O3 O3 3.18(2) 6
O3 O2 3.379(17) 5_455
O3 O3 3.33(2) 6_556
O3 Ga2 3.477(8) 2_566
O3 Ga3 3.650(8) 4_346
O3 O2 3.866(11) 1_565
O3 O3 3.908(18) 5_345
O3 Ga2 4.004(8) 1_565
O3 O3 4.03(2) 5_346
O3 Nb 4.151(13) 1_456
O3 Ga1 4.151(13) 1_456
O3 O2 4.236(14) 2_566
O3 La 4.240(8) 2_455
O3 Ga3 4.358(11) 2_464
O3 O1 4.395(13) 2_465
O3 La 4.364(12) 4_456
O3 O2 4.436(14) 6_456
O3 O2 4.522(13) 2_565
O3 O2 4.709(13) 6_455
O3 La 4.742(8) 2_465
O3 Ga2 4.793(12) 2_565
O3 O1 4.812(18) 2_466
O3 O2 4.831(11) 1_455
O3 O1 4.913(15) 2_455
O3 La 4.903(8) 1_455
O3 Ga3 4.921(7) 4_456
O3 Ga3 5.069(10) 4_345
O3 O3 5.0690 1_556
O3 O3 5.0690 1_554
O3 O2 5.135(11) 6_556
O3 O2 5.132(12) 2_456
O3 La 5.266(10) 1_556
O3 O2 5.323(11) 4_445
O3 O1 5.289(14) 2_456
O3 O2 5.372(14) 6
O3 O2 5.377(10) 3_465
O3 O2 5.370(13) 2_455
O3 O1 5.385(9) 1_455
O3 Ga2 5.468(10) 1_564
O3 O3 5.465(14) 3_565
O3 O3 5.466(14) 4_455
O3 O2 5.513(16) 4_454
O3 O2 5.508(18) 3_454
O3 Ga2 5.572(10) 2_466
O3 La 5.616(8) 2_565
O3 La 5.595(9) 2_456
O3 O1 5.73(2) 1_556
O3 O3 5.740(6) 4_344
O3 O3 5.740(6) 4_346
O3 O3 5.740(6) 3_464
O3 O3 5.740(6) 3_466
O3 O1 5.815(7) 1_445
O3 La 5.984(12) 2_466
O3 O2 6.099(17) 1_564
O3 La 6.132(7) 1_565
O3 O2 6.106(19) 4_456
O3 La 6.113(11) 1_456
O3 O3 6.156(15) 5_455
O3 O3 6.156(15) 5_445
O3 O2 6.102(17) 3_456
O3 O1 6.22(2) 1_554
O3 La 6.231(7) 4_345
O3 O3 6.232(13) 5_456
